Crystallography Walter Borchardt-Ott Crystallography An Introduction Third Edition Translated by Robert O. Gould 123 Dr. Walter Borchardt-Ott Ludgerusstr. 9 48341 Altenberge Germany walter@borchardt-ott.de Translator Dr. Robert O. Gould 33 Charterhall Road Edinburgh EH9 3HS United Kingdom bob@gould.ca ISBN 978-3-642-16451-4 e-ISBN 978-3-642-16452-1 DOI 10.1007/978-3-642-16452-1 Springer Heidelberg Dordrecht London New York Library of Congress Control Number: 2011921698 © Springer-Verlag Berlin Heidelberg 1993, 1995, 2011 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting reproduction on microﬁlm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Cover design: deblik, Berlin Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com) Dedicated to Sigrid† Preface to the Seventh German and Third English Edition Kristallographie has now appeared, after 32 years, in its seventh edition (Crystallography in its third). The book has changed greatly over these 32 years, and, I hope, for the better! I have always been very keen that it retain its character as a basic text, suitable for use at an early stage in a course of study. I also attach great importance to the exercises – now more than a hundred in number – which give many possibilities for deepening the study. In the last few years, I have become increasingly aware that an increasing number of my readers are undertaking the study of crystallography independently. It thus seems sensible to assist these readers – and not only them – by including material designed to assist their study. Even in the ﬁrst edition (1976), I included a pattern from which to build a model of a crystal, with instructions on how to build others. Unfortunately, this proved to be too diﬃcult for many, so now there are 22 patterns included, which have now been used in Münster for several decades. Genuinely three-dimensional models are of great assistance in determining symmetry, indexing, recognizing forms, and assigning the crystal system and point group of a crystal. Further, they help to give the three-dimensional training that is so important in crystallography. On the other hand, it is diﬃcult to give simple instructions for the building of three-dimensional models. It is, however, my experience that, with practice, drawing the parallel projections of structures can also help the student to appreciate their spatial nature. This book deals with the fundamentals of crystallography. Today, of course, there are many websites available with help in learning more about the subject. A good place to begin is the website of the International Union of Crystallography (IUCr) [www.iucr.org/education/resources] with many helpful suggestions. I am much indebted to Professor Elke Koch and Professor Heidrun Sowa for helpful discussion of symmetry problems. I am also very grateful to Dr. R.O. Gould, who has again translated the revised text with great expertise. Münster Autumn 2008 W. Borchardt-Ott Preface to the Second English Edition This second English edition has been required only 1 12 years after the ﬁrst; it appears shortly before the ﬁfth German edition, of which it is a translation. A major change is the expansion and revision of Chap. 4 by new exercises on the use of the stereographic, orthographic and gnonomic projections, and on indexing. Dr. R. O. Gould has again under taken the translation and has made a thorough revision of the text of the ﬁrst edition. I am very grateful to him for his eﬀorts. I should also like to thank Dr. Wolfgang Engel of Springer Verlag, Heidelberg, very much for his encouragement and his help during a collaboration of more than a decade. Münster Summer 1995 W. Borchardt-Ott Preface to the First English Edition This book is based on the lectures which I have now been giving for more than 20 years to chemists and other scientists at the Westfälische Wilhelms-Universität, Münster. It is a translation of the fourth German edition, which will also be appearing in 1993. It has been my intention to introduce the crystallographic approach in a book which is elementary and easy to understand, and I have thus avoided lengthy mathematical treatments. As will be clear from the contents, topics in crystallography have been covered selectively. For example, crystal structure analysis, crystal physics and crystal optics are only touched on, as they do not ﬁt easily into the scheme of the book. The heart of the book is ﬁrmly ﬁxed in geometrical crystallography. It is from the concept of the space lattice that symmetry operations, Bravais lattices, space groups and point groups are all developed. The symmetry of molecules is described, including the resulting non-crystallographic point groups. The treatment of crystal morphology has been brought into line with the approach used by International Tables for Crystallography. The relationship between point groups and physical properties is indicated. Examples of space groups in all crystal systems are treated. Much emphasis is placed on the correspondence between point groups and space groups. The section on crystal chemistry will serve as an introduction to the ﬁeld. Of the various methods of investigation using X-rays, the powder method is described, and an account is given of the reciprocal lattice. At the end of each chapter are included a large number of exercises, and solutions are given for all of them. The ﬁrst stimulus to have this book translated was given by Professor P. E. Fielding of the University of New England in Armidale (Australia). The translation was undertaken by Dr. R. O. Gould of the University of Edinburgh. I thank Dr. Gould for his enthusiasm and for the trouble he has taken over the translation. It was particularly beneﬁcial that we were able to consider the text together thoroughly. Professor E. Koch and Professor W. Fischer, both of the University of Marburg, have discussed each edition of this book with me, and their criticism has been invaluable. I wish to record my thanks to them also. Münster Autumn 1993 W. Borchardt-Ott Contents 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 2 2.1 The Crystalline State . . . . . . . . . . . . . . . . . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 8 3 3.1 3.2 3.3 3.4 3.4.1 3.4.2 3.4.3 3.5 3.5.1 3.5.1.1 3.5.1.2 3.6 The Lattice and Its Properties . . . Line Lattice . . . . . . . . . . . . . . Plane Lattice . . . . . . . . . . . . . . Space Lattice . . . . . . . . . . . . . . The Designation of Points, Lines and in a Space Lattice . . . . . . . . . . . The Lattice Point uvw . . . . . . . . . Lattice Lines [uvw] . . . . . . . . . . Lattice Planes (hkl) . . . . . . . . . . The Zonal Equation . . . . . . . . . . Applications of the Zonal Equation . Application 1 . . . . . . . . . . . . . Application 2 . . . . . . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Planes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 9 10 10 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 11 12 14 16 17 17 19 20 4 4.1 Crystal Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23 26 5 5.1 5.2 5.3 5.4 5.5 5.6 Morphology . . . . . . . . . . . . . . . . . . . . . . . Relationship Between Crystal Structure and Morphology Fundamentals of Morphology . . . . . . . . . . . . . . Crystal Growth . . . . . . . . . . . . . . . . . . . . . . The Stereographic Projection . . . . . . . . . . . . . . . The Reﬂecting Goniometer . . . . . . . . . . . . . . . . The Wulﬀ Net . . . . . . . . . . . . . . . . . . . . . . . 29 29 30 32 36 38 40 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xiv Contents 5.7 5.8 5.8.1 5.8.2 5.9 Indexing of a Crystal . . . . . . . . . . . . . The Gnomonic and Orthographic Projections The Gnomonic Projection . . . . . . . . . . The Orthographic Projection . . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44 50 50 51 52 6 6.1 6.2 6.3 6.4 6.4.1 6.4.2 6.5 Principles of Symmetry . . . . . Rotation Axes . . . . . . . . . . . The Mirror Plane . . . . . . . . . The Inversion Center . . . . . . . Compound Symmetry Operations Rotoinversion Axes . . . . . . . . Rotoreﬂection Axes . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61 63 66 67 68 70 71 72 7 7.1 7.2 7.2.1 7.2.2 7.2.3 7.2.4 7.2.5 7.2.6 7.3 7.4 7.5 The 14 Bravais Lattices . . . . . . . . . The Primitive Space Lattices (P-Lattices) . The Symmetry of the Primitive Lattices . Symmetry of the Triclinic P-Lattice . . . Symmetry of the Monoclinic P-Lattice . . Symmetry of the Orthorhombic P-Lattice Symmetry of the Tetragonal P-Lattice . . Symmetry of the Hexagonal P-Lattice . . Symmetry of the Cubic P-Lattice . . . . . The Centered Lattices . . . . . . . . . . . The Symmetry of the Centered Lattices . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 75 80 95 96 96 97 99 101 103 103 108 109 8 The Seven Crystal Systems . . . . . . . . . . . . . . . . . . . . . 119 9 9.1 9.2 9.2.1 9.2.2 9.2.3 9.2.4 Point Groups . . . . . . . . . . . . . . . . . . . . . . The 32 Point Groups . . . . . . . . . . . . . . . . . . Crystal Symmetry . . . . . . . . . . . . . . . . . . . . Crystal Forms of the Tetragonal System . . . . . . . . Crystal Forms of the Hexagonal (Trigonal) System . . Crystal Forms of the Cubic System . . . . . . . . . . . Crystal Forms in the Orthorhombic, Monoclinic and Triclinic Systems . . . . . . . . . . . . . . . . . . . . Molecular Symmetry . . . . . . . . . . . . . . . . . . Determination of Point Groups . . . . . . . . . . . . Enantiomorphism . . . . . . . . . . . . . . . . . . . . Point Groups and Physical Properties . . . . . . . . . Optical Activity . . . . . . . . . . . . . . . . . . . . . Optical Activity as a Property of a Crystal . . . . . . . 9.3 9.4 9.5 9.6 9.6.1 9.6.1.1 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 123 128 128 139 139 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 139 147 149 154 154 154 155 Contents 9.6.1.2 9.6.2 9.6.3 9.6.4 9.7 9.8 Optical Activity as a Property of Molecules Piezoelectricity . . . . . . . . . . . . . . . Pyroelectricity . . . . . . . . . . . . . . . . Molecular Dipole Moments . . . . . . . . . Noncrystallographic Point Groups . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 155 155 156 166 166 170 10 10.1 10.1.1 10.1.2 10.2 10.3 10.4 10.5 10.6 10.7 Space Groups . . . . . . . . . . . . . . . . . . . . . . . Glide Planes and Screw Axes . . . . . . . . . . . . . . . Glide Planes . . . . . . . . . . . . . . . . . . . . . . . . Screw Axes . . . . . . . . . . . . . . . . . . . . . . . . . The 230 Space Groups . . . . . . . . . . . . . . . . . . . Properties of Space Groups . . . . . . . . . . . . . . . . International Tables for Crystallography . . . . . . . . . Space Group and Crystal Structure . . . . . . . . . . . . Relationships Between Point Groups and Space Groups Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 189 189 190 193 195 201 210 211 212 215 11 11.1 11.2 11.2.1 11.2.2 11.3 11.4 11.5 Symmetry Groups . . . . . . . . . . . . . . . . . . Representation of Symmetry Operations by Matrices Properties of a Group . . . . . . . . . . . . . . . . . Finite Symmetry Groups . . . . . . . . . . . . . . . Inﬁnite Symmetry Groups . . . . . . . . . . . . . . Derivation of a Few Point Groups . . . . . . . . . . Group Multiplication Tables . . . . . . . . . . . . . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 223 223 237 238 239 239 241 243 12 12.1 12.2 12.3 12.4 12.4.1 12.4.2 12.4.3 12.4.4 12.5 12.6 12.7 12.7.1 12.7.1.1 12.7.1.2 12.7.2 12.7.2.1 12.7.2.2 Fundamentals of Crystal Chemistry . . . . Coordination . . . . . . . . . . . . . . . . . Metal Structures . . . . . . . . . . . . . . . . Structures of Noble Gases and Molecules . . Ionic Structures . . . . . . . . . . . . . . . . Ionic Radii . . . . . . . . . . . . . . . . . . . Octahedral Coordination [6] . . . . . . . . . Cubic Coordination [8] . . . . . . . . . . . . Tetrahedral Coordination [4] . . . . . . . . . Covalent Structures . . . . . . . . . . . . . . Isotypes, Solid Solutions and Isomorphism . Polymorphism . . . . . . . . . . . . . . . . . Transformations of First Coordination . . . . Dilatational Transformations . . . . . . . . . Reconstructive Transformations . . . . . . . Transformations in Secondary Coordination Displacive Transformations . . . . . . . . . . Reconstructive Transformations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 245 246 248 252 253 253 256 258 260 263 264 266 266 266 267 268 268 268 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xv xvi Contents 12.7.3 12.7.4 12.8 12.9 Order-Disorder Transformations . . . . . . . Transformations Involving Changes in Type of Bonding . . . . . . . . . . . . . . . . . . . Further Information on Crystal Structures . . Exercises . . . . . . . . . . . . . . . . . . . . 13 13.1 13.2 13.3 13.4 13.5 13.6 Studies of Crystals by X-Ray Diﬀraction The Bragg Equation . . . . . . . . . . . . . The Debye-Scherrer Method . . . . . . . . The Reciprocal Lattice . . . . . . . . . . . . Laue Groups . . . . . . . . . . . . . . . . . The Determination of a Crystal Structure . Exercises . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 277 277 278 282 287 289 292 14 14.1 14.1.1 14.1.2 14.1.3 14.2 14.2.1 14.2.2 14.3 14.3.1 14.3.2 14.3.3 Crystal Defects . . . . . . . . Point Defects . . . . . . . . . Substitution Defects . . . . . . Solid Solutions . . . . . . . . . Schottky and Frenkel-Defects . Line Defects . . . . . . . . . . Edge Dislocations . . . . . . . Screw Dislocations . . . . . . Plane Defects . . . . . . . . . Small Angle Grain Boundaries Stacking Faults . . . . . . . . . Twin Boundaries . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 293 293 294 294 294 295 295 296 296 296 297 297 15 15.1 15.2 15.2.1 15.2.2 15.3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 301 301 302 302 303 15.4 15.5 15.5.1 Appendix . . . . . . . . . . . . . . . . . . . . . Symbols for Crystallographic Items . . . . . . . Symmetry Elements . . . . . . . . . . . . . . . . Symmetry Elements (Planes) . . . . . . . . . . . Symmetry Elements (Axes) . . . . . . . . . . . . Calculation of Interatomic Distances and Angles in Crystal Structures . . . . . . . . . . . . . . . . Crystal Forms . . . . . . . . . . . . . . . . . . . Patterns for Polyhedra . . . . . . . . . . . . . . . Patterns to Construct Models of Polyhedra . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 305 306 309 309 16 Solutions to the Exercises . . . . . . . . . . . . . . . . . . . . . 321 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 269 . . . . . . . . . . . . 271 . . . . . . . . . . . . 271 . . . . . . . . . . . . 272 Literature References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 347 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 349 Inside Back Cover (Wulﬀ Net) 1 Introduction At the heart of crystallography lies an object – the crystal. Crystallography is concerned with the laws governing the crystalline state of solid materials, with the arrangement of atoms in crystals, and with their physical and chemical properties, their synthesis and their growth. Crystals play a role in many subjects, among them mineralogy, inorganic, organic and physical chemistry, physics, metallurgy, materials science, geology, geophysics, biology and medicine. This pervasiveness is perhaps better understood when it is realized how widespread crystals are: virtually all naturally occurring solids, i.e. minerals, are crystalline, including the raw materials for chemistry, e.g. the ores. A mountain crag normally is made up of crystals of diﬀerent kinds, while an iceberg is made up of many small ice crystals. Virtually all solid inorganic chemicals are crystalline, and many solid organic compounds are made up of crystals, among them benzene, naphthalene, polysaccharides, proteins, vitamins, rubber and nylon. Metals and alloys, ceramics and building materials are all made up of crystals. The inorganic part of teeth and bones is crystalline. Hardening of the arteries and arthritis in humans and animals can be traced to crystal formation. Even many viruses are crystalline. This enumeration could be continued endlessly, but it is already obvious that practically any material that can be regarded as solid is crystalline. Crystallography is a study that overlaps mineralogy, geology, physics, chemistry and biology, and is a unifying factor among these sciences. In many countries, especially in Germany, crystallography is mainly taught as a part of mineralogy, while elsewhere, notably in Britain and North America, it is more often taught as a part of physics or chemistry. The world-wide organization of crystallographers is the International Union of Crystallography (IUCr), which unites many local and regional organizations, themselves made up of biologists, chemists, mineralogists, geologists and physicists. The IUCr publishes the eight-volume International Tables for Crystallography providing essential background information for crystallographers, and eight important scientiﬁc journals, the six parts of Acta Crystallographica, the Journal of Applied Crystallography, and the Journal of Synchrotron Radiation. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_1, C Springer-Verlag Berlin Heidelberg 2011 2 The Crystalline State The outward appearance of a crystal is exceptionally variable, but all the variations which occur can be explained in terms of a single fundamental principle. To grasp this, we must ﬁrst come to terms with the nature of the crystalline state. The following are a few properties that are characteristic of crystals: • Many crystals not only have smooth faces, but, given ideal growth conditions, have regular geometric shapes. Fig. 2.1 shows a crystal of garnet with the form called a rhomb-dodecahedron. This is a polyhedron whose faces are 12 rhombi. Turn to Fig. 15.3, a pattern which you can (and should!) use to make a model of a rhomb-dodecahedron. • If some crystals (e.g. NaCl) are split, the resulting fragments have similar shapes with smooth faces – in the case of NaCl, small cubes. This phenomenon is known as cleavage, and is typical only of crystals. • Figure 2.2 shows a cordierite crystal and the colors that an observer would see when the crystal is viewed from the given directions. The colors that appear depend on the optical absorption of the crystal in that particular direction. For example, if it absorbs all spectral colors from white light except blue, the crystal will appear blue to the observer. When, as in this case, the absorption diﬀers in the three directions, the crystal is said to exhibit pleochroism. Fig. 2.1 A garnet crystal with the shape of a rhombdodecahedron W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_2, C Springer-Verlag Berlin Heidelberg 2011 4 2 The Crystalline State Fig. 2.2 Pleochroism as shown by a crystal of cordierite • When a crystal of kyanite (Al2 OSiO4 ) is scratched parallel to its length with a steel needle, a deep indentation will be made in it, while a scratch perpendicular to the crystal length will leave no mark (see Fig. 2.3). The hardness of this crystal is thus diﬀerent in the two directions. • If one face of a gypsum crystal is covered with a thin layer of wax and a heated metal tip is then applied to that face, the melting front in the wax layer will be ellipsoidal rather than circular (Fig. 2.4), showing that the thermal conductivity is greater in direction III than in direction I. Such behavior – diﬀerent values of a physical property in diﬀerent directions – is called anisotropy, (see also Fig. 2.5c). If the melting front had been circular, as it is, for example, on a piece of glass, it would imply that the thermal conductivity is the same in all directions. Such behavior – the same value of a physical property in all directions – is called isotropy (see Fig. 2.5a, b). Anisotropy of physical properties is normal for crystals. It is, however, not universal, as there are some crystals whose properties are isotropic. If, for example, the above c (010) III I Fig. 2.3 a Fig. 2.4 Fig. 2.3 A crystal of kyanite, with a scratch illustrating the anisotropy of its hardness Fig. 2.4 A crystal of gypsum covered with wax showing the melting front. The ellipse is an isotherm, and shows the anisotropy of the thermal conductivity 2 The Crystalline State Fig. 2.5a–c Schematic representation of the states of matter. (a) gas, (b) liquid, (c) crystal 5 6 2 The Crystalline State experiment with wax had been carried out on a face of a cubic crystal of galena, the melting front would have been circular. Similarly, if a sphere is cut from a crystal of copper, and heated, it will remain spherical as its radius increases. The thermal conductivity in these cases is the same in all directions, and thus isotropic. The origin of all of the phenomena listed above lies in the internal structure of crystals. In order to understand this better, let us now consider the various states of aggregation of matter. All matter, be it gas, liquid or crystal, is composed of atoms, ions or molecules. Matter is thus discontinuous. Since, however, the size of the atoms, ions and molecules lies in the Å region (1 Å = 10–8 cm = 0.1 nm) matter appears to us to be continuous. The states of matter may be distinguished in terms of their tendency to retain a characteristic volume and shape. A gas adopts both the volume and the shape of its container, a liquid has constant volume, but adopts the shape of its container, while a crystal retains both its shape and its volume, independent of its container (see Fig. 2.5). Gases. Figure 2.5a illustrates the arrangement of molecules in a gas at a particular instant in time. The molecules move rapidly through space, and thus have a high kinetic energy. The attractive forces between molecules are comparatively weak, and the corresponding energy of attraction is negligible in comparison to the kinetic energy. What can be said about the distribution of the molecules at that particular instant? There is certainly no accumulation of molecules in particular locations; there is, in fact, a random distribution. A. Johnsen has illustrated this by a simple analogy (Fig. 2.6a): we scatter 128 lentils over the 64 squares of a chessboard, and observe that in this particular case some squares will have no lentils, some 1, 2, or even 3 – but on average 2. If, instead of single squares we considered blocks of four squares, the number of lentils in the area chosen would fall between 7 and 9, while any similar block of 16 squares would have exactly 32 lentils. Thus, two distinct areas of the same size will tend to contain the same number of lentils, and this tendency will increase as the areas considered become larger. This kind of distribution is considered to be statistically homogeneous, i.e. it shows the same behavior Fig. 2.6a, b Statistical (a) and periodic (b) homogeneity after Johnsen 2 The Crystalline State in parallel directions, and it may easily be seen that the physical properties of the distribution are isotropic, i.e. are equal in all directions. Liquids. As the temperature of a gas is lowered, the kinetic energies of the molecules decrease. When the boiling point is reached, the total kinetic energy will be equal to the energy of attraction among the molecules. Further cooling thus converts the gas into a liquid. The attractive forces cause the molecules to “touch” one another. They do not, however, maintain ﬁxed positions, and Fig. 2.5b shows only one of many possible arrangements. The molecules change position continuously. Small regions of order may indeed be found (local ordering), but if a large enough volume is considered, it will also be seen that liquids give a statistically homogeneous arrangement of molecules, and therefore also have isotropic physical properties. Crystals. When the temperature falls below the freezing point, the kinetic energy becomes so small that the molecules become permanently attached to one another. A three-dimensional framework of attractive interactions forms among the molecules and the array becomes solid – it crystallizes. Figure 2.5c shows one possible plane of such a crystal. The movement of molecules in the crystal now consists only of vibrations about a central position. A result of these permanent interactions is that the molecules have become regularly ordered. The distribution of molecules is no longer statistical, but is periodically homogeneous; a periodic distribution in three dimensions has been formed (see also Fig. 3.1a). How can this situation be demonstrated using the chessboard model? (Fig. 2.6b). On each square, there are now precisely two lentils, periodically arranged with respect to one another. The ordering of the lentils parallel to the edges and that along the diagonals are clearly diﬀerent, and therefore the physical properties in these directions will no longer be the same, but distinguishable – in other words, the crystal has acquired anisotropic properties. This anisotropy is characteristic of the crystalline state. D A crystal is an anisotropic, homogeneous body consisting of a threedimensional periodic ordering of atoms, ions or molecules. All matter tends to crystallize, if the temperature is suﬃciently low, since the ordered crystalline phase is the state of lowest energy. There exist, however, materials, such as glass, which never reach this condition. Molten glass is very viscous, and the atoms of which it is made cannot come into a three-dimensional periodic order rapidly enough as the mass cools. Glasses thus have a higher energy content than the corresponding crystals and can best be considered as a frozen, viscous liquid. They are amorphous or “formless” bodies. Such materials do not produce ﬂat faces or polyhedra since an underlying order is missing. (cf. Chap. 5, “Morphology”) What then may be said about the relationship of liquid, crystal, and glass? One possibility is to examine the change in speciﬁc volume as the temperature is raised or lowered (Fig. 2.7). As a liquid is cooled, its volume decreases smoothly. When the melting point (Tm ) is reached, the liquid crystallizes, leading to a sharp change in 7 2 The Crystalline State Fig. 2.7 Temperature dependence of the speciﬁc volume of a liquid as it forms a crystalline or a glass phase. uid Liq d ole Specific Volume 8 rco pe Su uid Liq Glass l Crysta Tg Tm Temperature volume. Further cooling results in a smooth decrease in the volume of the crystalline phase. If cooling does not cause a liquid to crystallize, the volume continues to decrease as shown by the dashed line in Fig. 2.7, corresponding to a “supercooled liquid”. When the transformation temperature, or better transformation range, Tg is reached, the curve bends and continues more or less parallel to that for the crystal. This bend corresponds to a large increase in viscosity. The liquid “freezes”, but the resulting glass is still actually a supercooled liquid. There are many other ways in which crystals diﬀer from amorphous material. One of these is that while a crystal has a deﬁnite melting point, a glass has a softening region. Another diﬀerence is in their diﬀerent properties relative to an incident Xray beam. The three-dimensional ordering of the atoms in crystals gives rise to sharp interference phenomena, as is further examined in Chap. 13. Amorphous bodies, as they do not have underlying order, produce no such eﬀect. 2.1 Exercises Exercise 2.1 Determine the volume of gas associated with each molecule at standard temperature and pressure (0◦ C, 101.3 kPa). What is the edge of a cube with that volume? Exercise 2.2 Determine the packing eﬃciency of gaseous neon (RNe = 1.60 Å) at standard conditions, where the packing eﬃciency is the ratio of the volume of a neon atom to the volume determined in Exercise 2.1. For comparison, a copper atom in a crystal has a packing eﬃciency of 74%. Exercise 2.3 Discuss the use of the term “crystal glass”! 3 The Lattice and Its Properties A three-dimensional periodic arrangement of atoms, ions or molecules is always present in all crystals. This is particularly obvious for the α-polonium crystal illustrated in Fig. 3.1a. If each atom is represented simply by its center of gravity, what remains is a point or space lattice (Fig. 3.1b). ! A point or space lattice is a three-dimensional periodic arrangement of points, and is a pure mathematical concept. The concept of a lattice will now be developed from a lattice point via the line lattice and the plane lattice, ﬁnally to the space lattice. Fig. 3.1a, b Three-dimensional periodic arrangement of the atoms in a crystal of α-polonium (a) and the space lattice of the crystal (b) 3.1 Line Lattice In Fig. 3.2, we may consider moving from the point 0 along the vector a to the point 1. By a similar movement of 2a, we will reach point 2, etc. By this movement, one point is brought into coincidence with another, and a repetition operation takes place. By means of this operation, called a lattice translation, a line lattice has been generated. All points which may be brought into coincidence with one another by W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_3, C Springer-Verlag Berlin Heidelberg 2011 10 3 The Lattice and Its Properties Fig. 3.2 Fig. 3.3 Fig. 3.2 Line lattice with its lattice parameter |a| = a0 Fig. 3.3 Plane lattice with the unit mesh deﬁned by the vectors a and b a lattice translation are called identical points or points equivalent by translation. |a| = a0 is called the lattice parameter, and this constant alone completely deﬁnes the one-dimensional lattice. 3.2 Plane Lattice If a lattice translation b b ∦ a is then allowed to operate on the line lattice in Fig. 3.2, the result is the plane lattice or plane net (Fig. 3.3). The vectors a and b deﬁne a unit mesh. The entire plane lattice may now be constructed from the knowledge of three lattice parameters, | a | = a0 | b | = b0 and γ , the included angle. If any point is moved by any arbitrary lattice translation, it will come into coincidence with another point. but also to A plane lattice thus has lattice translations not only parallel to a and b, any number of combinations of them, i.e. an inﬁnite number of lattice translations. 3.3 Space Lattice If yet another lattice translation c is now introduced in a direction not coplanar with its action on the plane lattice in Fig. 3.3 generates the space lattice shown a and b, in Fig. 3.4. This space lattice can also be produced solely by the operations of three dimensional lattice translations. In contrast to a ﬁnite crystal, a space lattice is inﬁnite and c, we may introduce an According to the arrangement of the vectors a, b, and c and axial system with the crystallographic axes a, b and c. The vectors a, b, their respective crystallographic axes a, b and c are chosen to be right-handed. That is, if the right thumb points in the direction of a (a) and the index ﬁnger is along b (b), the middle ﬁnger will point in the direction of c (c). A lattice, or a crystal described by it, may always be positioned so that a (a) points toward the observer, b (b) toward the right, and c (c) upwards, as is done in Fig. 3.4. and c deﬁne a unit cell, which may alternatively be described by The vectors a b, six lattice parameters (Table 3.1): 3.4 The Designation of Points, Lines and Planes in a Space Lattice Fig. 3.4 Space lattice with the unit cell deﬁned by the vectors a, b and c Table 3.1 Lattice constants of a unit cell Length of lattice translation vectors |a| = a0 = b0 |b| |c| = c0 Interaxial lattice angles a ∧ b = γ a ∧ c = β b ∧ c = α Further application of lattice translations to the unit cell will produce the entire space lattice. The unit cell thus completely deﬁnes the entire lattice. Every unit cell has eight vertices and six faces. At all vertices there is an identical point. Can all of these points be considered part of the unit cell? The lattice point D in Fig. 3.4 is not only part of the marked-out unit cell, but part of all eight cells which meet at that point. In other words, only one eighth of it may be attributed to the marked unit cell, and since 8 × 18 = 1, the unit cell contains only one lattice point. Such unit cells are called simple or primitive, and are given the symbol P. ! A space lattice contains inﬁnitely many lattice planes, lines, and points 3.4 The Designation of Points, Lines and Planes in a Space Lattice 3.4.1 The Lattice Point uvw Every lattice point is uniquely deﬁned with respect to the origin of the lattice by and c are simply the lattice the vector τ = ua + vb + wc. The lengths of a, b, parameters, so only the coordinates u, v and w require to be speciﬁed. They are written as a “triple” uvw. In Fig. 3.5, the vector τ describes the point 231 (which 11 12 3 The Lattice and Its Properties Fig. 3.5 Designation of lattice points using the coordinates uvw that deﬁne the vector from the origin to the lattice point uvw, τ = ua + vb + wc is read as two-three-one). The coordinates u, v and w normally are integers, but can also have values of integers + 12 ; 13 or 23 , as is further explained in Sect. 7.3 and Table 7.5. When they have integral values, the points uvw are the coordinates of the points of a P-lattice. The coordinates of the vertices of a unit cell are given in Fig. 3.5. 3.4.2 Lattice Lines [uvw] A line may be speciﬁed mathematically in any coordinate system by two points. The lattice line I in Fig. 3.6 contains the points 000 and 231. Since the lattice line passes through the origin, the other point on its own describes the direction of the line in the lattice, and the coordinates of this point thus deﬁne the line. For this purpose, they are placed in square brackets [231], or in general [uvw], to show that they represent the direction of a line. The lattice line II’ passes through the points 100 and 212. Line II is parallel to this line, and passes through the origin as well as the point 112 and consequently both lines are represented by the symbol [112]. Fig. 3.6 Designation of lattice lines using the coordinates [uvw] (in square brackets) that deﬁne the vector from the origin to the given point τ = ua + vb + wc (I: [231], II: [112]) 3.4 The Designation of Points, Lines and Planes in a Space Lattice Fig. 3.7 Projection of a lattice onto the a, b-plane showing parallel sets of lattice lines [110], [120] and [310] Fig. 3.8 Projection of a space lattice along c onto the a, b-plane. The lattice line A is deﬁned by the triple [210], while B may be given as [130] or [130] ! Note that the triple [uvw] describes not only a lattice line through the origin and the point uvw, but the inﬁnite set of lattice lines which are parallel to it and have the same lattice parameter. Figure 3.7 shows parallel sets of lattice lines [110], [120] and [310]. The repeat distance along the lines increases with u, v, w. Figure 3.8 shows a projection of a space lattice along c onto the a, b-plane. The lattice line A intersects the points with coordinates 000, 210, 420 and 2 10. Note that minus signs are placed above the numbers to which they apply – this applies to all crystallographic triples. Each point on the line has diﬀerent values uvw, but the ratio u: v: w remains constant. In this case, the smallest triple is used to deﬁne the lattice line. Lines parallel to a or b are thus identiﬁed as [100] or [010] respectively, while the line B is given as [130] or [130]; note that these two representations deﬁne opposite directions for the lattice line. Similarly [210] and [2 10] describe the two directions of a single line. 13 14 3 The Lattice and Its Properties 3.4.3 Lattice Planes (hkl) Consider a plane in the lattice intersecting the axes a, b and c at the points m00, 0n0 and 00p. (These coordinates are given as mnp and not uvw to show that the values need not be integral). An example of a lattice plane which does not intersect the axes at lattice points is plane D in Fig. 3.11. The coordinates of the three intercepts completely deﬁne the position of a lattice plane (Fig. 3.9). Normally, however, the reciprocals of these coordinates are used rather than the coordinates themselves: a-axis: h ∼ 1/m b-axis: k ∼ 1/n c-axis: l ∼ 1/p The smallest integral values are chosen for the reciprocal intercepts, and they are then written as a triple (hkl) in round brackets. ! The values (hkl) are called Miller indices, and they are deﬁned as the smallest integral multiples of the reciprocals of the plane intercepts on the axes. The lattice plane shown in Fig. 3.9 has the intercepts m | n | p = 2 | 1 | 3. The reciprocals of these are 12 |1| 13 , leading to the Miller indices (362). Fig. 3.9 The intercepts on the axes of a lattice plane with the Miller indices (362) Fig. 3.10 The indexing of lattice planes by Miller indices, the smallest integral multiples of the reciprocals of the intercepts on the axes; I (111), II (211) 3.4 The Designation of Points, Lines and Planes in a Space Lattice Table 3.2 Indexing of the lattice planes shown in Fig. 3.10 m n p 1 m 1 n 1 p (hkl) I 1 1 1 1 1 1 (111) II 1 2 2 1 1 2 1 2 (211) In the space lattice shown in Fig. 3.10, two lattice planes have been drawn in, which are indexed in Table 3.2. In Fig. 3.11, a projection of a lattice is shown together with the lines representing the traces of lattice planes perpendicular to the plane of the paper and parallel to the c-axis. These lattice planes are indexed as shown in Table 3.3. The lattice planes A to G belong to a set of equally spaced, parallel planes resulting in the same indices. Since the plane E intersects the origin, it cannot be indexed in this position. Note that (210) and (2 10) deﬁne the same parallel set of planes. ! Generally, the triple (hkl) represents not merely a single lattice plane, but an inﬁnite set of parallel planes with a constant interplanar spacing. Fig. 3.11 Projection of a space lattice along c onto the a, b-plane. The “lines” A-G are the traces of the lattice planes parallel to c with the Miller indices (210). The “line” H is the trace of a lattice plane (230) Table 3.3 Indexing of the lattice planes shown in Fig. 3.11 m A 2 B 3 2 n 4 3 p 1 m 1 n 1 p (hkl) ∞ 1 2 1 4 0 (210) ∞ 2 3 1 3 0 (210) 1 1 2 0 (210) (210) C 1 2 ∞ D 1 2 1 ∞ 2 1 0 E – – – – – – F 1 2 1 ∞ 2 1 0 (2 10) ∞ 1 1 2 0 (2 10) ∞ 1 3 1 2 0 (230) G H 1 3 2 2 15 16 3 The Lattice and Its Properties Fig. 3.12 Projection of a lattice onto the a, b-plane, with the projections of six sets of lattice planes Figure 3.12 gives the projection of a lattice onto the a,b-plane. This projection has a square unit mesh (a0 = b0 ). The projections of six sets of lattice planes with various indices are also shown. As the indices rise, the spacing between the planes decreases, as does the density of points on each plane. Planes which are parallel to b and c will thus only have intercepts with a and are indexed as (100). Similarly, (010) intersects only the b-axis, and (001) only c. 3.5 The Zonal Equation We may ask what the relationship is between the symbols [uvw] and (hkl) if they represent sets of lines and planes that are parallel to one another. The equation of any plane may be written: Y Z X + + = 1, m n p (3.1) where X, Y and Z represent the coordinates of points lying on the plane, and m, n and p are the three intercepts of this plane on the crystallographic axes a, b and c (see Sect. 3.4.3). If the substitution is then made h ∼ m1 , k ∼ n1 , and 1 ∼ p1 , the equation may be written hX + kY + 1Z = C, (3.2) where C is an integer. The equation describes not only a single lattice plane, but a set of parallel lattice planes. For positive h, k and 1, giving C a value of + 1 describes that plane of the set which lies nearest to the origin in the positive a, b and c directions. 3.5 The Zonal Equation Similarly, a value of –1 deﬁnes the nearest plane in the negative a, b and c directions from the origin. The plane (hkl) which cuts the origin has the equation: hX + kY + 1Z = 0. (3.3) As an example, the planes D, E and F in Fig. 3.11, are deﬁned by the above equation where (hkl) = (210) and C takes on the values 1, 0 and –1 respectively. For any of these planes, the triple XYZ represents a point on the plane. In particular, on the plane passing through the origin (C = 0) this triple XYZ could describe a lattice line – the line connecting the point XYZ to the origin 000. In this case, we would replace XYZ by uvw giving the relationship: hu + kv + lw = 0. (3.4) For reasons which will appear later this relationship is called the zonal equation. 3.5.1 Applications of the Zonal Equation 3.5.1.1 Application 1 (a) Two lattice lines [u1 v1 w1 ] and [u2 v2 w2 ] will describe a lattice plane (hkl) (cf. Fig. 3.13), whose indices may be determined from the double application of the zonal equation: hu1 + kv1 + lw1 = 0 (3.5) hu2 + kv2 + lw2 = 0. (3.6) The solution of these two simultaneous equations for hkl may be expressed in two ways as the ratio of determinants: v1 w1 w1 u1 u1 v1 : : h:k:1= v2 w2 w2 u2 u2 v2 v2 w2 w2 u2 u2 v2 : : h̄ : k̄ : l̄ = v1 w1 w1 u1 u1 v1 Fig. 3.13 The lattice lines [u1 v1 w1 ] and [u2 v2 w2 ] deﬁne the lattice plane (hkl) or (h̄k̄l̄) (3.7) (3.8) 17 18 3 The Lattice and Its Properties The lattice plane symbols (hkl) and (h̄k̄l̄), however, describe the same set parallel planes. h : k : l = (v1 w2 − v2 w1 ) : (w1 u2 − w2 u1 ) : (u1 v2 − u2 v1 ). (3.9) The following form is particularly convenient: (3.10) Example. What is the set of lattice planes common to the lines [101] and [121]? 1 1 0 1 1 0 1 2 1 1 2 1 2 2 2 → (111) This result can also be obtained geometrically, as in Fig. 3.14. The lattice lines [101] and [121] (– • – • – •) lie in the lattice plane (–––). Other lines lying in the plane are also shown (– • – • – •) in order to make it more obvious. The indicated lattice plane cannot be indexed, as it passes through the origin. The choice of an alternative origin N makes it possible to index it: m | n| p| = 1|1|1 → (111). If the determinant is set up in the alternative manner: 1 2 1 1 2 1 1 0 1 1 0 1 2 2 2 → (1 1 1). (cf. Eq. 3.8) Fig. 3.14 The lattice lines [101] and [121] lie in the lattice plane indicated by the dashed lines. Since, however, that plane passes through the origin, it is necessary to consider an alternative origin such as N in order to assign its indices (111) c′ c N a b N′ b′ [121] [101] a′ 3.5 The Zonal Equation (111) and (1 1 1 ) belong to the same set of parallel lattice planes (cf. Exercise 3.11) ! In the description of crystal faces (Chap. 5) the symbols (hkl) and (h̄k̄l̄) are taken to represent a crystal face and its parallel opposite. 3.5.1.2 Application 2 Two lattice planes (h1 k1 l1 ) and (h2 k2 l2 ) intersect in the lattice line [uvw] (Fig. 3.15), which can be identiﬁed by the solution of the equations: h1 u + k1 v + l1 w = 0 (3.11) h2 u + k2 v + l2 w = 0. (3.12) Proceeding in the same method as above leads to the required lattice line [uvw]: (3.13) ! Note that, as in (a), two solutions are possible: [uvw] and [ūv̄w̄]. In this case, these represent the opposite directions of the same line. Example. Which lattice line is common to the lattice planes (101) and 112? 1 1 1 2 1 1 2 0 1 1 0 1 [1 3 1] If the values of (hkl) are interchanged, the result will be [1 31] Fig. 3.15 The lattice planes (h1 k1 l1 ) and (h2 k2 l2 ) intersect in the lattice line [uvw] 19 20 3 The Lattice and Its Properties 3.6 Exercises Exercise 3.1 Make a copy on tracing paper of the lattice points outlining a single unit cell in Fig. 3.5. Lay your tracing on top of a unit cell in the original drawing and satisfy yourself that you can reach any other cell by suitable lattice translations. Exercise 3.2 (a) Examine the lattice below, and give the coordinates of the points P1 , P2 , P3 and P4 , the values of [uvw] for the lattice lines that are drawn in. (b) On the same diagram, draw in the lines [211], [120] and [212]. (c) Determine the lattice planes to which the lines [131] and [111] belong. Exercise 3.3 The diagram below is the projection of a lattice along the c-axis onto the a,b-plane. The dark lines labeled I and II are the traces of planes that are parallel to the c-axis. 3.6 Exercises (a) Index planes I and II. (b) Calculate [uvw] for the line common to the two planes. (c) Draw the traces of the planes (320) and (120) on the projection. Exercise 3.4 Give (hkl) for a few planes containing the line [211], and give [uvw] for a few lines lying in the plane (121). Exercise 3.5 What condition must be fulﬁlled to make (a) [100] perpendicular to (100), (b) [110] perpendicular to (110) and (c) [111] perpendicular to (111)? Exercise 3.6 What are the relationships between (110) and (1 10); (211) and (21 1); [110] and [1 10]; [211] and [21 1]? 21 4 Crystal Structure In order to progress from a lattice to a crystal, the points of the lattice must be occupied by atoms, ions or molecules. Because the points are all identical, the collections of objects occupying them must also be identical. In general, crystals are not built up so simply as the crystal of α -polonium in Fig. 3.1! Let us consider the construction of a crystal by means of a hypothetical example. Figure 4.1a shows a lattice with a rectangular unit cell projected on the a, b-plane. We now place the molecule ABC in the unit cell of the lattice in such a way that A lies at the origin and B and C within the chosen cell (Fig. 4.1b). The position of B or C with respect to the origin may be described by a vector r in terms of the lattice and c (cf. Fig. 4.3): translations a, b, r = xa + yb + zc (4.1) The coordinates are yet another triple: x,y,z, where 0 ≤ x,y,z < 1 for all positions within the unit cell. In our example, the atoms have the following coordinates: A : 0,0,0 B : x1 ,y1 ,z1 , C : x2 ,y2 ,z2 . This arrangement of atoms within a unit cell is called the basis. Lattice translations reproduce the atoms throughout the entire lattice (Fig. 4.1c), or: lattice + basis = crystal structure. It follows that not only the A-atoms but also the B- and C-atoms lie on the points of congruent lattices, which diﬀer from one another by the amount indicated in the basis (see Fig. 4.2). Every atom in a crystal structure is repeated throughout the crystal by the same lattice translations. Thus, the following simple deﬁnition of a crystal is possible. D Crystals are solid chemical substances with a three-dimensional periodic array of atoms, ions or molecules. This array is called a crystal structure. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_4, C Springer-Verlag Berlin Heidelberg 2011 24 4 Crystal Structure Fig. 4.1a–c Interrelationship of the lattice (a), the basis or the arrangement of atoms in the unit cell (b) and the crystal structure (c), all shown as a projection on the a, b-plane Fig. 4.2 All atoms of the crystal structure shown in Fig. 4.1 lie on the points of congruent lattices 4 Crystal Structure Fig. 4.3 Description of a point in a unit cell by the coordinate-triple x,y,z deﬁning the vector r = xa + yb + zc An example of a simple crystal structure is cesium iodide. The unit cell is a cube (a0 = b0 = c0 = 4.57 Å, α = β = γ = 90◦ ).1 The basis is I− : 0,0,0; Cs+ : 12 , 12 , 12 . In Fig. 4.4a, a unit cell is shown as a perspective picture, with the relative sizes of the ions indicated. For more complex structures, this method of illustration is less useful, as it prevents the positions of atoms from being clearly seen. Consequently, it is more usual merely to indicate the centers of gravity of the atoms, as in Fig. 4.4b. Figure 4.4c shows the same structure represented as a parallel projection on one cube face. An important quantity for any structure is Z, the number of chemical formula units per unit cell. For CsI, Z = 1 as there are only one Cs+ ion and one I– ion per cell. Using only structural data, it is thus possible to calculate the density of CsI, since = m g cm−3 , V Fig. 4.4a–c The CsI structure shown in a perspective drawing taking account of the relative sizes of the ions (a), with ions reduced to their centers of gravity (b) and as a parallel projection on (001) (c) 1 The Ångström unit (Å): 1 Å = 10–8 cm = 0.1 nm. If a row of spheres with a radius of 1 Å is made, these will be 50,000,000 of them per centimeter! 25 26 4 Crystal Structure Fig. 4.5 The description of lines and planes in a unit cell by means of coordinates x,y,z where m is the mass of the atoms in the unit cell and V is the volume of the cell. The mass of one chemical formula is M/NA , where M is the molar mass and NA is the Avogadro number, so Z·M and NA Z·M g cm−3 = NA · V m= Thus, taking NA as 6.023 × 1023 mol–1 , for CsI, where M = 259.81 g mol–1 CsI = 1 · 259.81 = 4.52 g cm−3 . 6.023 · 1023 · 4.573 · 10−24 In a structure determination, this operation is carried out in reverse: from the measured density, the number of formula units per cell is estimated. Using the values (hkl) and [uvw] we have so far only described the orientations of sets of planes and lines. Consideration of the contents of a unit cell makes it necessary to describe speciﬁc planes and lines in the cell. Use of the coordinates x,y,z makes this possible. For example, the coordinates x,y,1/2 identify all points in the plane parallel to a and b which cuts c at 1/2. Figure 4.5 shows the planes x,y,1/2 and 3/ ,y,z. The line of intersection may easily be seen to be described by the coordinates 4 3 /4,y,1/2. 4.1 Exercises Exercise 4.1 Cuprite, an oxide of copper, has the lattice: a0 = b0 = c0 = 4.27 Å, α = β = γ = 90◦ and the basis: Cu: 14 , 14 , 14 ; 34 , 34 , 14 ; 34 , 14 , 34 ; 14 , 34 , 34 . O: 0,0,0; 12 , 12 , 12 . 4.1 Exercises (a) Draw a projection of the structure on x,y,0 (the a, b-plane) and a perspective representation of the structure. (b) What is the chemical formula of this compound? What is Z (the number of formula units per unit cell)? (c) Calculate the shortest Cu-O distance. (d) What is the density of cuprite? Exercise 4.2 The cell dimensions for a crystal of AlB2 were determined to be a0 = b0 = 3.00 Å, c0 = 3.24 Å, α = β = 90◦ , γ = 120◦ . There is an Al-atom at 0,0,0, and B-atoms at 13 , 23 , 12 and 23 , 13 , 12 . (a) Draw a projection of four unit cells of this structure on (001). (b) Calculate the shortest Al-B distance. (c) Calculate the density of AlB2 . Exercise 4.3 In the accompanying drawing of the unit cell of a lattice, give the coordinates of the points occupied by small circles, which, as we will later learn, represent inversion centers (Sect. 6.3). 27 28 4 Crystal Structure Exercise 4.4 Draw the unit cell of a lattice and give the coordinates which describe its ‘edges’. Exercise 4.5 For the same unit cell, give the coordinates which describe its ‘faces’. Exercise 4.6 Give the coordinates for the planes and lines drawn in the unit cell shown below. Exercise 4.7 Draw a unit cell with the shape of a cube. On it, sketch a plane with co-ordinates x,x,z and lines with the co-ordinates x,x,0 and x,x,x. 5 Morphology By the term “morphology”, we refer to the set of faces and edges which enclose a crystal. 5.1 Relationship Between Crystal Structure and Morphology The abundance of characteristic faces and, at least in ideal circumstances, the regular geometric forms displayed externally by crystals result from the fact that internally, crystals are built upon a crystal structure. What is, then, the relationship between the crystal structure (the internal structure) and morphology (the external surfaces)? Figure 5.1 shows the crystal structure and the morphology of the mineral galena (PbS). The faces of a crystal are parallel to sets of lattice planes occupied by atoms, while the edges are parallel to lattice lines occupied by atoms. In Fig. 5.1a, these atoms are represented by points. A lattice plane occupied by atoms is not actually ﬂat. This may be seen for the lattice plane (100), (010) or (001) in Fig. 5.1c when the size of the spherical atoms is taken into account, and is even more marked for crystals of molecular compounds. Atomic radii are very small – of the order of 1 Å – so crystal faces appear smooth and ﬂat to the eye. A crystal face contains a twodimensionally periodic array of atoms. The relationship between crystal structure and morphology may be summarized thus: ! (a) Every crystal face lies parallel to a set of lattice planes; parallel crystal faces correspond to the same set of planes. (b) Every crystal edge is parallel to a set of lattice lines. The reverse conclusions must, however, certainly not be drawn, since a crystal will have a very large number of lattice planes and lines, and generally only a few edges and faces. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_5, C Springer-Verlag Berlin Heidelberg 2011 30 5 Morphology Fig. 5.1a, b Correspondence between crystal structure (a) and morphology (b) in galena (PbS). In a, the atoms are reduced to their centers of gravity. (c) shows the atoms occupying the (100), (010) or (001) face Furthermore, it should be noted that the shapes in Fig. 5.1 have been drawn to vastly diﬀerent scales. Suppose the edge of the crystal marked with an arrow is 6 mm in length; then that edge corresponds to some 107 lattice translations, since the lattice parameters of galena are all 5.94 Å. Since crystal faces lie parallel to lattice planes and crystal edges to lattice lines, Miller indices (hkl) may be used to describe a crystal face, and [uvw] a crystal edge. The morphology of the crystal gives no information about the size of the unit cell, but can in principle give the ratio between one unit cell edge and another. Normally, however, the lattice parameters are known, so the angles between any pair of lattice planes can be calculated and compared with the observed angles between two crystal faces. The crystal of galena in Fig. 5.1 has been indexed, i.e. the faces have been identiﬁed with (hkl). Thus, with the origin chosen suitably inside the crystal, (100) cuts the a-axis and is parallel to b and c; (110) is parallel to c and cuts a and b at the same distance from the origin; (111) cuts a, b and c all at the same distance from the origin. 5.2 Fundamentals of Morphology Morphology is the study of the external boundary of a crystal, built up of crystal faces and edges. In morphology, the words “form”, “habit” and “zone” have special meanings. 5.2 Fundamentals of Morphology (a) Form. The morphology of a crystal is the total collection of faces which characterize a particular crystal. The morphology of the crystals shown in Fig. 5.2 consists of the combination of a hexagonal prism and a “pinacoid”; a pinacoid is a pair of parallel faces which in this case make up the ends of this prism. The prism and the pinacoid are examples of a crystal form, which is further discussed in Chap. 9. In the meantime, we will simply consider a crystal form as a set of “equal” faces. It is thus possible to describe the morphology as the set of forms of a crystal. Fig. 5.2a–c The three basic habits: (a) equant, (b) planar or tabular, (c) prismatic or acicular with the relative rates of growth in diﬀerent directions shown by arrows a) b) c) (b) Habit. This term is used to describe the relative sizes of the faces of a crystal. There are three fundamental types of habit: equant, planar or tabular, and prismatic or acicular (needle-shaped). These habits are illustrated in Fig. 5.2 by the relative sizes of the hexagonal prism and the pinacoid. (c) Zone. The crystals in Figs. 2.1, 2.2, 2.3 and 2.4 show several examples of three or more crystal faces intersecting one another to form parallel edges. A set of crystal faces whose lines of intersection are parallel is called a zone (Fig. 5.3). Faces belonging to the same zone are called tautozonal. The direction parallel to the lines of intersection is the zone axis. Starting from any point inside the crystal, the normals to all the faces in a zone are coplanar, and the zone axis is normal to this plane. Only two faces are required to deﬁne a zone. Fig. 5.3 A zone is a set of crystal faces with parallel lines of intersection. The zone axis is perpendicular to the plane of the normals to the intersecting faces, and is thus parallel to their lines of intersection (After [32]) 31 32 5 Morphology The galena crystal in Fig. 5.1b shows several zones. For example, the face (100) belongs to the zones [(101)/101̄)] = [010], [(110)/11̄0)] = [001], [(111)/11̄1̄)] = [011̄] and [(11̄1)/111̄)] = [011]. All intersecting faces of a crystal have a zonal relationship with one another. This is evident from consideration of Fig. 5.1b. The faces or the lattice planes (h1 ,k1 ,l1 ), (h2 ,k2 ,l2 ), and (h3 ,k3 ,l3 ), are tautozonal if and only if h1 k1 l1 h2 k2 l2 = 0 h3 k3 l3 (5.1) i.e. h1 k2 l3 + k1 l2 h3 + l1 h2 k3 − h3 k2 l1 − k3 l2 h1 − l3 h2 k1 = 0. (5.2) Do the planes (hkl) belong to the zone [uvw]? The answer depends on whether or not the zonal equation hu + kv + lw = 0 (Eq. 3.4) is fulﬁlled. For example, (11̄2) does lie in the zone [1̄11] since 1× (–1) + (−1) × 1 + 2× 1 = 0. 5.3 Crystal Growth It is easier to understand the morphology of a crystal if the formation and growth of crystals is considered. Crystals grow from, among other things, supersaturated solutions, supercooled melts and vapors. The formation of a crystal may be considered in two steps. 1. Nucleation. This is the coming together of a few atoms to form a threedimensional periodic array – the nucleus – which already shows faces, although it is only a few unit cells in size (see Fig. 5.4a). 2. Growth of a Nucleus to a Crystal. As the nucleus attracts further atoms, they take up positions on its faces in accordance with its three-dimensional periodicity. In this way, new lattice planes are formed (Fig. 5.4b–d). Note that the illustration is two-dimensional only. The growth of the nucleus, and then of the crystal, is characterized by a parallel displacement of its faces. ! The rate of this displacement is called the rate of crystal growth, and is a characteristic, anisotropic property of a crystal. Figure 5.5 shows a few stages in the growth of a quartz crystal. The nucleus shown in Fig. 5.6 is bounded by two diﬀerent types of faces, and the rates of growth of these faces, v1 and v2 are thus, in principle, distinguishable. Figure 5.6a illustrates the case in which these rates of growth are similar, while in Fig. 5.6b, they are very diﬀerent. A consequence of this diﬀerence is that the 5.3 Crystal Growth Fig. 5.4a–d Nucleation and growth of the nucleus to a macrocrystal illustrated in two dimensions. (a) Nucleus, e.g. in a melt. (b) Atoms adhere to the nucleus. (c) Growth of a new layer on the faces of a nucleus. (d) The formation of a macrocrystal by the addition of further layers of atoms Fig. 5.5 Quartz crystal showing its stepwise growth 33 34 5 Morphology Fig. 5.6a, b Crystal growth showing a small (a) and a large (b) diﬀerence in growth rate with direction faces corresponding to the slow growth rate become steadily larger, while those corresponding to rapid growth disappear entirely. In addition, it should also be noted that crystal growth rates are aﬀected by temperature, pressure, and degree of saturation of the solution. The actual crystal faces which eventually enclose the crystal depend on the ratios of the growth rates of the various faces, the slowergrowing ones becoming more prominent than those that grow more rapidly. Those faces which do eventually develop generally have low Miller indices and are often densely populated with atoms. The three basic types of crystal habit may be understood in terms of the relative growth rates of the prism and pinacoid faces, which are indicated in Fig. 5.2 by arrows. Figure 5.7 shows how crystals of diﬀerent shapes can result from the same nucleus. Crystal I is regular in shape, while crystals II and III have become very much distorted as a result of external inﬂuences on the growth rate. None the less, the angles between the normals to the crystal faces remain constant, since the growing faces have simply been displaced along their normals. A parallel displacement of the faces cannot change interfacial angles. This observation applies equally to all growing faces of a crystal. 5.3 Crystal Growth Fig. 5.7 Despite diﬀerence in rates of growth of diﬀerent parts of a crystal, the angles between corresponding faces remain equal This observation is the basis of the law of constancy of the angle: in diﬀerent specimens of the same crystal, the angles between corresponding faces will be equal. This law, which is valid at constant temperature and pressure, was ﬁrst formulated by N. Steno in 1669, without any knowledge of crystal lattices! The relative positions of the normals to the faces of the crystals in Fig. 5.7 remain constant. It is possible, by measurement of the angles between faces, to determine these relative positions and thus eliminate the distortion. So far, our discussion has assumed the existence of a single crystal nucleus, or only a few, which can grow separately into single crystals like those shown in Fig. 2.1. The term single crystal, as it is used here, implies one which has grown as such. It will normally display characteristic faces, but those grown in the laboratory often do not. If many nuclei are formed simultaneously, they may grow into one another in a random fashion, as illustrated in Fig. 5.8. This disturbance will prevent the development of crystal faces and forms. Instead, a crystal aggregate or polycrystal results. Figure 5.8 shows an example of single phases in the development of such an aggregate. The individual crystallites of an aggregate are themselves single crystals. Fig. 5.8a–c Development of a crystal aggregate. (a) Formation of several nuclei, which initially can grow independently. (b) Collision of growing crystallites leads to interference and irregularity in growth of the polyhedra. Eventually, the polyhedral shape of the crystallites is entirely lost. (c) The single crystal domains of the aggregate with their grain boundaries 35 36 5 Morphology 5.4 The Stereographic Projection Since crystals are three-dimensional objects, it is necessary to use projections in order to work with them on a ﬂat surface. One such projection is the parallel projection onto a plane, which was illustrated in Fig. 4.4c for representing a crystal structure. For morphological studies, the stereographic projection has proved to be particularly useful. The principle of this projection is shown in Fig. 5.9. A crystal, in this case galena (PbS), is placed at the center of a sphere. The normals to each face, if drawn from the center of the sphere, will then cut the surface of the sphere in the indicated points, the poles of the faces. The angle between two poles is taken to mean the angle between the normals n, not the dihedral angle f between the faces. These two angles are simply related as: n (angle of normals) = 180◦ − f (dihedral angle) (Fig. 5.10). The poles are not randomly distributed over the surface of the sphere. In general they will lie on a few great circles, i.e. circles whose radius is that of the sphere. Those faces whose poles lie on a single great circle will belong to a single zone. The zone axis will lie perpendicular to the plane of the great circle. Fig. 5.9 Crystal of galena at the center of a sphere. The normals to the faces of the crystal cut the sphere at their poles, which lie on great circles Fig. 5.10 In a stereographic projection, lines are drawn between the poles of the faces in the northern hemisphere and the south pole, and the intersection of these lines with the equatorial plane is recorded 5.4 The Stereographic Projection Considering the sphere as a terrestrial globe, a line from each of the poles in the northern hemisphere is projected to the south pole, and its intersection with the plane of the equator is marked with a point • or a cross + (see Fig. 5.11). Lines from poles in the southern hemisphere are similarly projected to the north pole, and their intersections with the equatorial plane are marked with an open circle O. For those poles lying exactly on the equator, a point or cross is used. The mathematical relationships of the stereographic projection are shown in Fig. 5.33. Figure 5.12 shows the stereogram of the crystal in Fig. 5.9, only those planes belonging to the northern hemisphere being shown. Poles belonging to a single zone lie on the projections of the relevant great circles. The points resulting from the projections of each face are indexed Figure 5.13a shows the stereographic projection of a tetragonal prism and a pinacoid, while Fig. 5.13b gives that of a tetragonal pyramid and a pedion. A pedion is the name given to a crystal form which consists of a single face. In both cases, the altitude of the prism or pyramid is set in the N–S direction. Both the tetragonal prism and the tetragonal pyramid have square bases and square cross-sections. The faces of the prism are perpendicular to the plane of the stereographic projection, so Fig. 5.11 Stereographic projection of the crystal in Fig. 5.9; see also Fig. 5.1b. Only the poles with positive values of l are included Fig. 5.12 Relationship between the angle of intersection of the normals (n) and the dihedral angle (f) between the faces F1 and F2 . The poles of the faces lie on a great circle, the zone circle 37 38 5 Morphology Fig. 5.13a, b Stereographic projection of a tetragonal prism and a pinacoid (a) and of a tetragonal pyramid and a pedion (b). The angular coordinates φ and ρ are given for one of the pyramid faces their poles lie on the circumference of the circle of that projection. The faces of the pyramid make equal angles with the equatorial plane, so the poles of these faces are at equal distances from the center of the plane of projection. The representation of the stereographic projection in Figs. 5.9, 5.11, and 5.12 is only intended to explain the principles of the method. In practice, the projection is based on the values of measured angles. The stereographic projection is also very useful for the description of the point groups. In this case, there is a departure from the normal convention of plotting the stereogram. For rotation axes and rotoinversion axes, the symbols of these axes are used to indicate their intersection with the surface of the sphere of projection. Similarly, for mirror planes, the corresponding great circle of intersection is indicated (for an example, see Fig. 7.8e). 5.5 The Reﬂecting Goniometer The angles between crystal faces may conveniently be measured with a reﬂecting goniometer. The crystal is mounted on a goniometer table, which is essentially a rotating plate with a graduated angle scale (see Fig. 5.14). The crystal mount 5.5 The Reﬂecting Goniometer Fig. 5.14 Light path for a one-circle reﬂecting goniometer Fig. 5.15 Two-circle reﬂection goniometer with azimuthal circle φ and pole distance circle ρ (After de Jong [22]) (or goniometer head) is a construction of arcs and slides which makes it possible to bring a zone axis of the crystal into coincidence with the rotation axis of the goniometer table. The crystal is then rotated until the light beam from a lamp mounted horizontally is reﬂected from a crystal face onto the cross-hairs of a telescope, also mounted horizontally. The reading on the scale of the table then ﬁxes the position of that crystal face. The table is then rotated until another face comes into the reﬂecting position, and the angular reading for this position is taken. The diﬀerence between the two readings is the angle between the normals to the crystal faces. Continuing to rotate the table through 360◦ will allow the angles corresponding to the selected zone to be measured. This is the principle of the one-circle reﬂection 39 40 5 Morphology goniometer. For the measurement of the angles corresponding to other zones on a one-circle reﬂecting goniometer, the crystal must be remounted. A two-circle reﬂection goniometer makes it possible to rotate and measure the crystal about two mutually perpendicular axes (Fig. 5.15). In this way, all possible faces can be brought into the reﬂecting position. From the position of the two circles, the angular coordinates φ and ρ may be measured. These coordinates uniquely deﬁne the orientation of a crystal face, and the values can be directly plotted on a stereographic projection. 5.6 The Wulﬀ Net The Wulﬀ net is a device to enable measured crystal angles to be plotted readily as a stereographic projection. The Wulﬀ net is itself the stereographic projection of the grid of a conventional globe orientated so that the N –S direction lies in the plane of projection (Fig. 5.16). The N–S direction of the stereographic projection (Fig. 5.9) is thus perpendicular to the N –S direction both of the grid net of the globe and of the Wulﬀ net (Fig. 5.16). Figure 5.16a shows the grid of only one hemisphere. The equator and all meridians of the globe are great circles, while all of the parallels except the equator are small circles. With the help of the Wulﬀ net, the angle between any two poles on the surface of the sphere can now be plotted directly on the stereographic projection. The angle measured between any two crystal faces is the angle between their normals or the angle between their poles. The two normals deﬁne the plane of a great circle (Fig. 5.9). The arc of the great circle between the two normals is the measured angular value. It is thus crucial that only arcs of great circles are used when angles are plotted on or estimated from a stereographic projection! We shall now demonstrate the use of the Wulﬀ net to plot the two angles measured with a two-circle goniometer (the azimuthal angle ϕ and the pole distance ρ) Fig. 5.16a, b The stereographic projection of the grid net of a globe (N –S ⊥ N–S) produces the Wulﬀ net; the positions of the angular coordinates ϕ (the azimuthal angle) and (the pole distance) are indicated. The pole P has coordinates ϕ = 90◦ and = 30◦ 5.6 The Wulﬀ Net on a stereographic projection. The circle of the plane of projection is taken as the azimuth ϕ, so possible ϕ-values run from 0 to 360◦ . The front face of the tetragonal pyramid in Fig. 5.13b thus has a ϕ-value of 90◦ . The ρ-axis is perpendicular to the ϕ-axis. The faces of the tetragonal pyramid have ϕ-coordinates of 0◦ , 90◦ , 180◦ and 270◦ respectively and all faces have the same ρ-value. A similar consideration of a tetragonal dipyramid, e.g. no. 6 in Exercise 5.4 results in the following angular coordinates (ϕ, ρ) for the eight faces: • As above, ϕ = 0◦ , 90◦ , 180◦ , 270◦ • For both ρ and – ρ Note that faces in the northern hemisphere are assigned values 0◦ ≤ ρ ≤ 90◦ , while those in the southern hemisphere have −90◦ ≤ ρ ≤ 0◦ where both 90◦ and −90◦ represent positions on the equator. For an example, see the table of ϕ, ρ -values for the galena crystal in Exercise 5.13. For practice, a Wulﬀ net with a diameter of 20 cm and a 2◦ -grid is bound inside the rear cover. For best results, this should be carefully removed and pasted on a card with a minimum thickness of 1 mm. Drawings are then made on tracing paper secured by a pin at the center of the net so as to be readily rotated. The stereographic projection has two important properties: (1) The projections of two vectors onto the sphere intersect with the same angle as do the vectors themselves. The parallels and the meridians of the global net are mutually perpendicular. Since the Wulﬀ net is the projection of these circles, the corresponding great and small circles of the Wulﬀ net are perpendicular to one another, cf. Fig. 5.16. (2) All circles, great and small, on the sphere will project as circles or arcs on the equatorial plane (Fig. 5.17). Exceptionally, the meridians which are parallel to the N–S-direction, will project as straight lines. This property has several consequences. For example, consider a circle with a radius of 30◦ on the surface of the sphere. Select a general point on the Wulﬀ net, place the pole M there, and construct the locus of all points that are 30◦ from it. By rotating the tracing paper, the poles lying 30◦ from M on each of the great circles will be found (Fig. 5.18). These poles will indeed be found to lie on the circumference of a circle. However, M is not at the center of this circle. The actual center M may be found by bisecting the diameter K1 K2 . The following examples illustrate the principles of the stereographic projection and the use of the Wulﬀ net. (1) Given the two poles 1 and 2, determine the angle between them: Place the tracing paper over the Wulﬀ net and rotate it until both poles lie on a great circle, the zone circle (cf. Fig. 5.19a). The value of the angle can then be read from the great circle. If one of the poles lies in the southern hemisphere, it must be treated appropriately (cf. Fig. 5.19b). 41 42 5 Morphology Fig. 5.17 A circle on the surface of a sphere remains a circle in its stereographic projection on the equatorial plane Fig. 5.18 Detail of the equatorial plane of a stereographic projection. Points 30◦ from a pole M are shown. These poles lie on the circumference of a circle, whose center M may be found by bisecting the diameter K1 K2 Fig. 5.19a, b The angle between two poles may be read from the great circle on which they both lie (2) Two faces deﬁne a zone. Their line of intersection is the zone axis, which is normal to the plane deﬁned by the normals to the faces (cf. Fig. 5.3). The zone circle is perpendicular to the pole of the zone axis. (a) Draw the pole corresponding to a zone circle: Rotate the zone circle onto a great circle of the Wulﬀ net; the zone pole will then be 90◦ from the zone circle along the equator (cf. Fig. 5.20). 5.6 The Wulﬀ Net Fig. 5.20 The zone circle and the zone pole () are mutually perpendicular Fig. 5.21 The angle ε between the planes of two zone-circles is the angle between the poles of the corresponding zones () Fig. 5.22 Construction of the two poles 3, which make an angle κ with pole 1, and an angle ω with pole 2 (b) Draw the zone circle corresponding to a given zone pole: Rotate the pole onto the equator of the Wulﬀ net. The zone circle is then the meridian 90◦ away from the pole (cf. Fig. 5.20). (3) The angle ε between the planes of two zone-circles is the angle between the poles of the corresponding zones (cf. Fig. 5.21). (4) Find the pole 3, which is separated from pole 1 by an angle κ and from pole 2 by an angle ω: This will lie at the intersections of the two circles with the given radii. Note that the centers and the radii of the circles must ﬁrst be speciﬁed. The center of the κ-circle is the midpoint of the diameter K1 K2 (cf. Fig. 5.18); the center of the ω-circle is found by constructing the perpendicular bisector of a chord. Note that there are two solutions to this problem (cf. Fig. 5.22). 43 44 5 Morphology Fig. 5.23a, b, c The octahedron in (a) is rotated into the position in (b). This rotation is shown in the stereogram in (c). The crosses in the stereogram correspond to the faces in (a), the points to the faces in (b). The poles move along small circles (5) Change the plane of projection of a stereographic projection: An octahedron is a crystal form consisting of eight equilateral triangular faces (Fig. 5.23a). Fig 5.23c gives the stereographic projection of this octahedron. The poles of the faces are marked with a cross; those lying in the southern hemisphere are not shown. The stereogram is now to be altered, so that the pole of one of the octahedral faces is moved to the center of the plane of projection. This may be done by rotating one of the poles onto the equatorial plane of the Wulﬀ net. The pole will lie on the equator at 54◦ 44 from its center. Rotating the pole about the N –S axis of the net by 54◦ 44 then brings it to the center of the projection. The other poles move along their own small circles by an angle of 54◦ 44 . The new positions of the poles of the faces, which are shown by points in Fig. 5.23c, correspond to the orientation of the octahedron in Fig. 5.23b, which sits on a face. 5.7 Indexing of a Crystal Today, it is rarely necessary to index a crystal whose lattice constants are unknown. In general, lattice constants give no indication of which faces of a crystal will actually be prominent, but it is possible to produce a stereogram showing all the poles representing faces that are possible for that lattice. Since crystals usually develop faces with low Miller indices, the number of poles which must be drawn is small. We shall now draw the stereogram of the poles of a crystal of topaz. The lattice parameters are a0 = 4.65, b0 = 8.80, c0 = 8.40 Å, α = β = γ = 90◦ . The six faces (100), (100), (010), (010), (001), (001) which are normal to the crystallographic axes can be entered immediately into the stereogram (Fig. 5.24). These faces lie on 5.7 Indexing of a Crystal Fig. 5.24 Stereogram of the poles of a few of the faces of a topaz crystal allowed by the lattice which have low indices the following zone-circles: [100] ≡ [(001)/(010)], [010] ≡ [(100)/(001)], [001] ≡ [(100)/(010)]. The zone axis is normal to the plane of the zone-circle, and is parallel to the set of lattice lines which are common to the lattice planes making up the zone. Figure 5.25 shows a (010)-section through the crystal lattice with the traces of the planes (100), (101), and (001), which belong to the [010]-zone. The angle δ is the angle between the normals to (001) and (101). Since tan δ = c0 /a0 , δ = 61.03◦ . Similarly, Fig. 5.26, showing the (100)-section of the same lattice, gives the angle between the normals to (001) and (011). In this case, tan δ’ = c0 /b0 , and δ = 43.67◦ . With the help of the Wulﬀ net, the angles δ and δ can be placed on the great circles corresponding to the zones [010] and [100] respectively, giving the positions of the poles of the planes (101) and (011). Since the planes (101), (101) and (101) have the same inclination to the crystallographic axes as (101), while (01 1), (011) and (011) have that of (011), they may likewise be entered on the stereogram (Fig. 5.24). The great circles for the zones [(100)/(011)] and [(101)/(010)] may now be drawn in, and the two intersections of these circles will occur at the poles with Miller indices (111) and (1 1 1). These traces of zone-circles lying in the southern hemisphere are given as dashed lines.1 1 Application of the zonal equation leads to 1 0 0 1 0 0 0 1 1 0 1 1 ——————————[0 1 1] 0 0 1 0 0 1 1 0 1 1 0 1 ——————————[1 0 1] 1 0 1̄ 1 0 1̄ 1̄ 1 0 1̄ 1 0 ——————————[1 1̄ 1] If the values of [uvw] are interchanged, the result is (1 1 1). Two zone circles intersect in two poles. In morphology, (hkl) and (h k l) represent two parallel faces, which are related to only one set of lattice planes, which may be designated as (hkl) or (h k l). 45 46 5 Morphology Fig. 5.25 Fig. 5.26 Fig. 5.25 Section parallel to (010) through the lattice of a topaz crystal, showing the traces of the planes (001), (101) and (100), all of which belong to the zone [010]. δ is the angle between the normals to (001) and (101) Fig. 5.26 Section parallel to (100) through the lattice of a topaz crystal, showing the traces of the planes (001), (011) and (010), all of which belong to the zone [100]. δ is the angle between the normals to (001) and (011) The drawing in of the circles for further zones gives the poles for further faces. From these, the poles can be located for all faces with the same axial inclination as (111), viz. (111), (111), (1 11), (111), (111), (11 1) and (1 1 1). For further faces, the zonal equation is used. Eventually, a stereogram, like that in Fig. 5.27 may be produced showing the poles for all faces (hkl) with 2̄ ≤ h, k ≤ 2 and 0 ≤ l ≤ 2. An actual topaz crystal is shown in Fig. 5.28. Once such a crystal has been indexed with the aid of a stereogram, it is only necessary to measure a few angles on the actual crystal in order to bring the angles of the crystal into correspondence with the angles in the stereogram. The indexing of the stereogram in Fig. 5.27 may be accomplished very easily using the complication rule, formulated by V. Goldschmidt. This rule allows all of the faces of a zone to be indexed by addition or subtraction of the indices of two standard faces. The application of this rule is shown in Fig. 5.29. Let the starting faces be (100) and (010). Addition of (100) + (010) gives (110); (010) + (110) gives (120); (110) + (120) gives (230), etc. It should be clear that subtraction will in the end lead to similar results. All of the calculated planes belong to the zone [001]. In Fig. 5.30, two zone circles are shown, each having two indexed poles on it. The complication rule may be used to index the pole at the point of intersection. In zone 1, (011) + (110) gives (101), while in zone 2, (010) + (211) gives (201). These poles lie between their generating poles. The problem is solved when further addition or subtraction leads to a common point. In this case, from zone 1: (110) + (101) gives (211); while from zone 2, (201) + (010) gives (211), so the pole corresponding to 5.7 Indexing of a Crystal Fig. 5.27 Stereogram of the poles of those faces of a topaz crystal allowed by the lattice which have indices (2 ≤ h, k ≤ 2; 0 ≤ l ≤ 2) Fig. 5.28 Topaz crystal. (After [37]) 47 48 5 Morphology Fig. 5.29 Complication of the faces (100) and (010) Fig. 5.30 Indexing of the point of intersection of two zone circles by complication of the (hkl) for faces lying in these zones the intersection, has been indexed. This example is taken from Fig. 5.27. Note the relative positions of (101) and (201). A corollary of the complication rule is that all the faces of a crystal may be indexed by complication of the four simple planes (100), (010), (001) and (111). Table 5.1 gives the φ and ρ values for a crystal which has been measured on a two-circle reﬂection goniometer. Figure 5.31 gives the corresponding stereographic projection, in which the poles in the other octants may be inferred. The faces are to be indexed without reference to lattice constants. The crystallographic axes have been chosen to be parallel to the main zone axes of the stereographic projection. The faces normal to a, b and c can then be indexed directly. Since only (001) and (001) actually appear in the crystal, the positions of (100), (100), (010) and (010) have been added as auxiliary poles, and represented by open circles. One plane must then be chosen as the unit face (111), which cuts each crystallographic axes a, b, c, at unit length. These unit lengths give the relative spacings at which the unit face cuts the crystallographic axes, a, b, c. They are calculated below. The only faces that can be considered for this purpose are 5 and 6, as only they cut a, b and c all in a positive sense. It is reasonable to choose face 6 as the unit face, as the zone circles including this pole contain more poles than those cutting 5. It is now possible to index faces making equal intercepts on a, b and c, viz. (111), (111), (111) and (1 11), together with those having poles in the southern hemisphere, (111), (111), (11 1) and (1 1 1). These last have not been included in the stereogram, nor have any others in the southern hemisphere, i.e. those with negative ρ. Using 5.7 Indexing of a Crystal Table 5.1 φ and ρ angles for the topaz crystal in Fig. 5.28 φ Face 1,1 – ρ ± (hkl) 0◦ 001 2,2 0◦ ±43◦ 39 011 3,3 0◦ ±62◦ 20 021 4 43◦ 25 90◦ 120 5,5 62◦ 08 ±45◦ 35 112 6,6 62◦ 08 ±63◦ 54 111 7 62◦ 08 90◦ 110 8,8 90◦ ±61◦ 0 101 Fig. 5.31 Indexing of the topaz crystal in Fig. 5.28 the complication rule, it is now possible to index the following faces and their equivalents: (101) = (100) + (001) = (111) + (111), (011) = (010) + (001) = (111) + (111), (110) = (100) + (010) = (111) + (111). The remaining faces are then: 5 : (111) + (001) = (101) + (011) = (112) 3 : (010) + (011) = (111) + (110) = (021) 4 : (110) + (010) = (111) − (011) = (120) The crystal is now fully indexed, and is, in fact, the topaz crystal shown in Fig. 5.28. 49 50 5 Morphology Fig. 5.32 The all-positive octant of the topaz stereogram from Fig. 5.31 with the constructed trace of the (110) face The morphological axial ratios a:b:c, normally given as ba : 1 : bc , are characteristic of a crystal. The values for topaz can now be calculated: The (110) face cuts a and b at unit length (Fig. 5.32). The angle δ is the angle between (110) and (100), and from Table 5.1 (7), it is 90◦ − 62◦ 08 = 27◦ 52 . Thus ba = tan(27◦ 52 ) = 0.529. From Fig. 5.26, δ is the angle between (011) and (001), and from Table 5.1(2), δ = 43◦ 39 . Hence, bc = tan (43◦ 39 ) = 0.954, and the normalized morphological axial ratios may be given as ba : 1 : bc = 0.529 : 1 : 0.954. The numbers 0.529, 1 and 0.954 give the relative spacings (unit lengths) at which the unit face cuts the crystallographic axes a, b and c. Today, it is usual to formulate the structural axial ratio in terms of the lattice constants; for topaz . ba00 : 1 : bc00 = 0.528 : 1 : 0.955. 5.8 The Gnomonic and Orthographic Projections In addition to the stereographic projection, mention should be made of the gnomonic and orthographic projections. 5.8.1 The Gnomonic Projection As in the stereographic projection, the crystal is considered to lie at the center of a sphere. The normals to the faces produce points PG on a plane of projection, which is tangential to the sphere at the north pole (Fig. 5.33). The poles corresponding to the faces of a zone lie in straight lines on the projection plane. Figure 5.34 shows a gnomonic projection of the galena crystal in Fig. 5.9. As ρ approaches 90◦ , the distances N – PG approach inﬁnity. The poles of those faces with ρ = 90◦ are represented in the projection by arrows. The distance N – PG is R. tan ρ. 5.8 The Gnomonic and Orthographic Projections Fig. 5.33 The relationship of the stereographic, gnomonic and orthographic projections Fig. 5.34 Fig. 5.35 Fig. 5.34 Gnomonic projection of the galena crystal in Fig. 5.9 Fig. 5.35 Orthographic projection of the galena crystal in Fig. 5.9 5.8.2 The Orthographic Projection As in the stereographic projection, the crystal is again considered to lie at the center of a sphere. In distinction to the stereographic projection, the poles in the northern hemisphere are projected onto the equatorial plane along the N–S direction, and not toward the south pole (Fig. 5.33). Figure 5.35 shows an orthographic projection of the galena crystal in Fig. 5.9. The distance M – PO is R. sin ρ. Compare Figs. 5.12 and 5.35. The orthographic projection is widely used in the description of the symmetry of cubic space groups (Fig. 10.15). 51 52 5 Morphology 5.9 Exercises Exercise 5.1 Plot the poles of the faces of the following objects on a stereogram. Exercise 5.2 Plot the directions corresponding to the following axial systems on a stereogram. Fig. 5.36 Axial Systems 5.9 Exercises Exercise 5.3 Using copies of the patterns in Fig. 15.5(1)–(12), construct models of the polyhedral models given in Fig. 5.37. Plot the poles of the faces of the polyhedra you have made on a stereogram with the orientation chosen such that the altitude of each crystal is perpendicular to the plane of projection. The drawings below give the geometric shapes of the base or of any section normal to the altitude. Fig. 5.37 Crystal Polyhedra Exercise 5.4 Which faces of the hexagonal prism and pinacoid and of the tetragonal dipyramid belong to a single zone? Draw in the zone circle on the appropriate stereogram in Fig. 5.37. 53 54 5 Morphology Fig. 5.37 (Continued) Exercise 5.5 What is represented by the following stereograms? 5.9 Exercises Exercise 5.6 In a stereographic projection, choose a pole at random and draw in points 30◦ away from it in all directions. What is the locus of the points produced? Exercise 5.7 Construct a Wulﬀ net using a ruler, a protractor and a compass. Make the circles at intervals of 30◦ . Exercise 5.8 Insert poles of a stereographic projection with the following φ and values: (1) 80◦ , 60◦ ; (2) 160◦ , 32◦ ; (3) 130◦ , 70◦ . Determine the angle between (a) 1 and 2; (b) 1 and 3; (c) 2 and 3. Indicate the zone pole for the zones determined by (a) 1 and 2; (b) 1 and 3; (c) 2 and 3, and give φ and values for their positions. Exercise 5.9 The poles for the faces with angular coordinates 40◦ , 50◦ and 140◦ , 60◦ lie on zone circle A, while the poles 80◦ , 70◦ and 190◦ , 30◦ are on zone circle B. These zone circles have two points of intersection. Determine the angular coordinates φ, for these points. How are these faces orientated relative to each other? Exercise 5.10 What is the relationship among the normals to the faces comprising a zone? How are they related to the zone axis? Exercise 5.11 In the cubic unit cell shown in Fig 5.38 three diﬀerent sorts of axes are shown. Three axes () pass through the midpoints of opposite faces (x, 12 , 12 ; 12 ,y, 12 ; and 12 , 12 ,z). Four axes () lie along the body diagonals. Six axes (()) pass through the mid points of opposite edges. All of these axes intersect in the center of the unit cell. Fig 5.38 Cubic unit cell showing the axes through the midpoints of opposite faces (), along the body diagonals (), and through the midpoints of opposite edges (0). (After Buerger [8]) Draw the axes on a stereographic projection making use of the Wulﬀ net. It is convenient to place one of the axes () at the center of the plane of projection. The angles between the various axes may be taken from Fig. 5.39 and 5.40, which shows cross-sections through the center of the cube. 55 56 5 Morphology Fig. 5.39 Fig. 5.40 Fig 5.39 Section through the center of the cubic unit cell in Fig. 5.38 parallel to a cube face ( 21 ,y,z or x, 12 ,z or x,y, 12 ) Fig 5.40 Section x,x,z or x,1-x,z throught the cubic unit cell of Fig. 5.38. The angle O is 54.73◦ , half of the tetrahedral angle (the H-C-H angle in methane) of 109.46◦ Exercise 5.12 In the cubes illustrated below, planes have drawn parallel to the cube faces (a), and diagonal to them (b), so that each of these planes bisects the cube. Draw these planes as great circles and their respective projections on the accompanying stereographic diagram. Now draw all these great circles from (a), (b)1, (b)2, and (b)3 in the ﬁnal diagram, and label the axes with the symbols (), , and as in Exercise 5.11. Compare your stereogram with that in Fig. 7.13e. 5.9 Exercises 57 58 5 Morphology Exercise 5.13 The galena crystal in Fig. 5.41 (see also Fig. 5.1) was measured using a reﬂection goniometer. The angular coordinates φ and ρ are given in Table 5.2. (a) Draw a stereogram of the pole faces. (b) Compare this stereogram of galena with stereograms (a) and (b) in Exercise 5.12. Fig 5.41 Crystal of galena Table 5.2 Angular coordinates of the galena crystal in Fig. 5.41 Face ϕ 1.1 – ±0◦ 2,2 0◦ ±45◦ 3 0◦ 90◦ 4,4 45◦ ±54.73◦ 5 45◦ 90◦ 6,6 90◦ ±45◦ 7 90◦ 90◦ 8,8 135◦ ±54.73◦ 9 135◦ 90◦ 10,10 180◦ ±45◦ 11 180◦ 90◦ 12,12 225◦ ±54.73◦ 13 225◦ 90◦ 14,14 270◦ ±45◦ 15 270◦ 90◦ 16,16 315◦ ±54.73◦ 17 315◦ 90◦ Exercise 5.14 Draw a stereogram showing the pole faces of a crystal of rutile (TiO2 ), The lattice parameters are: a0 = b0 = 4.59 Å, c0 = 2.96 Å, α = β = γ =90◦ . Compare your stereogram with that given in Table 9.11.15. 5.9 Exercises Exercise 5.15 Draw the stereogram of a cube in its normal setting, i.e. with one face normal to the N–S direction. Rotate the cube to bring a body diagonal of the cube parallel to N–S, and draw the resulting poles of the faces on the stereographic projection. Exercise 5.16 Draw an orthographic projection of the axes of the cube-shaped unit cell shown in Fig. 5.38. The necessary angular values my be taken from Exercise 5.11. Sketch the main zone circles. Exercise 5.17 Draw a gnomonic projection of the topaz crystal in Fig. 5.28. The lattice constants are: a0 = 4.65, b0 = 8.80, c0 = 8.40 Å, α = β = γ = 90◦ . Exercise 5.18 The rate of growth of a crystal is an anisotropic property. What shape would a crystal have if its growth rate were isotropic? 59 6 Principles of Symmetry Up to now, the only repetition operation that we have used formally has been the lattice translation: the operation of three non-coplanar lattice translations on a point which gives rise to the space lattice. Fig. 6.1 This wheel may be considered either as derived from an object consisting of a single spoke which is repeated by rotation every 45◦ or as an object which is brought into coincidence with itself by a rotation of 45◦ In addition to lattice translations, there are other repetition operations, such as rotations and reﬂections. In these cases, an object is brought into a coincidence with itself by rotation about an axis or reﬂection in a plane. D All repetition operations are called symmetry operations. Symmetry consists of the repetition of a pattern by the application of speciﬁc rules. In the wheel illustrated in Fig. 6.1, the spokes are repetitions of one another at intervals of 45◦ , or alternatively, as the wheel rotates, it is brought into coincidence with itself by every rotation of 45◦ . D When a symmetry operation has a “locus”, that is a point, a line, or a plane that is left unchanged by the operation, this locus is referred to as the symmetry element. Figure 6.2 is an illustration of a crystal of gypsum. The right-hand half of the crystal can be brought into coincidence with the left-hand half through a reﬂection W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_6, C Springer-Verlag Berlin Heidelberg 2011 62 6 Principles of Symmetry Fig. 6.2 Reﬂection of either side of this gypsum crystal in the hatched plane indicated brings it into coincidence with the other side. This plane is called a mirror plane in the hatched plane, which will equally bring the left-hand side into coincidence with the right. Every point in the crystal will be moved by this reﬂection operation except those which actually lie on the reﬂection plane itself. The plane containing these points is thus the symmetry element corresponding to the symmetry operation of reﬂection; it is called a mirror plane. Rotation through 180◦ about the axis marked with an arrow will bring either half of the pair of scissors in Fig. 6.3 into coincidence with the other half. Alternatively, rotation of the pair of scissors through 180◦ brings it into coincidence with itself. Every point on the scissors moves during this operation except those that lie on the rotation axis (the arrow) itself. The points comprising this axis make up the symmetry element corresponding to the symmetry operation of rotation: the rotation axis. Fig. 6.3 Rotation of the pair of scissors through 180◦ about the axis marked with an arrow brings it into coincidence with itself. This axis is called a rotation axis Fig. 6.4 Either pentagon is brought into coincidence with the other by reﬂection in a point. This is called inversion, and the point which remains unmoved by the operation is called an inversion center or center of symmetry 6.1 Rotation Axes Another type of symmetry is shown by the pair of irregular pentagons in Fig. 6.4. Reﬂection of either pentagon through the indicated point will bring it into coincidence with the other pentagon. In this symmetry operation, which is called inversion, only a single point remains unchanged, it is the symmetry element of the symmetry operation inversion and is called an inversion center or a center of symmetry. 6.1 Rotation Axes What symmetry elements are present in a general plane lattice, such as that shown in Fig. 6.5? Make a copy of the ﬁgure on tracing paper and lay the copy directly over the original. Then rotate the copy about the central lattice point A until both lattices come into coincidence once more. In this case, this will happen after a rotation of 180◦ , and a further rotation of 180◦ makes a full 360◦ rotation, returning the upper lattice to its original position. The symmetry element corresponding to the symmetry operation of rotation is ◦ called a rotation axis. The order of the axis is given by X where X = 360 ε , and ε is the minimum angle (in degrees) required to reach a position indistinguishable from ◦ the starting point. In the above case, X = 360 180◦ = 2, and the axis is called a 2-fold rotation axis. The symbol for this operation is simply the digit 2. In a diagram, it is if it is normal to the plane of the paper, or as → if it is parallel to it. represented as Whenever a 2-fold axis passes through a point A, a 2-fold axis must pass through all points equivalent by translation to A. 2-fold axes normal to the lattice plane will Fig. 6.5a, b A general plane lattice (a) and its symmetry (b). Symmetry elements marked with the same letter are equivalent to one another 63 64 6 Principles of Symmetry also pass through all points B, C and D which lie on the midpoints of a translation vector. There are thus an inﬁnite number of rotation axes normal to this plane. Objects are said to be equivalent to one another if they can be brought into coincidence by the application of a symmetry operation. If no symmetry operation except lattice translation is involved, the objects are said to be “equivalent by translation” or “identical”. In Fig. 6.5, all rotation axes A are equivalent to one another, as are all axes B, C and D. On the other hand, the axes A are not equivalent to B, and so forth. A crystal, in which congruent lattice planes (Fig. 6.5) lie directly one above the other, may develop a morphology in which the lower and upper faces are corresponding parallelograms (pinacoid), and the side faces are all perpendicular to these (Fig. 6.6). Such a crystal will come into coincidence with itself if it is rotated through 180◦ about an axis through the middle of the upper and lower faces. It thus contains a single 2-fold axis. This observation may be generalized as follows: Fig. 6.6 A crystal with upper and lower parallelogram faces and sides perpendicular to them has – so far as its morphology is concerned – only a single 2-fold axis ! The morphology of a single crystal will show only one symmetry element of a particular type in a particular direction, although both its lattice and its crystal structure will show inﬁnitely many parallel elements. Let us now consider whether it is possible to have axes of order higher than 2. An axis with X > 2 operating on a point will produce at least two other points lying in a plane normal to it. Since three non-colinear points deﬁne a plane, this must be a lattice plane. Thus, rotation axes must invariably be normal to lattice planes, and we must decide whether the points generated by a rotation axis can fulﬁll the conditions for being a lattice plane, speciﬁcally, that parallel lattice lines will have the same translation period. Threefold Rotation Axis 3 (graphical symbol ). Figure 6.7a shows a 3-fold rotation ◦ , axis normal to the plane of the paper. By its operation, a rotation of 120◦ = 360 3 point I comes into coincidence with point II, and, by a second rotation of 120◦ with point III. A further rotation of 120◦ returns it to its original location. A lattice 6.1 Rotation Axes translation moves point I to point IV, and the four points thus generated produce the unit mesh of a lattice plane. Thus, 3-fold axes are compatible with space lattices. Fourfold Rotation Axis 4 (graphical symbol ). Fourfold axes are also compatible with space lattices. As shown in Fig. 6.7b, the action of a 4-fold axis on a point results in a square of points which is also the unit mesh of a lattice plane. Fig. 6.7a–c The arrays of points resulting from the operation on a point of (a) 3-fold, (b) 4-fold, and (c) 6-fold axes normal to the plane of the paper can lead to lattice planes. additional points produced by lattice translations Fivefold Rotation Axis 5. The operation of this axis on a point results in a regular pentagon of points, as shown in Fig. 6.8a. The line through points III and IV is parallel to that through II and V. If these are to be lattice lines, the spacings of the two pairs of points must either be equal or have an integral ratio. Since this is clearly not the case, the points in Fig. 6.8a do not constitute a lattice plane, and we may conclude that 5-fold axes are impossible in space lattices! Fig. 6.8a–c The arrays of points resulting from the operation on a point of a 5-fold, b 7-fold, and c 10-fold axes do not fulﬁll the conditions for a lattice plane, in that parallel lines through equivalent points do not have equal spacings. These rotation symmetries cannot occur in lattices Sixfold Rotation Axis 6 (graphical symbol ).1 This operation, applied to a single point, results in a regular in a regular hexagon (Fig. 6.7c). A lattice translation places 1 The standard international symbols for 2, 3, 4 and 6 are , , , and , respectively. For are also used here. In Chap. 9, ﬁlled and unﬁlled symbols are used to convenience, , , and distinguish the ends of a polar rotation axis Xp . 65 66 6 Principles of Symmetry Table 6.1 Derivation, using Eq. (6.5), of the rotation axes X which are compatible with a space lattice cos ε ε X 0 0 90◦ 4 1 1 2 60◦ 6 1 m 2 1 0◦ , 360◦ –1 – 12 120◦ 3 –2 –1 180◦ 2 a lattice point on the axis itself, and the resulting array meets the condition for a lattice plane. Inspection of Fig. 6.7a,c will show that the lattices resulting from 6-fold and 3-fold axes are, in fact, equal. Rotation Axes of Order Higher Than 6. Figure 6.8b,c shows the eﬀect of attempting to build up a lattice plane by applying 7-fold and 10-fold axes to a point. The results are analogous to those for the 5-fold axis described in paragraph (c) above. These arrays do not produce equal spacings of points in parallel lines and so cannot occur in lattices. The same result will occur for any rotation axis with X > 6. This result can also be formulated mathematically. Figure 6.8 shows 10 equivalent points resulting from a 10-fold rotation axis. Points I and V lie on a line parallel to that connecting points II and IV. If these are to be lines of a plane net, then I–V must either equal II–IV or be an integral multiple of it. (1) I − V = m · II − IV (6.1) (2) I − V = 2r · sin 2ε = 4r · sin ε · cos ε (6.2) (3) II − IV = 2r · sin ε (1) 4r · sin ε · cos ε = m · 2r · sin ε cos ε = m/2 (6.3) (6.4) (6.5) Since –1 ≤ cos ε ≤ +1, m must be 0, 1, 2, –1 or –2. Table 6.1, along with Eq. (6.5) (cos ε = m/2) establishes the rotation axes that are compatible with a space lattice. ! In space lattices and consequently in crystals, only 1-, 2-, 3-, 4-, and 6-fold rotation axes can occur. 6.2 The Mirror Plane A further symmetry operation is reﬂection and the corresponding symmetry element is called a plane of symmetry or, more commonly, a mirror plane, and given the symbol m. The graphical symbol for a plane normal to the paper is a bold line, 6.3 The Inversion Center Fig. 6.9 The operation of a mirror plane m on an asymmetric molecule. The mirror plane, perpendicular to the paper, transforms A into B and likewise B into A Fig. 6.10a, b Operation of m on a lattice line: in a the lattice line is parallel to m. The resultant plane lattice is primitive with a rectangular unit cell. In b, the lattice line is tilted with respect to m. The resultant plane lattice again has a rectangular unit cell, but is now centered. additional points produced by lattice translations as in Fig. 6.9. A mirror plane parallel to the paper is represented by a bold angle; an example of this is in Sect. 15.2. Any point or object on one side of a mirror plane is matched by the generation of an equivalent point or object on the other side at the same distance from the plane along a line normal to it (Fig. 6.9). Figure 6.10 shows the operation of a mirror plane on a lattice line A, generating another lattice line A . Whether the line A is parallel to the mirror plane or not, the result is a rectangular unit mesh. The generation of the lattice plane in Fig. 6.10b requires that a lattice point lies on m; this lattice contains two points per unit mesh and is called centered. A primitive mesh is not chosen in this case since the rectangular cell (with the symmetry plane parallel to an edge) is easier to work with. 6.3 The Inversion Center The symmetry operation called inversion relates pairs of points or objects which are equidistant from and on opposite sides of a central point (called an inversion center or center of symmetry). The symbol for this operation is 1, and is explained in Sect. 6.4.1a. An illustration of this operation on a molecule is given in Fig. 6.11. The graphical symbol for an inversion center is a small circle. Every space lattice has this operation and is thus centrosymmetric, see Fig. 6.12. 67 68 6 Principles of Symmetry Fig. 6.11 The operation of an inversion center (0) on asymmetric molecules Fig. 6.12 The unit cell of a general lattice, showing the inversion at 12 , 21 , 21 . All lattices are centrosymmetric The operation of an inversion center on a crystal face generates a parallel face on the opposite side of the crystal. An example of this is the crystal of malonic acid in Table 9.11.2 which has no symmetry other than inversion, and is entirely enclosed by pairs of such parallel faces (or pinacoids). The occurrence of such pairs of parallel faces is important for the detection of inversion symmetry in crystals. 6.4 Compound Symmetry Operations The operations of rotation, inversion, reﬂection and lattice translation may be linked with one another. There are two possibilities to be considered here: (a) Compound Symmetry Operation. Two symmetry operations are performed in sequence as a single event. This produces a new symmetry operation but the individual operations of which it is composed are lost. (b) Combination of Symmetry Operations. In this case, two or more individual symmetry operations are combined which are themselves symmetry operations. Both they and any combination of them must be compatible with the space lattice. 6.4 Compound Symmetry Operations Fig. 6.13a, b Compound symmetry operation a and combination of symmetry elements b of a 4-fold rotation and an inversion, illustrated by the eﬀect on the point 1. In a the rotation and the inversion are not present; in b they are present. The open circles in a represent auxiliary points occupied when only one part of the compound operation has been applied. In b, the combination of the rotation and the inversion results also in a mirror plane normal to the axis These diﬀerent cases may be illustrated for 4-fold rotation and inversion by considering the examples given in Fig. 6.13. (a) Compound Symmetry Operation. Figure 6.13a shows an operation which consists of a rotation of 90◦ about an axis followed by an inversion through a point on the axis. Successive applications of this compound operation move a point at 1 to 2, 3, 4, and back to 1. Note that the resulting array has neither an inversion center nor a 4-fold rotation axis. (b) Combination of Symmetry Operations. Figure 6.13b illustrates the result of the operations 4-fold rotation and inversion also being present themselves. Successive operations of the 4-fold axis move a point from 1 to 2, 3, 4 and back to 1, while the inversion center moves it from each of those positions to 7, 8, 5 and 6 respectively. Combinations of symmetry operations will be further examined in Chaps. 6, 8 and 9. Compound symmetry operations are summarized in Table 6.2, where the names Table 6.2 Compound symmetry operations of simple operations. The corresponding symmetry elements are given in round brackets Rotation Rotation × Reﬂection Inversion Translation Roto-reﬂection Roto-inversion Screw rotation 2-fold rotation Glide reﬂection Reﬂection (Roto-reﬂection axis) × Inversion (Roto-inversion axis) (2-fold rotation axis) Translation (Screw axis) (Glide plane) × (Inversion center) Inversion × 69 70 6 Principles of Symmetry of the symmetry elements corresponding to the symmetry operations are given in round brackets. Neither reﬂection plus inversion nor translation plus inversion results in a new operation. Glide and screw operations are beyond the needs of the present discussion and will be covered in Sect. 9.1. 6.4.1 Rotoinversion Axes The compound symmetry operation of rotation and inversion is called rotoinversion. Its symmetry elements are the rotoinversion axes, with the general symbol X (pronounced X-bar or bar-X). There are only ﬁve possible rotation axes X: 1, 2, 3, 4 and 6, and ﬁve corresponding rotoinversion axes X : 1, 2, 3, 4 and 6. (a) Rotoinversion Axis 1 (Fig. 6.14a). 1 implies a rotation of 360◦ followed by inversion through a point on the 1-fold rotoinversion axis. The operation of 1 on a point 1 returns it to its starting position, and the subsequent inversion takes it to point 2. The same operations on point 2 bring it to the original position of point 1. The rotoinversion operation 1 is thus identical to inversion through an inversion center. For this reason, 1 is used as a symbol for the inversion center. Fig. 6.14a–d The operation of rotoinversion axes on a point 1: a 1. b 2 ≡ m. c 3 ≡ 3 + 1. d 6 ≡ 3 ⊥ m. For 4, see Fig. 6.10a. The unﬁlled circles represent auxiliary points which are not occupied when the two operations of which the compound operation is composed are not themselves present (b) Rotoinversion Axis 2 (Fig. 6.14b). The eﬀect of rotation through an angle of 180◦ followed by inversion is to take a point from 1 to 2. A repetition of this compound operation returns it to its original position. The two points are, 6.4 Compound Symmetry Operations however, also related to one another by reﬂection in a plane normal to the axis. The operation 2 is thus identical with m, and need not be considered further. Note, however, that 2 represents a direction normal to m. (c) Rotoinversion Axis 3 (graphical Symbol ) (Fig. 6.14c). Successive applications of the operation 3 move a point to altogether six equivalent positions. In this case, both of the simple operations 3 and 1 are necessarily present , 3 ≡ 3 + 1 so the compound symmetry operation is here a combination of symmetry operations. (d) Rotoinversion Axis 4 (graphical symbol ) (Fig. 6.13a). The 4 axis has already been analyzed in the previous section. As may be seen in Fig. 6.13a, and as the graphical symbol indicates, 4 implies the presence of a parallel 2. (e) Rotoinversion Axis 6 (graphical symbol ) (Fig. 6.14d). Successive applications of 6 move a point to altogether six equivalent positions. It can be seen that 6 implies the presence of a parallel 3 and a perpendicular m: 6 ≡ 3⊥m. The unambiguous demonstration of the relationships: 1 ≡ inversion center, 2 ≡ m, 3 ≡ 3 + 1, 4 implies 2, and 6 ≡ 3⊥m in Figs. 6.13a and 6.14 is only possible when an object such as an unsymmetrical pyramid is operated upon by symmetry operations (see Exercise 6.1a). Note particularly that only rotoinversion axes of odd order imply the presence of an inversion center, e.g. 1 and 3. Note that this also applies to the non-crystallographic axes 5, 7 etc. 6.4.2 Rotoreﬂection Axes Like the rotoinversion axes, rotoreﬂection axes S1 , S2 , S3 , S4 , and S6 may be deﬁned. Rotoreﬂection implies the compound operation of rotation and reﬂection in a plane normal to the axis. However, these axes represent nothing new, since it is easy to demonstrate the correspondence S1 ≡ m; S2 ≡ 1; S3 ≡ 6; S4 ≡ 4; S6 ≡ 3. Rotoinversion axes are now invariably used in crystallography. The symmetry elements with which the crystallographer is concerned are the proper rotation axes X (1, 2, 3, 4 and 6) and the rotoinversion or improper axes X(1 ≡ inversion center, (2) ≡ m, 3, 4 and 6). In addition to these, there are screw axes and glide planes (see Sect. 10.1). ! The axes X and X, including 1 and m, are called point-symmetry elements, since their operations always leave at least one point unmoved. For 1, this property applies to every point in space, for m to every point on the plane, for 2, 3, 4, 6, to every point on the axis, and for 1, 3, 4 and 6 to a single point. A mathematical description of the point symmetry operations is given in Sect. 11.1 (see also Table 11.1) 71 72 6 Principles of Symmetry 6.5 Exercises Exercise 6.1 The ten crystallographic point symmetry operations are shown below. Carry out these operations on: (a) An unsymmetrical pyramid, whose base lies into the plane of the paper. Sketch the appearance of the generated pyramids, using dotted lines for those lying below the paper. (b) A general pole on a sterographic projection. 6.5 Exercises Exercise 6.2 Carry out the rotoreﬂection operations S1 , S2 , S3 , S4 and S6 on a general pole on a stereographic projection, and compare these with the stereograms of the rotation-inversion axes 1, 2 ≡ m, 3, 4 and 6 in Exercise 6.1. Exercise 6.3 When two faces are related by an inversion center 1, how must they lie with respect to one another? – Exercise 6.4 Carry out the rotoinversion operation (a) 5 (b) 8 (c) 10 on a general pole on a stereographic projection. 73 74 6 Principles of Symmetry Exercise 6.5 Analyse the rotoinversion axes (cf. Exercise 6.1 and 6.4) into simple symmetry elements, if it is possible. Exercise 6.6 Which rotoinversion axes contain an inversion center? Exercise 6.7 What crystal form is developed by the faces whose poles result from the operation of 3, 4, 6 and 6 on a general pole? (see Exercise 6.1b). Exercise 6.8 What shape is implied for the section of a prism which has a 2-, 3-, 4-, or 6-fold axis? Exercise 6.9 Determine the location of the rotation axes of a cube. Draw these axes, showing the points at which they enter the cube (see Fig. 15.6 (3)). 7 The 14 Bravais Lattices The general space lattice, with no restrictions on the shape of the unit cell (Fig. 3.4 with a0 = b0 = c0 , α0 = β0 = γ0 ), may be used to describe all crystals. In most cases, however, the lattices which occur are special in that they have special features, such as unit cell dimensions (lattice parameters) which are equal in two or three directions or angles between cell edges with particular values, such as 60◦ , 90◦ , 120◦ or 54.73◦ , such as the cubic unit cell in Fig. 3.1b (a0 = b0 = c0 , α0 = β0 = γ0 = 90◦ ). The general lattice has no point symmetry elements except inversion centers. The presence of rotation axes and mirror planes will restrict the cell parameters in some way, and give special lattices. These special lattices give rise to simpliﬁcations in the crystal morphology and in physical properties. ! When lattice translations in two directions are equivalent, all physical properties are equal in these directions. In addition to the general space lattice, there are several special lattices. Before we consider these space lattices, however, it is useful to develop the relevant concepts by consideration of general and special plane lattices. The General (Oblique) Plane Lattice If we take a point 1, and operate on it with a 2-fold axis, we will generate an equivalent point 2 (Fig. 7.1a). The application of a lattice translation a to point 1 generates an identical point 3 (Fig. 7.1b), and the 2-fold axis then relates point 3 to point 4 (Fig. 7.1c). We have now generated a unit mesh of the lattice. It has the shape of an oblique parallelogram, where a0 = b0 and γ = 90◦ . Note that here and throughout this book, in reference to symmetry, = means need not be equivalent while = means are required by symmetry to be equivalent. It is possible to vary a0 , b0 and γ in any way we like without losing the 2-fold axis. Thus this lattice is fully general. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_7, C Springer-Verlag Berlin Heidelberg 2011 76 7 The 14 Bravais Lattices Fig. 7.1a–c Development of the general plane lattice, with an oblique unit mesh Special Plane Lattices (a) Returning to Fig. 7.1a, point 3 could have been chosen so that the points 1, 2 and 3 described a right triangle, with the right angle at point 3 (Fig. 7.2a). The operation of the 2-fold axis now results in a rectangular unit mesh, a0 = b0 , γ = 90◦ . The arrangements of the points is now “special”, as further symmetry has been introduced, namely two mutually perpendicular mirror planes, parallel to the 2-fold axis (Fig. 7.2b). Fig. 7.2a, b Development of the special plane lattice with a rectangular unit mesh (a) and its symmetry (b) (b) A further possibility in Fig. 7.1a would be to choose the location of point 3 so that points 1, 2 and 3 formed an isosceles triangle with the two equal edges meeting at point 3. The unit mesh of the resulting lattice is a rhombus: a0 = b0 , γ = 60◦ , 90◦ or 120◦ (Fig. 7.3a). Extension of the edges 1–4 and 1–3 a further unit translation on the other side of 1, an alternative choice of unit mesh arises (Fig. 7.3b). It is rectangular (a 0 = b 0 , γ = 90◦ ), and is called centered because Fig. 7.3a–c Development of the special plane lattice with a rhombic unit mesh (a), and its alternative description by a centered rectangular mesh (b). Symmetry of the plane lattice (c) 7 The 14 Bravais Lattices it has a point at its center identical to those at the vertices. Consideration of the symmetry of this cell shows that there are a pair of mirror planes, similar to those in Fig. 7.2b, and several 2-fold axes (Fig. 7.3c). (c) Returning once more to Fig. 7.1a, we choose the position of point 3 in such a way as to make the points 1, 2 and 3 describe an isosceles right triangle, with the right angle at 3. The resultant lattice now has a square unit mesh: a0 = b0 , γ = 90◦ . As shown in Fig. 7.4b, there are now a 4-fold axis and four mirror planes parallel to it in the cell. Fig. 7.4a, b Development of the special plane lattice with a square unit mesh and its symmetry (d) Finally, let us choose the position of point 3 in Fig. 7.1a such that the points 1, 2 and 3 make an equilateral triangle (Fig. 7.5a). The unit mesh of the resulting hexagonal lattice is now a 120◦ rhombus, or a0 = b0 , γ = 120◦ . In addition to the 2-fold axis, there are now 3- and 6-fold axes as well as several mirror planes. The axes are shown in Fig. 7.5b (see also Fig. 6.7a, c). Fig. 7.5a, b Development of the special hexagonal plane lattice and its symmetry. The unit mesh is a 120◦ rhombus We have now developed all four of the possible special plane lattices (which were, in fact, introduced in a diﬀerent way in Chap. 6) from the general plane lattice. These plane lattices are summarized in Table 7.1 with their characteristic symmetry elements. The general lattice (see Fig. 7.5) possesses 2-fold axes only, but the special lattices (a)–(d) all have further symmetry elements, which are shown on their diagrams in Fig. 7.6. It should be noted that only point symmetry elements are shown here. There are compound symmetry elements involving translation, glide planes (see Sect. 10.1). 77 78 7 The 14 Bravais Lattices Table 7.1 Plane lattices Shape of unit mesh Lattice parameters Characteristic symmetry elements Parallelogram a0 = b0 γ = 90◦ 2 6.5 7.1c a Rectangle (primitive) a0 = b0 γ = 90◦ m 7.2a 7.6a b Rectangle (centered) a0 = b0 γ = 90◦ m 7.3b 7.6b c Square a0 = b0 γ = 90◦ 4 7.4a 7.6c d 120◦ Rhombus a0 = b0 γ = 120◦ 6 (3) 7.5a 7.6d General plane lattices Special plane lattice Fig. 7.6a,b Symmetry elements of the special lattice planes with a primitive (a) and a centered (b) rectangular unit mesh, and a square (c) and a hexagonal (120◦ rhombus) (d) unit mesh Figure 7 Fig. 7.6c,d (Continued) The 14 Bravais Lattices 79 80 7 The 14 Bravais Lattices 7.1 The Primitive Space Lattices (P-Lattices) The relationships between lattices and symmetry elements in three dimensions are similar to those in two. From the general space lattice, several special space lattices may be derived, in which congruent lattice planes are stacked above one another. If the symmetry of the lattice planes is not changed, the ﬁve space lattices with primitive unit cells (P-lattices) are produced. These are given in Table 7.2. Compare the stacking processes illustrated in Figs. 7.7, 7.8, 7.9a, b, 7.10 and 7.11a, b. Notice that the centered rectangular plane lattice (b) does not occur. The square lattice may be stacked either with c0 = a0 = b0 or c0 = a0 = b0 ; the former develops the tetragonal P-lattice and the latter the cubic P-lattice. The cubic lattice is a special case of the tetragonal, since new, characteristic symmetry elements appear (three-fold rotation axes along the body diagonals of the unit cell). The generation of the general or triclinic P-lattice by stacking is shown in Fig. 7.12a. All of the P-lattices are illustrated in Table 7.3. Table 7.2 P-lattices Shape of unit mesh in stacked layers Interplanar spacing Lattice Figure Parallelograma (a0 = c0 ) b0 Monoclinic P 7.8a, b Rectangle (a0 = b0 ) c0 Orthorthombic P 7.9a, b Square (a0 = b0 ) c0 = (a0 = b0 ) Tetragonal P 7.10a, b Square (a0 = b0 ) c0 = (a0 = b0 ) Cubic P 7.13a, b c0 Hexagonal P 7.12a, b 120◦ -Rhombus (a0 = b0 ) Note that for historical reasons, the description a0 = b0 , γ = 90◦ has been changed in this case to a0 = c0 , β = 90◦ a 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.7a–f The triclinic crystal system 81 82 7 The 14 Bravais Lattices Fig. 7.8a–d The monoclinic crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.8e,f (Continued) 83 84 7 The 14 Bravais Lattices Fig. 7.9a–d The orthorhombic crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.9e,f (Continued) 85 86 7 The 14 Bravais Lattices Fig. 7.10a–d The tetragonal crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.10e,f (Continued) 87 88 7 The 14 Bravais Lattices Fig. 7.11a–d The trigonal crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.11e,f (Continued) 89 90 7 The 14 Bravais Lattices Fig. 7.12a–d The hexagonal crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.12e,f (Continued) 91 92 7 The 14 Bravais Lattices Fig. 7.13a–d The cubic crystal system 7.1 The Primitive Space Lattices (P-Lattices) Fig. 7.13e,f (Continued) 93 94 7 The 14 Bravais Lattices Table 7.3 The 14 Bravais lattices 7.2 The Symmetry of the Primitive Lattices 7.2 The Symmetry of the Primitive Lattices Before considering the symmetry of lattices, it is useful to learn two rules governing the generation of a symmetry element by the combination of two others. In the following two cases, the presence of any two of the given symmetry elements implies the presence of the third. Combination of symmetry elements is no casual occurrence; it is fundamental to the nature of symmetry. ! In the following two rules the presence of any two of the given symmetry elements implies the presence of the third: Rule I. A rotation axis of even order (Xe = 2, 4 or 6), a mirror plane normal to Xe , and an inversion center at the point of intersection of Xe and m (Fig. 7.13).1 Rule II. Two mutually perpendicular mirror planes and a 2-fold axis along their line of intersection (Fig. 7.14) Every lattice is centrosymmetric and has inversion centers on the lattice points and midway between any two of them. Thus, in a P-lattice, there are inversion centers at 0,0,0; 12 ,0,0; 0, 12 ,0; 0,0, 12 ; 12 , 12 ,0; 12 ,0, 12 ; 0, 12 , 12 and 12 , 12 , 12 . Fig. 7.14a–c Symmetry rule I: (a) 2⊥m → 1̄ (at the intersection of 2 and m); (b) 1̄ on m → 2 (passing through 1̄ and normal to m); (c) 1̄ on 2 → m (passing through 1̄ and normal to 2) Fig. 7.15a–c Symmetry rule II: (a) m ⊥ m → 2 (along the intersection of m and m ; (b) 2 on m → m ⊥m" (with 2 as the line of intersection); (c) 2 on m → m ⊥m (with 2 as the line of intersection) 1 Xe = 2, 4 or 6. The illustration only includes the case Xe = 2. The rule is not completely general, since m + 1̄ can only generate 2. 95 96 7 The 14 Bravais Lattices 7.2.1 Symmetry of the Triclinic P-Lattice The only point symmetry elements of the triclinic lattice are inversion centers (Fig. 7.15) at the coordinates given above. A projection of the symmetry elements parallel to c onto x,y,0 is shown in Fig. 7.16. The z-coordinates implied for the inversion centers are 0 and 12 . Fig. 7.16 Triclinic P-lattice with the symmetry elements of space group P1̄ ( 1̄ on lattice point) Fig. 7.17 Projection of the symmetry elements of space group P1̄ onto x,y,0. The z-coordinates of 1̄ are 0 and 12 , cf. Fig. 7.16 D The complete set of symmetry operations in a lattice or a crystal structure, or a group of symmetry operations including lattice translations is called a space group. The space group of a primitive lattice which has only 1̄ is called P1̄, and the conditions for its unit cell parameters: a0 = b0 = c0 ; α = β = γ . 7.2.2 Symmetry of the Monoclinic P-Lattice The set of lattice planes from which we generated the monoclinic P-lattice (Fig. 7.8a) contain a set of 2-fold axes parallel to b. In addition, there are mirror planes normal to b at x,0,z and x, 12 ,z as well as the inversion centers that were present in the triclinic case. The location of the mirror planes follows from our ﬁrst rule: (2 and 1̄ generate 7.2 The Symmetry of the Primitive Lattices m ⊥ 2 at 1̄.) The array of symmetry elements of the lattice is shown in Fig. 7.8d in projections on x,0,z and x,y,0.2 Since the 2 is normal to the m, this combination is given the symbol 2/m, pronounced “two over m”. It is not necessary to represent the inversion center, since 2/m implies 1̄, by Rule I. The space group of the monoclinic P-lattice is P2/m, where it is conventional to choose the b-axis parallel to 2 and normal to m. The b-axis is called the symmetry direction. The a- and c-directions thus lie in the plane of m. This is called the “second setting”. Occasionally, the so-called “ﬁrst setting” is encountered, with the c-direction parallel to 2 and normal to m. When this convention is used, the lattice is formed in the more usual way by the stacking of parallel lattice planes with a0 = b0 , γ = 90◦ , and a spacing of c0 . 7.2.3 Symmetry of the Orthorhombic P-Lattice In addition to the symmetry of the stacked planes (Fig. 7.9a), the orthorhombic P-lattice (Fig. 7.9b) has mirror planes normal to c at x,y,0 and x,y, 12 and inversion centers (Fig. 7.9d). Further, the application of rule I (m + 1̄ ⇒ 2 ⊥ m) or rule II (m ⊥ m ⇒ 2) generates 2-fold axes at x,0,0; x,0, 12 ; x, 12 ,0; x, 12 , 12 ; 0,y,0; 0,y, 12 ; 12 ,y,0 and 12 ,y, 12 . An alternative approach, which leads to the same result is the following: the unit cell of the orthorhombic P-lattice is a rectangular parallelepiped; it is bounded by three pairs of lattice planes with primitive rectangular unit meshes. These planes all have the same symmetry, that shown in Fig. 7.9a. The arrangement of symmetry elements is shown in Fig. 7.18, which should be compared with Fig. 7.9d. This set of symmetry elements can be given a symbol. The symmetry elements are arranged in the order of the crystallographic axes: a,b,c. Each axis has a 2-fold rotation axis Fig. 7.18 Symmetry elements of space group P 2/m 2/m 2/m. The inversion centers are not shown 2 In the diagrams, the symbol indicates a mirror plane parallel to the plane of the page at heights of 0 and 12 . When the planes lie at other heights, such as 14 and 34 , this is shown by adding 1 1 1 3 4 . Note that if there is an m, 2 or 1̄ at 0, it is also found at 2 ; if it lies at 4 , it is also at 4 , etc. 97 98 7 The 14 Bravais Lattices Fig. 7.19 a Space group P 2/m 2/m 2/m. In the other diagrams, only the symmetry elements corresponding to the symmetry directions a, b, c are shown: b P2/m . . . . . . , c P . . . 2/m . . . , d P . . . . . . 2/m ↓ ↓ ↓ c b a 7.2 The Symmetry of the Primitive Lattices parallel to it and mirror planes normal to it. Thus, the symbol for this space group P2/m 2/m 2/m ↓ ↓ . is: ↓ a b c Here the a-, b- and c-axes are all called symmetry directions. Figure 7.19, gives a projection of all point symmetry elements of space group P2/m2/m 2/m, and separate projections showing those elements related to the symmetry directions a, b and c. 7.2.4 Symmetry of the Tetragonal P-Lattice In addition to the symmetry of the stacked planes (Fig. 7.10a), the tetragonal P-lattice (Fig. 7.10b) has mirror planes ⊥ c at x,y,0 and x,y, 12 and inversion centers (Fig. 7.10d). Further, the application of Rule I (m + 1̄ ⇒ 2 ⊥ m) or rule II (m ⊥ m ⇒ 2) generates several 2-fold axes. It should be noted in passing that the projection of the symmetry elements for this space group in Fig. 7.10d is incomplete, since there are also glide planes present (Sect. 9.1). The same is true for the space groups in Figs. 7.10d–7.13d, which in addition contain screw axes. These symmetry elements are essentially irrelevant to our present purpose, and will not be considered further here. The unit cell of a tetragonal P-lattice has the shape of a tetragonal prism; it is bounded by two lattice planes with square unit meshes and four planes with rectangular meshes, the symmetries of which are shown in Fig. 7.20. Compare Fig. 7.20 with Fig. 7.10d, noting that the 2-fold axes parallel to [110] and [11̄0] do not appear in Fig. 7.20. The 4-fold axes have the eﬀect of making a and b equivalent, and they are often denoted as a1 and a2 , as in Fig. 7.10d. Similarly, the directions [110] and [11̄0] are equivalent to one another. We must now introduce a further type of brackets, pointed brackets . The symbol uvw denotes the lattice direction [uvw] and all directions equivalent to it. Similarly, a denotes the a-axis and all equivalent axes. Fig. 7.20 Symmetry elements of space group P 4/m 2/m 2/m. The 2 along 110 and the inversion centers are not shown 99 100 7 The 14 Bravais Lattices Fig. 7.21 a Space group P 4/m 2/m 2/m. In the other diagrams, only the symmetry elements corresponding to the symmetry directions c, a, 110 are shown: b P 4/m . . . . . . , c P . . . 2/m . . . , d P . . . . . . 2/m ↓ ↓ ↓ a 110 c 7.2 The Symmetry of the Primitive Lattices For the tetragonal lattice, 110 implies both the [110] and the [11̄0] directions, and a implies both the a- and b-axes. In the space group symbol, the symmetry elements are given in the order: c, a, diagonal of the a-axes, viz. 110, all of which are called symmetry directions. Thus, equivalent symmetry operations are given only once. The space group symbol is thus P 4/m 2/m 2/m. ↓ ↓ ↓ a 110 . c Figure 7.21 gives a projection of all point symmetry elements of space group P4/m 2/m 2/m, and separate projections showing those elements related to the symmetry directions c, a and 110. 7.2.5 Symmetry of the Hexagonal P-Lattice In addition to the symmetry of the stacked planes, the hexagonal P-lattice, like the orthorhombic and tetragonal lattices, has mirror planes ⊥ c at x,y,0 and x, y, 12 , and inversion centers (Fig. 7.10d), so the application of Rule I (m + 1̄ ⇒ 2 ⊥ m) or rule II (m ⊥ m ⇒ 2) generates several 2-fold axes. Figure 7.22 shows the projection of a hexagonal P-lattice on (001). The 6-fold axis makes a = b, and a and b may also be written as a1 and a2 . Another direction, called the a3 -axis, may then be added, making an angle of 120◦ with a1 and a2 , and equivalent to them both. Thus, a now represents a1 , a2 , a3 . The diagonals bisecting the a-axes are [210], [1̄2̄0] and [1̄10]. As for the tetragonal lattice, the symmetry elements are arranged in the space group symbol in the order, c, a, diagonals of the a axes, viz. 210, all of which are called symmetry directions. P6/m 2/m 2/m. ↓ ↓ The space group symbol is thus: ↓ a 210 . c Fig. 7.22 Hexagonal P-lattice projected on (001) emphasizing the symmetry directions a = a1 , a2 , a3 and 210 = [210], [1̄10] and [12̄0] 101 102 7 The 14 Bravais Lattices Fig. 7.23 a Space group P 6/m 2/m 2/m. In the other diagrams, only the symmetry elements corresponding to the symmetry directions c, a, 210 are shown: b P6/m . . . . . . , c P . . . 2/m . . . , d P . . . . . . 2/m ↓ ↓ ↓ a 210 c 7.3 The Centered Lattices Figure 7.23 gives a projection of all the point-symmetry elements of space group P6/m2/m2/m, and separate diagrams showing those elements related to the symmetry directions c, a and210. 7.2.6 Symmetry of the Cubic P-Lattice The symmetry of the stacking planes is shown in Fig. 7.12a. The stacking results in a lattice with a cubic unit cell (a0 = b0 = c0 ). This means that the lattice planes 0,x,z and x,0,z have the same symmetry as x,y,0, see Fig. 7.12d. This equivalence of the planes generates four 3-fold axes along the body diagonals of the unit cell as well as inversion centers, so these axes are represented as 3̄ (≡ 3 + 1̄). Application of rule I (m + 1̄ ⇒ 2 ⊥ m) or rule II (m ⊥ m ⇒ 2) generates 2-fold axes parallel to [110] and equivalent directions. (These 2-fold axes are not included in Fig. 7.11d). In the space group symbol, the symmetry elements are given in the order: a, 111 = body diagonals of the unit cell, 110 = face diagonals of the unit cell. The P4/m 3̄ 2/m. ↓ ↓ space group symbol for the cubic P-lattice is thus: ↓ a 111 110 . Figure 7.24 gives a projection of all the point-symmetry elements of space group P4/m3̄2/m, and separate diagrams showing those elements related to the symmetry directions a, 111 and 110. 7.3 The Centered Lattices Consideration of the primitive lattices we have so far generated raises the question as to whether it is possible to import into the P-lattices one or more further lattice planes without destroying the symmetry. Let us ﬁrst consider the monoclinic P-lattice. Figure 7.25 shows the monoclinic P-lattice and its symmetry, P2/m, projected onto x,0,z (see also Fig. 7.8d). Each point of the lattice has 2/m symmetry, which implies the presence of an inversion center in the point. Insertion of new lattice planes parallel to (010) into the lattice is only possible if the lattice points fall on a position which also has symmetry 2/m, i.e. on 12 ,0,0; 0, 12 ,0; 0,0, 12 ; 12 , 12 ,0; 12 ,0, 12 ; 0, 12 , 12 , or 12 , 12 , 12 . These possibilities must each be considered. (a) Lattice Plane with Lattice Point at 12 , 12 ,0 (Fig. 7.26). These new lattice points center the a, b-face of the unit cell. This is called a C-face centered lattice, or more simply a C-lattice, although this name is formally inexact, being used to describe a “lattice with a C-face centered unit cell”. The monoclinic C-lattice is illustrated in Table 7.3. 103 104 7 The 14 Bravais Lattices Fig. 7.24 a Space group P 4/m 3̄ 2/m. In the other diagrams, only the symmetry elements corresponding to the symmetry directions a, 111, <110> are shown. 7.3 The Centered Lattices Fig. 7.25 The monoclinic P-lattice and its symmetry elements projected onto x,0,z ( lattice point with y = 0) Fig. 7.26 The monoclinic C-lattice projected on x,0,z ( represents a lattice point with y = 12 (b) Lattice Plane with Lattice Point at 0, 12 , 12 (Fig. 7.27). If the new plane centers the b, c-face, the result will be an A-face centered lattice. Since, however, in monoclinic cells, the a and c axes may lie anywhere in the mirror plane, they may be swapped, converting the A-lattice into a C-lattice. (c) Lattice Plane with Lattice Point at 12 ,0, 12 (Fig. 7.28). The result is now a B-lattice, from which a smaller, primitive unit cell can be chosen (outlined in bold) that still has monoclinic symmetry. (d) Lattice Plane with Lattice Point at 12 , 12 , 12 (Fig. 7.29). A lattice is formed, with a lattice point at the body center of the unit cell. This is called a body centered or I-lattice (from the German innenzentriert). As with the A-lattice, choice of diﬀerent axes convert this to a monoclinic C-lattice. Fig. 7.27 The monoclinic A-lattice (a0 , b0 , c0 ) can, by interchanging a and c, be converted to a monoclinic C-lattice (a0 , b0 , c0 ) 105 106 7 The 14 Bravais Lattices Fig. 7.28 The monoclinic B-lattice (a0 , b0 , c0 ) can be converted to a smaller monoclinic P-lattice (a0 , b0 , c0 ) Fig. 7.29 The monoclinic I-lattice (a0 , b0 , c0 ) can be converted to a monoclinic C-lattice (a0 , b0 , c0 ) (e) Lattice Plane with Lattice Point at 12 ,0,0; 0, 12 ,0 or 0,0, 12 . In any of these cases, the result is simply to halve the cell; no new type of lattice is formed. (f) It is also possible to introduce two lattice planes at the same time, for example, as in both (a) and (b), giving additional lattice points at 12 , 12 ,0 and 0, 12 , 12 (Fig. 7.30a). Since it is necessary that all lattice points have the same environment, and parallel lattice lines the same period a further lattice point (shown with a dashed outline) must be added at 12 ,0, 12 . Thus, all the faces of the unit cell are now centered, giving an all-face centered or F-lattice. A general principle following from this is that a lattice centered on two faces cannot exist because the requirement that all lattice points are identical and parallel lattice lines have the same lattice period will convert it to an all-face centered lattice. The monoclinic F-lattice can, in fact, be reduced to a C-lattice of half the volume, as is shown in Fig. 7.30b. We have now considered all the possibilities for introducing extra lattice planes into the monoclinic P-lattice, and have shown that all of these may be represented either as P- or C-lattices (A, I, F → C; B → P). The orthorhombic lattice may be developed in the same way, giving rise of orthorhombic A-, B-, C-, I- and F-lattices. The I- and F-lattices are now not 7.3 The Centered Lattices Fig. 7.30 a, b. The development of the monoclinic F-lattice (a). The monoclinic F-lattice (a0 ,b0 ,c0 ) can be converted to a monoclinic C-lattice (a0 ,b0 ,c0 ) (b) reducible as they were in the monoclinic case. The A-, B- and C-lattices are alternative representations of the same lattice; the a-, b-, and c-axes can always be chosen so as to generate a C-lattice. There are a few space groups which are customarily treated as having an A-lattice (see Table 10.2). The C-lattice may also be developed by the vertical stacking of planes with the centered rectangular unit mesh (Fig. 7.6b). Similar considerations to those in the monoclinic case lead from the tetragonal P-lattice to the tetragonal I-lattice, and from the cubic P-lattice to the cubic I- and F-lattices (Table 7.3). An examination of the hexagonal P-lattice will show that the only point with the same symmetry as 0,0,0 is 0,0, 12 . The addition of a lattice plane there will merely halve the size of the unit cell. A 6-fold axis always contains a 3-fold axis. Starting from this fact, the plane lattice with a 120◦ rhombus as unit mesh contains a 3-fold axes at 0,0,z; 13 , 23 ,z and 23 , 13 ,z (Fig. 7.11a). It is possible to add a second plane at a height of 13 c0 with a lattice point on the 3-fold axis at 23 , 13 ,z and a third plane at a height of 23 c0 with a lattice point on the 3-fold axis at 13 , 23 ,z (Fig. 7.11b). The fourth plane will then come at a height of c0 , directly above the ﬁrst. This new arrangement of lattice points reduces the 6-fold axes to 3-fold and removes the mirror planes at x,0,z; 0,y,z and x,x,z as well as the 2-fold axes parallel to the c-axis. The resulting lattice has the shape of a hexagonal lattice (a0 = b0 = c0 , α = β = 90◦ , γ = 120◦ ) but contains three lattice points per unit cell (0,0,0; 23 , 13 , 13 ; 13 , 23 , 23 ). It is possible, however, to describe this lattice by a primitive unit cell (a0 = b0 = c0 , α = β = γ ). If the ﬁrst cell is used to describe the lattice, it is called a trigonal R-lattice, if the second is used, the lattice is called rhombohedral P (Fig. 7.19b). The unit cell of the rhombohedral P-lattice has indeed the shape of a rhombohedron, with six rhombi as faces. 107 108 7 The 14 Bravais Lattices Special cases of the rhombohedral P-lattice are: (a) α = 90◦ gives the cubic P-lattice; (b) α = 60◦ gives the cubic F-lattice and (c) α = 109.47◦ gives the cubic I-lattice. 7.4 The Symmetry of the Centered Lattices With the exception of the trigonal R-lattice, the derivation above of the centered lattices always paid strict attention to retaining the full symmetry of the corresponding P-lattice. All the symmetry elements of the P-lattice remained, only the translation properties were altered. The centering does indeed introduce new symmetry elements, notably screw axes and glide planes (see Sect. 10.1). In spite of this, the symbols for the space groups of the centered lattices may easily be given, since the new symmetry elements do not appear in them. Now it is not diﬃcult to derive the symbol for the trigonal R-lattice from the reduced symmetry of the lattice planes. There are, in addition to the normal ones, further inversion centers, which, by Rule I (m + 1̄ ⇒ 2 ⊥ m), generate a set of 2-fold axes parallel to a1 , a2 , a3 (Fig. 7.11d). The 3-fold axis becomes 3̄ since 3 + 1̄ ⇒ 3̄. The order of the symmetry directions here is: c, <a>, giving the symbol R3̄ 2/m. ↓ ↓ c a The space group symbols of the 14 Bravais lattices are given in Table 7.4 in the same order as Table 7.3. Table 7.3 contains the 14 lattices, which are usually known as the Bravais lattices. ! The 14 Bravais lattices represent the 14 and only ways in which it is possible to ﬁll space by a three-dimensional periodic array of points. Table 7.4 The space group symbols for the 14 Bravais lattices P C Triclinic P 1̄ Monoclinic P 2/m C 2/m Orthorhombic P 2/m 2/m 2/m C 2/m 2/m 2/m Tetragonal P 4/m 2/m 2/m I F I 2/m 2/m 2/m F 2/m 2/m 2/m I 4/m 2/m 2/m Trigonal Hexagonal Cubic R 3̄ 2/m P 6/m 2/m 2/m P 4/m3̄ 2/m I 4/m3̄2/m F 4/m3̄2/m 7.5 Exercises All crystals are built up on one of these lattices. In Chap. 4, we deﬁned a crystal structure as a lattice plus a basis. While the number of lattices is ﬁxed at 14, there are inﬁnitely many possible ways of arranging atoms in cell. Any crystal structure, however, has only one Bravais lattice. The number and coordinates of the lattice points in the unit cells of the Bravais lattices is given in Table 7.5. Table 7.5 Number and coordinates of the lattice points in the unit cells of the Bravais lattices Lattice No. of lattice points in unit cell Coordinates of lattice points in unit cell P 1 0,0,0 A 2 0,0,0; 0, 21 , 21 B 2 0,0,0; 12 ,0, 21 C 2 0,0,0; 12 , 12 ,0 I 2 0,0,0; 12 , 12 , 21 R 3 0,0,0; 23 , 13 , 31 ; 13 , 23 , 32 F 4 0,0,0; 12 , 12 ,0; 12 ,0, 21 ; 0, 21 , 21 7.5 Exercises Exercise 7.1 Symmetry of plane lattices. (a) Determine the symmetry elements for the given plane lattices, and draw these in their places on the lattice. Note that only m, 2, 3, 4 and 6 normal to the plane of the paper need be considered. (b) Draw in the edges of the unit mesh and give the lattice parameters. Which lattice parameters are equivalent and why? (c) Determine which symmetry elements are themselves equivalent by symmetry. 109 110 7 The 14 Bravais Lattices 7.5 Exercises Exercise 7.1 (Continued) Exercise 7.2 For the given two-dimensional structures, determine: (a) The unit mesh. (b) The symmetry elements. It is only necessary to indicate those symmetry elements which lie within the unit mesh. As in Exercise 7.1, only m, 2, 3, 4 and 6 normal to the plane of the paper need be considered. Two dimensional structures after Kockel 111 112 7 The 14 Bravais Lattices 7.5 Exercises Exercise 7.2 (Continued) Exercise 7.3 (Refer to Symmetry rule I) (a) Draw the given combinations of two symmetry elements on the stereographic projection. As the inversion center is a single point, it cannot be shown on the stereogram, but may be taken to lie at the center of the projection. Draw in a pole which does not lie on any symmetry element, and allow the symmetry elements to operate on it. On the basis of the positions of the resulting poles, determine the third symmetry element generated by the combination of the gien symmetry elements, and draw it on the sterogram. (b) Below are given an orthorhombic unit cell and its projection on x,y,0. Draw the third symmetry element generated by the two given elements on either or both of these, give its symbol and the coordinates of its position. Note that only one symmetry element of each type is drawn in the cell. 113 114 7 The 14 Bravais Lattices Exercise 7.3 (Continued) 7.5 Exercises Exercise 7.3 (Continued) Exercise 7.4 (Refer to symmetry rule II) (a) On the following stereograms, draw in the third symmetry element generated by the combination of the given two. 115 116 7 The 14 Bravais Lattices (b) An orthorhombic unit cell and its projection on x,y,0 are given below. On either of them, draw the third symmetry element generated by the two given elements, and given its symbol and the coordinates of its position. 7.5 Exercises Exercise 7.5 Which of the 14 Bravais lattices are each of the following? 117 118 7 The 14 Bravais Lattices Exercise 7.6 (a) Draw the unit cells of each of the following lattices as a projection on x,y,0, or, in the monoclinic case, on x,0,z. Use a scale of 1 Å = 1 cm. Monoclinic P: a0 = 5.5, b0 = 4.0, c0 = 4.0 Å; β = 150◦ Orthorhombic P: a0 = 3.0, b0 = 4.5, c0 = 4.0 Å Tetragonal P: a0 = 4.0, c0 = 3.0 Å Hexagonal P: a0 = 4.0, c0 = 3.0 Å Trigonal R: a0 = 4.5, c0 = 3.0 Å (b) Determine the symmetry operations of lattices you have drawn, and plot the symmetry elements on the projection of the lattice. (c) Now use colored pens to color the symmetry elements, using colors so that symmetry elements with the same symmetry direction have the same color. (d) Give the space group symbol for each lattice, making use of the colors of symmetry elements you have chosen in (c). Exercise 7.7 Derive the three centered orthorhombic lattices (cf. Sect. 7.3). (a) What is the symmetry of a lattice point in the orthorhombic P-lattice? (b) Which points in the unit cell of the P-lattice have the same symmetry as the lattice points? Give their coordinates. (c) Bring a lattice plane, parallel to (001) into a position such that a lattice point comes into coincidence with each of the positions you have determined in (b). Repeat the above exercise with two planes. Exercise 7.8 Similarly, derive the centered tetragonal lattices. Exercise 7.9 The projection of a Bravais lattice onto x,y,0 is given below. (a) Name the lattice constants and give the coordinates of the lattice points. (b) Determine the symmetry of the lattice, and draw the symmetry elements on the projection. (c) What are the symmetry directions for this lattice? (d) What is its space group symbol? Exercise 7.10 Look at Figs. 7.19, 7.21, 7.23 and 7.24. How do the individual projections in each ﬁgure relate to one another? 8 The Seven Crystal Systems In the various lattices, the vectors a, b and c must be chosen and associated with a system of suitable crystallographic axes, a, b, c. This is not done arbitrarily. Generally, so far as is possible, the choices are made so that the direction of rota c. tion axes, rotoinversion axes and the normals to mirror planes are parallel to a, b, Thus: c; a, b, c // X, X̄, normal to m. a, b, It is possible to distinguish six axial systems (systems of crystallographic axes), which are given in Figs. 7.7c–7.13c and which correspond to the six primitive lattices. These axial systems naturally apply equally to the centered lattices. On this basis, we may deﬁne a crystal system: D All lattices, all crystal structures and all crystal morphologies which can be deﬁned by the same axial system belong to the same crystal system. This deﬁnition distinguishes six crystal systems. It is, however, usual to separate the system of crystallographic axes based on a = b = c, α = β = 90◦ , γ = 120◦ into a hexagonal and a trigonal crystal system. The hexagonal system is characterized by the presence of 6 or 6̄, while the trigonal is characterized by 3. In Table 8.1, the seven crystal systems are listed along with the restrictions on the axial system. It is important to remember, however, that equivalence of crystallographic axes and special values of the angles are simply a consequence of the underlying symmetry. Those symmetry elements which cause equivalences to arise between crystallographic axes are listed. A full list of the symmetry elements characterizing the various crystal systems is given in Table 9.9. The space groups of the lattices themselves have the highest symmetry which can occur in that crystal system (cf. Table 7.4). Symmetry elements in each crystal system can only be orientated in certain directions with respect to one another, since it is not those symmetry elements alone, but they and all their combinations which W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_8, C Springer-Verlag Berlin Heidelberg 2011 120 8 The Seven Crystal Systems Table 8.1 The seven crystal systems Crystal system Restrictions on the axial system Figure Triclinic a=b=c α=β=γ a 7.7c Monoclinic a=b=c α=γ =90◦ , β>90◦ 7.8c Orthorhombic a=b=c α=β=γ =90◦ 7.9c Tetragonal a=b=c (a1 =a2 =c) α=β=γ =90◦ Equivalences of crystallographic axes caused by: 7.10c 4, 4̄//c Trigonalb a=b=c (a1 =a2 =c) α=β=90◦ , γ =120◦ 7.12c 3//c Hexagonal a=b=c (a1 =a2 =c) α=β=90◦ , γ =120◦ 7.12c 6, 6̄//c Cubic a=b=c (a1 =a2 =a3 ) α=β=γ =90◦ 7.13c 3// 111 usual, the signs=and=are to be read as must be equivalent and need not be equivalent respectively as a consequence of symmetry. b An alternative deﬁnition divides the hexagonal and trigonal systems diﬀerently, giving a hexagonal and a rhombohedral system. The rhombohedral system (see Fig. 7.11b) has the restrictions on its axial system: a=b ´ =c ´ ;´α =β ´ =γ ´ .´ a As must be in accordance with the properties of the space lattice. The symmetry of the lattice automatically determines all the angles which the symmetry elements of the particular crystal system may make with one another. The symmetry directions in crystal systems are summarized in Table 8.2. These symmetry directions are used for point groups (Chap. 9) and space groups (Chap. 10). Symmetry directions are deﬁned diﬀerently for each crystal system. For some subgroups, a symmetry element does not necessarily exist in the second and/or third position of the symmetry directions (cf. Table 9.10). The normalized axial ratios from morphology ba : 1 : bc or from the crystal structure ba00 : 1 : bc00 for an orthorhombic crystal are discussed in Section 5.7. These ratios are summarized in Table 8.3 for all crystal systems. They may be expressed more simply for systems of higher symmetry. The U.S. Department of Commerce: National Institute on Standards and Technology (NIST) and the International Centre for Diﬀraction Data have produced a series of volumes Crystal Data – Determinative Tables. These contain an extensive listing of important crystallographic data. Triclinic (anorthic), monoclinic and orthorhombic crystals are listed in the order of the ba00 ratio, where c0 < a0 < b0 . Tetragonal, trigonal and hexagonal crystals are arranged by the ac00 ratio, and cubic crystals by the value of the lattice constant a0 . 8 The Seven Crystal Systems Table 8.2 Symmetry directions in the seven crystal systems Crystal system Position in the international symbol First Second Third Triclinic – – – Monoclinic b – – Orthorhombic a b c Tetragonal c <a>a <110>b Trigonal c <a>c –d Hexagonal c <a>c <210>e Cubic <a>f <111>g <110>h a a, b; (a1 , a2 ). [110],[11̄0]. c a, b; (a , a , a ). 1 2 3 d Some space groups require a third symmetry direction <210>, as in the hexagonal system. Examples are P3̄1m and P312 which have m or 2 in the direction <210> (cf. Table 10.2). e [210], [1̄10], [1̄2̄0]. f a, b, c; (a , a , a ). 1 2 3 g [111], [11̄1̄], [1̄11̄], [1̄1̄1]. h [110], [11̄0], [101], [1̄01], [011], [011̄]. b Table 8.3 Normalized axial ratios as used for the various crystal systems Crystal system Axial ratios Morphological Structural a c :1: b b c0 a0 :1: b0 b0 c a c0 a0 – a0 Triclinic Monoclinic Orthorhombic Tetragonal Trigonal Hexagonal Cubic 121 9 Point Groups 9.1 The 32 Point Groups As has been noted, the space groups of the Bravais lattices are those with the highest possible symmetry for the corresponding crystal systems. When the lattice points are now replaced by actual atoms, ions or molecules, they must themselves possess at least the full symmetry of the lattice point if the space group is to remain unchanged. Now the symmetry of a lattice point is easily determined from the space group; it consists of all of the point symmetry elements of the space group that pass through the point (X, X̄, m) or lie on it (1̄). In each crystal system, only the space group of the P-lattice or, in the trigonal system the R-lattice, need be considered (see Figs. 7.7d–7.13d), since the centered lattices in each system deﬁne identical points. Lattice translations, the most important of all the symmetry operations for space groups, are now discarded, and the set of symmetry elements remaining is called a point group. The symmetry elements of these point groups and their stereographic projections are set out in Figs. 7.7e–7.13e, and the conversion from space group to point group in Table 9.1. There is a great deal of useful information in the diagrams, and it is worth taking the trouble to study them carefully. D The point groups are made up from point symmetry operations and combinations of them. Formally, a point group is deﬁned as a group of point symmetry operations whose operation leaves at least one point unmoved. Any operation involving lattice translation is excluded. The symmetry directions have the same relationship to the symmetry elements of the point group as they do to those of the space group (Table 8.2). Those point groups derived from the space groups of the lattices are also the highest symmetry possible for the particular crystal system. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_9, C Springer-Verlag Berlin Heidelberg 2011 124 9 Point Groups Table 9.1 Correspondence of one of the space groups of highest symmetry in each crystal system with the point group of highest symmetry in that crystal system Crystal system Space group Point group Figure Triclinic P1̄ → 1̄ 7.7d, e Monoclinic P2/m → 2/m 7.8d, e Orthorhombic P2/m 2/m 2/m → 2/m 2/m 2/m 7.9d, e Tetragonal P4/m 2/m 2/m → 4/m 2/m 2/m 7.10d, e Trigonal R 3̄ 2/m → 3̄ 2/m 7.11d, e Hexagonal P6/m 2/m 2/m → 6/m 2/m 2/m 7.12d, e Cubic P4/m 3̄ 2/m → 4/m 3̄ 2/m 7.13d, e These point groups of highest symmetry in each crystal system all contain the symmetry elements of one or more point groups of lower symmetry (sub-groups). These will be developed below for some crystal systems: (a) Triclinic. The only subgroup of 1̄ is 1. Starting from the space group P1̄ (Fig. 7.16), all points which do not lie on inversion centers have the point symmetry 1. (b) Monoclinic. 2/m has the subgroups 2, m,1̄ (cf. Symmetry rule I) and 1. Since1̄ and 1 belong to the triclinic system, only 2 and m are monoclinic point groups (cf. Fig. 7.8f). They possess suﬃcient symmetry to deﬁne the monoclinic system: m ⊥ b in the a, c-plane, and 2 parallel to b and normal to the a, c-plane. In the space group P2/m (Fig. 7.8d), the point 0,0,0 has the point symmetry 2/m, while any point on x, 12 ,z has point symmetry m, and any point on the line 12 ,y, 12 has point symmetry 2 (cf. Fig. 10.13) (c) Orthorhombic. If inversion symmetry is removed from point group 2/m 2/m 2/m, each 2/m must be reduced either to 2 or to m (Symmetry rule I). The possible orthorhombic subgroups are thus mmm, mm2 (or m2m or 2 mm), m22 (or 2m2 or 22m) and 222. The symmetry elements of mmm are given on the stereogram in Fig. 9.1. By Symmetry rule II (m ⊥ m ⇒ 2), 2-fold rotation axes are formed at each intersection of planes, and the point group 2/m 2/m 2/m has been reformed. Similarly, the combination 22m also regenerates 2/m 2/m 2/m (cf. Fig. 9.2). The orthorhombic subgroups of 2/m 2/m 2/m are thus 222 and mm2 (Fig. 7.9f). As an example, in the space group P2/m 2/m 2/m (Fig. 7.9d), all points on 12 , 12 ,z (z = 0 or 12 ) have point symmetry mm2. In a similar way, the other crystal systems may be treated, giving in total 32 point groups or crystal classes, which are summarized in Table 9.2. They are called the crystallographic point groups. All crystallographic point groups are subgroups of either 4/m 3̄ 2/m or 6/m 2/m 2/m or both. The hierarchy of the subgroups is illustrated in Fig. 9.3. 9.1 The 32 Point Groups Fig. 9.1 Fig. 9.2 Fig. 9.1 The three mutually perpendicular mirror planes of mmm showing with dashed outline the automatically developed 2-fold axes (Symmetry rule II). Thus mmm is in fact 2/m 2/m 2/m and is used as an abbreviated symbol for it Fig. 9.2 The symmetry elements of m22 (fully drawn in) on the stereogram, automatically generate (Symmetry rule II) the other symmetry elements shown with dashed outline, generating 2/m 2/m 2/m. Thus, m22 is in fact identical with 2/m2/m 2/m Table 9.2 The 32 point groups Crystal system Point groups Symmetry and stereograms of the point groups in ﬁgure Triclinic Monoclinic Orthorhombic 1̄ 2/m 2/m 2/m 2/m (mmm) 1 m, 2 mm2, 222 7.8e, f 7.9e, f Tetragonal 4/m 2/m 2/m (4/mmm) 4̄2m, 4mm, 422, 4/m, 4̄, 4 7.10e, f Trigonal 3̄ 2/m (3̄m) 3m, 32, 3̄, 3 7.11e, f Hexagonal 6/m 2/m 2/m (6/mmm) 6̄m2, 6mm, 622, 6/m, 6̄, 6 7.12e, f Cubic 4/m 3̄ 2/m (m3̄m) 4̄3m, 432, 2/m3̄ (m3̄), 23 7.13e, f Some point groups have overdeﬁned symbols, as we have seen for 2/m 2/m 2/m (Fig. 9.1). In some of these cases, the symbol is abbreviated; the abbreviated symbols are shown in round brackets in Table 9.2. These abbreviated forms are also used for space groups (Chap. 10). They are called short symbols to distinguish them from the full symbols. Up to now, symmetry symbols have always been used in relation to the symmetry directions. The symbol on its own, however, clearly shows the relative orientation of the various symmetry elements. Thus: X2: Xm: X̄2: rotation axis X and 2-fold axes perpendicular to it, e.g. 42(2) (Fig. 7.10f). rotation axis X and mirror planes parallel to it, e.g. 3m (Fig. 7.11f). rotoinversion axis X̄ and 2-fold axes perpendicular to it, e.g. 4̄ 2(m) (Fig. 7.10f). X̄m: rotoinversion axis X̄ and mirror planes parallel to it, e.g. 6̄m(2) (Fig. 7.12f). X/mm: rotation axis X and mirror planes both parallel and perpendicular to it, e.g. 4/mm(m) (Fig. 7.10f). 125 126 9 Point Groups Fig. 9.3 The crystallographic point groups and their subgroups, after Hermann [19]. The circles corresponding to the highest symmetry group of each crystal system are outlined in bold. Double or triple lines indicate that the supergroup is related to the subgroup in two or three inequivalent settings. Connecting lines between point groups of the same crystal system are bold, all others are plain or dashed. The presence of a line of any sort indicates that the lower group is a subgroup of the higher. On the ordinate is given the order of the point group, i.e. the number of symmetry operations in the group. See also Sect. 11.2 The symbols we have been using so far for space groups and point groups are known as the International or Hermann-Mauguin symbols. In physics and chemistry, the older Schönﬂies symbols are widely used. Unfortunately, Schönﬂies symbols are impossible to adapt as useful space group symbols. Although they are adequate to deﬁne point groups, there is no particular advantage to using them. Table 9.3 gives the International equivalents of all the Schönﬂies symbols for the crystallographic point groups. 9.1 The 32 Point Groups Table 9.3 The Schönﬂies symbols for the point groups with the equivalent international symbols 127 128 9 Point Groups 9.2 Crystal Symmetry A space group reveals the entire symmetry of a crystal structure. When we consider only the morphology of a crystal, the lattice translations which characterize the space group are no longer relevant, and what is left is the point group which is implied by that space group. If the crystal is bounded by plane faces, the symmetry of its morphology will be compatible with that point group. Figure 9.4 illustrates the symmetry of a crystal of PbS (galena) (cf. Fig. 15.4). The symmetry elements which are apparent in the crystal are summarized on the stereographic projection. The point group of the crystal is 4/m 3̄ 2/m (Oh ). In Table 9.11, examples of crystals in various point groups are given in the right-hand column. 9.2.1 Crystal Forms of the Tetragonal System In Sect. 5.2, crystal form was provisionally deﬁned as a set of “equal” faces. We are now in a position to give an exact deﬁnition. Fig. 9.4a–d A galena crystal in point group 4 /m 3 2 /m. In a, only those symmetry ↓ ↓ ↓ < a >< 111 >< 110 > elements which relate to the a-axis and equivalent directions (i.e. the b- and c-axes) have been drawn in (4/m → <a>); in b, only those relating to the [111] and equivalent directions (3̄→ <111>); in c, only those relating to the [110] and equivalent directions (2/m → <110>). The stereogram of the symmetry elements is given in d 9.2 Crystal Symmetry Fig. 9.5a,b Stereograms of point group 4. a General form, tetragonal pyramid {hkl}. b Limiting form tetragonal prism {hk0} of general form tetragonal pyramid {hkl} When the symmetry operations of a point group are applied to a crystal face, a number of equivalent faces will be produced. Thus, as shown in the stereographic projection in Fig. 9.5a, application of the symmetry operation of the point group 4 on the pole of a face produces a tetragonal pyramid. D A set of equivalent faces is called a crystal form. (but see also Sect. 9.7) Exercise 6.1b gives a manipulation which will always result in the production of the stereogram of a crystal form. The individual faces of the tetragonal pyramid in Fig. 9.5a have been indexed, i.e. assigned the values of their Miller indices. A scheme for indexing the faces of tetragonal crystals will be given later (Fig. 9.9). A crystal form is identiﬁed by the indices of one of the faces belonging to that form. In the case of a form, the indices are placed in braces, thus: {hkl}, in order to distinguish between a face and a form. The relationship between (hkl) and {hkl} is the same as that between [uvw] and <uvw>. Each face of the tetragonal pyramid in Fig. 9.5a is itself unsymmetrical, as there is no symmetry element normal to it. On its own, it thus has face symmetry 1. Three types of crystal forms must now be distinguished: a general form, a special form and a limiting form. D A general form is a set of equivalent faces, each of which has face symmetry 1. In other words, when the poles of the faces of a general form are placed on a stereogram of the symmetry elements, they do not lie on any of them. General forms have general indices {hkl}. The tetragonal pyramid {hkl} in Fig. 9.5a is such a general form. The poles of the faces of a general form have two degrees of freedom, shown as arrows in the ﬁgure. The face can be displaced in two directions without causing the tetragonal pyramid to cease to be a crystal form. All that happens is that the inclination of the faces to one another is altered. The variation of the indices {hkl} gives rise not to only one, but to an inﬁnite number of general crystal forms. In some point groups, care must be taken with the signs of the indices. In any case, the possibility of inﬁnitely many crystal forms is only of theoretical interest; in practice, crystals normally have faces with small values of h, k and l. 129 130 9 Point Groups Fig. 9.6a,b Stereograms of point group 4mm. a Special form, tetragonal pyramid {hhl}. b Limiting form, tetragonal prism {110} of special form, tetragonal pyramid {hhl} D A special form is a set of equivalent crystal faces which themselves have a face symmetry higher than 1. In a stereogram of the symmetry elements, the poles of the faces of a special form lie on at least one of them. Figure 9.6a shows the stereogram of the symmetry elements of the point group 4 mm. If the pole of a face (hhl) is entered, the application of the symmetry elements gives a tetragonal pyramid {hhl}. This is a special form, as the poles of the faces lie on a symmetry element, and each has face symmetry ..m. The symmetry is given as ..m. with reference to the order of the symmetry directions used for point groups of the tetragonal system: c,<a>,<110>. The mirror planes with which we are concerned here are those normal to <110>. The poles of the faces of this special form have only a single degree of freedom. The form will remain a tetragonal pyramid only as long as the pole remains on the mirror plane ..m. Should the pole move until it coincides with the 4-fold axis, another special form arises, the pedion {001} with face symmetry 4 mm. This form no longer has any degree of freedom. A special form always has indices which are a special case of {hkl}, such as {hhl}, {h0l} or {100}. D A limiting form is a special case of either a general or a special form. It has the same number of faces, each of which has the same face symmetry, but the faces may be described diﬀerently. Consider the situation in Fig. 9.5a if the pole moves to the periphery of the equatorial plane of the stereographic projection. The result is a tetragonal prism {hk0} which is the limiting form of the general form tetragonal pyramid {hkl} with face symmetry 1. A similar movement of the pole {hhl} in Fig. 9.6b, along the mirror plane to the periphery of the equator gives rise to the tetragonal prism {110}, the limiting form of the special form {hhl} with face symmetry ..m. Each point group has characteristic forms. What follows is a description of those of the point group 4/mmm, the point group of highest symmetry in the tetragonal system. Figure 9.7a is a stereogram of the symmetry elements of this point group. A single, asymmetric face unit is shown hatched in Fig. 9.7a. 9.2 Crystal Symmetry Fig. 9.7a–g Crystal forms of point group 4/mmm, with their face symmetries. A stereogram of the symmetry elements is given, with the asymmetric face unit and stereograms of each form 131 132 9 Point Groups D The asymmetric face unit of a point group, in terms of its stereographic projection, is the smallest part of the surface of the sphere which, by the application of the symmetry operations, will generate the entire surface of the sphere. This particular asymmetric face unit is bounded by m.., .m. and ..m. The vertices have face symmetry 4mm, m2m. and m.m2. If a pole is entered in the asymmetric face unit on the stereogram and operated on by the symmetry 4/mmm, the result is a ditetragonal dipyramid, {hkl}, shown in Fig. 9.7a. This form has two degrees of freedom. A ditetragonal dipyramid will be generated as long as the pole does not move onto one of the symmetry elements which constitute the boundary of the asymmetric face unit. The ditetragonal dipyramid is a general form (face symmetry 1, two degrees of freedom, {hkl}). The size of the asymmetric face unit is simply the ratio of the surface area of the sphere to the number of faces in a general form. fasym.faceunit = fsurface area of the sphere number of faces in the general form (9.1) In this case, the number of such faces is 16, so the asymmetric face unit shown 1 hatched in Fig. 9.7a is 16 of the total surface area of the sphere. ! An asymmetric face unit of a point group contains all the information necessary for the complete description of the crystal forms in this point group. (This deﬁnition may be compared with that of the asymmetric unit in Eq. 10.3.) If the general pole (hkl) is moved onto the mirror plane m.., this pole, and all the others in the general form {hkl} will undergo a change. As the poles approach this mirror plane, the angle between (hkl) and (hkl̄) becomes progressively smaller, and is equal to 0 at the mirror plane. At this point, the two faces (hkl) and (hkl̄) have coalesced into a single face (hk0). As shown in Fig. 9.7b, the ditetragonal dipyramid has become a ditetragonal prism {hk0}. Figure 9.8 shows the stereographic projection of a ditetragonal prism {hk0} and the indices of the poles of its faces. In the stereogram, a section through the ditetragonal prism is shown in bold lines which are extended (dashed lines) to show the intercepts on the axes better, (hk0) = (210). A pole of a face on the mirror plane .m. gives, after the application of the symmetry operations, a tetragonal dipyramid, {h0l}, shown in Fig. 9.7c. A pole of a face on ..m gives a tetragonal dipyramid {hhl}, shown in Fig. 9.7d. The three forms {hk0}, {h0l} and {hhl} all have eight faces, i.e. half of the number of faces of the ditetragonal dipyramid. These three forms each have one degree of freedom. Each form retains its identity so long as the pole remains on the appropriate edge (m) of the asymmetric face unit. The poles of faces on the vertices of the asymmetric face unit have no degree of freedom. The application of the symmetry operations to a pole with face symmetry m2m. gives a tetragonal prism {100} (Fig. 9.7e). Similarly the pole with face 9.2 Crystal Symmetry Fig. 9.8 Section through a ditetragonal prism (outlined), in the equatorial plane of a stereographic projection, with the poles of the relevant faces and their indices, {hk0} (={210}) shown. The dashed lines serve to indicate the intercepts of the faces on the axes symmetry m.m2 gives a tetragonal prism {110} (Fig. 9.7f), while that on 4 mm gives a pinacoid {001} (Fig. 9.7 g). The forms {hk0}, {h0l}, {hhl}, {100}, {110} and {001} have the face symmetries > 1 given in Fig. 9.7 and are thus special forms. Figure 9.9 shows a stereogram with the poles of the crystal forms of point group 4/mmm, the highest point symmetry of the tetragonal system. The poles of the faces with negative indices l̄ are not shown. The heavy lines divide the surface into the 16 asymmetric face units of the point group 4/mmm. Those poles which lie on the corners of the asymmetric face unit have no degree of freedom. Those on the edges of the asymmetric face unit have one degree of freedom, and represent all other poles lying on the same edge. The poles lying within the asymmetric face unit have two degrees of freedom and represent all faces whose poles lie in this area. In every case, taken together, these faces produce ditetragonal dipyramids. If the poles of the faces of a ditetragonal prism {hk0} (Fig. 9.8) are split and moved an equal amount in the directions of (001) and (001̄), a ditetragonal dipyramid {hkl} will be formed. The indexing of the faces of this form arise from the {hk0} of the ditetragonal prism by the replacement of 0 with l and l̄, as in Fig. 9.9, the indices of all 16 faces of the ditetragonal dipyramid can be read from the stereogram in Fig. 9.9, as can the indices for the faces of all of the tetragonal forms. In 4/mmm, there are n = 16 poles for faces of the general form, and 2n + 2 = 34 poles for faces of special forms, each type of form being considered only once. The same relationship between the numbers of faces for the general form and the total number of faces for all special forms also applies to the point group of highest symmetry in the orthorhombic, hexagonal and cubic systems. Starting from the point group of highest symmetry in a crystal system, the subgroups can be developed – see Sect. 9.1. There is a similar relationship between the general crystal form of the point group of highest symmetry and those of its subgroups belonging to the same crystal system. These may be illustrated by starting from the stereogram of the crystal forms of 4/mmm in Fig. 9.9 and developing those of the subgroup 4mm. 133 134 9 Point Groups Fig. 9.9 Stereogram of the poles of the faces of all crystal forms of 4/mmm, the point group of highest symmetry in the tetragonal system. The stereogram shows the position and the indices for each face in each form. Poles of faces with negative values of l are not included. The spherical triangle with vertices (001), (100) and (110) is an asymmetric face unit of the point group 4/mmm Place a piece of tracing paper over the stereogram in Fig. 9.9, choose suitable symmetry directions and mark on it those symmetry elements which belong to 4 mm (Fig. 7.10f). A possible asymmetric face unit for this point group is a region bounded by the pole faces (001), (100), (001̄) and (110). Because half of this asymmetric face unit lies in the southern hemisphere, it is shown checked in Fig. 9.10a. It is twice the size of the asymmetric face unit of 4/mmm, and is made up by combining two such asymmetric face units. Now enter on the tracing paper the pole of a general face (hkl), and allow the symmetry operations of 4mm to act on it. The result is eight poles which deﬁne a ditetragonal pyramid {hk1} (Fig. 9.10a1 ). The pole (hkl̄) which belongs to the same asymmetric unit as (hkl) in 4mm gives a second ditetragonal pyramid {hkl̄} (Fig. 9.10a2 ). Thus, the ditetragonal dipyramid which is the general form in 4/mmm reduces to two ditetragonal pyramids in 4mm. The doubling of the size of the asymmetric face unit results in a halving of the number of faces in the general form. In the same way, the general forms of the other tetragonal point groups may be developed. The relevant asymmetric face units are given in Table 9.4. 9.2 Crystal Symmetry Fig. 9.10a–d Crystal forms of point group 4mm, in so far as these diﬀer from those in point group 4/mmm (Fig. 9.7), with their face symmetries. A stereogram of the symmetry elements is given, with the asymmetric face unit and stereograms of each form. The general form of point group 4/m is a tetragonal dipyramid. The poles (hkl) and (hk̄l) both give tetragonal dipyramids, {hkl} and {hk̄l}, by the action of the symmetry operations, and these two dipyramids may be distinguished by their positions. Figure 9.11 shows the square cross-sections of {hkl} and {hk̄l}. Taking them together, and ignoring the dashed lines, they make up the cross-section of the ditetragonal dipyramid {hkl} of 4/mmm. The general form of 4̄2m is the tetragonal scalenohedron, and of 422 the tetragonal trapezohedron (Fig. 15.2b). The combination of {hkl} and {hk̄l} regenerates in both point groups the ditetragonal dipyramid. The asymmetric face unit for 4 and 4̄ is four times the size of that of 4/mmm (Table 9.4). In 4, the ditetragonal dipyramid is split into four tetragonal pyramids, 135 9 Table 9.4 Crystal forms in the tetragonal system and their face symmetries 136 Point Groups 9.2 Crystal Symmetry 137 138 9 Point Groups Fig. 9.11 Square cross-sections through the tetragonal dipyramids {hkl} and {hk̄l}, general forms in point group 4/m. Together, they make up the fully outlined ditetragonal cross section of the ditetragonal dipyramid. The same relationship holds for the four tetragonal pyramids {hkl}, {hkl̄}, {hk̄l} and {hk̄l̄}, general forms in point group 4 {hkl}, {hk̄l}, {hk̄l̄}, {hkl̄}, while in 4̄, it becomes four tetragonal disphenoids, also {hkl}, {hk̄l}, {hk̄l̄}, {hkl̄}. [Fig. 15.2b(9)]. The special forms of point group 4/mmm in Fig. 9.7 are given in Table 9.4 with their face symmetries. With the help of the stereogram in Fig. 9.9, we may derive the limiting and special forms of point group 4 mm. As in 4/mmm, the pole of the face (hk0) gives rise to the ditetragonal prism {hk0} (Fig. 9.7b). This ditetragonal prism is the limiting form of the general form ditetragonal pyramid {hkl}. These forms both have face symmetry 1 and a total of eight faces. Application of the symmetry operations 4 mm to the pole of the face (h0l) results in a tetragonal pyramid {h0l} (Fig. 9.10b1 ), having point symmetry .m., a special form. Similarly, {h0l̄} is a tetragonal pyramid (Fig. 9.10b2 ). These pyramids are distinguished only by their settings, and their combination gives the tetragonal dipyramid {h0l} of point group 4/mmm. The tetragonal prism {100} is a limiting form of the special form tetragonal pyramid {h0l}, also having face symmetry .m., and a total of four faces. Tetragonal pyramids are also generated by {hhl} and {hhl̄} (Fig. 9.10c), this time with face symmetry ..m. These forms combine to give the tetragonal dipyramid {hhl} of 4/mmm. The tetragonal prism {110} is a limiting form of the special form tetragonal pyramid {hhl}. Finally, the pole of the face (001) gives the pedion {001}, with face symmetry 4 mm. All of the forms of the point group 4 mm are given in Table 9.4. The special and limiting forms of the rest of the tetragonal point groups are also to be found in Table 9.4. It will be seen that the various forms of the point groups of lower symmetry are greatly simpliﬁed. For point group 4, for example, all that remains beside the general form tetragonal pyramid is a single limiting form, the tetragonal prism, and a single special form, the pedion. In Table 9.4, the general forms and their limiting forms are separated from special forms by heavy lines, while dashed lines are used to separate the general forms from their limiting forms. Equal forms with the same face symmetry are collected together, as is also done in Tables 9.5, 9.6, 9.7. 9.2 Crystal Symmetry The face symmetries in Table 9.4 are always derived from a three-component symbol for the point group, which is expanded as required, e.g. 4/m(1) (1). Thus, the face symmetry in {hk0} is given as m.., and that in {001} is given as 4.. . The same expansion is used for those point groups in other crystal systems which have symbols with only 1 or 2 components, e.g. 3m(1), 23(1), etc. Crystal forms in the other crystal systems can be developed in the same way to that we have done for the tetragonal system. In the following pages, the crystal forms for the hexagonal (trigonal), cubic and orthorhombic systems are set out to show their interrelationships and to provide an aid in the indexing of faces. The crystal forms are given for each system (Tables 9.4, 9.5, 9.6, and 9.7), and Fig. 15.2 gives a summary of the 47 fundamental forms. The names used here are those in the International Tables for Crystallography [14]. 9.2.2 Crystal Forms of the Hexagonal (Trigonal) System In each crystal system, an axial system a, b, c must be chosen which is appropriate for the symmetry. For the hexagonal and trigonal systems, in addition to the unique c-axis, it is convenient to choose three equivalent axes a1 , a2 and a3 (cf. Fig. 7.22) and to use the Bravais-Miller indices (hkil). The index i corresponds to the a3 axis. The indices h, k and i are not independent, but are related by h + k + i = 0 or h + k = ī. The application of this relationship can be seen in Fig. 9.12. Joint consideration of the hexagonal and trigonal systems is useful since all of the trigonal forms may be derived from the dihexagonal dipyramid, the general form of 6/m 2/m 2/m, the highest symmetry point group of the hexagonal system (see Figs. 9.12 and 9.13 and Table 9.5). The trigonal and hexagonal crystal forms are all set out in Fig. 15.2c. 9.2.3 Crystal Forms of the Cubic System The cubic crystal forms are collected in Table 9.6 and Fig. 15.2d; see also Figs. 9.14 and 9.15. In the cubic, hexagonal (including trigonal) and tetragonal systems, all crystal forms except the pinacoid and the pedion are characteristic of the system. 9.2.4 Crystal Forms in the Orthorhombic, Monoclinic and Triclinic Systems All of the “rhombic” forms are listed in Fig. 15.2a. see also Fig. 9.16 and Table 9.7. Only relatively simple forms occur in the monoclinic system. The general form in 2/m is the rhombic prism; in m and 2, the general forms are both dihedra: a dome in m and a sphenoid in 2 (Fig. 15.2a). The pinacoid and the pedion are special or limiting forms. The triclinic system gives only the pinacoid (1̄) and the pedion (1). 139 Table 9.5 Crystal forms in the hexagonal/trigonal sysem and their face symmetries 140 9 Point Groups 9.2 Crystal Symmetry 141 Table 9.6 Crystal forms in the cubic system and their face symmetries 142 9 Point Groups Table 9.7 Crystal forms in the orthorhombic system and their face symmetries 9.2 Crystal Symmetry 143 144 9 Point Groups Fig. 9.12 a, b Section through a hexagonal prism {hki0} (a) and {khi0} (b), in the equatorial plane of a stereographic projection, with the poles of the relevant faces and their indices indicated. The dashed lines serve to indicate the intercepts of the faces on the axes [(hki0) = (213̄0); (khi0) = 123̄0)] Fig. 9.13 Stereogram of the poles of the faces in all crystal forms of the point group of highest symmetry in the hexagonal system, 6/m 2/m 2/m. The stereogram shows the positions and the indices of all hexagonal and trigonal forms. The poles of faces with negative 1 are excluded. The spherical triangle with vertices (101̄0), (0001), (112̄0) is an asymmetric face unit for the point group 6/m 2/m 2/m 9.2 Crystal Symmetry Fig. 9.14 Indices for the cubic faces belonging to the form {hk0} (= {210}). If these are shifted from their special position so that their poles move toward the pole of the (111) face, faces will be obtained with general indices {hkl} in the point group 4/m 3̄ 2/m (cf. Fig. 9.15) Fig. 9.15 Stereogram of the poles of the faces in all crystal forms of the point group of highest symmetry in the cubic system, 4/m 3̄ 2/m. The stereogram shows the positions and the indices of all cubic forms (hk0) = (310), (hkk) = (311), (hhk) = (221), (hkl) = (321). The poles of faces with the third index negative are excluded. The spherical triangle with vertices (100), (110), (111) is an asymmetric face unit for the point group 4/m 3̄2/m 145 146 9 Point Groups Fig. 9.16 Stereogram of the poles of the faces in all crystal forms of the point group of highest symmetry in the orthorhombic system, 2/m 2/m 2/m. The stereogram shows the positions and the indices of all orthorhombic forms. The poles of faces with negative 1 are excluded. The spherical triangle with vertices (100), (010), (001) is an asymmetric face unit for the point group 2/m 2/m 2/m The symmetry of a crystal form can be considered in two separate ways. A tetragonal pyramid is generated by the symmetry operations of 4; that is its generating symmetry. On the other hand, a tetragonal pyramid actually displays the symmetry of 4mm; that is its eigensymmetry.1 In Table 9.8, these eigensymmetries and generating symmetries are given for all tetragonal forms. Normally, crystals are not characterised by a single form but by a combination of forms, which must, of course, all conform to the point group of the crystal. The rutile crystal in Table 9.11.15 is a combination of a tetragonal dipyramid {111}, and two tetragonal prisms, {100} and {110}. Table 9.8 Eigensymmetry and generating symmetry of the tetragonal forms 1 Eigensymmetry Generating symmetry Tetragonal pyramid 4mm 4, 4mm Tetragonal disphenoid 42m 4, 42m Tetragonal prism 4/mmm 4, 4, 4/m, 422, 4mm 42m, 4/mmm Tetragonal trapezohedron 422 422 Ditetragonal pyramid 4mm 4mm Tetragonal scalenohedron 42m 42m Tetragonal dipyramid 4/mmm 4/m, 422, 42m, 4/mmm Ditetragonal prism 4/mmm 422, 4mm, 42m, 4/mmm Ditetragonal dipyramid 4/mmm 4/mmm eigen (German) = own 9.3 Molecular Symmetry 9.3 Molecular Symmetry Point symmetry is a very great help in the description of molecules, by which term we include polyatomic ions of any charge. Figure 9.17a shows a molecule of H2 O, on which the symmetry elements, two mirror planes and a 2-fold rotation axis, have been drawn. The point group mm2 (C2v ) is shown on the stereogram in Fig. 9.17b. In Table 9.11.1–32 (left hand column) molecular examples are given for several point groups. Some of these molecules are shown in the “Newman projection” used widely in organic chemistry. In other cases, bonds are shown as thick or thin line to indicate whether they are above or below the plane of the page. The stereogram for the point group is in most cases in the same orientation as the example molecule. The point groups of molecules are not limited to the 32 crystallographic groups. They may contain such symmetry elements as 5-fold axes which are incompatible with a crystal lattice. These non-crystallographic point groups are described in Sect. 9.7. The point group of a molecule indicates which atoms and which bonds are equivalent. Thus, in benzene, C6 H6 , with point group 6/mmm – D6h all C-atoms and all H-atoms are equivalent, as are all C–H and C–C bonds (Fig. 9.18a, and also Table 9.11.27). Coronene, C24 H12 , also belongs to point group 6/mmm – D6h . In Fig. 9.18b, equivalent carbon atoms are indicated by the letters a or b or c, and all bonds between pairs of similarly labelled atoms are equivalent. There are thus four symmetry independent C–C bonds in coronene (a–a, a–b, b–c and c–c). Further examples are naphthalene, C10 H8 , and pyrene, C16 H10 , both (mmm – D2h ) (Fig. 9.18c), and phenanthrene, C14 H10 , (mm2 – C2v ) (Fig. 9.18e). The equivalences can be particularly clearly shown by copying the stereogram of the appropriate point group (Table 9.11.7, 8 and 27) onto transparent paper and superimposing it on the molecules in Fig. 9.18. In PF5 , phosphorus is surrounded by ﬁve ﬂuorine atoms. Were this a planar pentagonal molecule, all F-atoms and all P-F bonds would be equivalent (point group 5/mm2 (10m2), Table 9.11.35). In fact, the molecule has the shape of a trigonal dipyramid (Fig. 9.19) with the P-atom at the center, and point symmetry 6̄ m2 (D3 h ). Fig. 9.17a, b Point symmetry (mm2 – C2v ) of the H2 O molecule. b Stereogram of the symmetry elements of this point group 147 148 9 Point Groups Fig. 9.18a–e Equivalence within molecules. Equivalent atoms have the same letter symbols; equivalent bonds have the same pair of letters. (a) Benzene and (b) coronene (6/mmm – D6h ); (c) naphthalene and (d) pyrene (mmm – D2h ); (e) phenanthrene (mm2 – C2v ) Fig. 9.19a, b The PF5 molecule (a) has point group 6̄m2 (D3h ) (b). All atoms marked Fa are equivalent, as are all marked Fb , but Fa and Fb are not equivalent to one another Thus, the two atoms labelled Fa are equivalent, as are the three labelled Fb , but Fa and Fb are not equivalent to one another. If one of the methyl groups of an ethane molecule is rotated about the C–C bond through 360◦ with respect to the other, various diﬀerent conformations will be generated. These are illustrated in Fig. 9.20 together with the stereograms of the respective point groups. Conformations are the spatial arrangements of the atoms of a molecule which result from rotation about a chemical single bond. 9.4 Determination of Point Groups Fig. 9.20a–d Conformations of ethane. a Eclipsed: ϕ = 0 or 120 or 240◦ : (6̄m2 − D3h ). b Skew: 0 < ϕ < 60◦ , 120 < ϕ < 180◦ or 240 < ϕ < 300◦ : (32 – D3 ). c Staggered: ϕ = 60 or 180 or 300◦ : (3̄m − D3d ). d Skew: 60 < ϕ < 120◦ , 180 < ϕ < 240◦ or 300 < ϕ < 360◦ : (32 − D3 ). The conformations in b and d are enantiomorphs 9.4 Determination of Point Groups Before the determination of the point group of a crystal (or a molecule having a crystallographic point group), it should be assigned to one of the seven crystal systems. For this, it is necessary to know the characteristic symmetry elements of the crystal systems; these are given in Table 9.9, and can be derived from the symmetry information given in Table 9.10. In determining the point group of molecules or crystals, it is in general not necessary to ﬁnd each and every symmetry element. Using Tables 9.9 and 9.10, it may generally be done by answering a few, well-chosen questions. In practice, it is best to consider ﬁrst an important property of rotation axes. ! All rotation axes are polar. This means that they have distinct properties in parallel and antiparallel directions The 2 in Fig. 9.17 and Table 9.11.18 and the 3 in Table 9.11.19 are examples of polar rotation axes. The ends of polar axes are represented in symmetry diagrams and stereograms by one solid and one open symbol (cf. Figs. 7.8f, 7.9f, 7.10f, 7.11, 7.12f, and 7.13f). ! Various other symmetry elements can destroy this polarity, viz.: • 1̄ • m⊥X • 2⊥X 149 150 9 Point Groups Table 9.9 Characteristic symmetry elements of the seven crystal systems Questions to use for point-group determination: ! 1. Are rotation axes higher than 2 present (3, 4, 6)? 2. Are these axes polar? or Is an inversion centre present? (crystals with an inversion center are characterized by sets of parallel faces opposite one another. (6.3)) Point group determination will be illustrated by two examples: (a) The methane molecule (CH4 ) (Table 9.11.31). It is easily seen that a polar 3-fold axis lies on each C–H bond. As there are four of these, the point group must belong to the cubic system, and it must be one with polar 3-fold axes (indicated in Table 9.10 by a subscript p by the graphical symbol (e.g. p ). This indicates either 23 or 4̄3m (Table 9.10). These are readily distinguished, since only 4̄3m has mirror planes. These planes are easily seen in CH4 , so the point group is 4̄3m. (b) A crystal of magnesium (Table 9.11.27). The crystal contains a 6-fold rotation axis, and so must belong to the hexagonal system. An inversion center is also easily found. This limits the point group to 6/m and 6/mmm (Table 9.10). These may be distinguished by the mirror planes parallel to 6 in 6/mmm and not in 6/m. Since these planes are evident in the crystal, the magnesium crystal may be assigned to point group 6/mmm. Table 9.10 Crystal systems, point groups, symmetry directions and symmetry-dependent physical properties 9.4 Determination of Point Groups 151 Table 9.10 (Continued) 152 9 Point Groups b Schönﬂies symbol. Hermann-Mauguin symbol (International symbol). c The number of symmetry elements of each type is given, p signiﬁes polar. d Rotation axes, rotoinversion axes and the normals to mirror planes are parallel to the respective symmetry directions. a 9.4 Determination of Point Groups 153 154 9 Point Groups Determination of the symmetry of a crystal is not always unambiguous. For example, the cube (hexahedron) occurs as a form in all ﬁve cubic point groups (Table 9.6). Determining the symmetry of a cube will naturally lead to the point group of highest symmetry, m3̄m (Table 9.11.32). The mineral pyrites, FeS2 (point group m3̄) has cube-shaped crystals. The cube-faces, however, frequently have characteristic striations which indicate the lower symmetry (Table 9.11.29). In other ambiguous cases, “etch-ﬁgures” will indicate the true symmetry of a crystal face and hence of the entire crystal. These ﬁgures are bounded by faces with high Miller indices and arise from the action of a solvent on a crystal face. Crystals of the mineral nepheline (Table 9.11.21) have a morphology (a hexagonal prism and a pinacoid) which indicate the point group 6/mmm. The etch ﬁgures show that the true symmetry is only 6. 9.5 Enantiomorphism The point group 1(C1 ) is asymmetric. All other point groups with no symmetry other than rotation axes are called chiral or dissymmetric. The relevant point groups are: X: (1), 2, 3, 4, 6 X2: 222, 32, 422, 622 X3: 23, 432 Cn : (C1 ), C2 , C3 , C4 , C6 Dn : D2 , D3 , D4 , D6 T, O D Asymmetric and dissymmetric crystals and molecules are those which are not superimposable on their mirror images by rotation or translation. These mirror images are said to be the enantiomorphs of each other. In Fig. 6.9 and Table 9.11.3 and 18, examples are given of enantiomorphic crystals and molecules. Enantiomorphic molecules are also called enantiomers. 9.6 Point Groups and Physical Properties We shall now examine a few properties of molecules and crystals which are related to their point groups, or whose eﬀects may be traced back to speciﬁc symmetry considerations. 9.6.1 Optical Activity Optical activity refers to the ability of certain crystals and molecules to rotate the plane of polarized light. It can only arise in those point groups which are enantiomorphic (cf. Sect. 9.5 and Table 9.10). The optical activity of a crystal may be distinguished from that of a molecule in two ways: 9.6 Point Groups and Physical Properties 9.6.1.1 Optical Activity as a Property of a Crystal The crystal is optically active only in the crystalline state. The activity is lost when the crystal is melted or dissolved. Examples include MgSO4 · 7H2 O, SiO2 (lowquartz) and NaClO3 (Table 9.11.6, 18 and 28). Not only the morphology but also the crystal structures exist in two enantiomorphic forms. The “left” form rotates the plane of polarized light to the left, and the “right” form an equal amount to the right. 9.6.1.2 Optical Activity as a Property of Molecules Some molecules are themselves enantiomeric, and both their solutions and the crystals they form are optically active. Well-known examples of this type of optical activity are the crystals of D- and L-tartaric acid (Table 9.11.3). In contrast, the “racemate” DL-tartaric acid is optically inactive and gives crystals with point group 1̄ (Ci ). Molecules of the isomeric form meso-tartaric acid (1̄, (Ci ), Table 9.11.2) are centrosymmetric and hence optically inactive. Optical activity is not limited to the 11 point groups in which enantiomorphism occurs (Sect. 9.5). It can also occur in crystals in the point groups m(Cs ), mm2(C2v ), 4̄ (S4 ) and 4̄2m (D2d ), cf. Table 9.10. 9.6.2 Piezoelectricity Some crystals, when subjected to pressure or tension in certain directions develop an electric charge; this property is called piezoelectricity. This eﬀect is clearly seen in plates of quartz (point group 32), cut normal to the a-axis or any polar 2-fold rotation axis (Fig. 9.21). The direction of the applied pressure or tension must be along a polar axis. Polar axes are those which have distinct physical properties in the parallel and antiparallel directions. These directions must thus not be themselves related by symmetry. It follows that within the crystal there will be an asymmetric charge distribution along polar axes. Application of pressure normal to such an axis will alter the separation of the centers of the negative and positive atoms of the crystal, since the dipole moment of the crystal will be parallel to a polar axis. Thus, the opposite faces, normal to a polar axis, develop electric charges when a pressure is applied along that axis. The direction of this electric ﬁeld is reversed when the pressure is replaced by a tension. Piezoelectricity is only observed in crystals which have polar axes. Polar directions only exist in point groups without a center of symmetry. There are 21 such point groups, as is shown in Table 9.10. The point group 432 is also excluded, as the symmetry is too high for the eﬀect to develop. 155 156 9 Point Groups Fig. 9.21a–c The piezoelectric eﬀect in a quartz plate arising from pressure along a polar axis, here parallel to the a1 axis The piezoelectric eﬀect is reversible. If an electric ﬁeld is applied in the direction of the polar axis of a quartz plate, the crystal will undergo compression or expansion. The application of an alternating ﬁeld will cause the crystal to vibrate. Other crystals which show piezoelectricity include D- and L-tartaric acid (2 − C2 ), Table 9.11.3; tourmaline (3m − C3v ), Table 9.11.19; NaClO3 (23 − T), Table 9.11.28; ZnS (sphalerite) (4̄3m − Td ), Table 9.11.31. Piezoelectricity has many technical applications, including ultrasonic generators, ampliﬁers, microphones and quartz time-pieces. 9.6.3 Pyroelectricity When a crystal of tourmaline (Table 9.11.19) is heated, the polar ends of the crystal develop electric charges. Heating causes the positive end of the c-axis to become positively charged relative to the negative end, and cooling has the opposite eﬀect. This eﬀect results from the fact that tourmaline has a permanent electric dipole. The charge which builds up is soon dissipated by conduction into the surroundings. Changes in temperature change the size of the electric dipole. The dipole moment is a vector. Pyroelectricity can only arise when the point group has no symmetry operations which alter the direction of this dipole. The vector must remain unchanged by all the symmetry operations. Point groups having this property include those with only a single rotation axis: 2(C2 ), 3(C3 ), 4(C4 ) and 6(C6 ) as well as those which have only these axes plus mirror planes parallel to them: mm2(C2v ), 3m(C3v ), 4 mm(C4v ) and 6 mm(C6v ). The dipole-moment vector lies in the rotation axis. The conditions for the presence of a dipole moment are also found in the point groups m (for all directions parallel to the mirror plane) and 1 (for every direction), cf. Table 9.10. Knowledge of the symmetry gives only a qualitative indication of the possible presence of pyroelectricity. It does not indicate the size of the dipole moment or the directions of the positive and negative ends. Sucrose, C12 H22 O11 , (2 − C2 ) and hemimorphite, Zn4 [(OH)2 /Si2 O7 ] · H2 O (mm2 − C2v ) are examples of crystals showing pyroelectricity. 9.6 Point Groups and Physical Properties Table 9.11 Examples of molecules and crystals for the point groups 157 158 9 Point Groups Table 9.11 (Continued) 9.6 Point Groups and Physical Properties Table 9.11 (Continued) 159 160 9 Point Groups Table 9.11 (Continued) 9.6 Point Groups and Physical Properties Table 9.11 (Continued) 161 162 9 Point Groups Table 9.11 (Continued) 9.6 Point Groups and Physical Properties Table 9.11 (Continued) 163 164 9 Point Groups Table 9.11 (Continued) 9.6 Point Groups and Physical Properties Table 9.11 (Continued) 165 166 9 Point Groups 9.6.4 Molecular Dipole Moments Many molecules have an asymmetric distribution of electric charge and hence an electric dipole moment. The relationship between the point group of a molecule and the direction of its dipole is the same as that developed above for the pyroelectricity of crystals (cf. Sect. 9.6.3). The measurement of a dipole moment can give important information about the shape of a molecule. PF3 has a dipole moment, while BF3 does not. Molecules of the formula AB3 may have the shape of an equilateral triangle with A at the center [6̄m2 – (D3d )] or a triangular pyramid with A at the apex [3m – (C3v )], cf. Table 9.11.19 and 26. The shape of BF3 is thus the former, while PF3 is the latter. 9.7 Noncrystallographic Point Groups Up to this point, we have only been concerned with the 32 crystallographic point groups, which are the most important ones for the purpose of this book. In order to give a complete picture, however, it must be emphasized that there are an inﬁnite number of point groups which cannot be assigned to a crystal system because they contain 5-, 7-, 8- . . .. . . up to ∞-fold axes. D Point groups which contain a rotation or rotation-inversion axis which is incompatible with a space lattice are called noncrystallographic point groups. Noncrystallographic point groups are, however, important for the description of molecular symmetry. Linear molecules such as CO, HCl and CN- , like a cone, have an ∞-fold rotation axis with an inﬁnite number of mirror plans parallel to it. The point group is ∞m. (Table 9.12.1) The symmetry of other linear molecules such as O2 and CO2 is that of a bicone or a cylinder; in addition to the symmetry of ∞m, there are a mirror plane and inﬁnitely many 2-fold axes normal to the ∞-fold axis. In addition there is an inversion center. The point group symbol is ∞/mm. (Table 9.12.2) The symmetry of the sulfur molecule S8 is that of the tetragonal antiprism, 8̄2m. (Table 9.12.3) The pentagonal prism has symmetry 5/mm2. (Table 9.12.4) and is not a crystal form!! All prisms, pyramids and bipyramids with X > 6 are also never crystal forms; they cannot form the natural boundary surfaces of a crystal. Although it has ﬁve equivalent faces, these do not constitute a crystal form. When non-crystallographic symmetry is considered, the deﬁnition of a crystal form in Sect. 9.2 must be extended to read “ . . ... but only when the equivalence is generated by the operations 1, 2, 3, 4, 6, 1̄, m, 3̄, 4̄, or 6̄. 9.7 Noncrystallographic Point Groups Table 9.12 A few noncrystallographic point groups Molecules, polyhedra and other geometric forms 1 Noncrystallographic point groups CO, HCl, CN– An ∞-fold rotation axis with inﬁnitely many mirror planes parallel to it ∞m – C∞v cone 2 H2 O2 Cl2 An ∞-fold rotation axis with inﬁnitely many mirror planes parallel to it, inﬁnitely many 2-fold rotation axes normal to it and a mirror plane normal to it CO2 ∞/mm – D∞h bicone cylinder 3 S8 8̄2m – D4d 167 168 9 Point Groups Table 9.12 (Continued) Molecules, polyhedra and other geometric forms Noncrystallographic point groups 4 ferrocene (eclipsed conformation) 5/mm2 – D5h 10m2 Pentagonal prism 5 pentagonal dodecahedron 2/m35 – D5h icosahedron 9.7 Noncrystallographic Point Groups Table 9.13 Elements of the platonic solids 6 8 6 12 Point group Type of symmetry 4̄3m Crystallographic m3m 6 8 12 Regular pentagon 12 20 30 Equilateral triangle 20 12 30 Icosahedron 4 Pentagonal dodecahedron 4 Square Edges (e) Cube Vertices (v) Octahedron Faces (f) Equilateral triangle Number of Tetrahedron Description of faces Polyhedron 2/m3̄5̄ Noncrystallographic D The ﬁve platonic solids, named for the Greek philosopher Plato, are those which are bounded by a set of equivalent regular polygons. Only three of these ﬁve solids can be crystal forms, namely the tetrahedron, the octahedron and the cube. (see Exercise 9.15: 15, 14, and 13.) The other two platonic solids are the pentagonal dodecahedron and the icosahedron (Table 9.12.5). In Table 9.13, all of the platonic solids are listed with their geometrical properties (number of faces, edges and vertices). The tetrahedron has point group 4̄3m, the octahedron and the cube m3̄m, and the icosahedron and the pentagonal dodecahedron 2/m3̄5̄, as shown in Table 9.12.5. It is certainly worthwhile to take the time to build models of both of these polyhedra in order fully to appreciate their symmetry (patterns are given in Exercise 15.9). It will be evident from the stereographic projection of the pentagonal dodecahedron along a 5-fold axis and of the icosahedron along a 3-fold axis that these solids have the point group 2/m3̄ 5̄. It will be noticed that the octahedron and the cube, and also the pentagonal dodecahedron and the icosahedron, are “duals” of one another. This means that the two solids have the same number of edges, while the number of faces in each equals the number of vertices in the other. (See the arrows in Table 9.13). Table 9.13 also illustrates the Euler equation for convex polyhedra: f faces + v (vertices) = e edges + 2. It is important not to confuse the (noncrystallographic) regular pentagonal dodecahedron with the various cubic dodecahedral crystal forms, especially the tetartoid and the pyritohedron with symmetry 23 and 2/m3̄ respectively (Fig. 15.2d.36 and 37), the faces of which are not regular pentagons. (Fig. 15.2d (37), (36) and Fig. 15.7(1)) 169 170 9 Point Groups 9.8 Exercises Exercise 9.1 (a) What is meant by a polar rotation axis? (b) Which symmetry elements can compensate the polarity of a rotation axis? The arrows in the diagram represent X-fold polar rotation axes, Xp. The polarity will be compensated by a symmetry operation which reverses the head of the arrows. Draw in the location of symmetry elements which can do this. (c) How can polar rotation axes be recognised in symmetry diagrams and in the stereograms of point groups? Exercise 9.2 Are there polar rotoinversion axes? If so, specify which; if not, state why not. Exercise 9.3 Combine the operations 1+1̄, 2+1̄, 3+1̄, 4+1̄, 6+1̄. Which point groups result? Give their symbols. Exercise 9.4 Combine the operations (A) 2+2, (B) m+m and (C) 2+m, where the elements intersect at angles of 30, 45, 60 and 90◦ . Take the direction of m to be the direction of its normal. Complete the stereographic projections shown in Table 9.14. Which symmetry elements are generated? What are the resultant point groups? Give the symbols for each. Copy the stereograms of the point groups in columns A, B or C into column D, and add 1̄. Which new point groups are generated? Give their symbols. For each point group, choose an axial system and assign each point group to a crystal system. The solution of that part of the exercise will explain the following symmetry rules: ε (A) The combination of two 2-fold axes at an angle of produces an X-fold 2 axis through their point of intersection perpendicular to their common 360◦ plane. X = . ε ε (B) The combination of two mirror planes at an angle of produces an X-fold 2 360◦ axis along their line of intersection. X = . ε 9.8 Exercises ε 2 produces an X̄ axis through the point of intersection of the axis with the normal to the plane and perpendicular to the common plane of the axis 360◦ . and the normal. X̄ = ε (C) The combination of a 2-fold axis with a mirror plane at an angle of Since only X=1, 2, 3, 4 and 6 or X̄ = 1̄, 2̄ ≡ m, 3̄, 4̄ and 6̄ are permitted, ε2 can only have the values 30, 45, 60, 90 and 180◦ . The combinations at an angle of 180◦ are not included in Table 9.14. Table 9.14 171 172 9 Point Groups Exercise 9.5 Combine the operations of (A) 2+3, (B) 4̄+3 and (C) 4+3, where the elements intersect at an angle of 54.73◦ (the angle between the edge and the body diagonal of a cube). Complete the stereographic projections shown in Table 9.15, and give the symbols for the resultant point groups. Copy the stereograms in E, F and G into H, I and K and add 1̄ to them. Give the symbols of the point groups which now result. Table 9.15 Exercise 9.6 Starting from the point of highest symmetry in the trigonal system 3 2/m, develop its trigonal subgroups. Exercise 9.7 Color the circles of the point groups in Fig. 9.3, using the same color for all point groups belonging to the same crystal system. Exercise 9.8 (a) How is it possible to identify the crystal system of a point group from its International symbol? (b) For each crystal system, give the characteristic point-symmetry elements, and, if necessary, the number of such elements or their relationship to one another. Mark the position these elements occupy in the International point-group symbol, and give an example for each crystal system. 9.8 Exercises Crystal system Characteristic symmetry elements number and relationship to one another Position of characteristic symmetry element(s) in the symbol 1st 2nd 3rd Example Triclinic Monoclinic Orthorhombic Tetragonal Trigonal Hexagonal Cubic Exercise 9.9 Determine the International symbol for the point groups whose symmetry elements are illustrated in the following sterograms: 173 174 9 Point Groups (a) First, ﬁnd the symmetry elements that charcterise the crystal system. (b) Indicate the crystallographic axes a, b, c on the sterogram, bearing in mind the orientation of the symmetry directions for the crystal system. (c) Give the International symbol and, in brackets, the Schönﬂies symbol. Exercise 9.10 In the stereograms below, indicate the symmetry elements for the given point group: (a) Determine the crystal system. (b) Draw the appropriate axial system on the stereogram. The c-axis should always be perpendicular to the plane of projection. (c) Analyse the point group symbol with respect to the symmetry directions. (d) Finally, draw the symmetry elements on the stereogram. Remember that rotations and rotoinversion axes, as well as the normals to planes are arranged parallel to their symmetry directions. 9.8 Exercises Exercise 9.11 Determination of point groups Determine the point groups of the molecules and ions given below, using the method described in Sect. 9.4. Give the International symbol and the Schönﬂies symbol, and draw the symmetry elements on the stereographic projection. (a) Which isomers of tetrachlorocyclobutane are enantiomers? (b) Which molecules possess a dipole moment? 175 176 9 Point Groups 9.8 Exercises 177 178 9 Point Groups 9.8 Exercises 179 180 9 Point Groups 9.8 Exercises 181 182 9 Point Groups Exercise 9.12 What information about the spatial arrangement of the atoms in the following molecules can you infer from the point group symmetry? 9.8 Exercises Exercise 9.13 Rotate one of the CH2 Cl groups of a 1,2-dichloroethane molecule about the C-C bond stepwise through 360◦ with respect to the other. Which symmetry distinct conformations are encountered? Given their point groups, and compare them with the corresponding conformations of ethane in Fig. 9.20. Exercise 9.14 Will measurements of their dipole moments distinguish the cis and trans forms of dichloroethene? Exercise 9.15 (a) Determine the point groups of the following crystals with the help of Table 9.10 and crystal models such as those illustrated in Exercise 5.4. Draw the symmetry elements on the stereogram, and give the International symbol for the group. (b) Indicate the position of the crystallographic axes on the stereograms and the crystal diagrams. (c) Estimate by eye the positions of the crystal faces, and enter the poles on the stereogram, using diﬀerent colors for diﬀerent forms. (d) Index the crystal forms. 183 184 9 Point Groups 9.8 Exercises 185 186 9 Point Groups Tetragonal Scalenohedron Pentagonal Dodecahedron Ditetragonal Scalenohedron Hexagonal Trapezohedron Exercise 9.16 Which of the crystals in Exercise 9.15 might, on the basis of its crystal forms, show the piezo-electric eﬀect? Mark the appropriate diagrams “Piezo-elect.” Exercise 9.17 There is a simple relationship between the numbers of faces, edges and vertices of a polyhedron. Work out what it is. Exercise 9.18 The ﬁgure shows the cross-section of a ditetragonal prism on the equatorial plane of a stereographic projection, together with the corresponding poles. The dashed lines have been added to point out the axial intercepts of the faces. 9.8 Exercises (a) Index all the faces of the crystal form {hk0} or {210}. (b) If the faces of a ditetragonal prism are inclined by a given angle in the direction of the positive and negative c-axis, the poles of the faces move a corresponding amount away from the periphery in the [001] and [001] directions. What is the resulting crystal form? Index all the faces of this form. Exercise 9.19 The ﬁgure shows the cross-section of a hexagonal prism on the equatorial plane of a stereographic projection, together with the corresponding poles. The dashed lines have been added to point out the axial intercepts of the faces. (a) Index all the faces of the crystal form {hki0} or {2130}. (b) If the faces of a hexagonal prism are inclined by a given angle in the direction of the positive and negative c-axis, the poles of the faces move a corresponding amount away from the periphery in the [0001] and [0001] directions. What is the resulting crystal form? Index all the faces of this form. Exercise 9.20 Derive the crystal forms of the following point groups: (1) 42m (4) mm2 (7) 3m (2) 4 (5) 6/mmm (8) m3m (3) mmm (6) 622 (9) 43m (a) Use the characteristic symmetry elements to determine the crystal system (cf. Table 9.9). 187 188 9 Point Groups (b) Look up the stereogram of the poles of the forms for the point group of highest symmetry in that system: Fig. 9.16 for orthorhombic, Fig. 9.9 for tetragonal, Fig. 9.13 for hexagonal or trigonal, and Fig. 9.15 for cubic. (c) Place a piece of tracing paper over the stereogram, and draw in the symmetry elements for the point group, appropriately orientated to the crystallographic axes. (d) Indicate the asymmetric face unit. (e) Draw in ﬁrst the poles for the faces of the general form. What is it called? Index all the faces. (f) If the general form has limiting forms, draw these in and name and index them. (g) Draw in the special forms and their limiting forms (if any). Name and index them and give the point symmetry of their gaces. (It is a good idea to use several pieces of tracing paper!) Exercise 9.21 In International Tables for Crystallography, Vol. A, for the point group 4/m32/m, the trapezohedron (or deltoidicositetrahedron), is given as the special form {hhl}, |h|<|l| and the trisoctahedron for {hhl}, |h|>|l|. In Table 9.6, however, the trapezohedron is given for {hkk} and the trisoctahedron for {hhk}. Explain this apparent inconsistency. Exercise 9.22 Which special forms in the hexagonal and trigonal systems have limiting forms? Exercise 9.23 Note that, as shown in Table 9.6, the {100} form in all cubic point groups is a cube. The highest face-symmetry in point group 4mm can also show cube-like faces, characteristic of m3̄m. Many of the cubic crystrals of pyrites, FeS2 , show characteristic striations on the cube faces, which reduce the face symmetry to mm2, indicating that the point group of the crystal is 2/m3̄. (a) Draw a cube, and decorate the faces so as to reduce the symmetry to 4̄3m, 432 and 23. (b) In each case, what has the face symmetry become? 10 Space Groups 10.1 Glide Planes and Screw Axes The 32 point groups are the symmetry groups of many molecules and of all crystals, so long as only the morphology is considered. Space groups give the symmetry not only of crystal lattices, but also of crystal structures. The space-group symbols for the 14 Bravais lattices are listed in Table 7.4. The space-group symbol does not in general enumerate all the symmetry elements of the space group. In particular, the space groups of centered lattices contain new symmetry operations. These are compound symmetry operations which arise through reﬂection and translation (1) and rotation and translation (2) (cf. Sect. 6.4 and Table 6.2). 1. In the orthorhombic C-lattice, reﬂection through a plane (– – –) at 1/4,y,z, fol lowed by a translation of b2 moves the lattice point 0,0,0 to 1/2,1/2,0 (Fig. 10.1a). This symmetry operation is called a glide reﬂection, and the corresponding element is a glide plane (in this case, a b-glide plane). Fig. 10.1 a Location of a b-glide plane in an orthorhombic C-lattice. b. Position of 2-fold screw axis in an orthorhombic I-lattice. ( lattice point with z = 1/2) 2. In the orthorhombic I-lattice, a 180◦ rotation about an axis ( ) at 1/4,1/4,z, followed by a translation of 2c , moves the lattice point 0,0,0 to 1/2,1/2,1/2 (Fig. 10.1b). This symmetry operation is called a screw rotation, and the corresponding element is a screw axis (in this case, a 2-fold screw axis). W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_10, C Springer-Verlag Berlin Heidelberg 2011 190 10 Space Groups 10.1.1 Glide Planes The compound symmetry operation “glide reﬂection” implies: (A) a reﬂection and (B) a translation by the vector g parallel to the plane of glide reﬂection where |g| is called the glide component. Figure 10.2 contrasts the operation of a mirror plane with that of a glide plane on a point lying oﬀ the planes. Fig. 10.2a,b Operation of a mirror plane m (a) and of a glide plane c (b) on a point shown in perspective and as a projection on (001) A second application of the glide reﬂection brings one to a point identical to the starting point. ! |g| is one-half of a lattice translation parallel to the glide plane, |g| = 12 | τ |. Glide planes are developments of mirror planes, and can only occur in an orientation that is possible for a mirror plane. For this reason, in the orthorhombic system, glide planes only occur parallel to (100), (010) and (001). Compare the space group P2/m 2/m 2/m in Fig. 7.9d with the point group 2/m 2/m 2/m in Fig. 7.9e. Since the glide component |g| must be half of a lattice translation parallel to the glide plane, in an orthorhombic space group the only possible glide planes parallel to (100) will have glide components 1 1 c|, 12 |b + c| and 14 |b + c|, and this last type will only occur in centered 2 |b|, 2 | 10.1 Glide Planes and Screw Axes Fig.10.3 Glide planes in the orthorhombic system lattices, where 14 |b + c| can be half of a lattice translation. In Fig. 10.3, these cases are illustrated, together with those parallel to (010) and (001). Glide planes are designated by symbols indicating the relationship of their glide or components to lattice vectors a, b and c. Those with axial components: 12 |a|, 12 |b| 1 c| are given the symbols a, b and c respectively, those with diagonal components 2 | 1 1 | 2 τ1 ± τ2 |, have the symbol n, while those with component 4 | τ1 ± τ2 |, known as diamond glides, have the symbol d. (See Fig. 10.3). Finally, in some centered lattices, These a plane may have glide components in both of two directions, e.g. 1/2a and 1/2b. are given the symbol e (Fig. 10.4f). Since glide planes play so important a role in space groups, the operation of a few examples will be given in an orthorhombic cell projected on x,y,0. In these projection diagrams, only a single glide plane is shown – see Sect. 15.2 for an explanation of the graphical symbols. • In Fig. 10.4a, an a-glide is shown at x,1/4,z. Reﬂection of a point x,y,z in this plane gives x,1/2−y,z, called an “auxiliary” point and the translation 12 a then moves this auxiliary point to 1/2+x,1/2−y,z. • The b-glide plane at x,y,0 in Fig. 10.4b reﬂects a point x,y,z to the auxiliary point x,y,z, which the translation of 12 b then moves to x,1/2+y,z̄. • The c-glide plane at x,1/2,z in Fig. 10.4c reﬂects a point x,y,z to the auxiliary point, x,1−y,z which the translation of 1/2c then moves to x,1−y,1/2+z. 191 192 10 Space Groups Fig. 10.4a–f Operation of glide planes on a point. In each case, only a single glide plane is shown projected on x,y,0 in an orthorhombic cell 10.1 Glide Planes and Screw Axes • The n-glide plane at x,y,1/4 in Fig. 10.4d is parallel to the a, b-plane, and thus has a It reﬂects a point x,y,z to the auxiliary point x,y,1/2−z, glide component 12 |a + b|. then moves to 1/2+x,1/2+y,1/2−z. which the translation of 12 (a + b) • The n-glide plane at 0,y,z in Fig. 10.4e has a glide component 12 |b + c|. It reﬂects a point x,y,z to the auxiliary point x̄, y, z, which the translation of 12 (b + c) then moves to x̄, 12 + y, 12 + z. 10.1.2 Screw Axes The compound symmetry operation “screw rotation” implies: 360◦ ; (X = 1, 2, 3, 4, 6) and X • a translation by a vector s parallel to the axis, where |s| is called the screw component. • a rotation of an angle ε = For rotation axes and rotoinversion axes, the direction of rotation was unimportant. This is not the case for screw axes; for a right-handed axial system, X,Y,Z (Fig. 10.5) a rotation about an axis on Z from the X-axis toward the Y-axis is linked with a positive translation along Z. This is the motion of a right-handed screw, which corresponds to the motion of advancing the thumb of the right hand in the direction of the vector s as the ﬁngers of this hand point in the sense of rotation. Figure 10.6 shows the operation of a 6-fold screw axis (ε = 60◦ ) on a point lying oﬀ the axis. The points 1, 2, 3 . . . are arranged like the treads of a spiral staircase. After X rotations (X = 6) through the angle ε (X · ε = 360◦ ), the point 1 would return to its starting point. In this case, however, the rotations have been accompanied by a translation of X · s, and the point 1 has been reached, which is identical to the Fig. 10.5 The handedness of a screw axis Fig 10.6 Operation of a 6-fold screw axis 61 on a point lying oﬀ the axis Fig. 10.5 Fig. 10.6 193 194 10 Space Groups starting point. The vector 1–1 is not necessarily a single lattice translation τ, but may be any integral multiple σ of τ. X · |s| = σ | τ | or |s| = σ | τ |. X Since |s| < | τ |, σ < X and can have the following values: σ = 0, 1, 2, . . . X–1 and |s| = 0, X1 | τ |, X2 | τ |, .... X−1 τ| X | since the screw component |s| = σ | τ| , X screw axes are designated Xσ = X0 , X1 , X2 , . . .. XX–1 For X = 4, σ = 0, 1, 2, 3. The resulting screw axes are 40 (a 4-fold rotation axis), τ |, 24 | τ | and 34 | τ |. (Note that the screw 41 , 42 and 43 , with screw components 0, 14 | component is directly derivable from the symbol, by inverting it and considering Fig. 10.7a,b Operation of a 4-fold rotation axis and the three 4-fold screw axes on a point lying oﬀ the axes. (a) shows perspective views and (b) projections on x,y,0 10.2 The 230 Space Groups it as a fraction, e.g. 41 → 14 .) The 4-fold rotation and screw axes are compared in Fig. 10.7. Successive operations of the 4-fold screw axes on a point lying oﬀ the axis move point 1 to 2, 3 and 4. A lattice translation of τ generated the points 1 , 2 , 3 and 4 . The operations of the screw axes are also illustrated in Fig. 10.7b by projection of the points within a single lattice translation onto the plane normal to the axis. Note that the sets of points generated by 41 and 43 are mirror images of one another, i.e. they are a pair of enantiomorphs. Since 41 represents a right-handed screw, 43 may be described as a left-handed screw with a screw component |s | = 14 | τ | also. Figure 10.8 shows all of the other screw and rotation axes possible for crystals (see also Sect. 15.2). The enantiomorphous pairs are 31 and 32 , 41 and 43 , 61 and 65 , and 62 and 64 . Screw axes can only occur in crystals parallel to those directions which are possible for rotation axes in the corresponding point group. 10.2 The 230 Space Groups The 32 crystallographic point groups have been derived from the point groups of highest symmetry in each crystal system (see Table 9.2). All of the space groups can be derived in a similar manner. Starting from the space groups of highest symmetry in each crystal system, i.e. those of the 14 Bravais lattices (see Table 7.4), it is possible to derive an analogous scheme for determining all of their subgroups. It must, however, be borne in mind that screw axes can replace rotation axes, and glide planes mirror planes thus: 2 ← 21 3 ← 31 , 32 4 ← 41 , 42 , 43 6 ← 61 , 62 , 63 , 64 , 65 m ← a, b, c, n, e, d. Fig. 10.8 Operation of rotation and screw axes on a point lying oﬀ them. The enantiomorphous pairs 31 –32 , 61 –65 and 62 –64 are given together. 4, 41 , 42 and 43 are shown in Fig. 10.7 195 196 10 Space Groups Fig. 10.8 (Continued) 10.2 The 230 Space Groups a. Space groups of point group 2/m Fig. 10.9a The monoclinic space groups projected on x,y,0. The c-axis is not normal to the plane of projection, but is tilted such that β > 90◦ 197 198 10 Space Groups b. Space groups of point group m c. Space groups of point group 2 Fig. 10.9b,c (Continued) The space groups of the monoclinic system will be derived as an example for all crystal systems. We start from the two monoclinic space groups of highest symmetry; P2/m and C2/m (Fig. 10.9). Additionally, in C2/m, there are a-glide planes at x,1/4,z and x,3/4,z, and 21 -axes at 1/4,y,0; 1/4,y,1/2; 3/4,y,0 and 3/4,y,1/2. The monoclinic subgroups of the point group 2/m are m and 2. The pointsymmetry elements 2 and m can be replaced by 21 and a glide plane respectively. Since m is parallel to (010), only a-, c- and n-glides are possible. However, a diﬀerent 10.2 The 230 Space Groups Fig. 10.10a–c In the monoclinic system, a-, c-, and n-glide planes parallel to (010) are all possible. These are shown in a, b and c respectively. Suitable alteration of the choice of axes will convert aand n- into c-glides choice of the a and c axes will convert either an a- or an n-glide into a c-glide (Fig. 10.10). Thus, only the c-glide need be considered. (Note, however, that in the C2/m, it is an a-glide that is produced by the centering operation.) Replacement of 2 and m by 21 and c results in the 13 monoclinic space groups shown in Table 10.1 as subgroups of P2/m and C2/m. The sets of symmetry elements for these space groups are shown in Fig. 10.9, in the same order as Table 10.1, as projections on x,y,0. Additionally, a- and n-glide planes occur in C-centered space groups. Thus it can be seen that the pairs of symbols C2/m and C21 /m, C2/c and C21 /c, and C2 and C21 represent only a single space group each, cf. Exercise 10.4. In the same way, inspection of the other crystal systems leads to the entire 230 space groups. These 230 space groups are listed in Table 10.2, sorted by crystal system and point group. Only the standard abbreviated symbols (short symbols) are given. In every case, the point group is easily derived from the space group symbol. The screw axes are replaced by the corresponding rotation axis, the glide planes by a mirror plane, and the lattice symbol is omitted, the result being the point group to which the space group belongs. Table 10.1 The point and space groups of the monoclinic crystal system Point groups 2/m m 2 a Space groups P2/m C2/m P21 /m -a P2/c C2/c P21 /c -b Pm Cm Pc Cc P2 C2 P21 -c C21 /m ≡ C2/m, b C21 /c ≡ C2/c, c C21 ≡ C2 199 200 10 Space Groups Table 10.2 The 230 Space groups Crystal system Point group Space groups Triclinic 1 1̄ P1 P1̄ Monoclinic 2 m 2/m P2 Pm P2/m P21 c P21 Pc P21 /m C2/c C2 Cm C2/m Cc P2/c 222 P222 C2221 I21 21 21 Pmm2 Pca21 Pna21 Ccc2 Aea2 Iba2 Pmmm Pmma Pbam Pmmn Cmcm Cmme Immm P2221 C222 P21 21 2 F222 P21 21 21 I222 Pmc21 Pnc2 Pnn2 Amm2 Fmm2 Ima2 Pnnn Pnna Pccn Pbcn Cmce Ccce Ibam Pcc2 Pmn21 Cmm2 Aem2 Fdd2 Pma2 Pba2 Cmc21 Ama2 Imm2 Pccm Pmna Pbcm Pbca Cmmm Fmmm Ibca Pban Pcca Pnnm Pnma Cccm Fddd Imma P4 I4 P4̄ P4/m I4/m P4/22 P42 22 I422 P4mm P4cc I4mm P4̄2m P4̄m2 I4̄m2 P4/mmm P4/mbm P42 /mmc P42 /mbc I4/mmm P41 I41 I4̄ P42 m I41 /a P421 2 P42 21 2 I41 22 P4bm P4nc I4cm P4̄2c P4̄c2 I4̄c2 P4/mcc P4/mnc P42 /mcm P42 /mnm I4/mcm P42 P43 P4/n P42 /n P41 22 P43 22 P41 21 2 P43 21 2 P42 cm P42 mc I41 md P4̄21 m P4̄b2 I4̄2m P4/nbm P/4nmm P42 /nbc P42 /nmc I41 /amd P42 nm P42 bc I41 cd P4̄21 c P4̄n2 I4̄2d P4/nnc P4/ncc P42 /nnm P42 /ncm I41 /acd P3 P3̄ P312 P32 12 P3ml R3m P3̄1m R3̄m P31 R3̄ P321 P32 21 P31m R3c P3̄1c R3̄c P32 R3 P31 12 R32 P3c1 P31 21 P3̄m1 P3̄c1 Orthorhombic mm2 mmm Tetragonal 4 4̄ 4/m 422 4 mm 4̄2m 4/mmm Trigonal 3 3̄ 32 3m 3̄m P31c 10.3 Properties of Space Groups Table 10.2 (Continued) Crystal system Point group Space groups Hexagonal 6 P6 P64 P6̄ P6/m P622 P64 22 P6mm P6̄m2 P6/mmm P61 P63 P63 /m P61 22 P63 22 P6cc P6̄c2 P6/mcc P23 I21 3 Pm3̄ Im3̄ P432 I432 P4̄3m F4̄3c Pm3̄m Fm3̄m Im3̄m 6̄ 6/m 622 6 mm 6̄m2 6/mmm Cubic 23 m3̄ 432 4̄3m m3̄m P65 P62 P65 22 P63 cm P6̄2m P63 /mcm P62 22 P62 22 P63 mc P6̄2c P63 /mmc F23 I23 P21 3 Pn3̄ Pa3̄ P42 32 P43 32 F4̄3m I4̄3d Pn3̄n Fm3̄c Ia3̄d Fm3̄ Ia3̄ F432 P41 32 I4̄3m Fd3̄ F41 32 I41 32 P4̄3n Pm3̄n Fd3̄m Pn3̄m Fd3̄c It would be useful to revise the space groups of the Bravais lattices, which are given in Figs. 7.7d–7.13d. The International (Hermann-Mauguin) symbols thus indicate the symmetry of each space group clearly. Schönﬂies symbols, on the other hand, merely assign an arbitrary number to each space group within a given point group. Thus, for point group m(Cs ), we have: Pm : (C1s ), Pc : (C2s ), Cm : (C3s ), Cc : (C4s ). This is the main reason that Schönﬂies symbols are rarely used in crystallography. 10.3 Properties of Space Groups It is certainly not necessary to study each of the 230 space groups individually, but a general knowledge of how space groups diﬀer from one another is useful. For this reason, the properties of a few space groups will be explored in detail. Figure 10.11a gives the symmetry elements for the space group Pmm2. The application of the symmetry operations to a point x,y,z will generate the points x,ȳ,z; x̄,y,z, and x̄,ȳ,z, as well as equivalent points such as x,1-y,z; 1-x,y,z and 1-x,1-y,z. 201 202 10 Space Groups Fig. 10.11a–c Symmetry elements of space group Pmm2 in projection on x,y,0. (a) The general position x,y,z. (b) the special position 1/2,y,z. (c) The special position 1/2,1/2,z D The number of equivalent points in the unit cell is called its multiplicity. In Fig. 10.11a, the position is “4-fold”, or said to have a multiplicity of 4. This position has no restrictions on its movement; it has three degrees of freedom, and, as long as it does not move onto a point symmetry element, it continues to have a multiplicity of 4. Such a position is called a general position. D A general position is a set of equivalent points with point symmetry (site symmetry) 1. It is asymmetric, and this is indicated in Fig. 10.11 by the tail on the circle. The ﬁgure is, of course, not really asymmetric, as it is unchanged on reﬂection in the plane of the paper, but it is suﬃciently unsymmetrical for our present purpose! If the point in the general site x,y,z is moved on to the mirror plane at 1/2,y,z, the point 1-x,y,z comes into coincidence with it; the two points coalesce at the mirror plane to a single point 1/2,y,z. At the same time, the points x,1-y,z and 1-x,1-y,z coalesce to the single point 1/2,1-y,z (Fig. 10.11a, b). From the 4-fold general position, we have obtained a 2-fold special position. The multiplicity of a special position is always an integral factor of the multiplicity of the general position. Special positions are not asymmetric; they possess site symmetry higher than 1, and in Fig. 10.11b, the site symmetry is m. 10.3 Properties of Space Groups D A special position is a set of equivalent points arising from the merging of equivalent positions. It has point symmetry (site symmetry) higher than 1. This particular special position has two degrees of freedom. As long as the point remains on the mirror plane, its multiplicity is unchanged. Other similar special positions arise from the mirror planes at x,0,z; x,1/2,z and 0,y,z. If a point on 1/2,y,z moves onto the 2-fold axis at 1/2,1/2,z the two points 1/2,y,z and 1/ ,1-y,z coalesce to 1/ ,1/ ,z. This special position retains only a single degree of free2 2 2 dom. The point symmetry of the position rises to mm2, and the multiplicity falls to 1. The positions 0,0,z; 1/2,0,z and 0,1/2,z are similar to 1/2,1/2,z. Some space groups have special positions with no degrees of freedom, and important case of this being a point on an inversion center (see Table 10.4). The general and special positions in space group Pmm2 are set out in Table 10.3. Table 10.3 Positions of the space group Pmm2 Position Degrees of freedom Multiplicity General 3 4 1 x,y,z; x̄,ȳ,z; x,ȳ,z; x̄,y,z 10.11a 2 m 1 1 2 ,y,z; 2 ,ȳ,z 10.11b 2 m 0,y,z; 0,ȳ,z 2 m x, 12 ,z; x̄, 21 ,z 2 m x,0,z; x̄,0,z 1 mm2 1 1 2 , 2 ,z 1 mm2 1 2 ,0,z 1 mm2 0, 21 ,z 1 mm2 0,0,z 2 Special 1 Site symmetry Coordinates of equivalent points Figure 10.11c Another space group in point group mm2 is Pna21 , shown in Fig. 10.12. The space group symbol indicates that the unit cell is orthorhombic, with n-glide planes c|, a-glides normal to the b-axis, normal to the a-axis with a glide component 1/2|b+ and 21 -screw axes parallel to the c-axis. The general position, x,y,z, as shown in Fig. 10.12, is again 4-fold. When, however, the point moves onto the a-glide at x,1/4,z, the multiplicity is unchanged. A special position does not arise, since glide planes and screw axes do not alter the multiplicity of a point. As a result, the space group Pna21 has no special positions. Figure 10.13 shows the projection of the space group P2/m on x,y,0. In addition to the general position, there are special positions with m, 2 and 2/m site symmetry. Table 10.4 shows these points, and gives the degrees of freedom, the multiplicities, and the site symmetries of each type of position. Note that as the site symmetry rises, the multiplicity falls. 203 204 10 Space Groups Fig. 10.12 Symmetry elements of the space group Pna21 in projection on x,y,0 showing the general position x,y,z (1). Even if a point lies on the a-glide plane at x,1/4,z (1 ), this does not reduce its multiplicity. Glide planes and screw axes, unlike point-symmetry elements, do not reduce the multiplicity of a position which lies on them Fig. 10.13 Space group P2/m shown in projection on x,y,0 with the general position x,y,z and the special positions on m, 2 and 2/m D The asymmetric unit of a space group is the smallest part of the unit cell from which the whole cell may be ﬁlled exactly by the operation of all the symmetry operations. Its volume is given by: Vasym.unit = Vunitcell multiplicity of the general position It has the property that no two points within it are related to one another by a symmetry operation, cf. the asymmetric face unit of a point group in Sect. 9.2.1. 10.3 Properties of Space Groups Table 10.4 Positions of the space group P2/m General Special Degrees of freedom -––––––––––––––––––––- Position Multiplicity Site symmetry Coordinates of equivalent points 3 4 1 x,y,z x,1-y,z 1-x,y,1-z 1-x,1-y,1-z 2 2 m x, 21 ,z 1-x, 21 ,1-z 1 2 2 1 1 2 ,y, 2 1 1 2 ,1-y, 2 0 1 2/m 1 1 1 2,2,2 Fig. 10.14a–c. a Operation of a 61 -screw axis at 0,0,z on a point in a general site x,y,z. b Displacement of the points originated in a by lattice translation into the unit cell(general position). c Space group P61 205 206 10 Space Groups An asymmetric unit of the space group P2/m is the volume limited by 0≤x≤ 12 ; 0≤y≤ 12 ; 0≤z≤1. Its volume is one quarter of that of the unit cell, so the equation above is fulﬁlled, as the multiplicity of the general position is 4. The tetragonal space group P42 /mnm will be described in Sect. 10.4, International Tables for Crystallography. The general position in the hexagonal space group P61 is illustrated in Fig. 10.14. Figure 10.14a shows the operation of a 61 -axis at 0,0,z on an asymmetrical point x,y,z. The coordinate for each generated equivalent point are easily determined. With diﬀerent z-values, these x- and y-coordinates will also arise from 6, 6̄, 62 , 63 , 64 , 65 , 3, 3̄, 31 , 32 -operations. In Fig. 10.14b, the equivalent points of 10.14a have been shifted to a single unit cell by lattice translations. From this arrangement of the points, the 21 at 1/2,1/2,z and the 31 at 23 , 13 ,z and 1 2 3 , 3 ,z are clearly shown. The symmetry elements of P61 are given in Fig. 10.14c. We shall now consider, as an example of the cubic system, the space group P4/m3̄2/m. This is the space group of the cubic P-lattice, which has already been introduced in Fig. 7.13d. That diagram of the space group P4/m3̄2/m is incomplete. It was, however, adequate for the introduction of symmetry relationships, and is Fig. 10.15 Space group P4/m3̄2/m [6], [14] projection on x,y,0 10.3 Properties of Space Groups also entirely suitable for the application of this space group, as we shall see later. M. J. Buerger [8] developed projections of the cubic space groups which have been included in the third edition of the International Tables [16]. Figure 10.15 shows such a projection on x,y,0 of the space group P4/m 3̄ 2/m. In order to include those symmetry elements which are parallel to < 110 > and < 111 > in the diagram, Buerger used an orthographic projection (see Sect. 5.8), and representations of the oblique rotation- and screw-axes. In order to understand the relationship of the various symmetry elements, it is useful to study Figs. 10.15 and 7.13d, to see that they are representations of the same thing. Even for so complex a space group as P4/m3̄2/m, it is relatively easy to describe a general position. Figure 10.16 a shows a section of a cubic unit cell. A 3-fold rotation axis lies along the body-diagonal of the unit cell x,x,x, but it is not shown here. Fig. 10.16a–d The 48-fold general position of space group P4/m3̄2/m. (a) Section of a unit cell showing the operation of the 3-fold rotation axis at x,x,x (not drawn) on a general point x,y,z with x = 0.3, y = 0.2, z = 0.1. (b) Projection of the equivalent points in a on x,y,0. (c) The operation of the mirror plane at x,x,z on the points in b generates six equivalent points in a planar, 6-membered ring. (d) The operations of the 4-fold axis at 0,0,z and the mirror plane at x,y,0 on the points in c complete the full set of 48 equivalent points of the general position. Only those points lying above the plane of the paper are shown. The rest may be generated by giving a minus sign to the third co-ordinate of each triple 207 208 10 Space Groups Fig. 10.16a–d (Continued) Starting from a point x,y,z (x = 0.3, y = 0.2, z = 0.1), the operation of the 3-fold axis generates the points z,x,y and y,z,x (Fig. 10.16a). Figure 10.16b shows the projection of these three points on x,y,0. The application of the mirror plane at x,x,z to these points converts them to a set of six points in a planar ring (Fig. 10.16c). The further application of the 4-fold axis at 0,0,z converts this ring to a set of four rings (Fig. 10.16d). Finally, the mirror plane at x,y,0 reﬂects these rings downwards and produces the full set of points for this 48-fold position. The coordinates of all 48 of these points are given in Fig. 10.16d, if each triple is taken to imply one with a minus sign on the third-co-ordinate as well. These 48 equivalent points are generated entirely by the symmetry of 4/m3̄m! There is a simple relationship between the number of faces in the general form of a crystal of a particular point group and the multiplicity of the general position of a space group in that point group (cf. Table 10.2). For space groups with a Plattice, the multiplicity of the general position is equal to the number of faces in the general form for the point group. For space groups with C-, A- and I-lattices, the multiplicity of the general position is twice as great as the number of faces, and for those with an F-lattice four times. The general form of the point group mm2 is the rhombic pyramid (cf. Exercise 9.15(5)) with four faces. The multiplicity of the general position in Pmm2 (Fig. 10.11a) or Pna21 (Fig. 10.12) is 4, while for Cmm2, Aba2, Imm2 or Ima2 it is 8, and for Fmm2, it is 16. If the point group includes an inversion center, all the corresponding space groups will be centrosymmetric, cf. the monoclinic space groups in Fig. 10.9a. Consider now the space group P42 /n 21 /c 2/m. Removing the lattice symbol and converting all glide planes and screw axes to the corresponding point symmetry elements (42 → 4; 21 → 2; n, c → m) gives the point group of this space group: 4/m 2/m 2/m. 10.3 Properties of Space Groups Fig. 10.17 Space group P42 /mnm, from International Tables for Crystallography, Vol. A. [16] 209 210 10 Space Groups 10.4 International Tables for Crystallography Many of the most important properties of the 230 space groups are collected in International Tables for Crystallography, Vol A. [16]. These tables are exceedingly useful. The information they contain may be illustrated with respect to the space group P42 /mnm (Fig. 10.17). (1) Short space group symbol, Schönﬂies symbol, point group, crystal system, number of the space group, full space group symbol. (2) Projection of the symmetry elements of the space group on x,y,0; a points down the page, b across to the right, and the origin is in the upper left corner. (3) Projection of a general position on x,y,0; the axial directions are as in (2), represents an asymmetric point. represents a point that is related to it by rotoinversion (1̄, 2̄ ≡ m, 3̄, 4̄, or 6̄); they are thus enantiomorphs of each other. represents a point projecting on top of another, while implies that one of the points is derived from the other by rotoinversion, in this case reﬂection in the mirror plane at x,y,0. The z-coordinate is indicated thus: + = z, – = z̄, 1/ + = 1/ + z, 1/ – = 1/ – z. 2 2 2 2 (4) Information about the choice of origin, here at an inversion center at the intersection of three mutually perpendicular mirror planes. Since this is a tetragonal space group, the symbols 2/m 1 2/m imply the symmetry directions, c, < a >, < 110 >. (5) The asymmetric unit: Vasym.unit = V unit cell (cf.Eq.10.3) multiplicity of the general position (6) The symmetry operations of the space group. They are numbered, here 1 – 16. Examples: • (3) 4+ is on the line 0,1/2,z, with the screw translation in parentheses: (0,0,1/2) = 1/2 c. It is thus a 42 -screw axis. The plus sign indicates that it is in the mathematically positive or right handed sense, as in Fig. 10.5. • (5) 2 is a 21 -screw axis on 1/4,y,1/4 with |s| = (0,1/2,0) = 1/2 |b|. 1 • (12) 4̄- is a 4-fold rotoinversion axis on 0, /2,z with an inversion center at 0,1/2,1/4. In this case, the minus sign adjacent to the 4̄ indicates that the screw sense is negative, i.e. left-handed. • (14) n is an n-glide plane at 1/4,y,z, with a glide translation of (0,1/2,1/2), = 1/ (|b| + |c|). 2 (7) General and special positions. Col. 1: the multiplicity of the position. Col. 2: the Wyckoﬀ letter assigned to this position; the letter furthest down the alphabet, here k, represents the general position. 10.5 Space Group and Crystal Structure Col. 3: the site symmetry (point symmetry of the position), in the order c, < a >, < 110 >. Col. 4: the coordinates of equivalent points in the position. 10.5 Space Group and Crystal Structure In Chap. 3, we deﬁned a crystal structure as lattice + basis. It is thus possible to describe it as a geometrical arrangement of atoms. Table 10.5 A gives the lattice and the basis for the rutile (TiO2 ) structure. The perspective drawing and the projection on x,y,0 in Fig. 10.18 are derived from these data. Every crystal structure can be similarly described by its space group and the occupation of general or special positions by atoms. The crystal structure of rutile is in space group P42 /mnm. The titanium atoms occupy the position a, and the oxygen atoms the position f with x = 0.3 (cf. the page of International Tables in Fig. 10.17). Table 10.5 Description of the crystal structure of rutile TiO2 A Lattice Tetragonal P a0 = 4.59 Å c0 = 2.96 Å B Basis Space group Ti: 0,0,0 P42 /mnm 1 1 1 2,2,2 –––––––––––– O: 0.3, 0.3, 0 a0 = 4.59 Å 0.8, 0.2, 12 c0 = 2.96 Å 0.2, 0.8, 12 0.7, 0.7, 0 Positions of the atoms a Ti: 0,0,0 1 1 1 2,2,2 ––––––––––––––––––– f O: x,x,0 1 1 1 2 +x, 2 −x, 2 1 1 1 x = 0.3 2 −x, 2 +x, 2 x̄,x̄,0 Fig. 10.18a,b The crystal structure of rutile, TiO2 , shown: (a) in a perspective drawing, (b) in projection on x,y,0 211 212 10 Space Groups The special position a is 2-fold, implying 0,0,0 and 1/2,1/2,1/2, f is 4-fold: x,x,0; 1/2+x, 1/ –x,1/ ; 1/ –x,1/ +x,1/ and x̄,x̄,0 (Table 10.5B). 0,0,0 and x,x,0 (x = 0.3) lie in a single 2 2 2 2 2 asymmetric unit of space group P42 /mnm, cf. Fig. 10.17. Substituting 0.3 for x in the coordinates for the O-atoms gives the speciﬁc coordinates listed for the basis in Table 10.5 A. The description of a crystal structure in terms of the space group is much simpler than that in terms of the basis when positions of high multiplicity are involved. In addition, the space group shows clearly which atoms are related to one another by the symmetry elements of the space group. This relationship is particularly important for positions with one or more degrees of freedom. Any movement in x (cf. position f in Fig. 10.17) alters the relationship of all the related atoms; for example, an increase of x results in the movement of the O-atoms indicated by the arrows in Fig. 10.18b. 10.6 Relationships Between Point Groups and Space Groups As is shown in Table 10.2, there is a fundamental relationship between the point groups of morphology and the space groups of crystal structure. In any crystal, the only crystal forms which can appear are those of its point group, and this may be derived from the space group of its crystal structure. For example, the rutile structure has the space group P42 /mnm, and consequently the point group 4/mmm. The only possible forms for this point group are those given in Fig. 9.7. The crystal illustrated in Table 9.11.15 thus shows only the forms {111}, {110}, and {100}. There are only a few exceptions to this correspondence between point groups and space groups, and these deviations can be traced back to adsorption eﬀects during crystal growth. Table 10.6 gives further relationships between point groups and space groups. Molecules may also be assigned a point group, and one may ask what part this plays when similar molecules group together in crystal growth. What relationship is there between the point group of the molecule and the space group of the crystal? Hexamethylenetetramine has the point group 4̄3m (Fig. 10.19a). In its crystal structure (Fig. 10.19b), with space group I4̄3m, the molecules occupy sites with point symmetry 4̄3m, giving a perfect correspondence. It must be emphasized, however, that this is far from a general rule! Ethylene, with point group 2/m2/m2/m, (mmm), Fig. 10.20a, crystallizes in space group P21 /n21 /n2/m (Pnnm), Fig. 10.20b, with its center of gravity occupying a point with point symmetry only 2/m. Similarly, benzene, Fig. 10.21a, with the very high point symmetry 6/mmm, crystallizes in the orthorhombic space group Pbca, Fig. 10.21b. In this case, the center of gravity of the molecule is on a site of only 1̄ symmetry. Again, the molecular symmetry is much higher than its site symmetry in the crystal. 10.6 Relationships Between Point Groups and Space Groups Table 10.6 Correspondence of point groups and space groups Point groups: A group of point symmetry operations, whose operation leaves at least one point unaltered. Any operation involving lattice translations is thus excluded 1 2 3 4 6 1̄ m 3̄ 4̄ 6̄ a, b, c α, β, γ Space groups: A group of symmetry operations which include lattice translations 1 2 3 4 6 1̄ m 3̄ 4̄ 6̄ 21 ; a, b, c, n, e, d 31 , 32 41 , 42 , 43 61 , 62 , 63 , 64 , 65 lattice translations a0 , b0 , c0 α, β, γ Order of the symmetry operations e.g. 4/m 2/m 2/m | | | c < a > < 110 > Order of the symmetry operations 2/m 2/m e.g. P42 /m | | | c < a > < 110 > General form: Set of equivalent faces each with face symmetry 1 General position: Set of equivalent points each with site symmetry 1 fasymmetric face unit = fsphere multiplicity of general form Vasymmetric unit = Vunit cell multiplicity of general point Multiplicity of general form of the point group Multiplicity of the general position in all space groups with a P-lattice that are isomorphous with that point group Special form: Set of equivalent faces each with face symmetry >1 Special position: Set of equivalent points each with site symmetry >1 Fig. 10.19a,b Symmetry of hexamethylenetetramine (C6 H12 N4 ). (a) molecule: 4̄3m. (b) crystal structure: I 4̄3m. (After[2]) 213 214 10 Space Groups Fig. 10.20a,b Symmetry of ethylene (C2 H4 ). (a) Molecule: 2/m 2/m 2/m (b) Crystal structure P21 /n 21 /n 2/m Fig. 10.21a,b Symmetry of benzene (C6 H6 ). (a) Molecule:6/mmm. (b) Crystal structure:Pbca The sulfur molecule, S8 , Table 9.12.3, with the non-crystallographic point symmetry 8̄2m (D4d ), crystallises in the orthorhomic space group Fddd with site symmetry 2. It will thus be seen that there is no general relationship between molecular and crystal symmetry, except that a molecule cannot occupy a site of higher symmetry than its molecular point group unless the structure is disordered. The actual crystal structure that occurs depends mainly on the packing of the molecules and the intermolecular interactions that are possible. 10.7 Exercises 10.7 Exercises Exercise 10.1 For the two-dimensional “Kockel” structures given below, indicate: (a) The unit mesh. (b) The symmetry elements, paying particular attention to glide planes. 215 216 10 Space Groups Exercise 10.2 Glide planes and screw axes. In the projections below of a unit cell onto x,y,0, only a single symmetry element is given. Allow this symmetry element ot operate on an asymmetric point (in a general site) at x,y,z and give the coordinates of the equivalent point(s) generated. 10.7 Exercises j) i) 0 k) 21 in 1 , 0, z 2 2 in 1 , y , 0 4 l) 1 4 1 4 2 in 1 , 1 , z 4 4 21 in 0 , y , 1 4 m) n) 41 in 0 , 0 , z 31 in 0 , 0 , z Exercise 10.2 (Continued) Exercise 10.3 The ﬁgures show the operation of a glide plane and a 21 -axis on a point. The arrangement of the points appears to be the same in the two diagrams. Discuss this apparent contradiction. 217 218 10 Space Groups Exercise 10.4 Show that (a) C21 /c ≡ C2/c, (b) C21 /m ≡ C2/m, and (c) C21 ≡ C2. Start from the projections of the space groups (a) P21 /c, (b) P21 /m and (c) P21 as given in Fig. 10.9. Place a point at x,y,z and another at 12 +x, 12 +y,z (Ccentering), and allow the symmetry elements to operate on them. This will give the general positions for: (a) C21 /c, (b) C21 /m and (c) C21 . Using these general positions, the complete symmetry of the space groups can be determined. Using Fig. 10.9, show the correspondence of (a) C21 /c with C2/c, (b) C21 /m with C2/m, and (c) C21 with C2, moving the origin of the diagram as necessary. Exercise 10.5 Determine the symmetry of the orthorhombic C-and I-lattices. Indicate the symmetry elements on a projection of the lattice onto x,y,0, and give the space group symbol. Exercise 10.6 Draw the symmetry diagram of space group Pmm2 on a piece of graph paper. Enter points in the general positions 0.1,0.1,0.1; 0.1,0.4,0.1; 0.25,0.25,0.1; and 0.4,0.4,0.1 and those points resulting from the operation of the symmetry elements on them. Exercise 10.7 The symmetry diagrams for seven space groups are given below as projections on x,y,0. (a) Enter on each diagram a point in a general site x,y,z, and allow the symmetry to operate on it. (b) Give the coordinates of the points equivalent to x,y,z. (c) What is the multiplicity of the general position? (d) Work out the space group symbol. (The graphical symbols for symmetry elements are given in Sect. 15.2). (e) Indicate a special position – if there are any – and give its multiplicity. 10.7 Exercises Exercise 10.7 (Continued) 219 220 10 Space Groups Exercise 10.7 (Continued) Exercise 10.8 Make a tracing of the projection of a hexagonal unit cell on x,y,0 (Fig. 10.14) and place at 0,0,z (a) a 62 -axis, (b) a 63 -axis. 1. Allow the symmetry elements to operate on a point in a general site, and give the coordinates of the resulting equivalent points. 2. Draw in the other symmetry elements of the space group in the unit cell. 3. Which symmetry elements are contained within 62 and 63 ? Exercise 10.9 Consider the space group P4/m 3̄ 2/m (Fig. 10.15 and 10.16). In a projection on x,y,0, draw in the special positions (a) x,x,z, (b) x,x,x, (c) x,0,0. Give the coordinates of the equivalent points and the multiplicities and site symmetry of the positions. 10.7 Exercises Exercise 10.10 Draw a representation of the general position for the space group P 2/m3̄. Note that P 2/m 3̄ is a sub group of P 4/m3̄ 2/m. Start from Fig. 10.16, noting that 3̄ contains the 1̄ that lies at 0,0,0. From that, the orientation of the 2 and the m may be seen. Exercise 10.11 Draw several projections of a tetragonal unit cell on x,y,0. Show each of the 16 symmetry operations of the space group P42 /mnm [Fig. 10.17(6)], let each of them operate on a point x,y,z, and give the coordinates of the generated points. Exercise 10.12 In a projection, draw in the symmetry elements of each of the following space groups: P21 /c, Pna21 , Pmna, Pbca, and P422. Exercise 10.13 Criticize the symbol Pabc. Exercise 10.14 For each of the following space groups: P1̄ (Fig. 7.7d), Pm and P2/m (Fig. 10.9) and P2/m2/m2/m (Fig. 7.9d), consider an atom A at 0,0,0 and an atom B at a general position (x,y,z < 1/4). (a) (b) (c) (d) (e) Give the chemical formula for the resulting structure. What is the value of Z (the number of “molecules” per unit cell)? Describe the shape of the resulting molecule. Determine the point symmetry of the molecule. Determine the actual point symmetry of that point in the unit cell. 221 11 Symmetry Groups In our discussion of point and space groups, the related sub- and supergroups were mentioned without establishing that all of these are true groups in the mathematical sense. In order to show this, we will begin by showing how symmetry operations can be represented by matrices and vectors. 11.1 Representation of Symmetry Operations by Matrices We will start with the symmetry operations of point groups, leaving such operations as glide planes, screw axes and translations until later. The orientation of symmetry elements will ﬁrst be described in terms of the crystallographic axes a,b,c, or a directional vector [uvw], since these are relatively easy for a beginner to understand. For example, 4c represents a 4-fold rotation axis parallel to c, while m[110] is a mirror plane normal to the [110]-direction. The symbols used in International Tables for Crystallography [16] will be also given. Consider a 3-fold rotation axis in the c-direction as an example. Figure 11.1 c of the co-ordinate system shows this rotation axis and the lattice vectors a,b, in a stereographic projection. This rotation axis in fact comprises two symmetry Fig. 11.1 Transformation of the c into coordinate system a, b, a , b , c by the operation of the 3-fold axis 31c and into a , b , c by 32c , shown in a stereographic projection. These operations also convert (hkl) into (ihl) and (kil) a′′ b′ –a – b ihl kil b a′ hkl a b′′ W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_11, C Springer-Verlag Berlin Heidelberg 2011 224 11 Symmetry Groups operations, the 3-fold axes 31c and 32c , taken in the mathematically positive, or counterclockwise direction. The rotation 32c implies two successive operations of 31c . 31c may be written 3+ 0,0,z and 32c as 3– 0,0,z, where 3– 0,0,z implies a mathematically negative or clockwise rotation. the vector b into • 31c (3+ 0,0,z) transforms the vector a into the vector a = b, b = –a – b, and the vector c into c =c. This may be written: a = 0 · a + 1 · b + 0 · c (11.1) b = −1 · a − 1 · b + 0 · c (11.2) c = 0 · a + 0 · b + 1 · c (11.3) These equations may be summarized as follows in matrix-vector terminology: ⎞ 0 1̄ 0 c) · (M) c) · ⎝ 1 1̄ 0 ⎠ = (a, b, (a , b , c ) = (a, b, 001 ⎛ (11.4) The coeﬃcients of the three equations thus become the columns of the matrix (M). A minus-sign is written above the number to which it refers as in crystallographic triples. the vector b into • 32c (3– 0,0,z) transforms the vector a into the vector a = –a –b, b = a, and the vector c into c =c. This gives a second matrix: ⎛ ⎞ 1̄ 1 0 ⎝ 1̄ 0 0 ⎠ 001 (11.5) The two matrices are the inverses of each other, so their multiplication gives the unit matrix (E). ⎞ ⎛ ⎞ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ ⎛ 100 0 1̄ 0 0 1̄ 0 1̄ 1 0 1̄ 1 0 ⎝ 1 1̄ 0 ⎠ · ⎝ 1̄ 0 0 ⎠ = ⎝ 1̄ 0 0 ⎠ · ⎝ 1 1̄ 0 ⎠ = ⎝ 0 1 0 ⎠ (11.6) 001 001 001 001 001 or (M) · (M)−1 = (M)−1 · (M) = (E) (11.7) Let us now make the symmetry operations 31c and 32c operate on a point with coordinates x,y,z. • 31c (3+ 0,0,z) transforms the point x,y,z into the point ȳ,x – y,z. If the coordinates are given as a column vector, the following equation is obtained: ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ x 0 1̄ 0 x 0·x−1·y+0·z −y (M) · ⎝ y ⎠ = ⎝ 1 1̄ 0 ⎠ · ⎝ y ⎠ = ⎝ 1 · x − 1 · y + 0 · z ⎠ = ⎝ x − y ⎠ → ȳ, x − y, z z 001 z 0·x+0·y+1·z z (11.8) 11.1 Representation of Symmetry Operations by Matrices • 32c (3– 0,0,z) transforms the point x,y,z into the point y – x,x̄,z, or, in matrix notation: ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ x −x + y 1̄ 1 0 ⎝ 1̄ 0 0 ⎠ · ⎝ y ⎠ = ⎝ −x ⎠ → y − x, x̄, z (11.9) z z 001 Note that the column vector is placed to the right of the matrix. In Fig. 11.2, the three points have been drawn in a hexagonal coordinate system. They represent the general positions of point group 3. Fig. 11.2 Operation of the axes 31c and 32c on a point x,y,z Similarly, the indices of the planes which are equivalent to the plane (hkl) by the 3-fold rotations 31c and 32c can be calculated using the matrices (M) and (M)–1 . It is important to notice that the matrices (M) and (M)–1 now reverse their roles: (M)–1 describes the counterclockwise rotation of (hkl), while (M) describes its clockwise rotation. • 31c (3+ 0,0,z) : ⎛ ⎞ 1̄ 1 0 (hkl) · (M)−1 = (hkl) · ⎝ 1̄ 0 0 ⎠ 001 = (h · 1̄ + k · 1̄ + 1 · 0, h · l + k · 0 + l · 0, h · 0 + k · 0 + l · 1) = (−h − k, h, l) → (h̄ + k̄hl) = (ihl) (11.10) 2 – • 3c (3 0,0,z) : ⎞ ⎛ 0 1̄ 0 (hkl) · (M−1 ) = (hkl) · ⎝ 1 1̄ 0 ⎠ 001 = (h · 0 + k · 1 + l · 0, h · 1̄ + k · 1̄ + l · 0, h · 0 + k · 0 + l · 1) = (k, − h − k, l) → (kh̄ + k̄l) = (kil) (11.11) Note that the row vector is placed to the left of the matrix. 225 226 11 Symmetry Groups The poles of the three planes, constituting the trigonal pyramidal form, are drawn in Fig. 11.1, which may be compared with Fig. 9.13. In Chap. 6 (Principles of Symmetry) it was shown that only 10 distinct symmetry operations are possible for crystallographic point groups. This number, however, increases to 64, if the possible orientations of the symmetry elements to the crystallographic axes and the full set of operations implied by rotation and rotoinversion axes are counted. These 64 cases are given in Table 11.1. The ﬁrst column enumerates the operations, and the second gives their symbols. The direction of a rotation or rotoinversion axis or that of the normal to a mirror plane is given by the appropriate crystallographic axis a, b or c, or by a direction symbol [uvw]. The third column gives this symbol as it is represented in International Tables for Crystallography (I.T.) [16]. If a symmetry element implies further operations, these are given sequentially. For a rotation axis, the ﬁrst is always the one implying a counterclockwise rotation; for a rotoinversion axis, it is the one including a counterclockwise rotation. In the I.T. notation, these always have an index of 1 or a +-sign. The index π indicates that the ﬁrst operation is applied π times. The last operation in this set is that which is opposite to the ﬁrst. For a 4-fold axis parallel to c, these will be: 41c or 4+ 0,0,z (no. 49), 42c ≡ 2c or 2 0,0,z (no. 7), and 43c or 4– 0,0,z (no. 50). The operation of one symmetry operation after another is represented by the product of their matrices. The operation performed ﬁrst is placed to the right: ⎛ 0 ⎝1 0 ⎛ 0 ⎝1 0 ⎛ 0 ⎝1 0 · 41c = 42c ≡ 2c ⎞ ⎛ ⎞ ⎛ ⎞ 1̄ 0 0 1̄ 0 0 1̄ 0 0 0 ⎠ · ⎝ 1 0 0 ⎠ = ⎝ 0 1̄ 0 ⎠ 01 001 001 (11.12) · 42c = 43c ⎞ ⎛ ⎞ ⎛ ⎞ 010 1̄ 0 0 1̄ 0 0 0 ⎠ · ⎝ 0 1̄ 0 ⎠ = ⎝ 1̄ 0 0 ⎠ 01 001 001 (11.13) · 43c = 44c ≡ 1 ⎞ ⎞ ⎛ ⎞ ⎛ 010 100 1̄ 0 0 0 ⎠ · ⎝ 1̄ 0 0 ⎠ = ⎝ 0 1 0 ⎠ 001 01 001 (11.14) 41c 41c 41c The fourth column gives the crystal systems in which this operation is possible (a = triclinic (anorthic), m = monoclinic, o = orthorhombic, t = tetragonal, h = hexagonal, r = rhombohedral, and c = cubic). The matrix representation (M) of the element is given in the ﬁfth column. In the sixth column are given the coordinates into which x,y,z is converted by the given operation. The seventh column contains the inverse matrices (M)–1 . The ﬁnal column gives the indices of the plane into which (hkl) is converted by the operation. 11.1 Representation of Symmetry Operations by Matrices Symmetry operation Nr. I.T. 1 1 1 2 1 1 3 2a Crystal systems Table 11.1 Matrices and inverse matrices for the point symmetry operations; the coordinates of the points to which they convert x,y,z; and the Miller indices of the planes to which they convert (hkl) ( hkl) . (M) − 1 (M) . 100 010 001 x,y,z hkl c 100 0 10 00 1 x,y,z hkl o t c 100 0 10 00 1 x,y,z h kl 1 10 0 10 00 1 x − y,y,z hh + kl 100 010 00 1 x,y,z hkl 100 110 00 1 x,y − x,z 100 0 10 001 x,y,z hkl a (M) − 1 2 x,0,0 4 h 5 2b x y z (M) 2 0,y,0 6 m o t c h = ( M) h + kkl 7 2c 2 0,0,z m o t h c 8 2[ 110] 2 x,x,0 t h c 010 100 00 1 y,x,z khl 0 10 100 00 1 y,x,z khl 9 2[ 110] 2 x,x,0 t r h c 10 2[ 101] 2 x,0,x c 001 0 10 100 z,y,x lkh 11 2[ 101] 2 x,0,x r c 00 1 0 10 100 z,y,x lkh 227 11 Symmetry Groups Table 11.1 (Continued) Crystal systems 228 (M) 12 2[ 011] 2 0,x,x c 100 001 010 x,z,y hlk 13 2[ 011] 2 0,x,x r c 100 00 1 0 10 x,z,y hlk 14 2[ 210] 2 2x,x,0 100 1 10 00 1 x,x − y,z h + kkl 110 010 00 1 y − x,y,z hh + kl Symmetry operation Nr. I.T. h 15 2[ 120] 16 2 x,2x,0 18 (M) − 1 (hkl) . (M) − 1 o t c 100 010 001 x,y,z hkl m x,2x,z h 110 010 001 y − x,y,z hh + kl m x,0,z m o t c 100 0 10 001 x,y,z hkl m 2x,x,z h 100 1 10 001 x,x − y,z h + kkl mb 19 x y z m 0,y,z ma 17 (M) . = ( M) 20 mc m x,y,0 m o t h c 100 010 00 1 x,y,z hkl 21 m[ 110] m x,x,z t h c 0 10 100 001 y,x,z khl 22 m[ 110] m x,x,z t r h c 010 100 001 y,x,z khl 23 m[ 101] m x,y,x c 00 1 010 100 z,y,x lkh 11.1 Representation of Symmetry Operations by Matrices Crystal systems Table 11.1 (Continued) (M) 24 m[101] m x,y,x r c 001 010 100 z,y,x lkh 25 m[011] m x,y,y c 100 001 010 x,z,y hlk 26 m[011] m x,y,y r c 100 001 010 x,z,y 27 m[210] m 0,y,z 100 110 001 x,y − x,z h + kkl 28 m[120] m x,0,z 110 010 001 x − y,y,z hh + kl 29 31c 3+ 0,0,z 010 110 001 y,x − y,z 110 100 001 h + khl 30 32c 3− 0,0,z 110 100 001 y − x,x,z 010 110 001 kh + kl 31 31[111] 3+ x,x,x 001 100 010 z,x,y 010 001 100 lhk Symmetry operation Nr. I.T. h r c x (M) . y z (M)− 1 = ( M) ( hkl) . (M)−1 hlk 32 32[111] 3− x,x,x 010 001 100 y,z,x 001 100 010 klh 33 31[111] 3+ x,x,x 001 100 010 z,x,y 010 001 100 lhk 34 32[111] 3− x,x,x 010 001 100 y,z,x 001 100 010 klh c 35 31[111] 3+ x,x,x 001 100 010 z,x,y 010 001 100 lhk 36 32[111] 3− x,x,x 010 001 010 y,z,x 001 100 010 klh 229 11 Symmetry Groups Table 11.1 (Continued) Symmetry operation Nr. 37 I.T. 3[1111] Crystal systems 230 3+ x,x,x c x y z (M) (M) . 00 1 100 0 10 z,x,y 010 00 1 100 lhk (M) − 1 (hkl) . (M) − 1 38 3[2111] 3− x,x,x 010 00 1 100 y,z,x 00 1 100 0 10 klh 39 3c1 3+ 0,0,z 010 110 00 1 y,y − x,z 1 10 100 00 1 h + khl (30) 3c2 3c2 (2) 3c3 1 (29) 3c4 3c1 40 3c5 3− 0,0,z 1 10 100 00 1 x − y,x,z 010 110 00 1 kh + kl 41 3[1111] 3+ x,x,x 00 1 100 0 10 z,x,y 0 10 00 1 100 lhk (32) 3[2 111] 3[2 111] (2) 3[3 111] 1 (31) 3[4 111] 3[1 111] 42 3[5111] 3− x,x,x 0 10 00 1 100 y,z,x 00 1 100 0 10 klh 43 3[1111] 3+ x,x,x 001 100 0 10 z,x,y 010 00 1 100 lhk (34) 32 32 (2) 33 1 (33) 34 31 44 3[5111] 010 00 1 100 y,z,x 001 100 0 10 klh [ 111] [ 111] [ 111] 3− 0,0,z 1 h 3+ 0,0,z 3− x,x,x 1 [ 111] 3+ x,x,x 3− x,x,x 1 [ 111] r c c 3+ x,x,x 3− x,x,x 11.1 Representation of Symmetry Operations by Matrices Symmetry operation Nr. I.T. 45 31[111] (36) 32[ 111] 32[ 111] (2) 33 1 (35) 34[ 111] 31[ 111] 46 35[111] [ 111] Crystal systems Table 11.1 (Continued) 3+ x,x,x x y z (hkl) . (M)− 1 (M) (M) . 001 100 010 z,x,y 010 001 100 lhk 010 001 100 y,z,x 001 100 010 klh 001 100 010 z,x,y 010 001 100 lhk (M) − 1 3− x,x,x 1 3+ x,x,x 3− x,x,x c 47 31[111] (38) 32[ 111] 32[ 111] (2) 33[ 111] 1 (37) 34[ 111] 31[ 111] 48 35[ 111] 3− x,x,x 010 001 100 y,z,x 001 100 010 klh 49 41c 4+ 0,0,z 010 100 001 y,x,z 010 100 001 khl (7) 42c 50 43c 4− 0,0,z 010 100 001 y,x,z 010 100 001 khl 51 41a 4+ x,0,0 100 001 010 x,z,y 100 001 010 hlk (3) 42a 52 43a 100 001 010 x,z,y 100 001 010 hlk 2c 2a 3+ x,x,x 3− x,x,x 1 3+ x,x,x 2 0,0,z 2 x,0,0 4− x,0,0 t c c 231 11 Symmetry Groups Table 11.1 (Continued) Symmetry operation Nr. I.T. Crystal systems 232 4+ 0,y,0 (M) (M) . 001 010 100 x y z (M) − 1 ( hkl) . (M)− 1 z,y,x 001 010 100 lkh 53 41b (5) 42b 54 43b 4− 0,y,0 001 010 100 z,y,x 001 010 100 lkh 55 41c 4+ 0,0,z 010 100 001 y,x,z 010 100 001 khl (7) 42c 56 43c 4− 0,0,z 010 100 001 y,x,z 010 100 001 khl 57 41a 4+ x,0,0 100 001 010 x,z,y 100 001 010 hlk (3) 42a 58 43a 100 001 010 x,z,y 100 001 010 hlk 001 010 100 z,y,x 001 010 100 lkh 001 010 100 z,y,x 001 010 100 lkh 2b 2c 2a 2 0,y,0 2 0,0,z c t c 2 x,0,0 4− x,0,0 c 59 41b (5) 42b 60 43b 4+ 0,y,0 2b 2 0,y,0 4− 0,y,0 11.1 Representation of Symmetry Operations by Matrices Symmetry operation Nr. I.T. Crystal systems Table 11.1 (Continued) 6+ 0,0,z (M) (M) . 110 100 001 x y z (M) − 1 (hkl) . (M) − 1 x − y,x,z 010 110 001 kh + kl 61 61c (29) 62c 31c 3+ 0,0,z (7) 63c 2c 2 0,0,z (30) 64c 32c − 62 65c 6− 0,0,z 010 110 001 y,y − x,z 110 100 001 h + khl 63 61c 6+ 0,0,z 110 100 001 y − x,x,z 010 110 001 kh + kl (29) 62c 31c 3+ 0,0,z (20) 63c mc m x,y,0 (30) 64c 32c 3− 0,0,z 64 65c 010 110 001 y,x − y,z 110 100 001 h + khl h 3 0,0,z 6 0,0,z h Now we will consider screw rotations and glide reﬂections. These operations consist of the coupling of a rotation or a reﬂection with a translation. The matrix-vector representation of these operations consists of a matrix (M) giving the rotation or reﬂection followed by a vector representing the screw (s) or glide (g) component. For a pure translation, (M) is the unit matrix (E). 41 -screw axis in 0,0,z: 41c ⎞ ⎞ ⎛ ⎞ ⎛ s ⎞ ⎛ 0 −y x 0 1̄ 0 (41 )1c ⎝ 1 0 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ x ⎠ → ȳ,x,z + 1 z 001 z + 14 4 ⎛ 1 4 ⎛ 4c ≡2c ⎞ ⎛ ⎞ ⎛ 2s ⎞ ⎛ ⎞ 0 −x x 1̄ 0 0 (41 )2c ⎝ 0 1̄ 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ −y ⎠ → x̄, ȳ, z + 1 z 001 z + 12 2 (11.15) 2 1 2 (11.16) 233 234 11 Symmetry Groups ⎛ 43c ⎞ ⎛ ⎞ ⎛ 3s ⎞ ⎛ ⎞ 0 y 010 x (41 )3c ⎝ 1̄ 0 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ −x ⎠ → y, x̄, z + 3 z 001 z + 34 4 3 4 (11.17) 4c ≡1 ⎞ ⎛ ⎞ ⎛ 4s ⎞ ⎛ ⎞ 100 x 0 x (41 )4c ⎝ 0 1 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ y ⎠ → x,y,z + 1 001 z 1 z+1 ⎛ 4 (11.18) The fourfold application of this symmetry operation results in a unit translation parallel to the screw axis. a-glide plane in x,0,z: ⎛ m1b 10 a1 ⎝ 0 1̄ 00 ⎞ ⎛ ⎞ ⎛ 1g ⎞ ⎛ ⎞ 0 x x + 12 2 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ −y ⎠ → x + 12 , ȳ, z z 1 0 z (11.19) ⎛ mb ≡1 ⎞ ⎛ ⎞ ⎛2g⎞ ⎛ ⎞ 100 x 1 x+1 a2 ⎝ 0 1 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ y ⎠ → x + 1,y,z 001 z 0 z 1 (11.20) n-glide plane in 0,y,z: 2g ⎞ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ 0 −x x 1̄ 0 0 1⎟ ⎜1⎟ ⎜ n1 ⎝ 0 1 0 ⎠ ·⎝ y ⎠ + ⎝ 2 ⎠ = ⎝ y + 2 ⎠ → x̄, y + 12 , z + 1 z 001 z+ 1 ⎛ m1a 2 1 2 (11.21) 2 ⎛ ma ≡1 ⎞ ⎛ ⎞ ⎛2g⎞ ⎛ ⎞ 100 x 0 x n2 ⎝ 0 1 0 ⎠ · ⎝ y ⎠ + ⎝ 1 ⎠ = ⎝ y + 1 ⎠ → x, y + 1, z + 1 001 z 1 z+1 2 (11.22) Applying a glide-operation twice always results in a lattice translation parallel to the glide plane. When a symmetry element does not pass through the origin 0,0,0, this situation requires a further vector, the position vector l, giving the separation of the symmetry element from the lattice origin. Usually, l is combined with the vector s or g to give a composite vector v. 11.1 Representation of Symmetry Operations by Matrices 2 in 12 , 14 , z ⎛ 1̄ ⎝0 0 ⎞ ⎛ ⎞ ⎛ l ⎞ ⎛ ⎞ 0 x̄ + 1 x 00 1̄ 0 ⎠ ·⎝ y ⎠ + ⎝ 12 ⎠ = ⎝ ȳ + 12 ⎠ → 1 − x, 12 − y,z z 01 0 z 2c a in x, 14 , z mb ⎞ ⎛ ⎞ ⎛ 1g ⎞ ⎛ l ⎞ ⎛ 0 100 10 x 2 ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ + ⎝ 0 ⎠ + ⎝ 1 ⎠ = ⎝ 0 1̄ 2 z 001 00 0 0 ⎞ ⎛ x + 12 ⎟ ⎜ =⎝ ȳ + 1 ⎠ → 12 + x, 12 − y,z 2 z ⎛ 21 in 14 , y, 14 ⎞ ⎛ ⎞ ⎛ s ⎞ ⎛ 1l ⎞ ⎛ 0 x 1̄ 0 0 1̄ 0 2 ⎝0 1 0⎠·⎝y⎠ + ⎝ 1 ⎠+⎝ 0 ⎠ = ⎝0 1 2 1 z 0 0 1̄ 00 0 2 ⎞ ⎛ 1 x̄ + 2 ⎟ ⎜ =⎝ y + 12 ⎠ → 12 − x, 12 + y, 12 − z ⎛ 2b z̄ + v ⎞ ⎛ ⎞ ⎛1⎞ 2 0 x ⎜ ⎟ 0 ⎠ · ⎝ y ⎠ + ⎝ 12 ⎠ z 1 0 v ⎞ ⎛ ⎞ ⎛1⎞ x 0 2 ⎜ ⎟ 0 ⎠ · ⎝ y ⎠ + ⎝ 12 ⎠ 1 z 1̄ 2 1 2 In the following examples, the eight equivalent points of the general position in the space group P21 /b 2/c 21 /n are calculated using matrices (see also Fig. 11.3): Fig. 11.3 Space group P21 /b 2/c 21 /n showing a set of general positions: (1) x,y,z (2) x̄,ȳ,z̄ (3) 12 +x, 12 –y,z̄ (4) 12 –x, 12 +y,z (5) x̄,y, 21 –z (6) x,ȳ, 12 +z (7) 12 –x, 21 –y, 12 +z (8) 12 +x, 21 +y, 21 –z 235 236 11 Symmetry Groups 1. 1 ⎛ 1 10 ⎝0 1 00 ⎞ ⎛ ⎞ ⎛ ⎞ 0 x x 0 ⎠ · ⎝ y ⎠ = ⎝ y ⎠ → x,y,z 1 z z 2. 1̄in 0,0,0 ⎛ 1̄ ⎞ ⎛ ⎞ ⎛ ⎞ 1̄ 0 0 x x̄ ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ = ⎝ ȳ ⎠ → x̄,ȳ,z̄ z z̄ 0 0 1̄ 3. 21 in x, 14 ,0 ⎞ ⎛ ⎞ ⎛1⎞ ⎛ 2a ⎞ ⎛ ⎞ ⎛ 1s ⎞ ⎛ l̄ ⎞ ⎛ 0 100 1 0 0 x x 2 2 ⎟ ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ + ⎝ 0 ⎠ + ⎝ 1 ⎠ = ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ + ⎜ 1⎠ ⎝ 2 2 z z 0 0 1̄ 0 0 1̄ 0 0 0 ⎛ ⎞ 1 x+ 2 ⎜ ⎟ = ⎝ ȳ + 1 ⎠ → 12 + x, 12 − y,z̄ 2 z̄ 4. b-glide in 14 ,y,z ⎛ ma ⎞ ⎛ ⎞ ⎛ g ⎞ ⎛ 1l̄ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛1⎞ 0 x x 1̄ 0 0 1̄ 0 0 2 2 ⎟ ⎝0 1 0⎠·⎝y⎠ + ⎝ 1 ⎠+⎝ 0 ⎠ = ⎝0 1 0⎠ · ⎝y⎠ + ⎜ 1⎠ ⎝ 2 2 z z 001 001 0 0 0 ⎛ ⎞ 1 x̄ + 2 ⎜ ⎟ = ⎝ y + 1 ⎠ → 12 − x, 12 + y,z 2 z 5. 2 in 0,y, 14 ⎛ 2b ⎞ ⎛ ⎞ ⎛ 1 ⎞ ⎛ ⎞ 0 x̄ 100 x ⎝ 0 1 0 ⎠ ·⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ y ⎠ → x̄,ȳ, 1 − z 2 1 z 0 0 1̄ z̄ + 12 2 6. c-glide in x,0,z ⎛ mb ⎞ ⎛ ⎞ ⎛ g ⎞ ⎛ ⎞ 0 x 100 x ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ + ⎝ 0 ⎠ = ⎝ ȳ ⎠ → x,ȳ, 1 + z 2 1 z 001 z + 12 2 11.2 Properties of a Group 7. 21 in 14 , 14 , z v 1̄ ⎞ ⎛ ⎞ ⎛1⎞ ⎞ ⎛ ⎞ ⎛ s ⎞ ⎛ 1 ⎞ ⎛ 0 1̄ 0 0 x 1̄ 0 0 x 2 2 ⎟ ⎜ ⎟ ⎝0 1 0⎠·⎝y⎠ + ⎝ 0 ⎠+⎜ ⎝ 12 ⎠ = ⎝ 0 1̄ 0 ⎠ · ⎝ y ⎠ + ⎝ 12 ⎠ 1 1 z z 0 0 1̄ 0 0 1̄ 0 2 2 ⎞ ⎛ 1 x̄ + 2 ⎟ ⎜ = ⎝ ȳ + 12 ⎠ → 12 − x, 12 − y, 12 + z ⎛ 2c z+ 8. 1 2 n-glide in x,y, 14 g v ⎞ ⎛ ⎞ ⎛ 1 ⎞ ⎛ l̄ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛1⎞ 0 100 100 x x 2 2 ⎜ ⎟ ⎟ ⎝0 1 0⎠·⎝y⎠ + ⎜ ⎝ 12 ⎠ + ⎝ 0 ⎠ = ⎝ 0 1 0 ⎠ · ⎝ y ⎠ + ⎝ 12 ⎠ 1 1 001 z z 0 0 1̄ 0 2 2 ⎞ ⎛ 1 x+ 2 ⎟ ⎜ = ⎝ y + 12 ⎠ → 12 + x, 12 + y, 12 − z z̄ + 12 ⎛ mc 11.2 Properties of a Group A point or space group, or, in general, any symmetry group, is a combination of symmetry elements which together constitute a mathematical group. For this to be the case, four conditions must be met: D • If two symmetry operations of a group are performed sequentially, the result must be some symmetry operation of the group. Thus, the operation 2[110] followed by the operation 2a of the point group 422 results in the rotation 43c , which is also is an operation of 422. 2a · 2[110] = 43c ⎞ ⎛ ⎞ ⎛ ⎞ 100 010 010 ⎝ 0 1̄ 0 ⎠ · ⎝ 1 0 0 ⎠ = ⎝ 1̄ 0 0 ⎠ 0 0 1̄ 001 0 0 1̄ ⎛ • The symmetry operation 1, or the identity, is found in every symmetry group. It is the basic element of any group, and multiplication of any symmetry element with it leaves that symmetry element unchanged. Examples: 2[110] · 1 = 1 · 2[110] = 2[110] , 31c · 1 = 1 · 31c = 31c , ma · 1 = 1 · ma = ma 237 238 11 Symmetry Groups • In any symmetry group, the presence of an operation implies the presence of its inverse. The multiplication of these two elements gives the identity. Examples: 41c · 43c = 43c · 41c = 1 (4+ · 4− = 4− · 4+ = 1), 2[110] · 2[110] = 1, ma · ma = 1, 1̄ · 1̄ = 1. In the case of a two-fold rotation, a reﬂection or an inversion, the operation is its own inverse. • The multiplication of symmetry operations is always associative: Examples: (ma · mb ) · mc = ma · (mb · mc ) 2c · mc = ma · 2a = 1̄ (41c · m[110] ) · 2c = 41c · (m[110] · 2c ) mb · 2c = 41c · m[11̄0] = ma . ! The symmetry operations of a group constitute the elements of that group. The number of elements is called the order of the group. Point group 422 has the elements 41c , 42c ≡ 2c , 43c , 2a , 2b , 2[110] , 2[11̄0] , and 1. Thus, its order is 8. 2/m, with the elements 2, m, 1̄ and 1, has order 4. The order of a point group is always the same as the number of faces in its general form (422: tetragonal trapezohedron, 8 faces, order 8; 2/m: rhombic prism, 4 faces, order 4.) Some groups are commutative. In them, the order of multiplication of the elements does not aﬀect the result Example: 2/m 2/m 2/m: ma . mb = mb . ma = 2c ; 2a . 2b = 2b . 2a = 2c etc. D Calling a group G’ a subgroup of another group G implies that the elements of G’ are a subset of those of G. Similarly, G is then called a supergroup of G’. Some symmetry groups have a ﬁnite number of elements, while others have an inﬁnite number. 11.2.1 Finite Symmetry Groups Crystallographic point groups are all of this type. The elements of the group are the point symmetry operations, i.e. inversions, rotations, rotoinversions and reﬂections. 11.3 Derivation of a Few Point Groups The orders of these groups range from 1 (point group 1) to 48 (4/m3̄2/m). The others have the following orders: • • • • • • • • 2 (1̄, 2, m) 3 (3) 4 (4, 4̄, 2/m, 222, mm2) 6 (3̄, 6, 6̄, 32, 3m) 8 (2/m2/m2/m, 4/m, 422, 4mm, 4̄2m) 12 (3̄2/m, 6/m, 622, 6mm, 6̄m2, 23) 16 (4/m2/m2/m) 24 (6/m2/m2/m, 2/m3̄, 432, 4̄3m) The sub- and supergroups of the crystallographic point groups are given in Fig. 9.3. 11.2.2 Inﬁnite Symmetry Groups Space groups are of this type. The elements of the group are point symmetry operations as above, together with translations, screw rotations and glide reﬂections. All space groups allow translations in three linearly independent directions. By successive applications of translations, screw rotations or glide reﬂections, an inﬁnite number of identical points can be reached. This characteristic distinguishes such symmetry operations from those of point symmetry. All of the translations of a space group taken together constitute a subgroup of it, known as the translational subgroup. The translations taken alone obey the deﬁning axioms for a group. Furthermore, translations are commutative, meaning that the order in which they are applied has no eﬀect on the result. Translational subgroups of space groups are thus Abelian groups. Space groups, with the exception of P1, and the more complicated point groups are not Abelian groups. 11.3 Derivation of a Few Point Groups In Chap. 9 (Point Groups), point groups were derived as subgroups of the point group of highest symmetry in each crystal system, e.g. 2, m, 1̄ and 1 from 2/m. In Exercises 9.4 and 9.5, the derivation of a point group was carried out geometrically by combining symmetry elements at speciﬁc angles to one another. This may, of course, also be done by calculation. A few examples will be shown here: • Exercise 9.4A Combination of two 2-fold axes at 30◦ to one another: (a) 2[210] · 2a ⎞ ⎛ ⎛ 100 1 1̄ ⎝ 1 1̄ 0 ⎠ ·⎝ 0 1̄ 0 0 1̄ 00 ⎞ = 61c ⎛ ⎞ 0 1 1̄ 0 0⎠ = ⎝1 0 0⎠ 001 1̄ 239 240 11 Symmetry Groups (b) 62c (≡ 31c ) · 2a = 2[110] (c) 63c (≡ 2c ) · 2a = 2[120] (d) 64c (≡ 32c ) · 2a = 2b (e) 65c · 2a = 2[11̄0] as seen in the stereogram, the point group 622 has been derived. • Exercise 9.4B Combination of two mirror planes at 45◦ to one another: (a) · m[11̄0] = 41c ⎞ ⎛ ⎞ ⎛ ⎞ 010 1̄ 0 0 0 1̄ 0 ⎝0 1 0⎠ · ⎝1 0 0⎠ = ⎝1 0 0⎠ 001 001 001 ⎛ ma (b) 42c (≡ 2c ) · ma = mb (c) 41c · ma = m[110] as seen in the stereogram, the point group 4mm has been derived. • Exercise 9.4C Combination of a 2-fold axis and a mirror plane at 60◦ to one another: (a) · mb = 3̄1c ⎞ ⎞ ⎛ ⎞ ⎛ 010 100 1 1̄ 0 ⎝ 0 1̄ 0 ⎠ · ⎝ 1 1̄ 0 ⎠ = ⎝ 1̄ 1 0 ⎠ 001 0 0 1̄ 0 0 1̄ ⎛ 2a (b) 3̄2c (≡ 32c ) · 2a = 2b (c) 3̄4c (≡ 31c ) · 2a = 2[110] (d) 3̄3c (≡ 1̄) · 2a = ma (e) 3̄3c (≡ 1̄) · 2[110] = m[110] as seen in the stereogram, the point group, 3̄2/m has been derived. • Exercise 9.4D Combination of two 2-fold axes at 90◦ to one another plus an inversion center: (a) ⎛ 2a ⎞ · ⎛ 2b ⎞ = ⎛ 2c ⎞ 100 1̄ 0 0 1̄ 0 0 ⎝ 0 1̄ 0 ⎠ · ⎝ 0 1 0 ⎠ = ⎝ 0 1̄ 0 ⎠ 0 0 1̄ 0 0 1̄ 001 This produces the point group 222, cf. Fig. 7.9f 11.4 Group Multiplication Tables (b) 2a ·1̄ =ma 2b ·1̄ =mb 2c ·1̄ =mc This now produces the point group 2/m 2/m 2/m, cf. Fig. 7.9e • Exercise 9.5E Combination of a 2-fold and a 3-fold axis at 54◦ 44 to one another: 2a · 31 = 31 ⎞ ⎛ [111] ⎞ ⎛ [1̄11̄] ⎞ 001 100 001 ⎝ 0 1̄ 0 ⎠ · ⎝ 1 0 0 ⎠ = ⎝ 1̄ 0 0 ⎠ 010 0 1̄ 0 0 0 1̄ (a) ⎛ (b) 31[111] · 31[1̄11̄] = 32[1̄11̄] (c) 31[111] · 31[11̄1̄] = 32[1̄1̄1] (d) 31[111] · 32[1̄1̄1] = 2b (e) 31[111] · 32[11̄1̄] = 2c This combination produces the point group 23, as shown in the stereogram. • Exercise 9.5H Combination of a 2-fold and a 3-fold axis at 54◦ 44 to one another plus an inversion center: (a) 2a · 1̄ = ma 2b · 1̄ = mb 2c · 1̄ = mc (b) 3̄1[111] ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ 0 0 1̄ 1̄ 0 0 001 ⎝ 1 0 0 ⎠ · ⎝ 0 1̄ 0 ⎠ = ⎝ 1̄ 0 0 ⎠ etc. 010 0 1̄ 0 0 0 1̄ 31[111] · 1̄ = This combination produces the point group 2/m 3̄, as shown in Fig. 7.13a-f. 11.4 Group Multiplication Tables A group multiplication table allows the formation and the characteristics of a ﬁnite point group to be summarized conveniently. In the table, all the products of any two elements are shown in a square array. Figure 11.4 shows the tables for the ﬁve point groups of order 4, each symmetry element having one row and one column. The tables in Fig. 11.4 are symmetric about the diagonal from top left to bottom right (the leading diagonal). This implies that the order of multiplication of the matrices does not aﬀect the result. These groups are thus all Abelian groups. 241 242 11 Symmetry Groups Fig. 11.4a-e Group tables for the point groups of order 4, (a ) 2/m, (b) 222, (c) mm2, (d) 4, (e) 4̄ Figure 11.5 shows the group table for 3m. This table is not symmetrical, so 3m is not an Abelian group. For the correct interpretation of such a group table, it is essential to understand in which order the elements are applied to an object. The rule is that the symmetry operation in the top row is applied ﬁrst, and then the operation in the left-most column. The group tables for 2/m, 222 and mm2 in Fig. 11.4 are built up in the same way. If the four symmetry operations are simply represented as a, b, c and d, the three tables will become identical. Finite groups with this property are called isomorphic groups. Such groups always have the same order. The groups 4 and 4̄ (Fig. 11.4b, e) are isomorphic with each other, but not with 2/m, 222 and mm2. Here are some important relationships that can be read directly from the tables in Fig. 11.4. 11.5 Exercises Fig. 11.5 Group table for the point group 3m • 2/m (Fig. 11.4a) 2·2 = 1 m·m = 1 1̄ · 1̄ = 1 2, m and 1̄ are thus their own inverses. Further, symmetry rule I (p. 95) is seen directly: 2b · mb =1̄ 2b · 1̄ = mb mb · 1̄ = 2b 2a · 2c = 2b etc. • 222 (Fig. 11.4b): 2a · 2b = 2c • mm2 (Fig. 11.4c): symmetry rule II (p. 95) is here seen directly: ma · mb = 2c ma · 2c = mb etc. • 3m (Fig. 11.5) ma ·mb = 31c 11.5 Exercises Exercise 11.1 Write the matrices for the following symmetry operations: (a) 1̄ (b) 2b (c) m[210] (d) 3[111] (e) 4̄1b (f) 61c 243 244 11 Symmetry Groups Exercise 11.2 What are the inverse matrices for 1̄, 2c and m[110] ? Exercise 11.3 In this book, the monoclinic system is always treated in the second setting (2, m||b). Are the matrices in Table 11.1 also valid for the ﬁrst setting (2, m||c)? Exercise 11.4 Multiply the matrices for: (a) 2a and m[110] (b) 31c and mc (c) 41c and 1̄ Which symmetry operations and point groups are formed? Exercise 11.5 Derive using matrix multiplication the symmetry operations of symmetry rule I (Fig. 7.14) Exercise 11.6 Write the symmetry operations for point group 4̄2m. What is the order of this point group? Use these symmetry operations to derive the faces equivalent to (hkl). What crystal form do these faces represent? Compare the indices you have derived with those in Fig. 9.9. Exercise 11.7 Demonstrate that 3m and 32 are isomorphic groups. Is 32 an Abelian group? 12 Fundamentals of Crystal Chemistry Crystal chemistry is concerned with the crystal structure of the elements and of chemical compounds. It attempts to explain why particular types of crystal structures arise under speciﬁc conditions. It is, however, still only possible to understand how relatively simple crystal structures arise from the atoms that make them up. A fundamental concept in crystal structures is the idea of sphere packing. In this approach, the atoms or ions of which the structure is composed are regarded as hard spheres which pack with one another. Goldschmidt and Laves summarized this approach in three principles: ! 1. The Principle of Closest Packing. Atoms in a crystal structure attempt to arrange themselves in a manner which ﬁlls space most eﬃciently. 2. The Symmetry Principle. Atoms in a crystal structure attempt to achieve an environment of the highest possible symmetry. 3. The Interaction Principle. Atoms in a crystal structure attempt to achieve the highest coordination (Sect. 12.1), i.e. the maximum possible number of nearest neighbors with which they can interact. Chemical bonding is a very important factor in crystal chemistry, as it is concerned with the forces holding the atoms together in the structure. The atoms of a structure are held together in a characteristic order by the chemical bonding. This bonding arises from interaction of the electron shells of the atoms, and is conventionally divided into: (a) (b) (c) (d) metallic bonding van der Waals bonding ionic or heteropolar bonding and covalent or homopolar bonding. They are illustrated schematically in Fig. 12.1. Actual compounds rarely correspond exactly to one of these types. In most cases, the bonding is a mixture of two or more types, which should be regarded only as limiting cases. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_12, C Springer-Verlag Berlin Heidelberg 2011 246 12 Fundamentals of Crystal Chemistry Fig. 12.1a–d Schematic summary of bonding types in crystals. a Metallic bonding. Valence electrons of the metal atoms are delocalised in an “electron cloud”. This negatively charged cloud encloses the positively charged atom cores and holds them together. b Van der Waals bonding. This arises from random variations in the charge distributions of the atoms and is very weak. The atoms and molecules tend toward a closest packing. c Ionic bonding. In an ionic crystal, the positively and negatively charged ions are held together by electrostatic forces. d Covalent bonding. This represents the four sp3 -orbitals of a carbon atom in the diamond structure It is beyond the scope of this book to discuss the theory of chemical bonding. We shall restrict ourselves here, so far as bonding theory is concerned, to a small number of principles on which further study may be based. The principles stated above work well in rationalizing the structures of metallic and ionic materials. They also have some application to molecular crystals, those held together by van der Waals forces. For covalent structures, the principles of closest packing and of high coordination are rarely fulﬁlled. This results from the fact that covalent bonding is directional in nature. 12.1 Coordination In crystal chemistry, the immediate neighborhood of each atom and the forces which bind it to its neighbors play a leading role in the explanation of the overall geometry of the crystal. D The number of nearest neighbors of a central atom or ion is called its coordination number, and the polyhedron formed when the nearest neighbors are connected by lines is called its coordination polyhedron. Some important coordination polyhedra are given in Table 12.1 along with actual examples. The coordination number, in square brackets, can be inserted in the chemical formula as a superscript, and thus add signiﬁcant crystal-chemical information to the formula. Ideally, coordination polyhedra have a high point symmetry. However, a coordination polyhedron is nothing like so sharply deﬁned as a crystal form (Sect. 9.2.1). Even atoms of the same element coordinated to the same central atom are not necessarily equivalent. Strictly speaking, cubic (m3̄m), octahedral (m3̄m) and tetrahedral 12.1 Coordination Table 12.1 Important coordination polyhedra a The limiting value of the radius ration Ra /Rx is that at which spherical coordinating atoms X just touch one another, and the central atom A ﬁts precisely into the resulting hole. b cf. Exercise 4.2 247 248 12 Fundamentals of Crystal Chemistry (4̄3m) symmetries can only arise in the cubic system. Coordination polyhedra are often more or less distorted. The cubic coordination in cubic CsI (Fig. 3.4) and the octahedral coordination in NaCl (Fig. 12.17) are strictly regular, while the octahedral coordination in tetragonal rutile (Fig. 10.18) is distorted, cf. Exercise 12.10. 12.2 Metal Structures A simple picture of metallic bonding is that the valence electrons of the metal atoms are delocalised in an “electron cloud” (Fig. 12.1a). This negatively charged cloud encloses the positively charged atom cores (not ions) and shields them from one another. The bonding forces are not directional; they are equal in all directions. In a metal, one can consider the atoms as spheres. Each atom attempts to associate itself with the maximum number of similar atoms. This can be achieved for 12 nearest neighbors in two diﬀerent arrangements (coordination polyhedra), shown in Figs. 12.2a and 12.3a, and also Table 12.1a, b. Starting from these coordination polyhedra as nuclei, crystal growth will result in the formation of two distinct crystal Fig. 12.2a–c Cubic closest packing of spheres (Cu-type). a Coordination polyhedron [12] (cuboctahedron) as a perspective representation, using spheres reduced in size, and as a projection of the spheres on a close-packed layer. b The crystal structure. One of the layers parallel to (111) is shown together with the layer sequence ABCA. c A unit cell (cubic F-lattice). The spheres are reduced in size, and their correspondence to the stacked layers is indicated. The unit cell is also sketched in b 12.2 Metal Structures Fig. 12.3a–c Hexagonal closest packing of spheres (Mg-type). a Coordination polyhedron [12] (disheptahedron) as a perspective representation, using spheres reduced in size, and as a projection of the spheres on a close-packed layer. b The crystal structure. One of the layers parallel to (0001) is shown together with the layer sequence ABA. c A unit cell. The spheres are reduced in size, and their correspondence to the stacked layers is indicated. The unit cell is also sketched in b structures. These structures can be described as stackings of closest packed layers of spheres, and they diﬀer in the layer sequence. Structure I may be described by a cubic unit cell, with a cubic F-lattice, and is called the Cu-type, while structure II has a hexagonal unit cell, and is called the Mg-type. The two structures are thus called cubic and hexagonal closest packing respectively, abbreviated to ccp and hcp. Examples of each structure are given in Table 12.2. Some metals occur with both structure types, e.g. Ni. The atoms of the Cu or ccp structure are all related by simple lattice translations, and are thus identical. In the Mg or hcp structure, atoms in the A-layers are all identical, as are atoms in the B-layers. The A- and B-atoms are, however, equivalent but not identical to one another. This is shown by the positions given in Table 12.2. If the lattice constant is known, the radius of a sphere (the atomic radius) may be calculated. Figure 12.2b, c shows the diagonal of a (100) face of the cubic unit cell of the√ccp-structure. Its length is equal to four sphere radii (B-2C-A). Thus R = 1/4 a0 2 In the hcp-structure, R = 1/2 a0 (cf. Fig. 12.3b, c). Radii of metal atoms are given in Table 12.3. It is possible to ﬁll spaces completely by packing equal cubes, or, indeed, equal general parallelepipeds. This is not possible with spheres. In both types of closest sphere packings, there are interstices remaining of speciﬁc coordination; these are usually called “holes”. These may be bounded by four spheres (tetrahedral holes) or 249 250 12 Fundamentals of Crystal Chemistry Table 12.2 Data for the three most important metal structure types, Cu, Mg and W, and for α -Po Cu ccp Lattice + basis Mg hcp W bcc α-Po sc Cubic F Hexagonal P Cubic I Cubic P –––––––––––––––––––––––––––––––––––––––0,0,0 0,0,0; 23 , 31 , 21 0,0,0 0,0,0 Space group F 4/m 3̄ 2/m P 63 /m 2/m 2/c I 4/m 3̄ 2/m P 4/m 3̄ 2/m –––––––––––––––––––––––––––––––––––––––+ Positions occupied (a) 0,0,0 (c) 0,0,0; 23 , 13 , 12 (a) 0,0,0 (a) 0,0,0 Coordination Cuboctahedron Dishepatahedron Cube Octahedron polyhedron, number – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – – [12] [8] [6] √ √ 1 1 1 1 Atomic radii 4 a0 2 2 a0 4 a0 3 2 a0 Packing eﬃciency 0.74 Further examples Ag, Au Ni, Al Pt, Ir Pb, Rh Mg (1.62) Ni (1.63) Ti (1.59) Zr (1.59) Be (1.56) Zn (1.86) 0.68 0.52 Mo, V Ba, Na Zr, Fe – by six (octahedral holes), (Fig. 12.4) and are examples of tetrahedral and octahedral coordination (Table 12.1). D The packing eﬃciency is deﬁned as the ratio of the sum of the volumes of the spheres making up a unit cell to the volume of the unit cell. If the spheres are equal in size, it is given by Z · 43 π R3 . Vunitcell √ 4R As we have seen, in the ccp structure, R = 14 a0 2. Thus a0 = √ and 2 √ √ π 3 3 V = a0 = 16R 2. Since Z = 4, the packing eﬃciency is thus 6 2 = 0.74. The Fig. 12.4 a Tetrahedral [4] holes. b Octahedral [6] hole in closest packed arrays of spheres 12.2 Metal Structures corresponding calculation for the hcp structure gives the same result; both types of closest packing are equally eﬃcient. For the hcp structure, the ideal ac00 ratio may be calculated, since c0 is the height of two coordination tetrahedra of edge 2R = √ a0 , sharing a common vertex (cf. Fig. 12.3c). This gives a value for c0 / a0 of 2/3 · 6 = 1.63. In Table 12.2, the ac00 values for several metals are given; they tend to lie between 1.56 and 1.63. The value for Zn is considerably larger. In addition to the two types of closest packing, a further structure adopted by some metals is the W-type, with a cubic I-lattice, usually simply called body-centered cubic, and abbreviated bcc (Fig. 12.5). In this structure, the body-diagonal of the unit √ cell consists of four sphere radii, i.e. R = 1/4 a0 3. √ The packing eﬃciency of this structure is π8 3 = 0.68. The coordination number is [8], and the coordination polyhedron is a cube. An arrangement of metal atoms in a cubic P-lattice occurs only for α-polonium (Fig. 2.1, Table 12.2). It has a packing eﬃciency of 0.52, a coordination number of [6] and an octahedron as its coordination polyhedron. Considering the above data for the hcp and ccp structures, the Goldschmidt and Laves principles are very well fulﬁlled: • The packing eﬃciency is 0.74, the highest possible for the packing of equal spheres. • F4/m3̄2/m is one of the highest symmetry space groups of the cubic system, and P63 /m 2/m 2/c is one of the highest symmetry space groups of the hexagonal system. • [12] is the highest possible coordination number for spheres of equal size. The W-type or bcc structure has a packing eﬃciency of only 0.68 and its coordination number, [8], is smaller than that of the closest packed structures, but its symmetry, I4/m3̄2/m is also high. The α-Po structure also has a high symmetry (P4/m3̄2/m), but its packing eﬃciency and coordination of 0.52 and [6] respectively are very small. This is certainly the reason for α-Po being the sole example of this structure. Metals attempt to achieve a high symmetry and a high packing eﬃciency. The great majority of metals crystallize in one of the ﬁrst three given structure types. Fig. 12.5a,b Crystal structure of tungsten. a With atomic radii shown to scale. b Showing only the centers of gravity of the atoms 251 252 12 Fundamentals of Crystal Chemistry Metals have many characteristic properties which are related to their structure and bonding: (a) Electrical and Thermal Conductivity: Metals are good conductors of both heat and electricity. These properties arise from the fact that the electron clouds between the atom cores can move freely. (b) Plastic Deformation: Plastic deformation in a metal is a shearing parallel to closest packed layers. This property is most prominent for metals with cubic closest packing in which four equivalent (111)-planes can undergo shear eﬃciently. These metals are generally soft, malleable and ductile. Gold, for example, can be beaten to a thin foil that weakly transmits green light. Crystals with hexagonal closest packing of the atoms are less malleable, since they have only one shear plane, parallel to (0001). Body-centered cubic metals are yet more brittle. 12.3 Structures of Noble Gases and Molecules In noble gas and molecular structures, the atoms or molecules are held together by van der Waals forces. These forces are very weak. This is apparent from the very low melting points of such crystals, e.g. neon: −247.7◦ C, ethylene: −170◦ C, benzene: 5.5◦ C and phenyl salicylate 43◦ C. Noble gas atoms can also pack together as spheres, having a noble gas electron conﬁguration. The bonding forces, like those in metals are non-directional, and the same sphere packings occur: • cubic closest packing (cf. Fig. 12.2): Ne, Ar, Kr, Xe, Rn. • hexagonal closest packing (cf. Fig. 12.3): He. Molecular structures are characterized by the fact that the energy holding the atoms in the molecules together (covalent bonding) is large, while that holding one molecule to another is very weak. Most molecular compounds are organic, inorganic examples include sulfur (cf. the S8 molecule in Table 9.12.3) and C60 , see below. Three molecular structures were introduced in Figs. 10.19, 10.20 and 10.21 (hexamethylenetetramine, ethylene and benzene). As was made clear in Chap. 10, there is no simple relationship between crystal symmetry and molecular symmetry. Although molecules are not spherical in shape, they do attempt to pack as closely as possible in crystals. The hexamethylenetetramine structure (Fig. 10.1), for example, has a packing eﬃciency of 0.72. In the crystal structure of CO2 , the C-atoms occupy the positions of a cubic closest packing, the linear molecules being parallel to < 111 >. Since the forces holding the molecules together are weak, it follows that the lattice energies of organic compounds are, in general, low. Nonetheless, the great majority of organic compounds can be crystallised. Even “giant” molecules with very large unit cell dimensions have been crystallised, for example: 12.4 Ionic Structures Fig. 12.6a,b The C60 -molecule forms an almost spherical cage with 20 six-membered rings and 12 ﬁve-membered rings (a) ([41]). The non-crystallographic point group 2/m3 5(Ih ) of the molecule (b) ([14]) 1. vitamin B12 : C63 H88 N14 O14 PCo, P21 21 21 , a0 = 25.33 Å, b0 = 22.32 Å, c0 = 15.92 Å, Z = 4 2. pepsin: P61 22, a0 = 67 Å, c0 = 154 Å, Z = 12, M ≈ 40000 Fullerenes are molecules containing only carbon, the main one of which has the molecular formula C60 . In this molecule, the atoms form an almost spherical cage, made up of 20 six-membered rings and 12 ﬁve-membered rings. The structure is that of a soccer ball (Fig. 12.6a). The molecule has the non-crystallographic symmetry 2/m3 5 (Ih ) (Fig. 12.6b), and for this reason, all atoms are equivalent. C60 molecules have been crystallised with a ccp structure. 12.4 Ionic Structures Ionic crystals are built from positively and negatively charged ions, and the bonding energy is Coulombic forces, which are non-directional and equal in all directions. The strength of a bond is related to the charge on the ions, e, and the distance, d, between them: Coulomb’s Law: K = e1 ·e2 2 d Each cation seeks to maximize the number of neighboring anions, while each anion equally seeks to maximize its neighborhood of cations (Fig. 12.1c). The formation of ionic structures is thus another packing problem, but now the spheres are ions of opposite charge which generally are also diﬀerent in size. The relative sizes of the radius of the cation, RA , and that of the anion, Rx , the radius ratio RA /Rx , can suggest the appropriate coordination polyhedron and thus the crystal structure (Sects. 12.4.2, 12.4.3 and 12.4.4). 12.4.1 Ionic Radii Figure 12.7 gives ionic radii as a function of atomic number. The size of an ion, considering an ion as a sphere, depends on the charge on the nucleus and on the number of electrons. 253 Fig. 12.7 Atomic and ionic radii as a function of atomic number. (After Ramdohr and Strunz [35]) 254 12 Fundamentals of Crystal Chemistry Fig. 12.7 (Continued) 12.4 Ionic Structures 255 256 12 Fundamentals of Crystal Chemistry • Within a column of the periodic table, the ionic radius generally rises with the increasing nuclear charge. Li+ = 0.70 Å = 0.98 Å Na+ K+ = 1.33 Å Rb+ = 1.52 Å Cs+ = 1.70 Å F– = 1.33 Å Cl– = 1.81 Å Br– = 1.96 Å I– = 2.20 Å • For isoelectronic ions, an increase in the nuclear charge results in a lowering of the ionic radius. • For a particular element, the ionic radius falls as the positive charge rises: cf. S(16) or Mn(25) in Table 12.3. Table 12.3 Nuclear charge and ionic radius Na+ Mg2+ Al3+ Si4+ P5+ S6+ Cl7+ 0.98 Å 0.65 Å 0.57 Å 0.39 Å 0.34 Å 0.29 Å 0.26 Å 12.4.2 Octahedral Coordination [6] The octahedron as a coordination polyhedron is illustrated in Table 12.1e. The limiting value for the radius ratio RA /RX for this coordination may be determined by considering an octahedron composed of spherical anions which touch one another, and placing a cation precisely in the hole in its center. Figure 12.8 shows√a section through √ such an octahedron. It can be seen that RA + RX = RX 2, or RA /RX = 2 − 1 = 0.41. Octahedral coordination is only stable if RA /RX is greater than or equal to 0.41 (Fig. 12.9a, b). A section through an unstable octahedron is shown in Fig. 12.9c. Octahedral coordination occurs in the Na[6] Cl (Figs. 12.10 and 12.18) and rutile [6] Ti O2 (Fig. 10.18) structure types. The NaCl structure type can be considered as a cubic closest packing of anions with cations in the octahedral holes. For LiCl (RA /RX = 0.43), the ideal radius ratio for octahedral coordination is almost achieved. By contrast, NaCl itself has a radius ratio of 0.54 (Fig. 12.9a). The spinel structure Mg[4] Al2 [6] O4 is based on a cubic closest packed array of oxide ions. The Mg2+ ions occupy tetrahedral holes and the Al3+ ions octahedral holes. Let us consider how many of the octahedral and tetrahedral holes are occupied. Fig. 12.8 Cross-section through a coordination octahedron ([6]) 12.4 Ionic Structures Fig. 12.9a–c Section through a coordination octahedron, with the corresponding radius ratio, RA /RX . The arrangements in (a) and (b) are stable; that in (b) shows the limiting case with RA /RX = 0.41, and that in (c) is unstable Fig. 12.10 Na[6] Cl structure, Fm3̄m Lattice: cubic F Basis: Na+ at 0,0,0; Cl– at 1/2,0,0 Considering the NaCl structure as a cubic closest packing of Cl– ions (Fig. 12.9), it will be noted that all octahedral holes are occupied by Na+ ions. In NaCl, the ratio Cl– : Na+ is 1:1, thus each sphere in a ccp array (Cl– ) corresponds to an octahedral hole (Na+ ). Figure 12.11 shows the “antiﬂuorite” structure. The sulphide ions are in a ccp array (Fig. 12.11a), and the Li+ ions occupy all tetrahedral holes. In Li2 S, the ratio Li+ : S2– = 2:1, so each sphere in a ccp array (S2– ) corresponds to two tetrahedral holes (Li+ ). The relation 2[4], 1[6] per sphere applies equally to both closest packings. Returning now to the spinel structure, Mg[4] Al2 [6] O4 , we can see that 1/8 of the tetrahedral holes are occupied by Mg2+ and 1/2 of the octahedral holes by Al3+ . In the Ni[6] As (niccolite) structure (P63 /mmc), the As atoms are arranged as a hexagonal closest packing and the Ni atoms occupy all of the octahedral holes (Ni: Fig. 12.11a, b The ﬂuorite or Ca[8] F2 structure, and the “antiﬂuorite” structure (e.g. Li2 S), space group Fm3̄m. Lattice: cubic F. Basis: Ca2+ or S2− at 0,0,0; F− or Li+ at 1/4,1/4,1/4 and 3/4,1/4,1/4. (a) Fluorite structure with F− at 0,0,0 to emphasize cubic coordination. (b) 257 258 12 Fundamentals of Crystal Chemistry As = 1:1, Fig. 12.19). The O2– -ions of the corundum, Al2 [6] O3 similarly form a hexagonal closest packing. The Al3+ ions are in octahedral holes. From the above relationship, 2/3 of the octahedral holes are occupied. In corundum, every third octahedral hole is vacant, but in the ideal structure, all holes are equivalent. This results in a lowering of the space group symmetry to R3̄c. Thus, corundum is trigonal, while in NiAs, the symmetry of the hexagonal closest packing (P63 /mmc) is retained. The O2– ions in forsterite, Mg2 [6] Si[4] O4 , also are arranged as a hexagonal closest packing. The Si4+ ions occupy 1/8 of the tetrahedral holes, and the Mg2+ ions half of the octahedral holes. The symmetry is lowered to Pnma. The atoms or ions in tetrahedral or octahedral holes are usually not statistically disordered. In most cases, they are ordered in the structure. 12.4.3 Cubic Coordination [8] As the radius ratio increases, there should be a range in which the trigonal prism, with limiting RA /RX = 0.53, is stable (cf. Table 12.1d). In fact, for ionic structures, the stable structure becomes cubic [8]-coordination, cf. Table 12.1c. Making use of Fig. 12.12, which shows a section through a cube parallel to (110) (cf. Fig. 3.4), the limiting value for √ RA /RX for cubic coordination can be calculated: RA + RX = √ Rx · 3, so RA /RX = 3 − 1 = 0.73. This implies that octahedral coordination is stable for the range 0.41 < RA /RX < 0.73, while cubic coordination is preferred for RA /RX > 0.73. Cubic coordination is found in structures of the Cs[8] Cl-type, and for the ﬂuorite or Ca[8] F2 -type (Fig. 12.11). Cs[8] I (Fig. 4.4) has the Cs[8] Cl structure with an almost ideal radius ratio of 0.75. In Fig. 12.11b the CaF2 structure has been drawn with an F− -ion at 0, 0, 0. This makes the cubic coordination of the Ca2+ more evident. Ca2+ ions occupy every second cubic hole. The Cl– ions have the same arrangement in the CsCl structure; in that case, every cubic hole is occupied by Cs+ . The ﬂuorite structure is found for SrF2 , BaF2 , SrCl2 , UO2 etc., and also for a number of alkali metal sulphides, e.g. Li2 S, Na2 S, K2 S etc. As in indicated by the chemical formulae, in these sulphides, the positions of the cations and the anions must be reversed, i.e. S2– ions occupy the Ca2+ positions and the alkali metal cations occupy the F– positions. This structure is called the “antiﬂuorite” structure. In it, the S2– ions form a ccp array, and the cations occupy all of the tetrahedral holes (Fig. 12.11a). Fig. 12.12 Section, parallel to (110), through cubic coordination RA /RX 0.84 0.75 CsBr CsI RbI 0.89 0.82 RbF RbCl ScTe 1/0.80 0.76 0.75 0.74 CsF RbBr BaSe NaF 0.49 0.43 LiCl 0.50 CaTe 0.44 0.50 NaBr NaI 0.54 NaCl MgS 0.56 0.59 0.59 0.60 0.60 0.61 0.66 0.68 0.68 0.73 0.73 CaSe LiF MgO KI CaO CaS 0.82 0.80 BaS SrSe KBr SrS 0.96 KCi 1/0.94 AX BaO SrO KF 0.91 CsCl 1.00 0.73–0.41 Na[6] Cl-type >0.73 Cs[8] Cl-type LiI LiBr MgSe Table 12.4 Structures and radius ratios for some AX and AX2 compounds 0.35 0.40 0.41 CdF2 PrO2 CeO2 UO2 CaF2 ThO2 HgF2 SrF2 PbF2 BaF2 >0.73 0.74 0.76 0.77 0.79 0.80 0.83 0.84 0.95 0.99 1.05 HfO2 ZrO2 Flourite-Type Ca[8] F2 0.67 0.67 VO2 TiO2 RuO2 IrO2 OrO2 WO2 MoO2 NbO2 SnO2 MgF2 NiF2 ZnF2 CoF2 FeF2 PbO2 MnF2 0.73–0.41 0.46 0.48 0.49 0.50 0.51 0.52 0.52 0.52 0.56 0.58 0.59 0.62 0.62 0.62 0.64 0.66 GeO2 MnO2 Rutile-type Ti[6] O2 AX2 0.36 0.39 12.4 Ionic Structures 259 260 12 Fundamentals of Crystal Chemistry In Table 12.4, a number of AX and AX2 compounds are listed, arranged according to structure type. The radius ratio values are also given. The agreement between theory and experiment is reasonable, considering that the use of radius ratios makes the assumption that ions are hard spheres. 12.4.4 Tetrahedral Coordination [4] Table 12.1g shows the tetrahedron as a coordination polyhedron. A suitable radius ratio can also be calculated for tetrahedral [4]-coordination. In Fig. 12.13a, a coordination tetrahedron is shown inscribed in a cube. Figure 12.13b shows a section through the cube and tetrahedron parallel to (110), with the radii √ of ions drawn to scale. Since RA + RX is half the body diagonal of the cube ( 12 3) and RX is half of √ √ √ the face diagonal ( 12 2), (RA + RX )/RX = 3/ 2, and RA /RX = 32 − 1 = 0.225. This implies that tetrahedral coordination will have a range of stability for 0.225 < RA /RX < 0.41. Important examples of this coordination are the sphalerite or zinc blende (Zn[4] S) structure (Fig. 12.14), the wurtzite (Zn[4] S) structure (Fig. 12.15) and all modiﬁcations of SiO2 except stishovite. Figures 12.16 and 12.25 show the structures of diﬀerent modiﬁcations of Si[4] O2 . The SiO4 tetrahedra build a framework structure through the sharing of vertices. The radius ratio for SiO2 is 0.29. Fig. 12.13a,b Coordination tetrahedron A[4] X4 , inscribed in a cube (a); (110)-section through a coordination tetrahedron derived from sphere packing (b) Fig. 12.14 Fig. 12.15 Fig. 12.14 Zn[4] S-structure (sphalerite or zinc blende). Space group F4̄3m. Lattice: cubic F. Basis: S at 0,0,0; Zn at 14 , 14 , 14 Fig. 12.15 Zn[4] S-structure (wurtzite). Space group P63 mc. Lattice: hexagonal P. Basis: S at 0,0,0; 2 1 1 1 2 1 1 3 , 3 , 2 ; Zn at 0,0, 2 +z; 3 , 3 ,z (z ≈ 8 ) 12.4 Ionic Structures Fig. 12.16a,b Linking of pairs of tetrahedra (a) and octahedra (b) through a vertex, an edge and a face. The numbers give the relative distances apart of the two coordinated cations, after Pauling [34] The bonding in both Zn[4] S structures is, in fact, largely covalent in nature. If, however, the geometry alone is considered, the S-atoms in the sphalerite structure occupy the positions of a cubic closest packing, and in the wurtzite structure those of a hexagonal closest packing. In both structures, the Zn-atoms occupy half of the tetrahedral holes. How, then, do the basic principles for the formation of ionic structures work out in practice? • In general, ionic structures have space groups of high symmetry, e.g. CsCl: P4/m3̄2/m; NaCl and CaF2 : F4/m3̄2/m. Structures based on the closest packing of anions retain the space groups of those arrangements when the interstices of a particular type are completely ﬁlled, e.g. Na[6] Cl: F4/m3̄2/m (Fig. 12.10). When the interstices are only partly ﬁlled, the symmetry may be lowered, e.g. Al2 [6] O3 : R3c. • The packing eﬃciency of ionic structures is usually high: for the ideal CsCl type, with RA /RX = 0.73, it is 0.73; for the NaCl type with RA /RX = 0.41, it is 0.79. As the radius ratio increases for a particular structure type, the packing eﬃciency decreases. For the structure of the NaCl type, for example, with RA /RX = 0.54 (cf. Fig. 12.9a) it is 0.66. • In ionic structures, the commonly occurring coordination numbers, [8], [6], and [4], are dependent on radius ratio and are relatively small. A better correlation is obtained if only the coordinations of the anions are considered, e.g. NaCl and Al2 O3 : Coordination number [12]. Finally, the linking of coordination polyhedra in ionic compounds should be considered. Linking by shared vertices is favorable. The sharing of edges, and in particular the sharing of faces lowers the stability of a crystal structure. This eﬀect is greatest when a cation has a high charge or a low coordination number: Pauling’s 261 262 12 Fundamentals of Crystal Chemistry third rule. In Fig 12.16, the linking of pairs of tetrahedra and octahedra through a vertex, an edge and a face are shown. Taking the distance between cations in the vertex-sharing polyhedra to be 1, the values in Fig. 12.16 show the decrease in cation–cation distance in the edge- and face-sharing cases. Note that it is more severe for the linked tetrahedra (0.55, 0.38) than for the linked octahedra (0.71, 0.58). The closer the cations come to one another, the greater is the Coulombic repulsion, and the lower the stability of the structure. The eﬀect is greater when the cations have higher charge. The SiO4− 4 tetrahedra of numerous silicate structures, and of SiO2 structures, share vertices (cf. the Si[4] O2 structures in Figs. 12.17 and 12.25). There are a few exceptions; stishovite, Si[6] O2 , for example, has the rutile structure. In the ﬂuorite structure (Fig. 12.11b), the coordination cubes share edges. In the NaCl and NiAs structures, the cations have octahedral coordination. This coordination is indicated on the structures, in Figs. 12.18 and 12.19. In NaCl, the octahedra share edges, in NiAs, they share faces. Comparison in this respect of the Na[6] Cl and Cs[8] Cl structures favors the NaCl structure, since the Cs+ ions have a cubic coordination in which all cube faces are shared. The coordination octahedron of the rutile structure (Fig. 10.18) shares two edges. This becomes clear when the unit cells above and below that shown are considered. Fig. 12.17 Structure of high cristobalite, Si[4] O2 , Fd3̄m Fig. 12.18 The NaCl structure, showing the edge-sharing coordination octahedra. Every edge is shared by two octahedra 12.5 Covalent Structures Fig. 12.19a,b Ni[6] As structure, P63 /mmc. Lattice: hexagonal P. Basis: As 0,0,0; 23 , 13 , 12 Ni 13 , 23 , 14 ; 1 2 3 3 , 3 , 4 . a Perspective drawing. b As projection on (0001). The As-octahedra are face-sharing Two other forms of TiO2 , brookite and anatase, have coordination octahedra which share three and four edges respectively. The rutile structure is thus the most stable form of TiO2 , and, unlike brookite and anatase, its structure is adopted by many compounds. 12.5 Covalent Structures Covalent or homopolar bonding will be illustrated by the diamond structure, which consists entirely of carbon atoms. The outer shell of a carbon atom in free space is occupied by 2s2 2p2 -electrons. We may consider one electron promoted to give 2s1 2p3 and the resulting set mixed to form a set of four sp3 orbitals, pointing to the corners of a tetrahedron (Fig. 12.1g). Each C-atom can form bonds with a maximum of four other C-atoms. This results in the formation of a crystal structure, based on tetrahedra (Fig. 12.20), which has the same overall ordering of atoms as the sphalerite type in Fig. 12.14. Each C-atom is surrounded by a tetrahedron of four other C-atoms. In this case, the picture of bonding as sphere-packing is inapplicable as the main forces are due to the directional bonding of overlapping atomic orbitals. The packing eﬃciency of the C-atoms in diamond is not high. The bonding in diamond is exceptionally strong, resulting in its great hardness. Fig. 12.20 Diamond structure, Fd3̄m Lattice: Cubic F. Basis: C at 0,0,0 and 14 , 41 , 14 263 264 12 Fundamentals of Crystal Chemistry 12.6 Isotypes, Solid Solutions and Isomorphism D Crystals which have the same crystal structure are said to belong to a structure type or to be isotypes. Isotypes are generally characterized by having the same space group, analogous chemical formulae, and the same coordination polyhedra occupying the same sites. Neither the absolute size of the atoms nor the type of chemical bonding is important; ionic NaCl and metallic PbS crystals are isotypes, as are metallic Cu and van der Waals Ar crystals. The relationship between isotypic structures becomes closer if atoms in one structure can replace those in the other. The following experiment will illustrate this. Two single crystals of the isotypic structures Au and Ag are pressed together as the temperature is raised, but kept below the melting point of either crystal. By diffusion, silver atoms pass into the gold crystal and occupy the places vacated by gold atoms, while gold atoms similarly diﬀuse into the silver crystal. This diﬀusion can proceed to such an extent that eventually, in some parts of the mass, an atomic ratio Au: Ag of 1:1 is reached. The single crystal nature of the starting materials is apparently lost. In some regions, arrangements of atoms like that in Fig. 12.21 will occur. Figure 12.21a shows the initial situation, with separate crystals of Ag and Au, while Fig. 12.21b gives the situation after the diﬀusion process. The diﬀusion process has distributed the Au and Ag atoms statistically over the sites of the crystal structure. Fig. 12.21 a Single crystals of Ag and Au pressed against one another. b The resultant solid solution Ag, Au resulting from diﬀusion of one metal into the other. Only a single layer at x,y,0 is shown 12.6 Isotypes, Solid Solutions and Isomorphism D Crystals in which one or more positions are occupied by a statistical distribution of two or more diﬀerent atom types are called mixed crystals or solid solutions. The reciprocal exchange of atoms in crystals is referred to as diadochy or replacement. The chemical formula is also an indication that a crystal structure is actually a solid solution. Interchangeable atoms are written together in a chemical formula, separated by a comma. The solid solution described above would be written as Ag, Au. K(Cl, Br) describes a solid solution in which Cl– and Br– replace one another. In olivine, (Mg, Fe)2 SiO4 , the oxide ions form an hcp array. The Mg2+ and Fe2+ ions are statistically distributed over speciﬁc octahedral holes. Solid solutions form most commonly when the replaceable atoms or groups of atoms are most similar in chemical properties and size. A rule of thumb for solid solution formation is that the radii of the interchangeable atoms should diﬀer by no more than 15%. Silver and gold are miscible in all proportions (RAg = 1.44 Å, RAg = 1.44 Å, diﬀerence ~ 0.0%). Ag, Au solid solutions are generally formed by slow cooling of a mixture of melts of the two components. Copper and gold are only miscible in all proportions at high temperatures (RCu = 1.28 Å, ~ 11%). During slow cooling the (Cu, Au) solid solution is converted to ordered structures, called superstructures. The superstructures with composition Cu3 Au and CuAu are given in Fig. 12.22. Note that CuAu is tetragonal, and no longer cubic. Gold and nickel ( ~ 14%) are also miscible at high temperature. At lower temperature, the solution separates into Ni-rich and Au-rich solid solutions. The separation can be essentially complete, so that only pure Ni and Au domains remain. Solid solutions in which one atom directly replaces another are called substitutional solid solutions. Plagioclases are solid solutions whose limiting compositions are NaAlSi3 O8 (albite) and CaAl2 Si2 O8 (anorthite). Here, the formation of a solid solution occurs through the simultaneous substitution of Ca for Na and Al for Si, or vice versa. In order to keep the charges balanced, the general formula for a plagioclase is: (Na1–x Cax ) (Al1+x Si3–x ) O8 , where 0 < x < 1. (0: albite; 1: anorthite). When crystals of the same structure type (isotypic crystals) form solid solutions with one another, the structures are said to be isomorphous. As the following examples will show, however, solid solution formation is no criterion for isotypy. Fig. 12.22 a The CuAu structure. b The Cu3 Au structure as superstructures of the Cu, Au solid solution 265 266 12 Fundamentals of Crystal Chemistry Zn[4] S (sphalerite-type, Fig. 12.14) and FeS (Ni[6] As-type, Fig. 12.19) are clearly not isotypic. In sphalerite, however, a (Zn, Fe) substitution up to about 20% is possible. Fe2+ and Zn2+ are bivalent ions with almost equal radii of 0.74 Å. A substitution (Fe, Zn) in FeS does not occur. The occurrence of substitution is thus not only dependent on the size of the atoms but also on the properties of the crystal structures. Ag[6] Br (NaCl-type) and Ag[4] I (sphalerite-type) show limited solid solution formation. In AgBr, a (Br/I) substitution of up to 70% I− is possible, while in AgI, substitution of Br– occurs only very slightly. Li[6] Cl (NaCl-type) and MgCl2 (CdCl2 -type, a layer structure) have not only different crystal structures, but also diﬀerent chemical formulae. In both cases, the Cl– ions form ccp arrays, and Li+ and Mg2+ occupy octahedral holes in these arrays. All octahedral holes are occupied in LiCl, while in MgCl2 , only every second hole is occupied. When solid solutions are formed, a Mg2+ ion occupies one Li+ site in LiCl, and causes another Li+ site to be vacant. Similarly, when a Li+ ion occupies a Mg2+ site, another Li+ ion will occupy one of the empty octahedral holes in MgCl2 . 12.7 Polymorphism Under diﬀerent conditions, many solid substances can produce diﬀerent crystal structures of the same chemical constitution. This phenomenon is known as polymorphism. Nickel crystallises in both the Cu[12] -type (ccp) and the Mg[12] -type (hcp), zirconium in both the Mg[12] -type (hcp) and the W[8] -type (bcc), and Zn[4] S in both the sphalerite and wurtzite types. CaCO3 can give crystals of both the calcite-type (Ca[6] CO3 ) and the aragonite-type (Ca[9] CO3 ). These CaCO3 structures naturally produce diﬀerent morphologies (cf. Table 9.11.8 and 20). The interconversion of polymorphs, also called structure transformations, can proceed in a variety of ways. Buerger [7] distinguished the following types of transformation: 12.7.1 Transformations of First Coordination The transformation alters the coordination numbers, and thus the arrangement of nearest neighbors. The new structure thus has new coordination numbers. 12.7.1.1 Dilatational Transformations Cs[8] Cl is converted, above 445◦ C, to the Na[6] Cl type. The CsCl structure (Fig. 12.23a) is converted to the NaCl structure by a dilatation along a body diagonal 12.7 Polymorphism Fig. 12.23a,b Dilatational transformation in the ﬁrst coordination. The Cs[8] Cl structure (a) is converted by means of a dilitation along the body diagonal of the cube into the Na[6] Cl structure. (b) (After [5]) of the cube (Fig. 12.23b). From the cubic arrangement of the Cl– ions (a cube is a special rhombohedron with a 90◦ angle) arises a rhombohedral arrangement with a 60◦ angle. A rhombohedral P-cell with α = 60◦ is a cubic F-lattice (cf. Sect. 7.4). The movement of the Cl– ions causes the Cs+ ions to lose two neighbors, and the cubic coordination is transformed to octahedral. Dilatational transformations are rapid. 12.7.1.2 Reconstructive Transformations Ca[9] CO3 (aragonite) is converted about 400◦ C to Ca[6] CO3 (calcite). The coordination number falls from [9] to [6]. The bonds between Ca2+ and CO3 2− are broken and reformed. Another example of this type of transformation is the conversion of Zr from the Mg[12] -type (hcp) to the W[8] -type (bcc). Reconstructive transformations are very slow. In Table 12.5, examples are given of compounds crystallizing in the calcite and aragonite structure types, with the radii of the cations. RCa 2+ = 0.99 Å is the limiting radius for the two types. Smaller cations ﬁt well into the [6]-holes of the calcite Table 12.5 The occurrence of the calcite and aragonite structures as a function of cation radius Structure type Formula Cation radius (Å) Coordination number Calcite MgCO3 FeCO3 ZnCO3 MnCO3 CdCO3 CaCO3 0.66 0.74 0.74 0.80 0.97 0.99 [6] CaCO3 SrCO3 PbCO3 BaCO3 0.99 1.12 1.20 1.34 [9] Aragonite 267 268 12 Fundamentals of Crystal Chemistry structure, while larger ones ﬁt better into the [9]-holes of the aragonite structure. Ca2+ ions can form both structures. Raising the temperature favors the conversion of Ca[9] CO3 (aragonite) to Ca[6] CO3 (calcite), while raising the pressure converts calcite to aragonite. These observations may be summarized by the rules: ! higher temperatures favor lower coordination numbers; higher pressures favor higher coordination numbers 12.7.2 Transformations in Secondary Coordination In these cases, the arrangement of nearest neighbors, i.e. the coordination, is unchanged. The arrangement of next-nearest neighbors is changed. Figure 12.24 shows such a change diagrammatically. The three structures are all made up of planar AB4 “polyhedra” which are interconnected in diﬀerent ways. 12.7.2.1 Displacive Transformations These involve a direct conversion of (a) into (b) (Fig. 12.24). The polyhedra undergo rotation only, and no bonds are broken. An angle A-B-A which is less than 180◦ in (a) becomes equal to 180◦ in (b). The density falls and the symmetry rises. Low and high-quartz structures, Si[4] O2 are three-dimensional networks of SiO4 tetrahedra, which share vertices with one another. In right-handed low-quartz (P32 2) (cf. Table 9.11.18), these tetrahedra form a helix about a 32 -screw axis, parallel to the c-axis. In right-handed high-quartz (P62 22), this becomes a 62 -screw axis. Figure 12.24 gives a projection of both structures on to (0001). At 573◦ C, a displacive transformation between low- and high-quartz occurs. The two structures are very similar; only a small rotation of one tetrahedron relative to another has occurred. The conversion of low- to high-quartz lowers the density from 2.65 to 2.53 g cm–3 (600◦ C). 12.7.2.2 Reconstructive Transformations Consider the conversion of (b) to (c) in Fig. 12.24. For this to occur, the bonds in b must be broken, so that the 4-membered rings of (b) may be rebuilt into the 6-membered rings of (c). When high-quartz is heated above 870◦ C, it undergoes a reconstructive transformation to high-tridymite (P63 /mmc, Fig. 12.25c). The tridymite structure consists of 6-membered rings of SiO4 tetrahedra, which are packed above one another, normal to the c-axis. 12.7 Polymorphism Fig. 12.24a–c Transformations in the secondary coordination sphere for structures based on square AB4 coordinations. a ↔ b is displacive, b ↔ c is reconstructive. (After [5]) The transformation between sphalerite and wurtzite is also reconstructive. Displacive transformations require little energy and are relatively rapid; reconstructive ones require more energy and are very slow. 12.7.3 Order-Disorder Transformations Copper and gold are miscible in all properties at high temperatures. In the (Cu, Au)-solid solution, the Cu and Au atoms are statistically distributed over the sites of the ccp crystal structure (disorder). On cooling, there is an ordering through the formation of the CuAu and Cu3 Au superstructures (Figs. 12.21 and 12.22, cf. Sect. 12.6). 269 270 12 Fundamentals of Crystal Chemistry Fig. 12.25a–c Transformations in the secondary coordination of Si[4] O2 structures shown as projections on (0001). a ↔ b Displacive: right-handed low-quartz (P32 2) ↔ right-handed high-quartz (P62 22). b ↔ c Reconstructive: right-handed high-quartz (P62 22) ↔ high-tridymite (P63 /mmc). a, b after [39] 12.8 Further Information on Crystal Structures 12.7.4 Transformations Involving Changes in Type of Bonding Carbon occurs as diamond (Fig. 12.20), graphite (Fig. 12.26) and the various fullerenes (e.g. C60 , Fig. 12.6a). In diamond, the bonding throughout the crystal is covalent. In graphite and in the fullerenes, covalent bonds hold the atoms in the layers or molecules while van der Waals forces hold layers and molecules together. Transformations of this sort are very slow. In the graphite structure, the carbon atoms are ordered in 6-membered rings in the layers. The coordination “polyhedron” in this case is an equilateral triangle [3] (Table 12.1h). The layer stacking can repeat itself at intervals of either two or three layers (Fig. 12.26). Both of these structures have been observed. This special form of polymorphism is called polytypism. In these polytypic structures, (a) gives a hexagonal unit cell and (b) a rhombohedral. The structures are thus labelled as the 2H- and the 3R-polytypes of graphite, respectively. Fig. 12.26a,b Polytypes of graphite structure. a 2H; b 3R. After [37] 12.8 Further Information on Crystal Structures In this chapter, only a few, albeit very important, crystal structures have been described. The basic ideas and vocabulary have, however, been introduced to enable the reader to read the extensive literature on crystal structures. The following “classical” references are particularly recommended: [26], [42]–[45], [49]. The number of determined crystal structures has now reached several hundred thousand, and to deal with this ﬂood of information, various databanks have been established. The most important two of these are: 271 272 12 Fundamentals of Crystal Chemistry (1) ICSD (Inorganic Crystal Structure Database, FIZ, Karlsruhe, Germany and NIST, Gaithersburg MD, USA) [Inorganic and mineral structures – generally non-molecular] (2) CSD (Cambridge Crystallographic Database, Cambridge, UK) [Molecular organic and organometallic structures] (3) COD (Crystallography Open Database) The use of these databanks is not free, but in most countries arrangements have been made so that students can gain access to them. 12.9 Exercises Exercise 12.1 Calculate the ideal radius ratio RA/ RX for the coordination polyhedra: trigonal prism [6] and equilateral triangle [3] (cf. Table 12.1). Exercise 12.2 Give a description of the following structures in terms of lattice + basis: a) b) c) d) e) α-Polonium (cubic P-lattice), cf. Fig. 3.1. Tungsten (cubic I-latice), cf. Fig. 12.5. Magnesium (hexagonal closest packing) cf. Fig. 12.3. Copper (cubic closest packing) cf. Fig. 12.2. Draw four unit cells of the Mg-structure in projection on (0001). Find those symmetry elements which characterise the structure as hexagonal. Exercise 12.3 Calculate the radii of the atoms in the structures in Exercise 12.2, using the following lattice parameters: a) b) c) d) α-Po: a0 =3.35 Å. W: a0 =3.16 Å. Mg: a0 =3.21 Å, c0 =5.21 Å. Cu: a0 =3.61 Å. Compare these values with those given in Fig. 12.7. Exercise 12.4 Calculate the ideal c0 /a0 ratio for hexagonal closest packing. Exercise 12.5 The packing eﬃciency is the ratio of the sum of the volumes of the atoms making up a unit cell to the volume of the cell itself. Calculate the packing eﬃciencies of: a) b) c) d) α-Polonium (cubic P-lattice). Tungsten (cubic I-lattice). A hexagonal closest packing. A cubic closest packing. 12.9 Exercises Exercise 12.6 The diamond structure has: lattice: cubic F, a0 =3.57 Å basis: C: 0,0,0; 14 , 14 , 14 . a) Draw a projection of the structure on x,y,0. sketch tapered C–C bonds with colors indicating the height (use green for 0<z< 12 and red for 12 <z<1 b) c) d) e) Calculate the length of a C–C bond. What is the value of Z? Describe the structure. Compare the diamond structure with that of sphalerite (Fig. 12.14). Exercise 12.7 The graphite (2H) structure has lattice: hexagonal P: a0 =2.46 Å; c0 =6.70 Å. basis: C: 0,0,0; 0,0, 12 ; 13 , 23 ,0; 23 , 13 , 12 . a) Draw a projection on four unit cells on x,y,0. join each C-atom to its three nearest neighbors with the same z-coordinate with colored lines (z=0 green, z = 12 red). b) c) d) e) Calculate the length of a C–C bond. What is the value of Z? Describe the structure. How large is the inter-layer spacing? Calculate the densities of diamond and graphite and comment on the diﬀerence. Exercise 12.8 LiCl (NaCl-type; a0 =5.13 Å) has an arrangement of Cl− ions which is cubic closest packed (RA/ RX =0.43). Calculate the ionic radii of Cl– and Li+ and the packing eﬃciency of the LiCl structure. 273 274 12 Fundamentals of Crystal Chemistry Exercise 12.9 Draw the ions on the x,y,0-plane of the NaCl (a0 = 5.64 Å), LiCl (a0 =5.13 Å) and RbF (a0 =5.64 Å). The ionic radii can be taken from Fig. 12.7. Exercise 12.10 Calculate the Ti–O distance in the coordination octahedron of the rutile structure (cf. Table 10.5). Which distances are equivalent by symmetry, and hence required to be equal? Exercise 12.11 The pyrites structure (FeS2 ) has: a) Space group Pa3 (P21 /a3) Fe: 4a 3 0,0,0; 0, 12 , 12 ; 12 , 12 ,0; 1 1 2 +x, 2 −x,x; x,x,x; 12 −x, 12 +x,x; Lattice constant: a0 =5.41 Å. S: 8c 3 x,x,x; b) 1. 2. 3. 4. 5. 1 1 2 ,0, 2 . x, 12 +x, 12 −x; x, 12 −x, 12 +x; 1 1 2 −x,x, 2 +x; 1 1 2 +x,x, 2 −x, (x=0.386). Draw the structure as a projection on x,y,0 (let a0 =10 cm). Describe the structure. What is the value of Z? Calculate the shortest Fe–S and S–S distances. Draw the symmetry elements on the projection. Exercise 12.12 A compound of NH4 /Hg/Cl has: a) Space group P4/mmm. b) Lattice constants: a0 = 4.19 Å, c0 = 7.94 Å. c) Positions: Hg: 0,0,0 NH4 : 12 , 12 , 12 Cl(1): 12 , 12 ,0 Cl(2): ± (0,0,z) z = 0.3 1. Draw a projection of the structure on 0,y,z (1 Å=1 cm). 2. Give the chemical formula of the compound, and the value of Z. 3. Describe the coordination of Hg and NH4 , giving the coordination number and the coordination polyhedron. 4. Calculate the shortest Hg−Cl and NH4 −Cl distances. 5. What assumption has been made in assigning the space group in a)? Exercise 12.13 The cystal structure of BaSO4 has: a) Space group Pnma with special and general positions: (4c) ±(x, 14 ,z; 12 +x, 14 , 12 −z) (8d) ± (x,y,z; x, 12 +y,z; 12 +x, 12 −y, 12 −z; 12 −x,y, 12 +z) b) Lattice constants: a0 =8.87 Å, b0 =5.45 Å, c0 =7.15 Å. c) Occupation of positions: 12.9 Exercises Position multiplicity and Wyckoﬀ letter x Ba (4c) 0.18 S (4c) 0.06 O(1) (4c) −0.09 O(2) (4c) 0.19 O(3) (8d) 0.08 1. Draw a projection of the structure on x,0,z. 2. What is the value of Z? 3. Determine the coordination of O atoms around S. y 1 4 1 4 1 4 1 4 0.03 z 0.16 0.70 0.61 0.54 0.81 275 13 Studies of Crystals by X-Ray Diﬀraction Since the wavelengths of X-rays and the lattice parameters of crystals are of the same order of magnitude, X-rays are diﬀracted by crystal lattices. It was from the discovery of this eﬀect in 1912 by Max von Laue that we may date the beginning of modern crystallography. Only then did it become possible to determine the structures of crystals. We shall only describe here one X-ray method, the Debye-Scherrer technique, in detail, because it is a very important research tool for the scientist. Also, a brief description will be given of how a crystal structure may be determined. For a fuller description of X-rays and their properties, the reader is referred to textbooks of physics. 13.1 The Bragg Equation The diﬀraction of X-rays by crystals can be formally described as a reﬂection of X-rays from sets of lattice planes. Assume that a parallel, monochromatic beam of X-rays (i.e. one characterized by a single wavelength λ) falls on a set of lattice planes with a spacing of d, making a glancing angle of θ with them (Fig. 13.1). The waves I and II will be reﬂected at A1 and B, and will thus undergo interference. At the point A1 , the waves will have had a path diﬀerence Γ = BA1 −A1 B = BA3 −BC = CA3 , since BA1 = BA3 and B A1 = BC. Thus, sin θ = Γ 2d (13.1) An interference maximum will be observed when is an integral multiple n of λ, or = nλ, where n is the order of the interference. D This gives rise to the Bragg equation: nλ = 2 d sin θ W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_13, C Springer-Verlag Berlin Heidelberg 2011 (13.2) 278 13 Studies of Crystals by X-Ray Diﬀraction Fig. 13.1a Diﬀraction (“reﬂection”) of an X-ray beam by a set of lattice planes. b Interference of waves reﬂected by a set of lattice planes (Γ = 1λ) 13.2 The Debye-Scherrer Method In the Debye-Scherrer method, a ﬁne powder of a crystalline substance is irradiated with monochromatic X-rays. According to the Bragg equation, a set of parallel planes (hkl) will reﬂect X-rays with certain characteristic glancing angles θ (Fig. 13.2a). Since the crystallites are randomly arranged in a ﬁne powder, there will always be a large number of crystals orientated in such a way that a given set of planes (hkl), which make an angle θ with the X-ray beam can cause reﬂection to occur. These planes are tangent to the surface of a cone with a cone-angle of 2θ . The beams reﬂected by these planes lie on the surface of a cone with a cone angle of 4θ (Fig. 13.2b). Figure 13.2c shows the reﬂection cones of a few diﬀerent sets of planes. In the Debye-Scherrer method, a cylindrical camera is used with the powdered specimen, contained in a thin tube mounted along the cylinder axis. The cones of reﬂection intersect the ﬁlm in Debye-Scherrer lines (Fig. 13.2c, d). The angle between pairs of lines originating from the same cone is 4θ . Thus 4θ S = 2π R 360◦ (13.3) where R is the radius of the camera. For R = 28.65 mm (2π R = 180 mm), the measured value of S in mm is thus equal to the value of 2θ in degrees. In order to obtain information from X-ray photographs, it is necessary to index the reﬂections, i.e. to determine which set of lattice planes gave rise to the observed interference. Since the value of θ is easy to read from the photograph and λ is known, the Bragg equation allows d, the spacing of the lattice planes, to be calculated. How are these d-spacings related to (hkl)? The plane lying next to the one which passes through the origin in Fig. 13.3 intercepts the orthorhombic axes at the point m00 (a-axis), 0n0 (b-axis) and 00∞ (c-axis), cf. Sect. 3.4.3. 13.2 The Debye-Scherrer Method Fig. 13.2a Relationship between the primary beam and a ray diﬀracted by the lattice planes (hkl). b Possible orientations of the set of planes (hkl) in a crystalline powder. The result of the random orientation of the planes giving a glancing angle of θ is a cone with a generating angle of 4θ. c, d The rays diﬀracted from the various lattice planes lie on concentric cones about the primary beam. Their intersections with the ﬁlm give rise to the “lines” of the powder diagram. (After Cullity [13]) Fig. 13.3 Relationship between the Miller indices of a set of lattice planes and the spacing of the planes d for an orthorhombic crystal 279 280 13 Studies of Crystals by X-Ray Diﬀraction For a set of planes (hkl), considering only the plane nearest the origin: d h =d· m · a0 a0 d k =d· cos ϕb = n · b0 b0 cos ϕa = (13.4) (13.5) d l2 =d· p · c0 c0 cos ϕc = (13.6) Squaring these and adding them together gives: 2 2 2 2 cos ϕa + cos ϕb + cos ϕc = d · dhkl = h2 k2 l2 + + a20 c20 b20 =1 1 h2 k2 l2 + + a20 c20 b20 (13.7) (13.8) this relationship applies to the orthorhombic system. In the cubic system, it simpliﬁes to dhkl = a0 2 h + k2 + 12 . (13.9) Substituting this equation for the d-spacing into the Bragg equation and squaring gives: sin2 θ = λ2 · (h2 + k2 + 12 ). 4a20 (13.10) The right-hand side of this equation is the product of a constant factor λ2 /4a20 and an integer (h2 + k2 + l2 ). The values of sin2 θ for individual reﬂections are thus related to one another as integers. The powder pattern for tungsten in Fig. 13.4 was taken with CuKα radiation, λ = 1.54 Å. Table 13.1 shows the calculations for this photograph. Note that this Fig.13.4 Powder diagram of tungsten (reduced to 0.65 of original size) 13.2 The Debye-Scherrer Method Table 13.1 Interpretation of the powder pattern of tungsten S (mm) θ(◦ ) 1 40.3 20.15 2 58.3 29.15 3 73.2 4 Reﬂection number sin2 θ = λ2 · (h2 + k2 + l2 ) 4a20 hkl dhkl (Å) 0.1187 = 0.0594·2 110 2.24 0.2373 = 0.0593·4 200 1.58 36.60 0.3555 = 0.0592·6 211 1.29 87.1 43.55 0.4744 = 0.0593·8 220 1.12 5 100.8 50.40 0.5937 = 0.0594·10 310 1.00 6 115.0 57.50 0.7113 = 0.0592·12 222 0.91 7 131.2 65.60 0.8294 = 0.0592·14 321 0.85 8 154.2 77.10 0.9502 = 0.0592·16 400 0.79 table includes the reﬂections 200, 220 and 400, which contravene the deﬁnition of Miller indices as they do not represent the smallest integral multiples of the reciprocals of intercepts on the axes. In fact, they are Miller indices multiplied by the factor n, the order of diﬀraction. In other words, 200 may be regarded as the second order of diﬀraction from the (100) planes. These hkl triples, written without brackets, are called Laue symbols, and their use makes the factor n of the Bragg equation unnecessary. From the constant factor λ2 /4a20 = 0.0592, the lattice parameter a0 = 3.16 Å may be determined. Z, the number of formula units per unit cell, can also be determined (cf. Chap. 4) Z= · V · NA M (13.11) Z= 19.3 · 3.163 · 10−24 · 6.022 · 1023 183.86 (13.12) Z∼2 (13.13) A cubic structure of an element with Z = 2 can only occur if the substance has a cubic I–lattice, cf. Fig. 12.5. In Table 13.1, 100, 111 and 210 do not occur. Such absences occur in structures which have centered lattices or contain glide planes or screw axes. The absent reﬂections are said to be extinct. Those reﬂections which do occur in Table 13.1 obey the rule h+k+l = 2n, where n is an integer, and this is characteristic for all structures with an I-lattice. The number of reﬂections which can be observed on an X-rays photograph is λ λ , −1 ≤ sin θ ≤ +1. Thus 2d ≤ +1. and limited. In the Bragg equation sin θ = 2d λ d ≥ 2 . Diﬀraction can only arise from those sets of lattice planes for which d ≥ λ2 . For CuKα radiation, λ = 1.54 Å, the limiting value for d is thus 0.77 Å. The pattern for tungsten thus contains no reﬂections with a d-value ≤ λ2 = 0.77 Å. 281 282 13 Studies of Crystals by X-Ray Diﬀraction The greatest use of the Debye-Scherrer method is in the identiﬁcation of crystalline substances. Every sort of crystal produces a pattern of lines with characteristic positions and intensities. The intensity is roughly proportional to the blackness of a photograph. The American Society for Testing Materials published an index (the ASTM index) containing data for all crystalline inorganic and organic substances which have been studied by X-ray diﬀraction. This index is now administered by the Joint Committee for Powder Diﬀraction Standards (JCPDS) at the International Centre for Diﬀraction Data in Swarthmore, USA. The PDF now contains data for more than 200,000 crystalline samples on CD-Rom. Every substance has an “index card” which contains many crystallographic data: the crystal system, space group, lattice constants, number of formula units per unit cell and density, as well as the d-values or 2θ-values, the relative intensities (strongest = 100) and the hkl-values for individual reﬂections. The PDF-card for tungsten is given in Table 13.2. The identiﬁcation of an unknown substance depends on the correspondence between the powder diagram for the specimen and a diagram stored on the PDF. The search routine normally begins with the identiﬁcation of the three lines of highest intensity. The use of known chemical or physical properties, such as the density, can also assist the search. 13.3 The Reciprocal Lattice Crystals are three-dimensional systems. A stereographic projection, which gives a useful summary of the arrangements of the crystal faces with respect to one another, can be derived simply from a consideration of the morphology of a crystal. As described in Sect. 5.4, the normals to the crystal faces are used for this purpose. An alternative system for representing the lattice planes was proposed by P.P. Ewald to discuss the scattering of X-rays by the crystal lattice. Since, as is described in Sect. 13.1, the diﬀraction of X-rays can be interpreted as the reﬂection of the rays by sets of parallel lattice planes, it was important to devise an aid to illustrate both the orientations of the lattice planes and their diﬀraction. This aid is the “reciprocal lattice”. Each set of lattice planes in the crystal is represented by a point in the reciprocal lattice. The construction of a “reciprocal lattice” from the corresponding “direct lattice” may be performed as follows: For each set of lattice planes (hkl), the normal is drawn from the origin with a length d∗ = dC , where d is the lattice hkl spacing and C is a proportionality constant. The construction of the reciprocal lattice corresponding to the projection on (010) of a direct monoclinic P-lattice is shown in Fig. 13.5. The normal to the set C . The of lattice planes (001) is drawn from the origin and assigned a length d∗ = d001 ∗ resulting point is called P001 . A similar construction for the set of (100) planes gives the point P∗100 . The points P∗001 and P∗100 represent the relative orientations of the (001) and (100) lattice planes. d–sp: I/Icor.: 18.00 Beta Dm: SS/FOM: F8 =108 (.0093,8) Z: 2 mp: C: Color: Gray metallic Pattern taken at 26◦ C. Sample prepared at Westinghouse Electric Corp. CAS #: 7440-33-7. Analysis of sample shows SiO2 0.04%, K 0.05% Mo, Al2 O3 and 0.01% each. Merck Index, 8th Ed., p. 1087. W type. Also called: wolfram.PSC: cI2. Mwt: 183.85. Volume [CD]: 31.70. Dx: 19.262 Ref: Ibid. α: A: β: a: 3.1648 γ: S.G.: Im3m (229) c: b: Sys.: Cubic Ref: Swanson, Tatge, Natl. Bur. Stand. (U.S.). Circ. 539, I, 28 (1953) Filter: Ni 0.7912 0.8459 2 18 11 4 1.0008 0.9137 λ: 1.5405 8 1.1188 Int.: Diﬀract. 23 1.292 Rad.: CuKal 15 Cut oﬀ: 100 2.238 1.582 Tungsten Int. d(A) W 4 3 3 2 2 2 2 1 h 0 2 1 2 2 1 0 1 k 0 1 0 2 0 1 0 0 L Table 13.2 PDF index “card” for tungsten (© 2002 JCPDS- International Centre for Diﬀraction Data. All rights Reserved PCDFWIN v.2.3) 04–0806 Wavelength = 1.5405 13.3 The Reciprocal Lattice 283 284 13 Studies of Crystals by X-Ray Diﬀraction Fig. 13.5 Monoclinic P-lattice as a projection on (010) with the points P∗001 and P∗100 .P∗000 , P∗001 and P∗100 deﬁne a lattice, the reciprocal lattice Making use of the three points P∗000 , P∗100 and P∗001 , a two-dimensional lattice can be constructed. This reciprocal lattice plane is indicated by dashed lines in Fig. 13.5. It must now be shown that the reciprocal lattice points corresponding to all sets of lattice planes with indices (h0l) fall on this same plane. Figures 13.6, 13.7 and 13.8 show the relevant constructions for the sets of (101), (201) and (102) planes. When all relevant points are added to the drawing, its lattice-like nature is apparent (Fig. 13.9). This construction does not, however, lead to all of the points required by the reciprocal lattice. For example, P∗002 , P∗200 and P∗202 are missing since lattice planes with indices such as (002), (200) and (202) contravene the deﬁnition of Miller indices given in Sect. 3.4.3. It is, of course, possible to deﬁne a set of “lattice planes” d001 . In these “lattice planes”, only half of the planes (002) with a spacing d = 2 intersect points of the direct lattice. Furthermore, the Bragg equation (13.2) can be written in the form λ = 2 nd sin θ . If this is done, every n-th order diﬀraction with a plane spacing of d can be replaced by a ﬁrst-order diﬀraction from planes with a spacing of nd . P∗002 describes in the same way a second-order diﬀraction from the planes (001), P∗003 a third order, and so on. The same sort of reasoning applies to the points P∗200 , P∗202 , etc. (see also Sect. 13.2). The rule for constructing the reciprocal lattice given above (p. 284) is thus incomplete and should read: . . . with a length d∗ = dC , and all integral multiples thereof, where d is the lattice spacing.. . . hkl 13.3 The Reciprocal Lattice Fig. 13.6 Fig. 13.7 Fig. 13.6 Monoclinic P-lattice as a projection on (010) with the traces of the lattice planes (101) and the point P∗101 of the reciprocal lattice Fig. 13.7 Monoclinic P-lattice as a projection on (010) with the traces of the lattice planes (201) and the point P∗201 of the reciprocal lattice Fig. 13.8 Fig. 13.9 Fig. 13.8 Monoclinic P-lattice as a projection on (010) with the traces of the lattice planes (102) and the point P∗102 of the reciprocal lattice Fig. 13.9 Reciprocal lattice (a∗ c∗ -plane) corresponding to the monoclinic P-lattice of Fig. 13.5 285 286 13 Studies of Crystals by X-Ray Diﬀraction The reciprocal lattice, like the direct lattice, is deﬁned by six lattice parameters: ∗ a = a∗ = 0 1 b0 c0 sin α V a0 c0 sin β = V a0 b0 sinγ = V = d(100) 1 ∗ b = b∗0 = d(010) ∗ c = c∗ = 1 0 d (001) V = a0 b0 c0 · 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ (13.14) (13.15) (13.16) (13.17) (Volume of the unit cell) cos β cos γ − cos α α ∗ = b∗ ∧ c∗ ; cos α ∗ = sin β sin γ cos α cos γ − cos β β ∗ = a∗ ∧ c∗ ; cos β ∗ = sin α sin γ cos α cos β − cos γ ∗ ∗ ∗ ∗ γ = a ∧ b ; cos γ = sin α sin β (13.18) (13.19) (13.20) The use of the reciprocal lattice allows an elegant discussion of the application of the Bragg equation to the diﬀraction of X-rays by a lattice. Figure 13.10 shows a section through a reciprocal lattice. The direction of the primary beam is indicated by a straight line through the point P∗000 . A sphere (which in Fig. 13.10 becomes a circle) with a radius of Cλ and a center at the point M on the line is then constructed so that the surface of the sphere intersects the origin of the reciprocal lattice, P∗000 . This sphere is known as the sphere of reﬂection. In general, no point of the reciprocal Fig. 13.10 Ewald Construction 13.4 Laue Groups lattice other than P∗000 lies on the surface of the sphere. By choosing the direction of the primary beam appropriately, however, it may be possible to cause another point P∗hkl to lie on the surface of the sphere of reﬂection, as in Fig. 13.10. In this case, the condition for the Bragg equation n λ = 2d sin θ is fulﬁlled precisely for the set of planes (hkl). Diﬀraction occurs, and the diﬀracted beam has the direction MP∗hkl . The orientation of the planes (hkl) is shown in Fig. 13.10 by a dotted line. It is obvious that the diﬀracted beam with a glancing angle equal to θ can equally well be described as a reﬂection from the lattice planes (hkl). It will be noticed that for the triangle P∗hkl MT, sin θ = 1 2d 1 λ = λ 2d , fulﬁlling the Bragg condition. This geometrical construction is known as the Ewald construction. If a single crystal is rotated about an axis which is perpendicular both to the primary beam and to a selected plane of the reciprocal lattice, then the reciprocal lattice itself rotates about an axis through P∗000 . During this rotation, other points of the reciprocal lattice will pass through the surface of the sphere of reﬂection, and the corresponding lattice planes will come into the diﬀracting position. These relationships are the basis of rotating crystal methods. The precession method of M. Buerger produces an undistorted representation of the reciprocal lattice. In this technique, an axis of the crystal processes about the primary beam. The resulting picture is of the reciprocal lattice plane perpendicular to this axis. A precession photograph of β=eucryptite, LiAlSiO4 (space group P64 22) is shown in Fig. 13.11. It represents the a∗ b∗ -plane. The reciprocal lattice of a hexagonal lattice is itself hexagonal, as is shown in Fig. 13.12 which should be compared with Fig. 13.11. 13.4 Laue Groups In general, the intensity of an X-ray beam diﬀracted from one side of a set of lattice planes is equal to that diﬀracted from the other. A diﬀraction pattern is thus centrosymmetric. It follows that instead of 32 point groups only the 11 which contain an inversion center can characterize a diﬀraction pattern. These 11 point groups are known as Laue groups (cf. Table 9.10). As an example, the Laue groups of the tetragonal system will be explained. An inversion center is added to each point group: Laue group 4/m 4 + 1 → 4/m (Symmetry rule I) 4 + 1 → 4/m (cf. Fig. 6.13) The operation of an inversion center on the 4 array in (a) results in the 4/m array in (b). Laue group 4/m 2/m 2/m (4/mmm) 422 + 1 → 4/m 2/m 2/m (Symmetry rule I) 4 mm +1 → 4/m 2/m 2/m (Symmetry rule I) 42m + 1 → 4/m 2/m 2/m (4 + 1 → 4/m as above and symmetry rule I) 287 288 13 Studies of Crystals by X-Ray Diﬀraction Fig. 13.11 Precession photograph of β-eucryptite, LiAlSiO4 (space group P64 22): a∗ b∗ -plane (Photograph A. Breit) Fig. 13.12 a∗ b∗ -plane of a hexagonal reciprocal lattice, cf. Fig. 13.11 13.5 The Determination of a Crystal Structure Consideration of the ﬁrst symmetry rule together with the relationships 3 + 1 ≡ 3 and 6+1 ≡ 6/m will allow the Laue groups of the other crystal systems to be derived from each point group (cf. Table 9.10). 13.5 The Determination of a Crystal Structure Powder diﬀraction patterns allow the determination only of relatively simple structures. Techniques have been developed which make use of measurements of the intensities of the reﬂections of sets of lattice planes from single crystals. Study of relationships among intensities and “systematic absences” in the diﬀraction pattern can lead to the determination of the space group. Measurement of the density of the crystals gives Z (cf. Sect. 13.2), the number of formula units in the unit cell. The intensity of the individual reﬂections depends on the extent to which the sets of lattice planes are occupied by atoms. Since diﬀerent sets of lattice planes will vary greatly in both the number of atoms occupying them and the “heaviness”(in terms of electrons) of those atoms, the intensities of a very large number of reﬂections can allow the determination of the arrangement of atoms in the unit cell. For simple crystal structures, it is possible to make useful structural conclusions from only a small amount of data. This may be illustrated by the structure of SnO2 , cassiterite, for which the following data have been determined: 1. Lattice constants: a0 = 4.74 Å, c0 = 3.19 Å. 2. Space group: P42 /mnm 3. Density: 6.96 g cm–3 . The value of Z (the number of chemical formula units per unit cell) may be directly calculated (cf. Eq. 4.5): Z= 6.96 · 6.023 · 1023 · 4.742 · 3 · 19 · 10−24 · NA · V = = 1.99 ≈ 2 M 150.69 (13.21) Thus, there must be two formula units of SnO2 or two tin and four oxide ions per unit cell. The Sn4+ ions must then occupy a set of 2-fold positions in the unit cell, and the O2– ions a set of 4-fold positions, or (less likely) two sets of 2-fold positions. The space group, P42 / mnm, (Fig. 10.17) has two sets of 2-fold positions (a and b), and ﬁve sets of 4-fold positions (c – g). Let us see whether the ionic radii (R(Sn4+ ) = 0.71 Å, R(O2− ) = 1.32 Å) can help to select the sites which are actually occupied. In the following illustrations, the lattice constants and the ionic radii have been drawn to the same scale. First, consider the possible 4-fold position for the O2– ions. • Positions (c): These include the ﬁxed points 0,1/2,0 and 0,1/2,1/2 (Fig. 10.17). These are shown as points on the line 0,1/2,z in Fig. 13.13c, in which the lattice repeat is 289 290 13 Studies of Crystals by X-Ray Diﬀraction scaled to the actual length c0 . When the O2− ions are then drawn in to scale, it is clear that they overlap badly. • Positions (d): These also include ﬁxed points 0,1/2,1/4 and 0,1/2,3/4, which are shown as points on the line 0,1/2,z in Fig. 13.13d. When the O2− ions are then drawn in to scale, the overlap is the same as in (c). • Positions (e): Here, there is one degree of freedom to be considered. A pair of points 0,0,z and 0,0,z must both lie within the range of the lattice constant c0 (Fig. 13.13e). Whatever value is chosen for z, the overlap will be at least as bad as that in (c) and (d). Clearly, these three sets of positions are not possible for the SnO2 structure. • Positions (f): Again, there is one degree of freedom to be considered. In order to limit the possibilities for the O2− ions somewhat, the Sn4+ ions have been inserted at 0,0,0 (positions (a)) in a scale drawing of the x,y,0-plane (Fig. 13.14a). It is then possible to draw in the O2− ions at x,x,0 and x̄,x̄,0 along the diagonal between the Sn4− ions at 0,0,0 and 1,1,0. In fact, the ions ﬁll the gaps precisely! It is possible to estimate a value for x: RSn4+ + RO2− = 0.71 + 1.32 = 2.03 Å 2.03 √ = 1.44 2 1.44 = 0.304 = x a0 (13.22) (13.23) (13.24) Substituting the value x = 0.3(04) in the positions (f) gives 0.2,0.8,1/2 and 0.8,0.2,1/2 for ions 3 and 4. These are shown along with the Sn4+ ion at 1/2,1/2,1/2 in Fig. 13.14b. Figure 13.14c shows the x,x,z section through Figs. 13.14a, b. Each Sn4+ ion occupies an octahedral hole formed by six O2− ions. Fig. 13.13 Investigation of sites c, d, e in the structure of SnO2 . The O− ions cannot lie in the given places as required by the positions c to e of space group P42 /mnm 13.5 The Determination of a Crystal Structure Fig. 13.14a–c Structure of SnO2 . Placing the Sn4+ ions on positions a and the O2− ions on f leads to an acceptable arrangement. (a) the x,y,0 plane. (b) the x,y,1/2 plane. (c) the x,x,z plane The structural results may then be summarized thus: Space group P42 /mnm (Fig. 10.17). Sn4+ in 2a m.mm and O2– in 4f m.2m with x = 0.304. The currently accepted value for x is 0.3053. SnO2 has the same structure type as rutile (Fig. 10.18). • The positions (g) have not yet been considered. In fact, placing the O2− ions in these positions leads to an alternative description of the same structure. The following are a few still simpler examples; the calculation of Z will be omitted. • CsI: Z = 1. The space group is P4/m32/m, which has only two 1-fold positions: • 1 b m 3 m 1/2,1/2,1/2 • 1 a m 3 m 0,0,0 Thus, the Cs+ may be placed at 0,0,0 and the I− at 1/2,1/2,1/2 or vice-versa (cf. Fig. 4.4). • NaCl: Z = 4. The space group is F4/m32/m. Table 13.3 gives the coordinates of the positions a to d for this space group. There are two 4-fold sets of positions, so 291 292 13 Studies of Crystals by X-Ray Diﬀraction Na+ may be placed on a and Cl− on b or vice-versa, cf. Fig. 12.10. In Fig. 12.10, 1/ ,0,0 is given instead of the equivalent 1/ ,1/ ,1/ . 2 2 2 2 • CaF2 : Z = 4. Space group F4/m32/m (Table 13.3). The F− ions occupy the 8-fold positions c, while the Ca2+ ions may be placed either on a (0,0,0 etc.) or on b (1/2,1/2,1/2 etc). Either choice leads to the same structure. Table 13.3 Coordinates for some of the positions of space group F4/m3̄2/m., from [14]. (0, 0, 0)+ (0, 12 , 12 )+ 24 d m.mm 0, 41 , 41 0, 43 , 14 8 c 4̄3m 1 1 3 4,4,4 4 b m3̄m 1 1 1 4,4,4 1 1 1 2,2,2 4 a m3̄m 0,0,0 1 1 4 ,0, 4 ( 12 ,0, 12 )+ 1 3 4 ,0, 4 ( 12 , 12 ,0)+ 1 1 4 , 4 ,0 3 1 4 , 4 ,0 13.6 Exercises Exercise 13.1 Draw the (100)- and (001)-lattice planes of the rutile structure (cf. Fig. 10.18 and Table 10.5). Using the introduction in Sect. 13.3, construct the a∗ c∗ - and the a∗ b∗ -planes of the reciprocal lattice. Exercise 13.2 For the crystal structure of thallium, the lattice parameters are a0 = b0 = c0 = 3.88 Å, α = β = γ = 90◦ , and the density is 11.85 g cm-3 . Determine the crystal structure, and draw it, projected on x, y, 0. Exercise 13.3 Derive the cubic Laue groups. Exercise 13.4 A powder photograph has been taken of the cube-shaped crystals of KI, using Cu Kα radiation (λ=1.54 Å). The ﬁrst nine lines, measured from the position of the direct beam, give the following 2Θ-values: 21.80; 25.20; 36.00; 42.50; 44.45; 51.75; 56.80; 58.45; 64.65. 1. 2. 3. 4. Index these powder lines and calculate their d-values. Determine the lattice constant a0 . What is the value of Z? (The density of KI is 3.13 g cm-3 ) Suggest the structure type of KI. 14 Crystal Defects A crystal with a volume of 1 cm3 will contain about 1023 atoms. Lattice theory requires in principle that all of these atoms occupy a regular lattice. The array of atoms must conform to one of the 230 space groups. The equivalent points of a position of a space group must be fully occupied by atoms of the same type. This theoretical model is only achieved conceptually, by an ideal crystal. The observation of a large number of crystals will show that they in fact have cracks and ﬁssures, and that crystal faces are often not really ﬂat. At cleavage surfaces, crystalline domains are often displaced with respect to one another. Inclusions occur in crystals, which may themselves be crystalline, liquid or gas. In practice, a real crystal deviates considerably from the ideal model described above. All deviations from ideal crystalline behavior are described as crystal defects. Many important properties of crystals derive from defects, including luminescence, diﬀusion, mechanical properties, etc. Nevertheless, the ideal crystal structure is the starting point for all studies of crystals. Individual defects make themselves apparent in many ways. They can be categorized in terms of their dimensionality (Table 14.1). Table 14.1 Types of crystal defects 14.1 Point defects 14.2 Line defects 14.3 Plane defects (a) Subsititution defects (b) Solid solutions (c) Schottky and Frenkel defects (a) Edge dislocations (b) Screw dislocations (a) Small angle grain boundaries (b) Stacking faults (c) Twin boundaries 14.1 Point Defects Point defects are concerned with atomic dislocations. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_14, C Springer-Verlag Berlin Heidelberg 2011 294 14 Crystal Defects 14.1.1 Substitution Defects An ideal crystal must consist entirely of the substance to which its formula refers, and this situation never occurs. As there are about 1023 atoms in 1 cm3 of a crystal, even a purity of 99.99999% implies the presence of some 1016 foreign atoms! These foreign atoms will in general be larger or smaller than the atoms they replace. Furthermore, the foreign atoms may have diﬀerent bonding capacities. This can result in the propagation of further irregularities in the crystal which may no longer be of the point-defect type. In some cases, crystals with speciﬁc impurities are actually required. It is such impurities which control the electrical conductivity of many semiconductors. 14.1.2 Solid Solutions The statistical distribution of atoms in solid solutions (cf. Sect. 12.6) are also point defects. 14.1.3 Schottky and Frenkel-Defects Every crystal contains voids. These are places in a crystal where the expected atoms do not occur. If these missing atoms have “wandered” to a surface of the crystal, the result is called a Schottky defect, while if they have moved to places between other atoms (interstitial sites), the result is called a Frenkel defect. Both of these types are illustrated for an ionic crystal in Fig. 14.1. The concentration of faults in a crystal is in thermal equilibrium, and increases with rising temperature. The type of fault which occurs depends on the structure itself, its geometry and its bonding type. In alkali halides, Schottky defects predominate, while Frenkel defects predominate in silver halides. Measurement of the density of a crystal gives an indication of the defect type, since Schottky defects decrease the density (more volume for the same mass) while Frenkel defects leave the volume and hence the density unchanged. Fig. 14.1 a–c Schottky defects (a) and Frenkel defects (c) in an ionic crystal ( void); (b) the ideal crystal 14.2 Line Defects Wuestite (NaCl-structure type) does not have the ideal stoichiometry FeO, because the Fe2+ ions in some places are replaced by Fe3+ .This unbalanced charge results in a corresponding number of caption vacancies, giving a formula Fe1–x O. The occurrence of these faults gives rise to a number of properties. The defects make possible the diﬀusion of ions through the crystal. If a gold crystal and a silver crystal are pressed ﬁrmly against one another as the temperature is raised, Ag-atoms diﬀuse into the gold crystal, and Au-atoms into the silver, forming solid solutions (cf. Fig. 12.20). At suﬃciently high temperature, ionic crystals, such as NaCl, show a small electrical conductivity. This does not result from electronic conduction, as in metals, but is brought about by ionic movement. Without crystal defects, this would not occur. Solid-state reactions are almost always propagated by crystal defects. The heating of a mixture of ﬁnely powdered ZnO and Fe2 O3 crystals to a temperature well under their melting points brings about a reaction yielding crystals of the spinel zinc ferrite, ZnFe2 O4 . The rates of solid-state reactions are much less than those taking place in the gas or liquid phase. They do, however, rise with temperature as the concentration of crystal faults and the rates of diﬀusion rise. 14.2 Line Defects This type of defect forms along a line, the line of dislocation. 14.2.1 Edge Dislocations The upper portion of the crystal in Fig. 14.2a has been displaced by the vector BC (=B C ) in the plane ABA B relative to the lower portion in such a way that the line AA (the line of dislocation) marks the limit of the displacement. Figure 14.2b shows the structure of a plane normal to the line of dislocation AA . The displacement vector, which amounts to a displacement (=BC) is known as the Burgers vector b, and is normal to the line of dislocation AA . Fig. 14.2a,b Edge dislocation; pictorial (a), structural representation (b) (⊥ end of the line of dislocation) 295 296 14 Crystal Defects 14.2.2 Screw Dislocations The crystal in Fig. 14.3 contains a screw dislocation which arises from a displacement in the plane ABCD with the line of dislocation AD. In the region of the line of dislocation, the crystal does not consist of neatly stacked lattice planes, but of an arrangement of atoms which repeat through the structure in a helical manner (screw dislocation). In this case, the Burgers vector b is parallel to the line of dislocation. Fig. 14.3 Screw dislocation after Read ([36]) Edge- and screw dislocations, as described here, are only limiting cases; intermediates also occur. Dislocations are important in the plastic deformation of metals (Sect. 12.2) (movement of dislocations). Screw dislocations also play an important role in crystal growth. The deposition of atoms on a step of the helix is always energetically favorable, and these steps persist during the growth of the crystal, permanently. Dislocations are active regions in crystal faces, and etching gives rise there to characteristic etch-ﬁgures (cf. Table 9.11.21). By etching, the concentration of dislocations per cm2 can be estimated. This varies from virtually zero in the most perfect single crystals of germanium (semiconductor) to 1012 per cm2 in the most strongly deformed metals. “Whiskers”, or ultrathin, needle crystals, often form with the screw dislocation parallel to the needle axis. They display remarkable mechanical properties. For example, the breaking strength of a NaCl-whisker of 1 μm diameter is as much as 1080 N mm–2 . 14.3 Plane Defects 14.3.1 Small Angle Grain Boundaries It frequently occurs that diﬀerent domains of a single crystal are tilted by a small angle with respect to each other. Their boundary faces are small angle grain boundaries, and are built up by a series of dislocations. A small angle grain 14.3 Plane Defects Fig. 14.4 Small angle grain boundary formed from edge dislocations (θ = inclination angle) boundary, consisting entirely of step dislocations, is illustrated in Fig. 14.4. The inclination angle θ which the crystal domains make with each other, may be calculated from the Burgers vector b and the separation of the displacements D, since θ= b D 14.3.2 Stacking Faults Stacking faults are disturbances of the normal layer sequence in the building of a structure. They are most frequently observed in metals (ccp and hcp, Figs. 12.2 and 12.3) and in some layer structures (e.g. graphite, Fig. 12.26). Cobalt crystallises with both cubic and hexagonal closest packing, and it also occurs that both stacking sequences (ABCA...and ABA...) may alternate irregularly. Such an array is only periodic in two dimensions and thus does not qualify to be called a crystal. 14.3.3 Twin Boundaries D A twin is the regular growing together of crystals of the same sort. The crystals lie in a symmetric relationship to one another. The commonest twinning symmetry elements are 2 and m. Twins can arise during crystal growth (growth twins) or through mechanical stress (deformation twins). In Fig. 14.5, the twin element is a mirror plane parallel to (101). A spinel twin is shown in Figs. 14.6a and 15.8. The twin element is a mirror plane, which is the boundary of the two twin domains. The twin crystal in Fig. 14.6a may be 297 298 14 Crystal Defects Fig. 14.5 Twin with twin-plane (101) Spheres in cubic closest packing Spheres in hexagonal closest packing Spheres in cubic closest packing Fig. 14.6a,b Spinel twin on (111) (a). Sequence of layers of closest-packed O-atoms in the twin. The twin-boundary consists of an interruption with hexagonal closest packing.(b) described formally as the upper half of an octahedron rotated through 180◦ relative to the lower half about a direction normal to (111) (=[111]!) (Figs. 14.7 and 15.8). The twin is bounded by octahedral faces, and the twin plane m is also an octahedral face (111). This is called a spinel twin about (111). The spinel structure MgAl2 O4 is a ccp array of O2– ions with Mg in [4] and Al in [6] (see also Sect. 12.4.2). The octahedral faces lie parallel to the layers of closest packed O2– ions (Fig. 12.2b). A spinel twin is thus built about a plane parallel to these layers. Since the twin element m is one of these layers, it results in the alteration in stacking shown in Fig. 14.6b. There are two crystals with ccp layers joined by a lamella of hcp stacking, and this results in the observed twinning. Fig. 14.7 Octahedron. Rotation of the upper part by 180◦ about an axis normal to the octahedral face results in the spinel twin in Fig. 14.6a 14.3 Plane Defects Spinel twins are growth twins. Should only Al3+ ions approach a surface of O2– ions, the hcp packing of corundum (Sect. 12.2.3) will result. If, on the other hand, both Al3+ and Mg2+ are present, the O2– ions will continue to lay down ccp layers. Thus, if the solution containing Al3+ becomes enriched with Mg2+ , a region of hcp growth can revert to the more stable ccp layering, and this may then continue to grow as a twin to the original ccp layers. Metals with the Cu structure can also produce twins about (111) which build in the same way as a spinel twin. From an aqueous solution, NaCl will crystallize with cube-shaped crystals. If, however, a small amount of MnCl2 is added to the solution, these cubes can form twins as shown in Fig. 14.8a. These “pyramids” in the twins are the vertices of cubes. The twin plane is (111) and the twin element m. The NaCl structure may be described as cubic closest packing of Cl– with Na+ in all the octahedral [6] holes. The Spheres in cubic closest packing Trigonal prism Spheres in cubic closest packing Fig. 14.8a,b NaCl twin on (111) (a). Sequence of layers of closest-packed Cl-ions in the twin. The twin-boundary consists of an interruption in which the coordination polyhedron is a trigonal prism.(b) Fig. 14.9 Plane of a real crystal with mosaic blocks. ([1]) 299 300 14 Crystal Defects twin plane is once again parallel to the layers of closest packed ions. The twin element m, unlike that in spinel twinning, requires two successive layers to lie directly above one another. The Mn2+ ions can coordinate 6 Cl– to form a trigonal prism (Table 12.1d). If NaCl crystallizes from such a nucleus of MnCl6 polyhedra, it is possible for two twin components of NaCl to continue to develop cube faces as in Fig. 14.8. In general, because of the occurrence of a small angle grain boundaries, a crystal may be thought of as being built up of small mosaic blocks, which are only slightly displaced relative to one another. Figure 14.9 shows such a mosaic formation, with the inclination angles grossly exaggerated. 15 Appendix 15.1 Symbols for Crystallographic Items a, b, c a1 , a2 ; a1 , a2 , a3 Crystallographic axes Symmetrically equivalent crystallographic axes a Set of symmetrically equivalent crystallographic axes (a1 , a2 ; a1 , a2 , a3 ) Morphological axial ratio a b :1: → c b → → a, b, c Lattice vectors of the unit cell ⎫ ⎪ ⎪ ⎬ → |a| = a0 → b = b0 ⎪ ⎪ ⎭ ⎫ → → ⎪ α=b∧ c⎪ ⎬ → |c| = c0 → → → →⎪ ⎪ ⎭ β= a ∧ c Lengths of vectors Lengths of cell edges Interaxial angles ⎫ ⎪ ⎪ ⎪ ⎪ ⎬ ⎪ ⎪ ⎪ ⎪ ⎭ Lattice parameters γ=a∧b a0 b0 :1: c0 b0 Structural axial ratio Crystallographic “triples” → → → → x,y,z Coordinates of the vector r = x a +y b = z c Coordinates of a point in the unit cell, 0 ≤ x,y,z <1 uvw Coordinates of the lattice translation vector τ = u a +v b + w c → → → Coordinates of a lattice point, integers and integers + 1/2; 1/3 ; 2/3 W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_15, C Springer-Verlag Berlin Heidelberg 2011 → 302 15 Appendix [uvw] <uvw> (hkl) (hkil) {hkl} {hkil} hkl →∗ →∗ →∗ a ,b ,c Indices of a set of parallel lattice lines. Indices of a zone axis or parallel crystal edges Indices of a set of symmetrically equivalent lattice lines or directions Miller indices: Indices of a crystal face or of a set of parallel lattice planes Bravais-Miller indices: indices of a crystal face, or of a set of parallel lattice planes, for the hexagonal axes a1 , a2 , a3 , c Indices of a set of symmetrically equivalent crystal faces (crystal form) or lattice planes Indices of a set of symmetrically equivalent crystal faces (crystal form) or lattice planes, for the hexagonal axes a1 , a2 , a3 , c Laue symbol (indices): indices of a X-ray reﬂection from a set of parallel lattice planes (hkl) Vectors of the unit cell in the reciprocal lattice ⎫ ⎪ = a∗0 ⎪ ⎬ ⎫ →∗ Lengths of vectors ⎪ b = b∗ ⎪ 0 ⎪ ⎪ Lengths of cell edges ⎪ ⎪ → ⎪ ⎭ ⎬ ∗ ∗ |c | = c0 Parameters of the reciprocal lattice → → ⎫ ⎪ ⎪ α∗ = b∗ ∧ c ∗ ⎪ ⎪ ⎪ ⎬ ⎪ ⎪ → ⎭ → β∗ = a ∗ ∧ c∗ ⎪ Interaxial angles → → ⎪ ⎭ γ∗ = a∗ ∧ b∗ → |a∗ | 15.2 Symmetry Elements 15.2.1 Symmetry Elements (Planes) Table 15.1 Symmetry elements (planes) Symmetry element Mirror plane Plane of symmetry Glide plane with axial glide component Graphical symbol Glide component |g| Symbol ⊥ Plane of projection Plane of projectiona – → a 2 → b 2 → c 2 m a b c ····················· 15.2 Symmetry Elements Table 15.1 (Continued) Symmetry element Double glide plane with two glide vectors Glide plane with diagonal glide component Graphical symbol Glide component |g| Symbol ⊥ Plane of projection Plane of projectiona → a 2 → , b 2 → → → → → → → → → → → → → → → → e a + b 2 a + c 2 n b + c 2 →b a + b + c 2 “Diamond” glide plane a + b 4 a + c 4 d · b + c 4 →b a + b + c 4 a b If the z-coordinate is not 0 or 12 , its value is given. In tetragonal and cubic systems only. 15.2.2 Symmetry Elements (Axes) Table 15.2 Symmetry elements (axes) Symmetry element Screw component |s| Symbol Onefold rotation axis ≡ identity – 1 Inversion center Center of symmetry – 1̄ Twofold rotation axis – 2 Graphical symbol oa Plane of Projection Plane of projectiona Twofold screw axis 1 2 → |τ | 21 Plane of Projection Plane of projectiona 303 304 15 Appendix Table 15.2 (Continued) Symmetry element Screw component |s| Symbol Threefold rotation axis – 3 Threefold rotoinversion axis – 3 |τ | 2 3 |τ | 32 Fourfold rotation axis – 4 Fourfold rotoinversion axis – 4 Threefold screw axes → → 31 1 4 |τ | 2 4 |τ | 3 4 |τ | 43 Sixfold rotation axis – 6 Sixfold rotoinversion axis – 6 1 6 c0 61 2 6 c0 62 3 6 c0 63 4 6 c0 64 5 6 c0 65 Fourfold screw axes Sixfold screw axes a → 1 3 → → Graphical symbol 41 42 If the z-coordinate is not 0 or 1/2, its value is given. Symmetry directions in the seven crystal systems: cf. Table 8.2 Characteristic symmetry elements in the seven crystal systems: cf. Table 9.9. 15.3 Calculation of Interatomic Distances and Angles in Crystal Structures 15.3 Calculation of Interatomic Distances and Angles in Crystal Structures Speciﬁc interatomic distances (e.g. bond lengths) and the angles between the corresponding vectors (bond angles) are often of great interest. Interatomic Distances: The distance 1 between atoms A (x1 ,y1 ,z1 ) and B (x2 ,y2 ,z2 ) may be calculated by use of the following formulae: Table 15.3 Calculation of interatomic distances Crystal system l Triclinic {(Δx)2 a20 + (Δy)2 b20 + (Δz)2 c20 + 2ΔxΔya0 b0 cos γ +2ΔxΔza0 c0 cos β + 2ΔyΔzb0 c0 cos α}1/2 Monoclinic {(Δx)2 a20 + (Δy)2 b20 + (Δz)2 c20 + 2ΔxΔza0 c0 cos β}1/2 Orthorhombic {(Δx)2 a20 + (Δy)2 b20 + (Δz)2 c20 }1/2 Tetragonal {((Δx)2 + (Δy)2 )a20 + (Δz)2 c20 }1/2 Trigonal or hexagonal {((Δx)2 + (Δy)2 − ΔxΔy)a20 + (Δz)2 c20 }1/2 Cubic {((Δx)2 + (Δy)2 + (Δz)2 )a20 }1/2 Fig. 15.1 The triangle formed by atoms, A, B and C Angles: The angle ω, relating the atoms A, B and C (Fig. 15.1) may be readily calculated by calculating the lengths of the three edges, 11 , 12 and 13 of the triangle ABC and applying the cosine rule: cos ω = 121 − 122 + 123 . 211 13 305 306 15 Appendix 15.4 Crystal Forms Figure 15.2 shows the 47 crystal forms. 1. Pedion (Monohedron) Fig. 9.10d 2. Pinacoid (Parallelohedron), Fig. 9.7g 3. Dihedron (Sphenoid (2), Dome (m)) 4. Rhombic disphenoid 5. Rhombic pyramid, Exercise 9.15(5), Fig. 15.5(2) 6. Rhombic prism, Exercise 9.15(1), Fig. 15.5(1) 7. Rhombic dipyramid, Exercise 9.15(9), Fig. 15.5(3) Fig. 15.2a Forms of the triclinic, monoclinic and orthorhombic systems 8. Tetragonal pyramid, Fig. 9.10b, c, Fig. 15.5(5) 9. Tetragonal disphenoid 10. Tetragonal prism, Fig. 9.7e, f, Fig. 15.5(4) 11. Tetragonal trapezohedron 12. Ditetragonal pyramid, Fig. 9.10a 13. Tetragonal scalenohedron Fig. 15.7(2) 14. Tetragonal dipyramid, Fig. 9.7c, d, Fig. 15.5(6) 15. Ditetragonal prism, Fig. 9.7b 16. Ditetragonal dipyramid, Fig. 9.7a Some of the drawings of crystal forms are copied from Niggli [32] Fig. 15.2b Forms of the tetragonal system 15.4 Crystal Forms 17. Trigonal pyramid, Exercise 9.15(7), Fig. 15.5(8) 18. Trigonal prism, Exercise 9.15(3), Fig. 15.5(7) 19. Trigonal trapezohedron 20. Ditrigonal pyramid 21. Rhombohedron, Exercise 9.15(16), Fig. 15.7(1) 22. Ditrigonal prism 23. Hexagonal pyramid, Exercise 9.15(8), Fig. 15.5(11) 24. Trigonal dipyramid, Exercise 9.15(11), Fig. 15.5(9) 25. Hexagonal prism, Exercise 9.15(4), Fig. 15.5(10) 26. Ditrigonal scalenohedron Fig. 15.7(3) 27. Hexagonal trapezohedron Fig. 15.7(5) 28. Dihexagonal pyramid 29. Ditrigonal dipyramid 30. Dihexagonal prism 31. Hexagonal dipyramid, Exercise 9.15(12), Fig. 15.5(12) 32. Dihexagonal dipyramid Fig. 15.2c Forms of the hexagonal (and trigonal) system 307 308 15 Appendix 33. Tetrahedron, Exercise 9.15(15), Fig. 15.6(1) 34. Hexahedron (cube), Exercise 9.15(13), Fig. 15.6(3) 35. Octahedron, Exercise 9.15(14), Fig. 15.6(2) 36. Tetartoid (Tetrahedral pentagon-dodecahedron) 37. Pyritohedron (pentagon-dodecahedron) Fig. 15.7(4) 38. Deltoid-dodecahedron (deltohedron) 39. Tristetrahedron 40. Rhomb-dodecahedron, Fig. 2.1, Fig. 15.3 41. Diploid (disdodecahedron) 42. Trisoctahedron 43. Trapezohedron (deltoid-icositetrahedron) 44. Gyroid 45. Hexatetrahedron (hexakistetrahedron) 46. Tetrahexahedron (tetrakishexahedron) 47. Hexaoctahedron (hexakisoctahedron) Fig. 15.2d Forms of the cubic system 15.5 Patterns for Polyhedra 15.5 Patterns for Polyhedra 15.5.1 Patterns to Construct Models of Polyhedra To use the following patterns, photocopy the pages, enlarging them to A4 (U.S. letter) size onto heavy paper (about 200 gsm). Cut the patterns out, and score the fold-lines with a knife. Fold inwards along all of these lines. Then use the ﬂaps to glue the model together; a glue stick is useful for doing this. Fig. 15.3 Rhomb-dodecahedron 309 310 15 Appendix Fig. 15.4 Crystal of galena (PbS) 15.5 Patterns for Polyhedra Fig. 15.5 cf. Figs. 5.37 (1–12) 311 312 15 Appendix Fig. 15.5 (Continued) 15.5 Patterns for Polyhedra Fig. 15.5 (Continued) 313 314 15 Appendix Fig. 15.5 (Continued) 15.5 Patterns for Polyhedra Tetrahedron (1) Octahedron (2) Cube (hexahedron) (3) Fig. 15.6 Regular polyhedra that are crystal forms and platonic solids 315 316 15 Appendix Rhombohedron (1) Fig. 15.7(1)–(5) Patterns (2)–(5) were drawn using the program “Kristall2000” (www. kristall2000.de). cf. Exercise 9.15 (16)–(20) 15.5 Patterns for Polyhedra Tetragonal scalenohedron (2) Ditetragonal scalenohedron (3) Fig. 15.7(1)–(5) (Continued) 317 318 15 Appendix Pentagonal dodecahedron (4) Hexagonal trapezohedron (5) Fig. 15.7(1)–(5) (Continued) 15.5 Patterns for Polyhedra Fig. 15.8 Spinel twin on (111) in two parts, cf. Figs. 14.6a and 14.7 319 320 15 Appendix Regular dodecahedron (1) Icosahedron (2) Fig. 15.9 Two non-crystallographic polyhedra, after [17] 16 Solutions to the Exercises The solutions to a few exercises are incomplete, as the drawings would require too much space. Chapter 2 2.1 22.41 (the molar volume)/6.023×1023 (the Avogadro number, NA ) = 37,191 Å3 , which corresponds to a cube with an edge of 33.4 Å. 2.2 0.046% 2.3 No glass can be a crystal, nor any crystal a glass! Chapter 3 3.2 (a), (b) (c) (112). W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1_16, C Springer-Verlag Berlin Heidelberg 2011 322 16 Solutions to the Exercises 3.3 (a) (b) [001]. 3.4 (11̄1), (102), (12̄0), (1̄11̄) [11̄1], [101̄], [2̄10], [012̄]. 3.5 a) β = γ = 90◦ b) a0 = b0 ; α = β = 90◦ c) a0 = b0 = c0 ; α = β = γ 3.6 (hkl) and (h k l) belong to the same set of parallel planes; [uvw] and [u v w] are opposite directions. Chapter 4 4.1 (a) (b) Cu2O, Z = 2, (c) a0 4 3 = 1,85Å, (d) 6,1g/cm3. 4.2 (a) (b) 2.37 Å (c) 3.20g/cm3 4.3 All combinations of 0, 1/2, and 1 from 0,0,0, to 1,1,1. Figure 3.5 includes a partial solution; see also Sect. 7.2.1. 16 Solutions to the Exercises 4.4 x,0,0; 0,y,0; 0,0,z x,1,0; 1,y,0; 1,0,z x,0,1; 0,y,1; 0,1,z x,1,1; 1,y,1; 1,1,z 4.5 x,y,0; x,0,z; 0,y,z x,y,1; x,1,z; 1,y,z 4.6 x,y,1/4; x,1/2,z; x,1/2,1/4. 4.7 Chapter 5 5.1 (1) + (2) = Fig. 5.13a (lower part). (3) (4) 5.2 (1) = Solutions-Exercise 5.3 (4) (2) = Solutions-Exercise 5.3 (10). 5.3 323 324 16 Solutions to the Exercises 5.4 Cf. Exercise 5.3 (6) and (10). 5.5 1. Trigonal pyramid and pedion. 2. Tetragonal dipyramid. 3. Cube, tetragonal prism and pinacoid, rectangular box, orthogonal axes. 4. Hexagonal prism and pinacoid, hexagonal axes. 5.6 Cf. Fig. 5.18. 5.7 5.8 (a) 60◦ /229◦ ; 58◦ (b) 46◦ /260◦ ; 30◦ (c) 44◦ /32◦ ; 69◦ 5.9 100◦ ; 44◦ and 280◦ ; −44◦ , parallel 5.10 They lie in a plane, perpendicular to the zone axis, cf. Fig. 5.3. 5.11 Cf. Fig. 7.13f (432). 5.12 The stereograms are identical. 5.13 Cf. Fig. 5.11. The stereograms in Exercises 5.12 and 5.13 are geometrically equivalent. 5.14 (The pole faces with negative l have not been included) 16 5.15 Cube 1 + ; Cube 2 • 5.16 Cf. Orthographic projection in 0,0,0 of Fig. 10.15 5.17 5.18 A sphere. Chapter 6 6.1 See pp. 326 and 327. 6.2 Solutions to the Exercises 325 16 Solutions to the Exercises 6.1 326 Solutions to the Exercises 6.1 16 327 328 16 Solutions to the Exercises 6.3 Parallel. 6.4 6.5 1̄ ≡ Inversion center, 2̄ ≡ m, 3̄ ≡ 3 + 1̄, 5̄ ≡ 5 + 1̄, 6̄ ≡ 3 ⊥ m, 10 ≡ 5 ⊥ m. 6.6 X̄ (odd): 1̄, 3̄, 5̄ . . . . 6.7 Trigonal, tetragonal, and hexagonal pyramid; trigonal dipyramid. 6.8 Rhombus,1 equilateral triangle, square, regular hexagon. 6.9 Cf. Fig. 5.38. Chapter 7 7.1 (a) Cf. Figs. 7.6 and 6.5b. (b) (3) a0 = b0 because of the 4-fold axis (4) a0 = b0 because of the 6-fold axis (c) (3) m in x, 0, z and 0, x, z; m in x, x, z and x, x̄, z. (4) m in x, 0, z; x, x, z and 0, x, z. 7.2 (1) (4) 1 (2) Cf. Fig. 7.6a, (3) Cf. Fig. 7.6c, (5) Cf. Fig. 7.6d, (6) Cf. Fig. 6.5b, Solids with rectangular or parallelogram cross-sections are not prisms in the crystallographic sense as their faces are not all equivalent (cf. Sect. 9.2.1). 16 (7) Solutions to the Exercises (8) (9) No symmetry except lattice translation. (10) 7.3 (a) (b) (1) (3) (5) (7) 2 in x,1/2,0, (2) m in x,y,1/2, 1̄ in 1/2,0,1/2, (4) m in x,y,0, 1̄ in 1/2,1/2,1/2, (6) 2 in 1/2,y,1/2, 2 in 0,1/2,z. 7.4 (a) Cf. Fig. 7.9f (right) and Table 9.11.7 (b) (1) 2 in x,1/2,1/2, (2) m in x,y,1/2, (3) 2 in 1/2,1/2,z, (4) m in x,0,z. 7.5 (a) cubic P, (b) monoclinic P, (c) triclinic P, (d) orthorhombic P, (e) tetragonal P, (f) hexagonal P. 7.6 (a) Cf. Figs. 7.7a–7.12a, (b) Cf. Figs. 7.7d–7.12d, (c) and (d) Cf. Figs. 7.18–7.23. 7.7 (a) 2/m2/m2/m (b) and (c): 1/2,0,0; 0,1/2,0; 0,0,1/2 → halving of the unit cell. 1/ ,1/ ,0 → C-lattice; 1/ ,0,1/ → B-lattice; 2 2 2 2 0,1/2,1/2 → A-lattice 1 1 1 /2, /2, /2 → I-lattice 1/ ,1/ ,0; 1/ ,0,1/ ; and 0,1/ ,1/ → F-lattice 2 2 2 2 2 2 7.8 I. 7.9 Fig. 7.11d 7.10 In each case, a = b + c + d. 329 330 16 Solutions to the Exercises Chapter 9 9.1 (a) The directions parallel and antiparallel to a polar axis have distinct physical properties. (b) (1) 1̄, (2) m ⊥ X, (3) 2 ⊥ X [also valid for 4 and 6]. (c) On stereograms, the ends of neighboring polar axes are indicated by open and ﬁlled symbols (cf Fig. 7.10f for point group 422); in tables, a subscript p is placed by the axis, e.g. p or 3p . 9.2 No. Rotoinversion implies rotation through an angle followed by inversion. The two ends of the axis remain equivalent. 9.3 1̄, 2/m, 3̄, 4/m, 6/m. 9.4 622 6 mm 6̄ m2 6/m 2/m 2/m 422 4 mm 4̄ 2m 4/m 2/m 2/m 32 3m 3̄ 2/m 3̄ 2/m 222 mm2 mm2 2/m 2/m 2/m Cf. also Figs. 7.9e, f–7.12e, f. 9.5 23 4̄ 3m 432 2/m 3̄ 4/m 3̄ 2/m 4/m 3̄ 2/m Cf. also Fig. 7.13e, f. 9.6 3m, 32, 3̄, 3. 9.7 Cf. Table 9.10 9.8 Cf. Table 9.9 9.9 (1) 4̄2m, (2) m, (3) 32, (4) 6 mm, (5) mm2, (6) 4̄3m. 9.10 Cf. Figs. 7.8 e, f–7.13e, f. 9.11 (1) 6/m 2/m 2/m, (2)–(4) mm2, (5) 2/m 2/m 2/m, (6) mm2, (7) m, (8) 6̄ m2, (9) 4/m 3̄ 2/m, (10) 4 mm, (11) 4/m 2/m 2/m, (12) mm2, (13) 3m, (14) mm2, (15) 4̄ 3m, (16) 3m, (17) mm2, (18) = (16), (19) = (15), (20) 3m, (21) & (22) 6̄ m2, (23) m, (24) mm2, (25) m, (26) 2, (27) 2, (28) 3m, (29) m, (30) & (31) 1, (32) 3̄ 2/m, (33) mm2, (34) 2, (35) mm2, (36) 4/m 2/m 2/m, (37) 4 mm, (38) 4̄ 2m, (39) 2/m 2/m 2/m, (40) mm2, (41) 2/m, (42) & (43) m, (44) & (45) 2, (46)–(49) 1 (a) Enantiomers: (26)&(27), (30)&(31), (44)&(45), (46)&(47), (48)&(49). (b) Polar molecules: (2)–(4), (6), (7), (10), (12), (14), (16)–(18), (20), (23)–(31), (33)–(35), (37), (40), (42)–(49) 16 Solutions to the Exercises 9.12 (1) Bent (Fig. 9.17a), (2) pyramidal, (3) Table 9.11.14, (4) Fig. 9.19. 9.13 mm2 (0◦ ); 2 (0◦ < ϕ < 180◦ ); 2/m (180◦ ); 2 (180◦ < ϕ < 360◦ ). 9.14 Yes; mm2(+); 2/m(0). 9.15 (1) 2/m 2/m 2/m, (2) 4/m 2/m 2/m, (3) 6̄ m2, (4) 6/m 2/m 2/m, (5) mm2, (6) 4 mm, (7) 3m, (8) 6 mm, (9) 2/m 2/m 2/m, (10) 4/m 2/m 2/m, (11) 6̄ m2, (12) 6/m 2/m 2/m, (13) & (14) 4/m 3̄ 2/m, (15) 4̄ 3m, (16) 3̄ 2/m. 9.16 (3), (5), (6), (7), (8), (11), (15). 9.17 Faces + vertices = edges + 2 (Euler’s equation for polyhedra – cf. Table 9.11). 9.18 (a) Cf. Fig. 9.8. (b) Ditetragonal dipyramid; from (hk0) arise (hkl) and (hk1̄) etc., or from (210) arise, for example, (211) and (211̄) etc. 9.19 (a) Cf. Fig. 9.12a. (b) Hexagonal dipyramid; from (hki0) arise (hkil) and (hki1̄) etc. or from (213̄1) arise, for example, (213̄1) and (213̄1̄). 9.20 (1), (2): Table 9.4; (3), (4): Table 9.7; (5), (6), (7): Table 9.5; (8), (9): Table 9.6. 9.21 (Part of Fig. 9.15) The pole (113) corresponds to the crystal form trapezohedron or deltoid icositetrahedron {311} or {hkk}. (311) lies in the asymmetric face unit. 9.22 6̄ m2: (m..); ditrigonal prism {hki0}: hexagonal prism {112̄0} 3̄ 2/m: (.m.); rhombohedron {h0h̄l}: hexagonal prism {101̄0} 6 mm: (.m.); hexagonal pyramid {h0h̄1}: hexagonal prism {101̄0} (..m; hexagonal pyramid {hh2h1}: hexagonal prism {112̄0} 3m: (.m.), trigonal pyramid {h0h̄1}: trigonal prism {101̄0}. 331 332 16 Solutions to the Exercises 9.23 4 2 mm 43 m 432 2 23 Chapter 10 10.1 10.2 (a) x,y,1-z, (b) x,1/2-y,z, (c) 1/2+x,y,1/2-z, (d) 1/2-x,1/2+y,z, (e) x,1/2-y,1/2+z, (f) 1/2-x,1/2+y,1/2+z, (g) 1/2+x,1/2+y, z̄, (h) 1/2+x, ȳ,1/2+z, (i) 1/2-x,y, z̄, (j) 1-x, ȳ,1/2+z, (k) x̄,1/2+y,1/2-z, (l) 1/2-x,1/2-y,z, (m) ȳ,x,1/4+z; x̄, ȳ,1/2+z; y,x̄,3/4+z, (n) ȳ,x-y,1/3 +z; x̄+y,x̄,2/3 +z 10.3 The diﬀerence between the operation of a glide plane and a 21 is only evident when a “fully asymmetric point” is considered. An example is the asymmetric pyramid in the following ﬁgure. 16 10.5 10.6 Solutions to the Exercises 333 334 16 Solutions to the Exercises 10.7 (1) (a) (2) x,y,z; x̄,ȳ,z̄,2 (3) 2, (4) P1̄, (5) on all 1̄, 1-fold. (1) (b) (2) x,y,z; x, ȳ,z; 1/2+x,1/2-y,z; 1/2+x,1/2+y,z, (3) 4, (4) Cm, (5) on m, 2-fold. (1) (c) (2) x,y,z; 1/2+x,1/2-y,z; 1/2-x,1/2+y,z; x̄,ȳ,z, (3) 4, (4) Pba2, (5) on 2, 2-fold. (1) (d) (2) x,y,z; x,1/2-y,1/2+z; x̄,1/2+y,1/2+z; x̄,ȳ,z, (3) 4, (4) Pnc2, (5) on 2, 2-fold. 2 Coordinates are given as in International Tables [16], i.e. instead of 1-x,1-y,1-z is written x̄,ȳ,z̄. 16 Solutions to the Exercises (1) (e) (2) x,y,z; x,1/2-y,z; 1/2-x,y,1/2+z; 1/2-x,1/2-y,1/2+z; 1/2+x,1/2+y,1/2+z; 1/2+x,ȳ,1/2+z; x̄,1/2+y,z; x̄,ȳ,z. (3) 8, (4) Ibm2, (5) on 2, 4-fold. (1) (f) (2) x,y,z; 1/2-x,1/2-z; 1/2+x,y,1/2-z; x̄,y,z; x,ȳ,z̄; 1/2-x,ȳ,1/2+z; 1/2+x,ȳ,1/2+z; x̄,ȳ,z̄, (3) 8, (4) P2/m 2/n 21 /a, (5) on m and 2, 4-fold, on 1̄, 2-fold. (1) (g) (2) x,y,z; x̄,ȳ,z; ȳ,x,1/2+z; y,x̄,1/2+z; 1/2+x,1/2-y,z; 1/2-x,1/2+y,z; 1/2-y,1/2-x,1/2+z; 1 /2+y,1/2+x,1/2+z. (3) 8, (4) P42 bc, (5) on 2, 4-fold. 335 336 16 Solutions to the Exercises 10.8 (a) 1. x,y,z; x̄,ȳ,z; x-y,x,z+1/3 ; x̄+y,x̄,z+1/3 ; ȳ,x-y,z+2/3 ; y,x̄+y,z+2/3 2. 2 in 1/2,0,z; 1/2,1/2,z; 0,1/2,z; 0,1/2,z; 32 in 2/3 ,1/2,z; 1/3 ,2/3 ,z 3. 32 ,2 (b) 1. x,y,z; ȳ,x-y,z; x̄+y,x̄,z; x-y,x,z+1/2; x̄,ȳ,z+1/2 2. 21 in 1/2,0,z; 1/2,1/2,z; 0,1/2,z; 3 in 2/3 ,1/3 ,z; 1/3 ,2/3 ,z 3. 3, 21 10.9 16 Solutions to the Exercises (c) Coordinates are not given for those points which are reﬂected by m to locations below the plane x,y,0. The third coordinate of each triple must be taken to have both a plus and a minus sign. 10.10 Cf. the solution to Exercise 10.9. 10.11 Cf. Figure 10.17: the diagram in (2) and the general position in (7) 337 338 16 Solutions to the Exercises 10.12 P21 /c (Fig. 10.9 a), Pna21 (Fig. 10.12), Pmna (Exercise 10.7f). 10.13 This is absurd: an a-glide plane cannot be normal to the a-axis . . . 10.14 P1̄: (a) AB2 , (b) Z = 1, (c) linear, (d) ∞/mm, (e) 1̄. 16 Solutions to the Exercises Pm: (a) AB2 , (b) Z = 1, (c) bent, (d) mm2, (e) m. P2/m: (a) AB4 , (b) Z = 1, (c) planar [4]-coordination (rectangular), (d) 2/m 2/m 2/m, (e) 2/m. P 2/m 2/m 2/m: (a) AB8 , (b) Z = 1, (c) [8]-coordination (rectangular parallelepiped), (d) and (e) 2/m 2/m 2/m. Chapter 11 ⎛ ⎞ 100 c = −c; ⎝ 0 1 0 ⎠ 11.1 (a) for all coordinate systems a = −a, b = −b, 001 ⎛ ⎞ 100 (b) (1) m, o, t, c; a = −a, b = b , c = −c; ⎝ 0 1 0 ⎠ 001 ⎛ ⎞ 100 b = b; c = −c; ⎝ 1 1 0 ⎠ (2) h; a = −a − b; 001 339 340 16 Solutions to the Exercises ⎛ ⎞ 100 b = b; c = c; ⎝ 1 1 0 ⎠ h; a = −a − b; 001 ⎛ ⎞ 001 b = c, c = a; ⎝ 1 0 0 ⎠ r, c; 31[111] : a = b; 001 ⎛ ⎞ 010 ⎝0 0 1⎠ 32[111] : a = c; b = a; c = b; 100 ⎛ ⎞ 001 c = −a; ⎝ 0 1 0 ⎠ c; a = c, b = −b; 100 ⎛ ⎞ 110 b = −a; c = c; ⎝ 1 0 0 ⎠ h; a = a + b, 001 (c) (d) (e) (f) 11.2 For inversion, 2-fold rotation and reﬂection, the direct and inverse matrices are identical. 11.3 Yes. 3 2 5 3 11.4 (a) (1) t; 2a · m[110] = 4c ; (4c ≡ 2c ) · 2a = 2b; 2c · m[110] = m[110] ;42m (2) h; 2a · m[110] = 3c ; (3c ≡ 1) · 2a = ma ; 1̄ · m[110] = 2[110] etc.; 3 2/m 1 5 (b) 3c · mc = 6c ; 6 1 (c) 41c · 1 = 4c ; (42c ≡ 2c ) · 1 = mc ; 4/m. In 4/m, of course, 4 is implied. 11.5 (a) 2b · mb = 1; (42b ≡ 2b ) · mb ≡ 1; (63c ≡ 2c ) · mc = 1 (b) mb · 1 = 2b (c) 2b · 1 = mb ; (42b ≡ 2b ) · 1 = mb ; (63c ≡ 2c ) · 1 = mc 1 2 3 11.6 4c , 4c ≡ 2c , 4c , 2a , 2b , m[110] , m[110] , 1. Order 8 (hkl) cf. Table 11.1. Tetragonal scalenohedron. 11.7 Cf. the group multiplication tables for 32 and 3m. No. Group multiplication table for 32 16 1 31c 32c 2a 2b 2[110] 1 1 31c 32c 2a 2b 2[110] 31c 31c 32c 1 2[110] 2a 2b 32c 32c 1 31c 2b 2[110] 2a 2a 2a 2b 2[110] 1 31c 32c 2b 2b 2[110] 2a 32c 1 31c 2[110] 2[110] 2a 2b 31c 32c 1 Solutions to the Exercises Chapter 12 12.1 Cf. Table 12.1d and h. 12.2 (a) cub. P; Po: 0,0,0 (b) cub. I; W: 0,0,0 (c) hex. P; Mg: 0,0,0; 2/3 ,1/3 ,1/2 (d) cub. F; Cu: 0,0,0 (e) 63 in 1/3 ,2/3 ,z; 6̄ in 0,0,z 12.3 (a) 1.675 Å, (b) 1.37 Å, (c) 1.605 Å, (d) 1.28 Å. 12.4 1.63. 12.5 (a) 0.52, (b) 0.68, (c) 0.74, (d) 0.74. 12.6 (a) Cf. Fig. 12.20 (b) 1.546 Å, (c) 8, (d) each C is tetrahedrally coordinated by 4C. (e) The two structures have the same geometry. 12.7 (a) Cf. 11.15a (b) 1.42 Å, (c) 4, (d) 3.35 Å, (d); ρD = 3.50 g cm–3 ; ρG = 2.27 g cm–3 341 342 16 Solutions to the Exercises 12.8 Li+ : 0.76 Å; Cl− : 1.81 Å; 0.79 12.9 12.10 1.95 Å (distances indicated by thick lines), 1.97 Å (distances indicated by thin lines), cf. Fig. 10.18. 16 Solutions to the Exercises 12.11 The 3̄ are orientated parallel to < 111 >. (3) 4, (4) Fe–S: 2.27 Å; S–S: 2.06 Å. 12.12 (1) (2) HgNH4 Cl3 , Z = 1, (3) Hg[6] (octahedron), NH[8] 4 (cube), (4) Hg–Cl: 2.38 Å 2.96 Å, NH4 –Cl: 3.36 Å. (5) Only if the NH4 + ions are considered spherical. 343 344 16 Solutions to the Exercises 12.13 (2) 4, (3) S is tetrahedrally coordinated by 4O. Chapter 13 13.1 16 Solutions to the Exercises 13.2 Z = 2, W-type (Fig. 12.5). 13.3 23 2 / m3 432 43m 4 /m32 /m 2 + 1 = 2 /m, 3 + 1 = 3 2 / m3 4 + 1 = 4 /m, 3 + 1 = 3, 2 + 1 = 2 /m 4 + 1 = 4 /m, 3 + 1 = 3, m + 1 = 2 /m 4 /m32 /m 13.4 (1) 111 4.077; 200 3.534; 220 2.495; 311 2.127; 222 2.038; 400 1.766; 331 1.621; 420 1.579; 422 1.442. (2) a0 = 7.06 Å. (3) Z = 4. (4) Because Z = 4, so KI must have either the rock salt or the sphalerite structure. As RA /RX for KI is 0.61 (see Fig. 12.7) the structure should be the rock salt (NaCl) type. 345 Literature References This list makes no claim to being complete. It is merely intended to indicate some useful texts, tables and other publications, in particular those to which reference has been made in this book. 1. Allman R (2003) Röntgen-Pulverdiﬀraktometrie. Springer, Heidelberg. 2. Azaroﬀ LV (1968) Elements of X-ray Crystallography. McGraw-Hill, New York. 3. Bijvoet JM, Kolkmeyer NH, Macgillavry CH (1951) X-Ray Analysis of Crystals. Butterworth, London. 4. Bloss FD (1994) Crystallography and Crystal Chemistry. Holt, Rinehart & Winston, New York. 5. Bohm J (1995) Realstruktur von Kristallen. Schweizerbart, Stuttgart. 6. Borsdorf R, Dietz F, Leonhardt G, Reinhold J (1973) Einführung in die Molekülsymmetrie. Chemie Physik, Weinheim. 7. Buerger MJ (1951) Crystallographic Aspects of Phase Transformations. In: Smoluchowski R (ed) Phase Transformations in Solids. Wiley, New York. Chapman & Hall, London. 8. Buerger MJ (1978) Elementary Crystallography. Wiley, New York. 9. Buerger MJ (1971) Introduction to Crystal Geometry. McGraw-Hill, New York. 10. Buerger MJ (1977) X-Ray Crystallography. de Gruyter, Berlin. 11. Burzlaﬀ H, Zimmermann H (1993) Kristallsymmetrie - Kristallstruktur. Merkel, Erlangen. 12. Chernov AA (1984) Modern Crystallography, Vol III, Crystal Growth. Springer, Heidelberg. 13. Cullity BD (1978) Elements of X-ray Diﬀraction. Addison-Wesley, Reading Mass. 14. Fischer E (1966) Einführung in die mathematischen Hilfsmittel der Kristallographie. Bergakademie - Fernstudium, Freiberg. 15. Giacovazzo C (ed) (2002) Fundamentals of Crystallography. Oxford. 16. Hahn T (ed) (2005) International Tables for Crystallography, Vol A. Wiley, New York. 17. Hargittai I und M (1994) Symmetry. Shelter Publications, Bolinas California. 18. Haussühl S (2007) Physical Properties of Crystals. Wiley, New York. 19. Hermann C (ed) (1935) Internationale Tabellen zur Bestimmung von Kristallstrukturen, Bd I. Borntraeger, Berlin. 20. Jaﬀe HH, Orchin M (1973) Symmetry in Chemistry. Wiley, New York. 21. Jagodzinski H (1955) Kristallographie. In: Handbuch der Physik, Bd VII, Teil I. Springer, Heidelberg. 22. De Jong WF (1959) General Crystallography: a Brief Compendium. Springer, Heidelberg. 23. Kittel CH (2004) Introduction to Solid State Physics. Wiley, New York. 24. Kleber W (Bautsch J, Bohm J) (2002) Einführung in die Kristallographie. Technik, Berlin. 25. Klein C, Hurlbut CS (1985) Manual of Mineralogy. Wiley, New York. 26. Landolt-Bornstein (1971) Strukturdaten organischer Verbindungen, Bd 5. Springer, Heidelberg. 27. Landolt-Bornstein (1973–1986) Kristallstrukturen anorganischerVerbindungen, Bd 7. Springer, Heidelberg. 28. Lima-de-Faria J (1990) Historical Atlas of Crystallography. Kluwer, Dordrecht. W. Borchardt-Ott, Crystallography, 3rd ed., DOI 10.1007/978-3-642-16452-1, C Springer-Verlag Berlin Heidelberg 2011 348 Literature References 29. Massa W (2004) Crystal Structure Determination. Springer, Heidelberg. 30. McKie D, McKie C (1990) Essentials of Crystallography. Blackwell, Oxford. 31. Meyer K (1977) Physikalisch-chemische Kristallographie. Deutscher Verlag für GrundstoﬃnDustrie, Leipzig. 32. Niggli P (1941) Lehrbuch der Mineralogie und Kristallchemie. Borntraeger, Berlin. 33. Paufler P (1986) Physikalische Kristallographie. Chemie Physik, Weinheim. 34. Pauling L (1964) The Nature of the Chemical Bond. Cornell University Press, New York. 35. Ramdohr P, Strunz H (1978) Lehrbuch der Mineralogie. Enke, Stuttgart. 36. Read WT (1953) Dislocations in Crystals. McGraw-Hill, New York. 37. Schulz H, Tscherry V (1972) Acta Crystall., B28, 2168. 38. Schwarzenbach D (2001) Kristallographie. Springer, Heidelberg. 39. Shuvalov LA et al. (1988) Modern Crystallography, Vol IV, Physical Properties of Crystals. Springer, Heidelberg. 40. Stoddart JF (1991) Angew. Chem., 103, 71. 41. Stout GH, Jensen LH (1989) X-ray Structure Determination. Macmillan, London. 42. Strukturberichte (1913–1940) Akademische Verlagsgesellschaft, Leipzig. 43. Structure Reports (1956–1990) Springer, Heidelberg. 44. Strunz H, Nickel EH (1999) Strunz Mineralogical Tables: a Chemical-Structural Mineral Classiﬁcation System. Schweizerbart, Stuttgart. 45. Vainshtein BK (1996) Modern Crystallography, Vol 1, Symmetry of Crystals. Methods of Structural Crystallography. Springer, Heidelberg. 46. Vainshtein BK, Fridkin VM, Indenbom VL (2006) Modern Crystallography, Vol II, Structure of Crystals. Springer, Heidelberg. 47. Wells AF (1995) Structural Inorganic Chemistry. Clarendon Press, Oxford. 48. Wilke K-TH, Bohm J (1988) Kristallzüchtung. Deutscher Verlag der Wissenschaften, Berlin. 49. Wyckoﬀ RWG (1963–1971) Crystal Structures. 1963 (vol. l)–(vol. 6). Wiley, New York. Index A C Acicular 31 Ag, Au 250, 264–265 Aggregate 35 Amorphous 7–8 Angle between the normals 36, 39, 45–46 Ångström 25 Anisotropic 7, 32 Antiﬂuorite structure 257–258 Aragonite 266–268 Aragonite structure 267–268 Asymmetric face unit 130–135, 144–146, 188, 204, 231 unit 132, 134, 204, 206, 210, 212–213 Atomic radii 29, 250–251 Avogadro number 26 Axial ratio 50, 120–121, 301 Axial system 10, 52, 119–120, 170, 174, 193 Azimuthal angle 40 C60 252–253, 271 CaCO3 structure 266 CaF2 258–259, 261, 292 CaF2 structure 258 CaF2 -type 259 Calcite 266–268 Calcite structure 267 ccp 249–251, 253, 257–258, 266, 269, 297–299 Centered lattice 103–109, 119, 123, 189, 191, 281 Centrosymmetric 67–68, 95, 155, 208, 287 Characteristic symmetry elements 77–78, 80, 149–150, 173, 304 Chemical bonding 245–246, 264 Chiral 154 C-lattice 103, 105–107, 189 Cleavage 3, 293 Column vector 224–225 Combination of symmetry operations 68–69, 71 Complication rule 46, 48–49 Compound symmetry operation 68–71, 189–190, 193 Conformation 148–149, 168, 183 Continuous 6–7 Coordination number 246, 251, 261, 266–268, 274 polyhedron 246, 248–251, 253, 256, 260, 274, 299 Coronene 147–148 Corundum structure 258, 299 Coulombic force 253 Coulomb’s law 253 Covalent bonding 246, 252 Cristobalite 262 B Basis 23, 211 BaSO4 274 bcc 251, 266–267 Benzene 1, 147–148, 212, 214, 252 B-lattice 105–106 Bragg equation 277–278, 280–281, 284, 286–287 Bravais lattice 75–118, 123, 189, 195, 201 Bravais-Miller indices 139, 302 Buerger 55, 207, 266, 287 Burgers vector 295–297 350 Index Crystal aggregate 35 chemistry 245–275 data-determination tables 120 defects 293–300 edge 29–30, 301 face 19, 29–31, 34–35, 38–40, 68, 129–130, 154, 183, 282, 293, 296 form 31, 37, 44, 128–146, 166, 169, 212, 246 growth 32–35, 212, 248, 296–297 structure Ag, Au 250 AlB2 27 Antiﬂuorite 257–258 BaSO4 274 Benzene 214 CaF2 258–259, 261 Corundum-type (Al2 O3 ), 258, 299 Spinel-type 256–257 Cristobalite 262 CsCl-type 258–259, 266 Cu2 O 322 Cu3 Au 265, 269 CuAu 265, 269 Cubic closest packing 248, 252, 257 Cuprite 26 Cu-type 248–249 Diamond 246, 271 Ethylene 214 Fluorite 257–258, 262 Forsterite 258 Graphite 271, 297 Hexagonal closest packing 249, 252, 257, 261 Hexamethylenetetramine 212–213, 252 HgNH4 Cl3 343 LiCl 259 Mg-type 249 NaCl-type 266 NiAs-type 262 Pyrite 154 Quartz(high) 268 Quartz(low) 268 RbF 259 Rutile (TiO2 ) 211, 259, 263 SiO2 260, 262 Sphalerite 260–261 Tridymite 268 W-type 251 Wurtzite 260–261, 266 ZnS 156 α-Polonium 9, 251 structure determination 26 system 81–82, 84, 86, 88, 90, 92, 119–121, 123–126, 133, 139, 149–151, 166, 195, 198–201, 210, 226–233, 239, 282, 289 Crystallographic axes 10, 16, 44–45, 48, 50, 71, 97, 119–120, 223, 226 CsCl 258–259, 261, 266 CsCl structure 258, 266 CsCl-type 261 CsI 25–26, 248, 259, 291 CsI structure 25 Cu2 O 322 Cu3 Au 265, 269 CuAu 265, 269 Cubic closest packing 248, 252, 256–257, 261, 298–299 coordination 248, 257–260, 262, 267 Cu-type 248–249 D Debye-Scherrer line 278 Debye-Scherrer method 278–282 Degree of freedom 130, 132–133, 203, 290 Deltohedron 308 Deltoid-dodecahedron 308 Deltoid-icositetrahedron 308 Density 16, 25–26, 268, 282, 289, 294 Determinant 17–18 Determination of point groups 149–154 Diadochy 265 Diamond structure 246, 263 Dihedron 306 Dihexagonal dipyramid 139, 307 Dihexagonal prism 307 Dihexagonal pyramid 307 Dilatational transformation 266–267 Diploid 308 Dipole moment 155–156, 166 Discontinuous 6 Disdodecahedron 308 Dislocation 293, 295–297 Displacive transformation 268–269 Dissymmetric 154 Ditetragonal dipyramid 132–135, 138, 146, 306 Ditetragonal prism 132–133, 138, 146, 306 Ditetragonal pyramid 134, 138, 146, 306 Ditrigonal dipyramid 307 Ditrigonal prism 307 Ditrigonal pyramid 307 Index Ditrigonal scalenohedron Dome 139, 306 307 E Edge dislocation 293, 295, 297 Eigensymmetry 146 Electrical conductivity 294–295 Enantiomeric 155 Enantiomorphism 154–155 Equant 31 Equivalent 10, 49, 63–67, 71, 75, 99, 101, 103, 109, 120, 126–130, 139, 147–148, 166, 169, 201–203, 205–208, 211, 213, 216, 218, 220, 225, 235, 246, 249, 252–253, 258, 293 Equivalent by translation 10, 63–64 Etch-ﬁgure 154, 296 Ethane 148–149 Ethylene 212, 214, 252 Ewald 282, 286–287 Ewald construction 286–287 Extinct 281 F Face centered 103, 105–106 Face symmetry 129–130, 132, 138–139, 213 Finite group 242 Fivefold rotation axis 65 Fluorite structure 257–258, 262 Fluorite-type 257–258, 262 Forsterite structure 258 Fourfold rotation axis 65, 304 Frenkel defect 293–295 Full symbol 125 G Galena 6, 29–30, 32, 36, 41, 50–51, 128, 310 Garnet 3 Gas 5–7, 252–253, 293, 295 General form 129–130, 132–135, 138–139, 188, 208, 213, 238, 265 General plane lattice 63, 76–77 General position 202–205, 207–208, 210, 213, 225, 235 Generating symmetry 146 Glancing angle 277–279, 287 Glass 4, 7–8 Glide component 190–191, 193, 203, 302–303 Glide plane 69, 71, 77, 99, 108, 189–195, 198–199, 203–204, 208, 210, 223, 234–281, 302–303 Glide reﬂection 69, 189–190, 233, 239 Gnomonic projection 50–51 Goldschmidt 46, 245, 251 Goniometer 38–40, 48, 58 Graphite structure 271 Great circle 36–38, 40–42, 45, 56 Group Inﬁnite 166–167, 239 Laue 287–289 multiplication table 241–243 Growth rate 34 Gypsum 4, 61–62 Gyroid 308 H Habit 30–31, 34 Handedness 193 Hardness 4 hcp 249, 251, 265–267, 297–299 Hermann 126, 153, 201 Hermann-Mauguin symbol 126, 153, 201 Heteropolar bonding 245 Hexagonal closest packing 249, 252, 257–258, 261, 297–298 dipyramid 139, 307 prism 31, 53, 144, 154, 187, 307 pyramid 307 trapezohedron 186, 307, 319 Hexahedron 154, 308 Hexakisoctahedron 308 Hexakistetrahedron 308 Hexamethylenetetramine 212–213, 252 Hexaoctahedron 308 HgNH4 Cl3 343 {hkil} 302 (hkil) 139, 302 {hkl} 129–130, 132–133, 135, 138, 145, 302 (hkl) 14–17, 19, 21, 26, 30, 32, 45–46, 48, 129–130, 132, 134–135, 138, 145, 223, 225–233, 278–282, 284, 287, 302 Homogeneous 6–7 Homopolar bonding 245, 263 I Ideal crystal 293–294 Idea of sphere packing 245 351 352 Index Identical 10–11, 23, 64, 70–71, 75–77, 106, 123, 125, 190, 193, 239, 242, 249 Identical points 10–11, 75, 123, 239 I-lattice 105–108, 189, 208, 251, 281 Indexing 14–15, 44–50, 129, 133, 139 Interaction principle 245 International symbol 65, 121, 127, 153 International tables for crystallography 1, 139, 206, 209–211 Interrelationship of point groups and space groups 212–214 Inverse 224, 226, 238, 243 Inversion 62–63, 67–71, 75, 95–97, 99, 101, 103, 108, 124, 150, 166, 203, 208, 210, 238, 287, 303 Inversion center 62, 67–71, 75, 95–97, 99, 101, 103, 108, 124, 150, 166, 203, 208, 210, 287, 303 Ionic bonding 246 Ionic radii 253–254, 289 Ionic structure 253–263 Isomorphism 264–266 Isotropic 4, 6–7, 32 Isotypes 264–266 J JCPDS 282–283 K Kyanite 4 L Lattice line 12–13, 17–20, 29–30, 45, 64–65, 67, 106, 301 parameter 10–11, 13, 30, 44, 75, 78, 109, 277, 281, 286, 301 plane 11, 14–19, 29–30, 32, 45, 63–67, 78, 80, 96–97, 99, 103, 105–108, 277–279, 281–282, 284–285, 287, 289, 296, 302 point 9, 11–16, 63, 66–67, 95–96, 103, 105–107, 109, 123, 189, 284, 301 translation 9–11, 23, 30, 61, 64–65, 67–68, 75, 96, 123, 128, 190–191, 194–195, 205–206, 213, 234, 249, 301 A-lattice 105, 107 F-lattice 106–108, 208, 248–249, 267 Laue 277, 281, 287–289, 292, 302 Laue symbol 281, 302 Law constancy of the angle 35 Limiting form 129–130, 138–139 Line defect 293, 295–296 Line lattice 9–10 Liquid 5–8, 293, 295 M Magnesium 150 Malonic acid 68 Metallic bonding 245–246, 248 Metal structure 248–252 Methane 150 Mg-type 249 Miller indices 14–15, 30, 34, 44–45, 129, 139, 154, 227, 279, 281, 284, 302 Mirror plane 38, 62, 66–67, 69, 75–77, 95–97, 99, 101, 105, 107, 119, 125, 130, 132, 147, 150, 153, 156, 166–167, 190, 195, 199, 202–203, 207–208, 210, 223, 226, 297, 302 Mixed crystals 265 Molecular dipole moment 166 Molecular structure 252 Molecular symmetry 147–149, 166, 212, 252 Monochromatic beam 277 Monoclinic 80, 82, 96–97, 103, 105–108, 118, 120–121, 124–125, 139–146, 173, 197–200, 208, 226, 282, 284–285, 305–306 Morphological axial ratio 50, 301 Morphology 7, 29–51, 64, 75, 120, 128, 154, 189, 212, 282 Mosaic blocks 299–300 Multiplicity 202–204, 206, 208, 210, 212–213 N NaCl 3, 155–156, 248, 256–257, 259, 261–262, 264, 266, 291, 295–296, 299–300 NaCl structure 256–257, 262, 266, 295, 299 NaCl-type 266 Naphthalene 1, 147–148 Nepheline 154 NiAs structure 262 NiAs-type 258, 262 Noble gas structure 252–253 Non-crystallographic point group 147, 253 Nucleation 32–33 Nucleus 32–35, 253, 300 Number of chemical formula units per unit cell 25, 289 Index O Octahedral coordination 248, 250, 256–258, 262 Octahedral hole 250, 256–258, 265–266, 290 Octahedron 44, 169, 250–251, 256–257, 262, 298, 308, 315 Olivine structure 265 One-circle reﬂection goniometer 39–40 Optical activity 154–155 Order-disorder transformation 269–270 Order (of a group) 101, 103, 126, 238 Order (of a rotation axis) 63, 95 Orthographic projection 50–51 Orthorhombic 84, 97–99, 101, 106, 108, 120–121, 124–125, 133, 139–146, 189–192, 200, 203, 212, 226, 278–280, 305–306 symmetry operation 71, 123, 213, 227, 238–239 Polar 65, 149–150, 153–156, 245, 263 Polar axis 155–156 pole 42–43 Pole distance 39–40 Pole of the face 138 α-Polonium 9, 251 Polymorphism 266–271 Polytypism 271 Powder diagram 279–280, 282 Powder pattern 280–281 Precession method 287 Principle of closest packing 245 Prismatic 31 Pyrene 147–148 Pyrite 154 Pyritohedron 169, 308 Pyroelectricity 156–166 P Q Packing eﬃciency 8, 250–252, 261, 263, 272–273 Parallelohedron 306 Pauling’s third rule 261–262 PDF index card 283 Pentagon-dodecahedron 308 Periodically homogeneous 7 Phenanthrene 147–148 Physical property 4 Piezoelectricity 155–156 Pinacoid 31, 34, 37–38, 53, 64, 68, 133, 139, 154, 306 Plagioclase 265 Planar 31, 147, 207–208, 268 Plane defect 293, 296–300 Plane lattice 9–10, 63, 67, 75–80, 107 Plastic deformation 252, 296 P-lattice 12, 80–99, 101, 103, 105–108, 118, 123, 206, 213, 251, 272, 282, 284–285 Pleochroism 3–4 Point defect 293–295 equivalent by translation 10, 63 group 38, 120, 123–188, 190, 195, 197–201, 203–204, 208, 210, 212–214, 223, 225–226, 237, 241–243, 253, 287, 289 lattice 9, 11–12, 14, 63, 66–67, 95–96, 103, 105–107, 109, 123, 189, 284, 301 symmetry elements 71, 75, 77, 96, 99, 101, 103, 123, 202, 204, 208 Quartz high 268, 270 low 155, 268, 270 structure 268 R Radius ratio 247, 253, 256–261 Rate of crystal growth 32 Real crystal 293, 299 Reciprocal lattice 282–288, 302 Reconstructive transformation 267–269 Reﬂection 39–40, 48, 61–63, 66, 68–71, 189–191, 202, 210, 233, 238–239, 277–278, 280–282, 286–287, 289, 302 Reﬂection goniometer 39–40, 48 Repetition operation 9, 61 Rhomb-dodecahedron 308–309 Rhombic dipyramid 306 Rhombic disphenoid 306 Rhombic prism 139, 238, 306 Rhombic pyramid 208, 306 Rhombohedral 107, 120, 226, 267, 271 Rhombohedron 107, 267, 307, 316 R-lattice 107–108, 123 Rotation 38–39, 44, 61–66, 68–71, 75, 80, 95, 97, 119, 124–125, 147–150, 153–156, 166–167, 189, 193–195, 199, 207, 223–226, 233, 237–239, 268, 287, 298, 303–304 353 354 Index Rotation axis 39, 62–66, 69, 95, 97, 125, 147, 150, 155–156, 167, 194, 199, 207, 223, 226, 303–304 Rotoinversion 38, 70–71, 119, 125, 153, 193, 210, 226, 304 Rotoinversion axis 70–71, 125, 210, 226, 304 Rotoreﬂection 71 Rotoreﬂection axis 71 Row Vector 225 Rutile 146, 211–212, 248, 256, 259, 262–263, 291 Rutile structure 212, 262–263 Rutile-type 259 S Schonﬂies symbol 126–127, 153, 201, 210 Schottky defect 294 Screw axis 69, 189, 193, 205, 210, 233–234, 268, 303 component 193–195, 303–304 dislocation 293, 296 rotation 69, 189, 193, 233, 239 Short symbol 125, 199 Single crystal 35, 64, 264, 287, 289, 296 SiO2 structure 262 Site symmetry 202–203, 205, 211–214 Sixfold rotation axis 65, 304 Small angle grain boundaries 293, 296–297, 300 Small circle 40–41, 44, 67 SnO2 structure 290 Solid solution 264–266, 269, 293–295 Space group C2 198, 200 C2/c 199 C2/m 199 Cc 198, 200 Cm 199–200 Ibm2 335 P1̄ 96, 108, 124, 200 P1 200, 239 P21 199–200 P2 199–200 P21 /b 21 /c 21 /n 235 P21 /c 199 P21 /m 199–200 P2/c 199–200 P2/m 2/m 2/m 99, 124, 190 P2/m 2/n 21 /a 335 P2/m 97–99, 103, 124, 190, 198–200, 203–206 P422 200 P42 bc 200 P4/m 3̄ 2/m 124, 206–207, 220, 251, 261, 291 P4/m 2/m 2/m 101, 124 P61 201, 205–206 P6/m 2/m 2/m 101, 124 Pba2 200 Pc 199–200 Pm 199–200 Pmm2 200–203, 208 Pna21 200, 203–204, 208 Pnc2 200 R 3̄ 2/m 108 Space lattice 9–16, 61, 65–68, 75, 80–94, 120, 166 Special form 120, 130, 133, 138, 271 Special plane lattice 75–79 Special position 145, 202–204, 210–213 Sphalerite 156, 260–261, 263, 266, 269 Sphalerite-type 266 Sphenoid 139, 146, 306 Spinel structure 256–257, 298 Stacking faults 293, 297 Statistically homogeneous 6–7 Steno 35 Stereographic projection 36–38, 40–42, 44, 48, 50–51 Structural axial ratio 50, 301 Subgroup 120, 124, 126, 133, 195, 198–199, 238–239 Substitutional solid solution 265 Substitution defect 294 Supergroup 126, 223, 238, 239 Superstructure 265, 269 Symmetry direction 97–101, 103–104, 108, 120–121, 123, 125, 130, 134, 151, 153, 210, 304 element 61–64, 66, 69–71, 75, 77–78, 80, 95–96, 108, 119–120, 123–125, 128–132, 134–135, 147, 149, 153, 189, 198–199, 201–202, 204, 206–208, 210, 212, 223, 226, 234, 237, 239, 241, 297, 302–304 operation 61–64, 66–71, 96, 101, 123, 126, 129, 132, 134–135, 138, 146, 156, 189–190, 193, 201, 204, 210, 213, 223–239, 242 operation matrix 223–237 principle 245 rules 95, 124–125, 243, 287, 289 Index T Tabular 31 Tartaric acid 155–156 Tautozonal 31–32 Tetragonal dipyramid 41, 132–135, 138, 146, 306 disphenoid 138, 146, 306 prism 37–38, 99, 129–130, 132–133, 138, 146, 306 pyramid 37–38, 41, 129–130, 134–135, 138, 146, 306 scalenohedron 135, 146, 306 trapezohedron 135, 146, 238, 306 Tetrahedral coordination 260–263 Tetrahedral hole 249–250, 256–258, 261 Tetrahedral pentagon-dodecahedron 308 Tetrahedron 169, 188, 260, 263, 268, 308, 315 Tetrahexahedron 308 Tetrakishexahedron 308 Thermal conductivity 4, 6, 252 Threefold rotation axis 64, 304 TiO2 58, 211, 259, 263 Topaz 44–50 Tourmaline 156 Transformation of ﬁrst coordination 267 Transformation involving changes in type of bonding 271 Transformation in secondary coordination 268, 270 Translational subgroup 239 Trapezohedron 135, 146, 238, 306–308 Triclinic 80–81, 96, 108, 120–121, 124–125, 139–146, 173, 200, 226, 305–306 Tridymite structure 268 Trigonal 88, 107–108, 119–121, 123–125, 139–140, 144, 147, 200, 226, 258, 299–300, 305, 307 Trigonal dipyramid 147, 307 Trigonal prism 258, 299–300, 307 Trigonal pyramid 226, 307 Trigonal trapezohedron 307 Trisoctahedron 308 Tristetrahedron 308 Twin 293, 297–300, 319 Twin element 297–300 Two-circle reﬂection goniometer Twofold rotation axis 303 39–40, 48 U Unit cell 10–12, 23–26, 30, 32, 67–68, 75, 80, 96–97, 99, 103, 105–107, 109, 202–207, 210, 213, 248–252, 262, 271, 281–282, 286, 289, 301–302 Unit length 48, 50 Unit mesh 10, 16, 65–67, 75–78, 80, 97, 99, 107 uvw 11–14, 17, 301 [uvw] 12–13, 16, 19, 26, 30, 32, 45, 99, 129, 223, 226, 301 <uvw> 129, 301 V Van der Waals bonding Vitamin B12 253 245–246 W Whisker 296 W-type 251 Wulﬀ net 40–45 Wurtzite structure 261 X X-ray 277–292, 302 X-ray diﬀraction 277–292 x, y, z 23, 25–26, 191, 193, 201–208, 224–228, 234, 236, 301 Z Zinc blende 260 ZnS 156 Zonal equation 16–19, 32, 45–46 Zone axis 31, 36, 39, 42, 45, 301 355 The Wulﬀ Net (reproduced by kind permission of Carl Zeiss, Oberkochen)

Descargar
# Crystallography